# SEMICONDUCTOR DEVICE PHYSICS AND...

### Transcript of SEMICONDUCTOR DEVICE PHYSICS AND...

SEMICONDUCTOR DEVICE PHYSICS AND DESIGN

Semiconductor Device Physicsand Design

UMESH K. MISHRAUniversity of California, Santa Barbara, CA, USA

and

JASPRIT SINGHThe University of Michigan, Ann Arbor, MI, USA

by

A C.I.P. Catalogue record for this book is available from the Library of Congress.

ISBN 978-1-4020-6480-7 (HB)ISBN 978-1-4020-6481-4 (e-book)

Published by Springer,P.O. Box 17, 3300 AA Dordrecht, The Netherlands.

www.springer.com

Printed on acid-free paper

All Rights Reservedc© 2008 Springer

No part of this work may be reproduced, stored in a retrieval system, or transmitted in any formor by any means, electronic, mechanical, photocopying, microfilming, recording or otherwise,without written permission from the Publisher, with the exception of any material suppliedspecifically for the purpose of being entered and executed on a computer system, for exclusiveuse by the purchaser of the work.

This book is dedicated to our parentsSrinibas Mishra and Sushila DeviGurcharn Singh and Gursharan Kaur

CONTENTS

Acknowledgements xii

Preface xiii

Introduction xx

1 Structural Properties of Semiconductors 11.1 INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.2 CRYSTAL STRUCTURE . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2

1.2.1 Basic Lattice Types . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2.2 Basic Crystal Structures . . . . . . . . . . . . . . . . . . . . . . . . . . 31.2.3 Notation to Denote Planes and Points in a Lattice: Miller Indices . . . . 71.2.4 Artificial Structures: Superlattices and Quantum Wells . . . . . . . . . 111.2.5 Surfaces : Ideal Versus Real . . . . . . . . . . . . . . . . . . . . . . . 121.2.6 Interfaces . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 151.2.7 Semiconductor Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . 15

1.3 LATTICE MISMATCHED STRUCTURES . . . . . . . . . . . . . . . . . . . . 171.4 STRAINED EPITAXY: STRAIN TENSOR . . . . . . . . . . . . . . . . . . . . 211.5 TECHNOLOGY CHALLENGES . . . . . . . . . . . . . . . . . . . . . . . . . 241.6 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 251.7 FURTHER READING . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27

2 Electronic levels in semiconductors 282.1 INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 282.2 PARTICLES IN AN ATTRACTIVE POTENTIAL:

BOUND STATES . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 292.2.1 Electronic levels in a hydrogen atom . . . . . . . . . . . . . . . . . . . 292.2.2 Electrons in a quantum well . . . . . . . . . . . . . . . . . . . . . . . . 30

2.3 ELECTRONS IN CRYSTALLINE SOLIDS . . . . . . . . . . . . . . . . . . . 332.3.1 Particle in a periodic potential: Bloch theorem . . . . . . . . . . . . . . 36

2.4 OCCUPATION OF STATES:DISTRIBUTION FUNCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . 41

vi

CONTENTS vii

2.5 METALS AND INSULATORS . . . . . . . . . . . . . . . . . . . . . . . . . . . 432.5.1 Electrons and Holes . . . . . . . . . . . . . . . . . . . . . . . . . . . . 45

2.6 BANDSTRUCTURE OF SOME IMPORTANTSEMICONDUCTORS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 462.6.1 Direct and indirect semiconductors . . . . . . . . . . . . . . . . . . . . 46

2.7 MOBILE CARRIERS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 502.7.1 Mobile electrons in metals . . . . . . . . . . . . . . . . . . . . . . . . . 502.7.2 Electrons and holes in semiconductors . . . . . . . . . . . . . . . . . . . 55

2.8 DOPING OF SEMICONDUCTORS . . . . . . . . . . . . . . . . . . . . . . . 602.9 DOPING IN POLAR MATERIALS . . . . . . . . . . . . . . . . . . . . . . . 652.10 TAILORING ELECTRONIC PROPERTIES . . . . . . . . . . . . . . . . . . . . 73

2.10.1 Electronic properties of alloys . . . . . . . . . . . . . . . . . . . . . . . 732.10.2 Electronic properties of quantum wells . . . . . . . . . . . . . . . . . . 73

2.11 STRAINED HETEROSTRUCTURES . . . . . . . . . . . . . . . . . . . . . . . 802.12 DEFECT STATES IN SOLIDS . . . . . . . . . . . . . . . . . . . . . . . . . . . 842.13 TECHNOLOGY ISSUES . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 862.14 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 862.15 FURTHER READING . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 90

3 Charge transport in materials 923.1 INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 923.2 CHARGE TRANSPORT: AN OVERVIEW . . . . . . . . . . . . . . . . . . . . 933.3 TRANSPORT AND SCATTERING . . . . . . . . . . . . . . . . . . . . . . . . 94

3.3.1 Quantum Mechanics and Scattering of electrons . . . . . . . . . . . . . 963.4 TRANSPORT UNDER AN ELECTRIC FIELD . . . . . . . . . . . . . . . . . . 104

3.4.1 Velocity–electric field relations in semiconductors . . . . . . . . . . . . 1043.5 SOME IMPORTANT ISSUES IN TRANSPORT . . . . . . . . . . . . . . . . . 1173.6 CARRIER TRANSPORT BY DIFFUSION . . . . . . . . . . . . . . . . . . . . 118

3.6.1 Drift and diffusion transport: Einstein’s relation . . . . . . . . . . . . . . 1213.7 CHARGE INJECTION AND QUASI-FERMI LEVELS . . . . . . . . . . . . . 124

3.7.1 Non-equilibrium Distributions . . . . . . . . . . . . . . . . . . . . . . . 1243.8 CARRIER GENERATION AND RECOMBINATION . . . . . . . . . . . . . . 125

3.8.1 Optical Absorption and Emission in Semiconductors . . . . . . . . . . . 1283.8.2 Schockley Read Hall Statistics . . . . . . . . . . . . . . . . . . . . . . . 133

3.9 CURRENT CONTINUITY(The law of conservationof electrons and holes separately) . . . . . . . . . . . . . . . . . . . . . . . . . . 137

3.10 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1423.11 FURTHER READING . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 145

4 Junctions in Semiconductors: P-N Diodes 1464.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1464.2 P-N JUNCTION IN EQUILIBRIUM . . . . . . . . . . . . . . . . . . . . . . . 1464.3 P-N DIODE UNDER BIAS . . . . . . . . . . . . . . . . . . . . . . . . . . . . 155

4.3.1 Drift and Diffusion Currents in the Biased Diode . . . . . . . . . . . . . 157

CONTENTS viii

4.3.2 Minority and Majority Currents in the p-n Diode . . . . . . . . . . . . . 1604.3.3 Narrow Diode Current . . . . . . . . . . . . . . . . . . . . . . . . . . . 160

4.4 REAL DIODES: CONSEQUENCES OF DEFECTS AND CARRIER GENER-ATION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1634.4.1 Generation-Recombination Currents . . . . . . . . . . . . . . . . . . . 164

4.5 Reverse Bias Characteristics . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1724.5.1 First Observation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1724.5.2 Quasi Fermi Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 175

4.6 HIGH-VOLTAGE EFFECTS IN DIODES . . . . . . . . . . . . . . . . . . . . . 1774.6.1 Forward Bias: High Injection Region . . . . . . . . . . . . . . . . . . . 1774.6.2 Reverse Bias: Impact Ionization . . . . . . . . . . . . . . . . . . . . . . 177

4.7 Avalanche Breakdown in a p-n junction . . . . . . . . . . . . . . . . . . . . . . 1784.7.1 Reverse Bias: Zener Breakdown . . . . . . . . . . . . . . . . . . . . . . 180

4.8 DIODE APPLICATIONS: AN OVERVIEW . . . . . . . . . . . . . . . . . . . . 1834.8.1 Applications of p-n diodes . . . . . . . . . . . . . . . . . . . . . . . . . 1834.8.2 The Solar Cell and Photodetector . . . . . . . . . . . . . . . . . . . . . 1844.8.3 The uses of diode non-linearity (Mixers, Multipliers, Power Detectors) . 1894.8.4 Power Devices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 191

4.9 Light emitting diode (LED) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1934.9.1 Emission Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1934.9.2 Carrier Injection and Spontaneous Emission . . . . . . . . . . . . . . . . 197

4.10 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2044.11 DESIGN PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2114.12 FURTHER READING . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 214

5 Semiconductor Junctions 2165.1 INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2165.2 METAL INTERCONNECTS . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2165.3 METAL SEMICONDUCTOR JUNCTION:

SCHOTTKY BARRIER . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2195.3.1 Schottky Barrier Height . . . . . . . . . . . . . . . . . . . . . . . . . . 2195.3.2 Capacitance Voltage Characteristics . . . . . . . . . . . . . . . . . . . . 2235.3.3 Current Flow across a Schottky Barrier: Thermionic Emission . . . . . . 2235.3.4 Comparison of Schottky and p-n diodes . . . . . . . . . . . . . . . . . 227

5.4 METAL SEMICONDUCTOR JUNCTIONSFOR OHMIC CONTACTS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 229

5.5 INSULATOR-SEMICONDUCTOR JUNCTIONS . . . . . . . . . . . . . . . . . 2305.5.1 Insulator-Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 230

5.6 SEMICONDUCTOR HETEROJUNCTIONS . . . . . . . . . . . . . . . . . . . 2325.6.1 Abrupt p-n heterojunction . . . . . . . . . . . . . . . . . . . . . . . . . 2325.6.2 Graded p-n heterojunction . . . . . . . . . . . . . . . . . . . . . . . . . 2375.6.3 Quasi-electric fields . . . . . . . . . . . . . . . . . . . . . . . . . . . . 238

5.7 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 240

CONTENTS ix

5.8 FURTHER READING . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 245

6 Bipolar Junction Transistors 2466.1 INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2466.2 BIPOLAR TRANSISTOR: A CONCEPTUAL PICTURE . . . . . . . . . . . . . 2486.3 STATIC CHARACTERISTICS: CURRENT-VOLTAGE

RELATION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2526.3.1 Current Flow in a BJT . . . . . . . . . . . . . . . . . . . . . . . . . . . 2536.3.2 BJT Biasing in circuits . . . . . . . . . . . . . . . . . . . . . . . . . . . 2596.3.3 Current-Voltage: The Ebers-Moll Model . . . . . . . . . . . . . . . . . . 259

6.4 DEVICE DESIGN AND DEVICE PERFORMANCE PARAMETERS . . . . . . 2626.5 BJT DESIGN LIMITATIONS: NEED FOR BAND

TAILORING AND HBTs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2656.5.1 The Generalized Moll-Ross Relationship . . . . . . . . . . . . . . . . . 2696.5.2 How much β do we need? . . . . . . . . . . . . . . . . . . . . . . . . . 270

6.6 SECONDARY EFFECTS IN REAL DEVICES . . . . . . . . . . . . . . . . . . 2746.6.1 High Injection: The Kirk Effect . . . . . . . . . . . . . . . . . . . . . . 2746.6.2 High Injection: Thermal Effects . . . . . . . . . . . . . . . . . . . . . . 2806.6.3 Base Width Modulation: The Early Effect . . . . . . . . . . . . . . . . 2806.6.4 Drift Effects in the Base: Nonuniform Doping . . . . . . . . . . . . . . . 2826.6.5 Avalanche Breakdown . . . . . . . . . . . . . . . . . . . . . . . . . . . 2836.6.6 Low Injection Effects and Current Gain . . . . . . . . . . . . . . . . . . 2846.6.7 Current Crowding Effect . . . . . . . . . . . . . . . . . . . . . . . . . . 284

6.7 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2906.8 DESIGN PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3016.9 FURTHER READING . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 303

7 Temporal Response Of Diodes and Bipolar Transistors 3047.1 INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3047.2 MODULATION AND SWITCHING OF A P -N DIODE: AC RESPONSE . . . 304

7.2.1 Small-Signal Equivalent Circuit of a p-n Diode . . . . . . . . . . . . . . 3067.2.2 Switching characteristics of diodes . . . . . . . . . . . . . . . . . . . . . 312

7.3 Temporal Response of a Schottky Diode . . . . . . . . . . . . . . . . . . . . . . 3177.4 BIPOLAR JUNCTION TRANSISTORS:

A CHARGE-CONTROL ANALYSIS . . . . . . . . . . . . . . . . . . . . . . . 3187.4.1 Junction Voltages at Saturation . . . . . . . . . . . . . . . . . . . . . . . 324

7.5 HIGH-FREQUENCY BEHAVIOR OF A BJT . . . . . . . . . . . . . . . . . . . 3257.5.1 Bipolar Transistor Small-Signal Equivalent Circuit . . . . . . . . . . . . 3337.5.2 Attenuation and Phase Shift of a Traveling Electron Wave . . . . . . . . 3367.5.3 Small Signal Figures of Merit . . . . . . . . . . . . . . . . . . . . . . . 340

7.6 BIPOLAR TRANSISTORS: A TECHNOLOGYROADMAP . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3457.6.1 Si Bipolar Technology . . . . . . . . . . . . . . . . . . . . . . . . . . . 3457.6.2 Si-Based HBTs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 346

CONTENTS x

7.6.3 GaAs/AlGaAs HBTs . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3477.6.4 InGaAs/InAlAs and InGaAs/InP HBTs . . . . . . . . . . . . . . . . . . 347

7.7 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3487.8 DESIGN PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 355

8 Field Effect Transistors 3568.1 INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3568.2 JFET AND MESFET: CHARGE CONTROL . . . . . . . . . . . . . . . . . . . 3568.3 CURRENT-VOLTAGE CHARACTERISTICS . . . . . . . . . . . . . . . . . . 362

8.3.1 The Ohmic Regime . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3628.3.2 A Nearly Universal Model for FET Behavior : The Saturation Regime . . 368

8.4 HFETs: INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3758.5 CHARGE CONTROL MODEL FOR THE MODFET . . . . . . . . . . . . . . 378

8.5.1 Modulation Efficiency . . . . . . . . . . . . . . . . . . . . . . . . . . . 3858.6 POLAR MATERIALS AND STRUCTURES . . . . . . . . . . . . . . . . . . . 388

8.6.1 Polar Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3888.6.2 Polar HFET Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . 394

8.7 DESIGN ISSUES IN HFETS . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3958.7.1 n+ Cap Layers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3958.7.2 Maximizing 2DEG Conductivity . . . . . . . . . . . . . . . . . . . . . . 3968.7.3 Back-barriers to Substrate Injection . . . . . . . . . . . . . . . . . . . . 3988.7.4 Gate Recess Design . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4008.7.5 Field Plates . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4018.7.6 Comparison of two disparate material systems:

AlInAs/GaInAs and AlGaN/GaN . . . . . . . . . . . . . . . . . . . . . 4028.7.7 Non-idealities in state-of-the-art transistors . . . . . . . . . . . . . . . . 403

8.8 SMALL AND LARGE SIGNAL ISSUES AND FIGURES OF MERIT . . . . . 4118.8.1 Small-Signal Characteristics . . . . . . . . . . . . . . . . . . . . . . . . 4118.8.2 Power-frequency limit . . . . . . . . . . . . . . . . . . . . . . . . . . . 4158.8.3 Classes of operation of transistor power amplifiers and necessary device

characteristics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4168.9 Implications on device technology and circuits . . . . . . . . . . . . . . . . . . . 4218.10 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4228.11 DESIGN PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4318.12 FURTHER READING . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 432

9 Field Effect Transistors: MOSFET 4339.1 INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4339.2 MOSFET: DEVICES AND IMPACT . . . . . . . . . . . . . . . . . . . . . . . 4349.3 METAL-OXIDE-SEMICONDUCTOR CAPACITOR . . . . . . . . . . . . . . . 4379.4 CAPACITANCE-VOLTAGE CHARACTERISTICS

OF THE MOS STRUCTURE . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4489.5 MOSFET OPERATION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 454

9.5.1 Current-Voltage Characteristics . . . . . . . . . . . . . . . . . . . . . . 454

CONTENTS xi

9.5.2 Substrate Bias Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . 4589.5.3 Depletion and Enhancement MOSFETs . . . . . . . . . . . . . . . . . . 4629.5.4 Complementary MOSFETs . . . . . . . . . . . . . . . . . . . . . . . . 464

9.6 IMPORTANT ISSUES AND FUTURE CHALLENGES IN REAL MOSFETS . 4669.6.1 Subthreshold Conduction . . . . . . . . . . . . . . . . . . . . . . . . . . 4669.6.2 Mobility Variation with Gate Bias . . . . . . . . . . . . . . . . . . . . . 4729.6.3 Important Effects in Short-Channel MOSFETs . . . . . . . . . . . . . . 4759.6.4 Parasitic Bipolar Transistors and Latch-up in CMOS . . . . . . . . . . . 478

9.7 SUMMARY . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4809.8 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4819.9 DESIGN PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4859.10 FURTHER READING . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 487

10 Coherent Transport and Mesoscopic Devices 48910.1 INTRODUCTION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48910.2 ZENER-BLOCH OSCILLATIONS . . . . . . . . . . . . . . . . . . . . . . . . 49110.3 RESONANT TUNNELING . . . . . . . . . . . . . . . . . . . . . . . . . . . . 49210.4 QUANTUM INTERFERENCE EFFECTS . . . . . . . . . . . . . . . . . . . . 49710.5 MESOSCOPIC STRUCTURES . . . . . . . . . . . . . . . . . . . . . . . . . . 500

10.5.1 Conductance Fluctuations and Coherent Transport . . . . . . . . . . . . 50010.5.2 Coulomb Blockade Effects . . . . . . . . . . . . . . . . . . . . . . . . 502

10.6 MAGNETIC SEMICONDUCTORSAND SPINTRONICS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 505

10.7 PROBLEMS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 50910.8 Further Reading . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 510

A List of Symbols 511

B Boltzmann Transport Theory 517B.1 BOLTZMANN TRANSPORT EQUATION . . . . . . . . . . . . . . . . . . . . 517

B.1.1 Diffusion-Induced Evolution of fk(r) . . . . . . . . . . . . . . . . . . . 518B.1.2 External Field-Induced Evolution of fk(r) . . . . . . . . . . . . . . . . 519B.1.3 Scattering-Induced Evolution of fk(r) . . . . . . . . . . . . . . . . . . . 519

B.2 AVERAGING PROCEDURES . . . . . . . . . . . . . . . . . . . . . . . . . . . 526

C Density of States 529

D Important Properties of Semiconductors 535

E Beyond the Depletion Approximation 544

F Design of Graded Heterojunctions for Bipolar Transistors 548

Index 552

ACKNOWLEDGEMENTS

Writing a book on Semiconductor Device Physics and Design is never complete and proba-bly never completely satisfying. The field is vast and diverse and it is difficult to decide whatshould be included in the book and what should not be. Of course it is always a good idea forauthors to not discuss areas that they are unfamiliar with and that helped narrow the scope ofthis book down greatly!! In all seriousness the flow and content of this book is a consequenceof the classes that we have taught at UC Santa Barbara and The University of Michigan andreflects what we believe can be taught in a manner that emphasizes physical understanding withan appropriate amount of rigor. At UCSB Prof Kroemer had developed a two-quarter sequenceclass on device physics which I (Umesh Mishra) took over when I arrived at UCSB in 1990.I developed the class over the past 15 years using his notes as a foundation and the new con-tent is reflected in this book. I am grateful to Prof Kroemer for allowing me to include partsof his notes and homework problems in this book. Prof Mark Rodwell contributed to under-standing that the answer to the question “How much β do we need” is application dependent.Prof Steve Long and Prof Rakesh Lal helped with the diode- applications section. Prof TomasPalacios of MIT contributed to the AlGaN/GaN HEMT description. Dr Karthik Krishnamurthy(RFMD) allowed use of his descriptions of classes of FET amplifiers. Lastly, Dr Jeff Shealy (VPRFMD) and Dr Rama Vetury (RFMD) are thanked for their help in illustrating how the mobilephone uses multiple semiconductor technologies for optimal system performance as describedin the introduction. Discussions with Profs. Lorenzo Faraone, Brett Nener and John Dell at TheUniversity of Western Australia were helpful (and fun). Drs., Lee McCarthy, Ilan Ben-Yaacov,Nicholas Fichtenbaum and Siddharth Rajan contributed significantly in helping the text layoutof the book. We thank several of our colleagues who contributed figures to the book and theyhave been acknowledged at the appropriate places. Umesh would like to thank his wife Susanfor not asking the question “Isn’t it finished?” too many times. Jasprit would like to thank hiswife Teresa for drawing numerous figures and YuhRennn Wu for providing device design studiesfor field effect transistors. We would also like to thank the editors at Springer Verlag for theirenthusiasm and support.

xii

PREFACE

It would not be an exaggeration to say that semiconductor devices have transformed humanlife. From computers to communications to internet and video games these devices and thetechnologies they have enabled have expanded human experience in a way that is unique inhistory. Semiconductor devices have exploited materials, physics and imaginative applications tospawn new lifestyles. Of course for the device engineer, in spite of the advances, the challengesof reaching higher frequency, lower power consumption, higher power generation etc. providenever ending excitement. Device performances are driven by new materials, scaling, and newdevice concepts such as bandstructure and polarization engineering. Semiconductor devices havemostly relied on Si but increasingly GaAs, InGaAs and heterostructures made from Si/SiGe,GaAs/AlGaAs etc have become important. Over the last few years one of the most excitingnew entries has been the GaN based devices that provide new possibilities for lighting, displaysand wireless communications. New physics based on polar charges and polar interfaces hasbecome important as a result of the nitrides. For students to be able to participate in this andother exciting arena, a broad understanding of physics, materials properties and device conceptsneed to be understood. It is important to have a textbook that teaches students and practicingengineers about all these areas in a coherent manner. While this is an immense challenge wehave attempted to do so in this textbook by judiciously selecting topics which provide depthwhile simultaneously providing the basis for understanding the ever expanding breath of devicephysics.

In this book we start out with basic physics concepts including the physics behind polar het-erostructures and strained heterostructures. We then discuss important devices ranging fromp − n diodes to bipolar and field effect devices. An important distinction users will find in thisbook is the discussion we have presented on how interrelated device parameters are on systemfunction. For example, how much gain is needed in a transistor, and what kind of device char-acteristics are needed. Not surprisingly the needs depend upon applications. The specificationsof transistors employed in A/D or D/A converter will be different from those in an amplifier in acell phone. Similarly the diodes used in a laptop will place different requirements on the deviceengineer than diodes used in a mixer circuit. By relating device design to device performanceand then relating device needs to system use the student can see how device design works in realworld.

It is known that device dimensions and geometries are now such that one cannot solve de-vice problems analytically. However, simulators do not allow students to see the physics of

xiii

PREFACE xiv

the problem and how intelligent choices on doping, geometry and heterostructures will impactdevices. We have tried to provide this insight by carefully discussing and presenting analyticalmodels and then providing simulation based advanced results. The goal is to teach the studenthow to approach device design from the point of view some one who wants to improve devicesand can see the opportunities and challenges. The end of chapter problems chosen in this bookare carefully chosen to allow students to test their knowledge by solving real life problems.

Umesh K. MishraUniversity of California

Santa Barbara

Jasprit SinghThe University of Michigan

Ann Arbor

Lesson Plan for a 1 Semester course: 35-40 lectures R© : Reading Assignment

Structural Properties: 2 Lectures

R© Crystals: Lattices, Basis, and Planes

• Heteroepitaxy: Strain tensor,

• Polar Effects: Spontaneous and Piezoelectric Effects

Electronic levels in Semiconductors: 3 Lectures

R© Particles in attractive potentials, quantum wells

R© Electrons in crystalline materials

• Important bandstructures

R© Distribution functions

R© Metals and insulators

• Mobile carriers

• Doping: Dopants and polar doping

• Heterostructures: Lower dimensional systems

• Strained heterostructures

Charge Transport: 4 lectures

• Transport and scattering

• Velocity-Field relations

• Transport by diffusion

• Carrier generation and recombination

• Current continuity equation

P-N Diodes- Steady State: 3 lectures

• P-N junction under equilibrium

• Junction under bias: Ideal case

• Non-Ideal effects

• High voltage effects

R© Diode applications

xv

LESSON PLAN FOR SEMESTER COURSE xvi

Semiconductor Junctions: 3 lectures

R© Metal interconnects

• Schottky Barrier Diode

• Ohmic contacts

R© Insulator semiconductor junctions

• Semiconductor heterojunctions

Bipolar Junction Transistor- Steady State: 4 lectures

• Current voltage relations

• Device design and optimization

• Secondary effects in BJTs

• Heterojunction bipolar transistors

Bipolar Devices- Temporal Response: 4 lectures

• P-N diode: Small and large signal

• Schottky diode temporal response

• Bipolar transistor: Charge control model

• High frequency response of bipolar transistors

• Technology roadmap and device needs

Field Effects Transistors- MESFET and HFETs: 6 lectures

• JFET and MESFET: Charge control and current-voltage

• Charge control for MODFETs

• Polar HFETs: Charge Control

• HFET Design issues

• Temporal response and high power issues

LESSON PLAN FOR SEMESTER COURSE xvii

MOSFET: 6 lectures

• MOS Capacitor

• Current-voltage characteristics

• Sub-threshold current flow

• Short channel and scaling issues in FETs

Mesoscopic Devices: 3 lectures

• Zener-Bloch oscillations

• Resonant tunneling devices

• Quantum interference effects

• Conductance fluctuations and Coulomb Blockade

• Spintronics: Overview

Lecture Plan for a two-quarter sequence of 10 weeks each with 3.5 hours of lecture per weekThe basis of this lecture plan is the experience gained from teaching graduate students at

UCSB. The experience has been that the class size is larger in the first quarter than in the secondwhere a large group of graduate students from many disciplines attend the class to understandimportant devices at a level higher than their exposure as undergraduates. It is therefore proposedthat the first quarter cover p-n junctions, heterojunctions, HBTs, FETs and MOSFETs operatingunder DC conditions. Here drift diffusion analysis and thermionic emission will be employed todescribe current flow. In the next quarter, it is suggested that the Boltzmann transport analysiscontained in the Appendix be covered and the basis for the drift-diffusion fomalism explained.Next the methodology for deriving the high frequency properties of devices such as HBTs andFETs along with their equivalent circuits is covered. Lastly, High Electron Mobility Transistorsand Gallium Nitride based devices may be covered

Quarter 1

Lecture 1: Shockley-Read-Hall analysis of lifetime (this introduces the concept of lifetime es-sential for p-n junction analysis)

Lecture 2: P-n junction electrostatics, P-n junction transport (Forward)

Lecture 3: P-n junction transport (Reverse) and Applications

Lecture 4: Schottky barrier electrostatics and current transport

Lecture 5: Graded materials, Quasi-fields and heterojuncions

Lecture 6: HBTs, Generalized Moll-Ross relationship Early effect, Kirk effect(quick descrip-tion)

Lecture 7: FETs and gradual channel analysis

Lecture 8: High Aspect Ratio design analysis

Lecture 9: MOS Capacitor and MOSFETs

Lecture 10: Non-ideal effects

Quarter 2

Lecture 1 and 2: Boltzmann Transport Equation and consequences (Drift Diffusion Equationderivation, relaxation times)

Lecutre 3: Charge Control Model (Description and application to HBTs)

Lecutre 4: Ramo-Shockley Theorem and the Kirk effect

Lecutre 5: High Frequency properties of HBTs

Lecutre 6: Equivalenbt Circuit derivation of HBTs; Figures of Merit

xviii

LECTURE PLAN FOR QUARTER xix

Lecutre 7: HEMTs; Electrostatics

Lecutre 8: Gallium Nitride; Polarization and device design

Lecutre 9: HEMTs; I-V characteristics, Design Issues

Lecutre 10: HEMTs and FETs; High Frequency Performance

INTRODUCTION

The pace of semiconductor materials and device development has been staggering, and theimpact on human society monumental. Leading this advance has been the development of thesilicon-based MOSFET device and its continuous high level of integration. Moore’s Law (shownin figure .1), which predicts the doubling of device density every 18 months, has been the gov-erning maxim of the industry. Sustaining Moore’s Law has required:

• The development of lithography tools to achieve the 45 nm gate length MOSFETs releasedinto production in 2006

• The continuous scaling of silicon wafers to 12 inch diameters (2005) and 15 inch in thefuture to enable large chip yields per wafer

• Tremendous advances in interconnect technology

• Device innovations to continuously maintain charge control and low gate leakage as theoxide thickness is scaled down along with the gate length

Though most of the chip and dollar volume of the industry has been driven by Si-based CMOSarchitecture, there have been critical advances made in other semiconductor technologies. Theability to grow epitaxial layers in a controlled fashion, initially by Liquid Phase Expitaxy (LPE)and Vapor Phase Epitaxy (VPE) and currently by Metalorganic Vapor Phase Epitaxy (MOVPE)and Molecular Beam Epitaxy (MBE), has enabled the compound semiconductor industry tomature into a small but critical component of the total space. The impact has been felt in both theelectronics and photonics arenas. In the former, development of the Heterojunction Field EffectTransistor (HFET) and the Heterojunction Bipolar Transistor (HBT) has had a large impact onanalog and mixed signal applications. In the low noise receiver area, GaAs and InP based HFETsare the preferred technology. The GaAs-based HBT is preferred for power amplifiers in cellularphones. The Si/SiGe HBT is being actively used in mixed signal applications such as A/Dconverters and in BiCMOS implementations.

In the optical arena, the development of Light Emitting Diodes (LEDs), lasers, and detectorshas been profound. LEDs are used in prolific applications such as signage displays and remotecontrols as well as in communication devices. The advent of GaN-based LEDs has raised thepossibility of a revolutionary advance in lighting with the emergence of solid-state lighting.

xx

INTRODUCTION xxi

Figure .1: Illustration of Moore’s Law.

Lasers and detectors have been the enabling elements in optical communications. Lasers havealso enabled entertainment devices such as the DVD.

The continuous expansion of the material and device tool set has enabled system designersto choose the correct technology for the application, resulting in phenomenal advances at thesystem level. This is best understood by studying a commercial widespread system - the cellularphone. Consider the Motorola V551 phone, illustrated in figure .2. The key components of thetransmit/receive chain in any radio architecture are the switch, filter, modulator/demodulator,LNA, mixer, gain blocks, and power amplifier. Integrating the different chips into a total radiosolution places varied specifications on the different chips used to achieve the radio solution. Inturn, these specifications drive the selection of the active device and process technology that isused to implement the functionality of the particular chip.

As an example of this technology selection process, consider the POLARIS total radio solutionfrom RFMD, which is a highly integrated transciever that performs all functions of the handsetradio section, operating under GSM/GPRS/EDGE standards. The POLARIS chipset consists ofthe following functional blocks, shown in figure .3:

1. The RF 2722 quad-band RF receiver.

2. The RF 3146 POWER STAR PA module with integrated power control.

3. The RF 6001 digital filter, fractional-N PLL, modulator, and power amplifier ramp control.

INTRODUCTION xxii

Figure .2: The Motoral V551 cellular phone. Picture courtesy of A. Upton, R. Vetury, and J.Shealy, RFMD.

The RF 2722 fulfills the functional requirement of a quad band LNA and mixer. It includesa VCO and supports very low IF (VLIF) and direct conversion receive (DCR) architectures,thus eliminating the need for IF SAW and RF interstage filters. The complexity of the circuitarchitecture needed and the noise and linearity requirements placed by the LNA and mixer makethe technology of choice SiGe-BiCMOS.

The RF 3146 fulfills the functional requirement of a power amplifier. It includes considerablepower control circuitry and can be driven from the DAC output, thus eliminating the need fordirectional couplers, detector diodes, and other power control circuitry. GaAs HBT technologyis chosen for this component in order to achieve the optimum combination of high power, highPAE, and excellent linearity requirements at the frequency of operation.

The RF 6001 fulfills the functional requirements of a synthesizer and signal processor. Toachieve the optimum combination of low cost, high levels of integration, and low power con-sumption, Si CMOS technology is chosen for this component.

INTRODUCTION xxiii

SiGe-BiCMOS

technology

GaAs HBT

technology

Si CMOS

technology

Figure .3: The POLARIS total radio solution from RFMD. Picture courtesy of A. Upton, R.Vetury, and J. Shealy, RFMD.

So what does the future hold for semiconductor based device development? There are brickwalls facing the conventional scaling of CMOS circuits. Beyond the year 2012 and the 18 nmnode, several of the pathways to continued scaling are not obvious. Also, the power dissipation inthe chip threatens to set a thermal limit to the size and the speed of processors in the future. Thisis best illustrated in figure .4, where it is clear that today’s chips seem hotter than a hot plate,and chips of the future in a tongue-in-cheek prediction may rival the sun’s surface (obviouslyimpossible). Hence now is the time for all of us to rethink the conventional CMOS scalingparadigm and consider what new pathways may open up. Could compound semiconductors,with their high electron mobilities and velocities, play a role in achieving high clock speedsand reduced power levels? Could large bandgap materials such as Gallium Nitride play a rolein applications where the operating temperature is continuously rising? Are there completelynew devices such as Carbon Nanotubes (CNTs) which operate in the ballistic regime of electronand hole transport that can emerge as the dark horse in future complementary circuits? Or ismolecular electronics, the use of the electronic states of the molecule to achieve computation, the

INTRODUCTION xxiv

Figure .4: Chip power density is increasing exponentially with time.

answer? Is the control of electron spin rather than the total charge in the channel of the device(the emerging field of spintronics) the holy grail? Are architectures based on single electrontransistors a high density, low power alternative?

The future is murky, and we as scientists and engineers have to help clarify it. This book seeksto provide an understanding of the materials, devices, and technology of the various alternativesbeing considerred, with detail appropriate to the maturity of the technology. A bias towardscompound semiconductors is obvious, as Si-based devices have been exclusively addressed overthe years in various forms. We hope that this book serves a function to academics teaching coursematerials, engineers and researchers in the field tackling the murky future, and today’s graduatestudents who will be the great engineers of tomorrow.

Watt

s/c

m2

Watt

s/c

m2

1

10

100

1000

1.5 μm 1 μm 0.7 μm 0.5 μm 0.35 μm 0.25 μm 0.18 μm 0.13 μm 0.1 μm 0.07 μm

i386i386

i486i486

PentiumPentium®®

PentiumPentium®® ProPro

PentiumPentium®® IIII

PentiumPentium®® IIIIIIHot plateHot plateHot plateHot plate

RocketNozzleRocketRocketNozzleNozzleRocketNozzleRocketRocketNozzleNozzle

Nuclear ReactorNuclear ReactorNuclear ReactorNuclear ReactorNuclear ReactorNuclear Reactor

PentiumPentium®® 44

Power doubles every 4 yearsPower doubles every 4 years

55--year projection: 200W total, 125 W/cmyear projection: 200W total, 125 W/cm2 2 !!

P=VI: 75W @ 1.5V = 50 A!P=VI: 75W @ 1.5V = 50 A!

Chapter 1

STRUCTURAL PROPERTIES OFSEMICONDUCTORS

1.1 INTRODUCTION

In this text we will be exploring state of the art electronic devices that drive modern informa-tion technology. Essentially all of these devices are based on semiconductors. Semiconductorstructures have also provided the stages for exploring questions of fundamental physics. As tech-nology advances the number of semiconductors that are used in technology steadily increases.Indeed many innovations have arisen as a result of using new materials and their heterostruc-tures. Thus while Si, GaAs and InP have been most widely used, other materials like InAs, GaN,InN etc. are finding important uses as well. It is important to recognize that the ability to exam-ine fundamental physics issues and to use semiconductors in state of the art device technologiesdepends critically on the purity and perfection of the semiconductor crystal.

Semiconductor structures can operate at their potential only if they can be grown with a highdegree of crystallinity and if impurities and defects can be controlled. For high structural qualityit is essential that a high quality substrate be available. This requires growth of bulk crystalswhich are then sliced and polished to allow epitaxial growth of thin semiconductor regions in-cluding heterostructures.

In this chapter we will discuss important semiconductor crystal structures. We also discussstrained lattice structures and the strain tensor for such crystals. Strained epitaxy and its resultantconsequences are now widely exploited in semiconductor physics. High speed SiGe devices arebased on strained systems as are InGaAs and AlGaN/GaN microwave devices.

We will start with some general properties of crystalline materials and then discuss somespecific crystal structures important for semiconductors.

1

2 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

1.2 CRYSTAL STRUCTURE

As noted above high performance semiconductor devices are based on crystalline materials.Crystals are periodic structures made up of identical building blocks. While in “natural” crystalsthe crystalline symmetry is fixed by nature, new advances in crystal growth techniques are allow-ing scientists to produce artificial crystals with modified crystalline structure. These advancesdepend upon being able to place atomic layers with exact precision and control during growth,leading to “low dimensional systems”. To define the crystal structure, two important conceptsare introduced. The lattice represents a set of points in space forming a periodic structure. Thelattice is by itself a mathematical abstraction. A building block of atoms called the basis is thenattached to each lattice point yielding the physical crystal structure.

To define a lattice one defines three vectors a1, a2, a3, such that any lattice point R′ can beobtained from any other lattice point R by a translation

R′ = R + m1a1 + m2a2 + m3a3 (1.2.1)

where m1, m2, m3 are integers. Such a lattice is called a Bravais lattice . The crystallinestructure is now produced by attaching the basis to each of these lattice points.

lattice + basis = crystal structure (1.2.2)

The translation vectors a1, a2, and a3 are called primitive if the volume of the cell formed bythem is the smallest possible. There is no unique way to choose the primitive vectors. It ispossible to define more than one set of primitive vectors for a given lattice, and often the choicedepends upon convenience. The volume cell enclosed by the primitive vectors is called theprimitive unit cell .

Because of the periodicity of a lattice, it is useful to define the symmetry of the structure. Thesymmetry is defined via a set of point group operations which involve a set of operations appliedaround a point. The operations involve rotation, reflection and inversion. The symmetry playsa very important role in the electronic properties of the crystals. For example, the inversionsymmetry is extremely important and many physical properties of semiconductors are tied tothe absence of this symmetry. As will be clear later, in the diamond structure (Si, Ge, C, etc.),inversion symmetry is present, while in the Zinc Blende structure (GaAs, AlAs, InAs, etc.), it isabsent. Because of this lack of inversion symmetry, these semiconductors are piezoelectric, i.e.,when they are strained an electric potential is developed across the opposite faces of the crystal.In crystals with inversion symmetry, where the two faces are identical, this is not possible.

1.2.1 Basic Lattice Types

The various kinds of lattice structures possible in nature are described by the symmetry groupthat describes their properties. Rotation is one of the important symmetry groups. Lattices canbe found which have a rotation symmetry of 2π, 2π

2 , 2π3 , 2π

4 , 2π6 . The rotation symmetries are

1.2. CRYSTAL STRUCTURE 3

denoted by 1, 2, 3, 4, and 6. No other rotation axes exist; e.g., 2π5 or 2π

7 are not allowed becausesuch a structure could not fill up an infinite space.

There are 14 types of lattices in 3D. These lattice classes are defined by the relationships be-tween the primitive vectors a1, a2, and a3, and the angles α, β, and γ between them. We willfocus on the cubic and hexagonal lattices which underly the structure taken by all semiconduc-tors.

There are 3 kinds of cubic lattices: simple cubic, body centered cubic, and face centered cubic.

Simple cubic: The simple cubic lattice shown in figure 1.1is generated by the primitive vec-tors

ax, ay, az (1.2.3)

where the x, y, z are unit vectors.

Body-centered cubic : The bcc lattice shown in figure 1.2 can be generated from the simplecubic structure by placing a lattice point at the center of the cube. If x, y, and z are threeorthogonal unit vectors, then a set of primitive vectors for the body-centered cubic lattice couldbe

a1 = ax, a2 = ay, a3 =a

2(x + y + z) (1.2.4)

A more symmetric set for the bcc lattice is

a1 =a

2(y + z − x), a2 =

a

2(z + x − y), a3 =

a

2(x + y − z) (1.2.5)

Face Centered Cubic: Another equally important lattice for semiconductors is the face-centeredcubic (fcc) Bravais lattice shown in figure 1.3. To construct the face-centered cubic Bravaislattice add to the simple cubic lattice an additional point in the center of each square face. Thisform of packing is called close-packed.

A symmetric set of primitive vectors for the face-centered cubic lattice (see figure 1.3) is

a1 =a

2(y + z), a2 =

a

2(z + x), a3 =

a

2(x + y) (1.2.6)

The face-centered cubic and body-centered cubic Bravais lattices are of great importance,since an enormous variety of solids crystallize in these forms with an atom (or ion) at eachlattice site. Essentially all semiconductors of interest for electronics and optoelectronics have aclose-packed structure, either fcc or Hexagonal Close Pack(HCP) as discussed below.

1.2.2 Basic Crystal Structures

Diamond and Zinc Blende StructuresMost semiconductors of interest for electronics and optoelectronics have an underlying fcc lat-tice, with two atoms per basis. The coordinates of the two basis atoms are

(000) and (a

4,a

4,a

4) (1.2.7)

4 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

x

y

z

a3

a2

a1a

a3

a2a1

z

y

x

a

a3

a2 a1

(a)

(b)

(c)

Figure 1.1: A simple cubic lattice showing the primitive vectors. The crystal is produced byrepeating the cubic cell through space.

1.2. CRYSTAL STRUCTURE 5

a

Two atoms per basisBasis atoms same: Diamond structureBasis atoms different: Zinc blende

Figure 1.2: The body centered cubic lattice along with a choice of primitive vectors.

z

y

x

a3

a2a1

a

fcc lattice

Figure 1.3: Primitive basis vectors for the face centered cubic lattice.

6 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

a

Figure 1.4: The zinc blende crystal structure. The structure consists of the interpenetratingfcc lattices, one displaced from the other by a distance (a

4a4

a4 ) along the body diagonal. The

underlying Bravais lattice is fcc with a two atom basis. The positions of the two atoms is (000)and (a

4a4

a4 ).

Since each atom lies on its own fcc lattice, such a two atom basis structure may be thought of astwo inter-penetrating fcc lattices, one displaced from the other by a translation along the bodydiagonal direction (a

4a4

a4 ).

Figure 1.4 shows this important structure. If the two atoms of the basis are identical, thestructure is called diamond. Semiconductors such as Si, Ge, C, etc., fall in this category. If thetwo atoms are different, the structure is called the Zinc Blende structure. Semiconductors suchas GaAs, AlAs, CdS, etc., fall in this category. Semiconductors with diamond structure are oftencalled elemental semiconductors, while the Zinc Blende semiconductors are called compoundsemiconductors. The compound semiconductors are also denoted by the position of the atoms inthe periodic chart, e.g., GaAs, AlAs, InP are called III-V (three-five) semiconductors while CdS,HgTe, CdTe, etc., are called II-VI (two-six) semiconductors.

Hexagonal Close Pack Structure The hexagonal close pack (hcp) structure is an importantlattice structure and many semiconductors such as BN, AlN, GaN, SiC, etc., also have this un-derlying lattice (with a two-atom basis). The hcp structure is formed as shown in figure 1.5a.Imagine that a close-packed layer of spheres is formed. Each sphere touches six other spheres,leaving cavities, as shown in figure 1.5. A second close-packed layer of spheres is placed on topof the first one so that the second layer sphere centers are in the cavities formed by the first layer.The third layer of close-packed spheres can now be placed so that center of the spheres do notfall on the center of the starting spheres (left side of figure 1.5a) or coincide with the centers ofthe starting spheres (right side of figure 1.5). These two sequences, when repeated, produce thefcc and hcp lattices.

1.2. CRYSTAL STRUCTURE 7

(a)

(b)

+

Spheres on the starting layer

Center s of spheres on the second layer

Center s of spheres on the third layer

+ + +

+ + + + + + + + + +

+ + + +

+

fcchcp

a b

c

a

b

a

(c)

Figure 1.5: (a) A schematic of how the fcc and hcp lattices are formed by close packing ofspheres. (b) The hcp structure is produced by two interpenetrating hexagonal lattices with adisplacement discussed in the text. (c) Arrangement of lattice points on an hcp lattice.

In figure 1.5b and figure 1.5c we show the detailed positions of the lattice points in the hcplattice. The three lattice vectors a1, a2, a3 are shown as a, b, c. The vector a3 is denoted by cand the term c-axis refers to the orientation of a3. The hexagonal planes are displaced from eachother by a1/3 + a2/3 + a3/2. In an ideal structure, if | a |=| a1 |=| a2 |,

c

a=

√8

3(1.2.8)

In table 1.1 we show the structural and some important electronic properties of some importantsemiconductors. Note that two or more semiconductors are randomly mixed to produce an alloy,AxB1−x, the lattice constant of the alloy is given by Vegard’s law according to which the alloylattice constant is the weighted mean of the lattice constants of the individual components

aalloy = xaA + (1 − x)aB (1.2.9)

1.2.3 Notation to Denote Planes and Points in a Lattice: Miller Indices

To represent the directions and planes in a crystalline structure an agreed upon scheme isused. The planes or directions are denoted by a series of integers called the Miller indices.

8 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

Zinc Blende and Wurtzite CRYSTAL STATIC LATTICE

MATERIAL STRUCTURE BANDGAP DIELECTRIC CONSTANT DENSITY

(EV) CONSTANT (¯) (gm-cm 3 )

C DI 5.50, I 5.570 3.56683 3.51525Si DI 1.1242, I 11.9 5.431073 2.329002SiC ZB 2.416, I 9.72 4.3596 3.166Ge DI 0.664, I 16.2 5.6579060 5.3234BN HEX 5.2, I ε|| = 5.06 6.6612 2.18 ε = 6.85 2.5040 BN ZB 6.4, I 7.1 3.6157 3.4870BP ZB 2.4, I 11. 4.5383 2.97BAs ZB 4.777 5.22AlN W 6.2,D ε = 9.14 3.111 3.255 4.981 AlP ZB 2.45,I 9.8 5.4635 2.401AlAS ZB 2.153,I 10.06 5.660 3.760AlSb ZB 1.615,I 12.04 6.1355 4.26GaN W 3.44,D ε||=10.4 3.175 6.095

ε = 9.5 5.158 GaP ZB 2.272,I 11.11 5.4505 4.138GaAs ZB 1.4241,D 13.18 5.65325 5.3176GaSb ZB 0.75,D 15.69 6.09593 5.6137InN W 1.89,D 3.5446 6.81 8.7034 InP ZB 1.344,D 12.56 5.8687 4.81InAs ZB 0.354,D 15.15 6.0583 5.667InSb ZB 0.230,D 16.8 6.47937 5.7747ZnO W 3.44,D ε||= 8.75 3.253 5.67526

ε = 7.8 5.213 ZnS ZB 3.68,D 8.9 5.4102 4.079ZnS W 3.9107,D ε = 9.6 3.8226 4.084

6.2605 ZnSe ZB 2.8215,D 9.1 5.6676 5.266ZnTe ZB 2.3941,D 8.7 6.1037 5.636 CdO R 0.84,I 21.9 4.689 8.15CdS W 2.501,D ε = 9.83 4.1362 4.82

6.714CdS ZB 2.50,D 5.818 CdSe W 1.751,D ε||=10.16 4.2999 5.81 ε = 9.29 7.0109CdSe ZB 6.052 CdTe ZB 1.475,D 10.2 6.482 5.87PbS R 0.41,D* 169. 5.936 7.597PbSe R 0.278,D* 210. 6.117 8.26PbTe R 0.310,D* 414. 6.462 8.219

a =c =

a =c =

a =c =

a =c =

a =c =

a =c =

a =c =

a =c =

Data are given at room temperature values (300 K).Key: DI: diamond; HEX: hexagonal; R: rocksalt; W: wurtzite; ZB: zinc blende; *: gap at L point; D: direct; I: indirect ε||: parallel to c-axis; ε : perpendicular to c-axis

Table 1.1: Structure, lattice constant, and density of some materials at room temperature

1.2. CRYSTAL STRUCTURE 9

These indicies are obtained using the following:

(1) Define the x, y, z axes (primitive vectors).(2) Take the intercepts of the plane along the axes in units of lattice constants.(3) Take the reciprocal of the intercepts and reduce them to the smallest integers.The notation (hkl) denotes a family of parallel planes.The notation (hkl) denotes a family of equivalent planes.

To denote directions, we use the smallest set of integers having the same ratio as the directioncosines of the direction.

In a cubic system the Miller indices of a plane are the same as the direction perpendicularto the plane. The notation [ ] is for a set of parallel directions; < > is for a set of equivalentdirection. Figure 1.6 shows some examples of the use of the Miller indices to define planes for acubic system.

Example 1.1 The lattice constant of silicon is 5.43 A. Calculate the number of siliconatoms in a Si MOSFET with dimensions of 50μm × 2μm × 1μm.

Silicon has a diamond structure which is made up of the fcc lattice with two atoms on eachlattice point. The fcc unit cube has a volume a3. The cube has eight lattice sites at the cubeedges. However, each of these points is shared with eight other cubes. In addition, thereare six lattice points on the cube face centers. Each of these points is shared by twoadjacent cubes. Thus the number of lattice points per cube of volume a3 are

N(a3) =8

8+

6

2= 4

In silicon there are two silicon atoms per lattice point. The number density is, therefore,

NSi =4 × 2

a3=

4 × 2

(5.43 × 10−8)3= 4.997 × 1022 atoms/cm3

The number in the MOSFET are

NMOSFET = 4.997 × 1012 atoms

Example 1.2 Calculate the surface density of Ga atoms on a Ga terminated (001) GaAssurface.

In the (001) surfaces, the top atoms are either Ga or As leading to the terminology Gaterminated (or Ga stabilized) and As terminated (or As stabilized), respectively. A squareof area a2 has four atoms on the edges of the square and one atom at the center of thesquare. The atoms on the square edges are shared by a total of four squares. The totalnumber of atoms per square is

N(a2) =4

4+ 1 = 2

The surface density is then

NGa =2

a2=

2

(5.65 × 10−8)2= 6.26 × 1014 cm−2

10 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

ATOMS ON THE (111) PLANE

Could be either Ga or As

1 bond connecting an adjacent plane on one side

3 bonds connecting an adjacent plane on the othe r side

ATOMS ON THE (110) PLANE

Each atom has 4 bonds:• 2 bonds in the (110) plane• 1 bond connects each atom to adjacent (110) planes

Cleaving adjacent planes requires breaking 1 bond per atom

ATOMS ON THE (001) PLANE

2 bonds connect each atom to adjacent (001) plane

Atoms are either Ga or As in a GaAs crystal

Cleaving adjacent planes requires breaking 2 bonds per atom

Figure 1.6: Some important planes in the cubic system along with their Miller indices. Thisfigure also shows how many bonds connect adjacent planes. This number determines how easyor difficult it is to cleave the crystal along these planes.

1.2. CRYSTAL STRUCTURE 11

1.2.4 Artificial Structures: Superlattices and Quantum Wells

Epitaxial crystal growth techniques such as molecular beam epitaxy (MBE) and metal or-ganic chemical vapor deposition (MOCVD) allow one to have monolayer (∼3 A) control in thechemical composition of the growing crystal. Nearly every semiconductor extending from zerobandgap (α-Sn,HgCdTe) to large bandgap materials such as ZnSe,CdS,AlN etc., has been grownby epitaxial techniques. This allows growth of quantum wells and heterostructures where elec-tronic properties can be altered. Heteroepitaxial techniques allow one to grow heterostructureswith atomic control, one can change the periodicity of the crystal in the growth direction. Thisleads to the concept of superlattices where two (or more) semiconductors A and B are grownalternately with thicknesses dA and dB respectively. The periodicity of the lattice in the growthdirection is then dA + dB . A (GaAs)/(AlAs) heterostructure is illustrated in figure 1.7.

In figure 1.8, we show a cross-sectional TEM image of a structure containing InGaAs/GaAsand AlGaAs/GaAs superlattices, indicating the precision with which these structures can beproduced using modern epitaxial growth techniques.

Ga

As

Al

Figure 1.7: Arrangement of atoms in a (GaAs)/(AlAs) heterostructure grown along (001) direc-tion.

12 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

Figure 1.8: (b) This transmission electron microscope picture shows the precision with whichsemiconductor compositions can be altered by epitaxial growth techniques. Individual semicon-ductor layers as thin as 10 A can be produced.

1.2.5 Surfaces : Ideal Versus Real

The arrangement of atoms on the surface can be quite different from that in the bulk. Thebulk crystal structure is decided by the internal chemical energy of the atoms forming the crystalwith a certain number of nearest neighbors, second nearest neighbors, etc. Since the surface,the number of neighbors is suddenly altered, the spatial geometries which were providing thelowest energy configuration in the bulk may not provide the lowest energy configuration at thesurface. Thus, there is a readjustment or “reconstruction” of the surface bonds toward an energyminimizing configuration.

An example of such a reconstruction is shown for the GaAs surface in figure 1.9. The figure(a) shows an ideal (001) surface where the topmost atoms form a square lattice. The surfaceatoms have two nearest neighbor bonds (Ga-As) with the layer below, four second neighborbonds (e.g., Ga-Ga or As-As) with the next lower layer, and four second neighbor bonds withinthe same layer. We could denote the ideal surface by the symbol C(1×1), representing the factthat the surface periodicity is one unit by one unit along the square lattice along [110] and [110].

1.2. CRYSTAL STRUCTURE 13

4 Å

4 Å

(2 x 4 unit cell)

(a) (b)

Top layer As atomsSecond layer Ga atomsThird layer As atoms

IDEAL SURFACE RECONSTRUCTED SURFACE

Figure 1.9: The structure (a) of the unreconstructed GaAs (001) arsenic-rich surface. The miss-ing dimer model (b) for the GaAs (001) (2×4) surface. The As dimers are missing to create a 4unit periodicity along one direction and a two unit periodicity along the perpendicular direction.

The reconstructed surfaces that occur in nature are generally classified as C(2×8) or C(2×4) etc.,representing the increased periodicity along the [110] and [110] respectively. The C(2×4) caseis shown schematically in figure 1.9, for an arsenic stabilized surface (i.e., the top monolayer isAs). The As atoms on the surface form dimers (along [110] on the surface to strengthen theirbonds. In addition, rows of missing dimers cause a longer range ordering as shown to increasethe periodicity along the [110] direction to cause a C(2×4) unit cell. Similar reconstructionoccurs for Si surfaces as well.

Example 1.1 Calculate the planar density of atoms on the (111) surface of GaAs.

As can be seen from figure 1.6, we can form a triangle on the (111) surface. There arethree atoms on the tips of the triangle. These atoms are shared by six other similartriangles. There are also 3 atoms along the edges of the triangle which are shared by twoadjacent triangles. Thus the number of atoms in the triangle are

3

6+

3

2= 2

The area of the triangle is√

3a2/2. The density of GaAs atoms on the surface is then7.29 × 1014 cm−2.

14 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

(a)

(b)

Figure 1.10: (a) Cross-sectional TEM images of a typical AlGaN/GaN HFET structure grown ona SiC substrate. First, a 50 nm AlN nucleation layer is grown, followed by a 450 nm GaN bufferlayer and a 29 nm AlGaN cap. A large number of defects are formed at the AlN/GaN interface,but many of the defects are annihilated as the GaN layer is thickened. The AlGaN cap layer iscoherently strained on top of the bulk GaN. No new defects are formed at this interface. (b) Highresolution X-ray diffraction scan of this structure. The close match between the data and theoryindicates the high crystalline quality of the structure. Images courtesy of Prof. J. Speck, UCSB.

1.2. CRYSTAL STRUCTURE 15

1.2.6 Interfaces

Like surfaces, interfaces are an integral part of semiconductor devices. We have already dis-cussed the concept of heterostructures and superlattices which involve interfaces between twosemiconductors. These interfaces are usually of high quality with essentially no broken bonds(see figure 1.10), except for dislocations in strained structures (to be discussed later). There is,nevertheless, an interface roughness of one or two monolayers which is produced because ofeither non-ideal growth conditions or imprecise shutter control in the switching of the semicon-ductor species. The general picture of such a rough interface is as shown in figure 1.11a forepitaxially grown interfaces. The crystallinity and periodicity in the underlying lattice is main-tained, but the chemical species have some disorder on interfacial planes. Such a disorder canbe quite important in many electronic devices. In figure 1.11b we show a TEM for a GaAs/AlAsinterface.

One of the most important interfaces in electronics is the Si/SiO2 interface. This interfaceand its quality is responsible for essentially all of the modern consumer electronic revolution.This interface represents a situation where two materials with very different lattice constants andcrystal structures are brought together. However, in spite of these large differences the interfacequality is quite good. In figure 1.12 we show a TEM cross-section of a Si/SiO2 interface. Itappears that the interface has a region of a few monolayers of amorphous or disordered Si/SiO2

region creating fluctuations in the chemical species (and consequently in potential energy) acrossthe interface. This interface roughness is responsible for reducing mobility of electrons andholes in MOS devices. It can also lead to “trap” states, which can seriously deteriorate deviceperformance if the interface quality is poor.

Finally, we have the interfaces formed between metals and semiconductors. Structurally, theseimportant interfaces are hardest to characterize and are usually produced in presence of hightemperatures. Metal-semiconductor interfaces involve diffusion of metal elements along withcomplex chemical reactions.

1.2.7 Semiconductor Defects

Semiconductor devices have both unintended and intentional defects. Some unintentional de-fects are introduced due to either thermodynamic considerations or the presence of impuritiesduring the crystal growth process. In general, defects in crystalline semiconductors can be char-acterized as i) point defects; ii) line defects; iii) planar defects and iv) volume defects. Thesedefects are detrimental to the performance of electronic and optoelectronic devices and are to beavoided as much as possible.Localized DefectsA localized defect affects the periodicity of the crystal only in one or a few unit cells. There area variety of point defects, as shown in figure 1.13. Defects are present in any crystal and theirconcentration is given roughly by the thermodynamics relation

Nd

NTot= kd exp

(− Ed

kBT

)(1.2.10)

where Nd is the vacancy density, NTot the total site density in the crystal, Ed the defect formation

16 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

Dl

AlAs (perfect crystal)

GaAs (perfect crystal)

GaAs

GaAs

2.1 ML AlAs

(a)

(b)

Figure 1.11: (a) A schematic picture of the interfaces between materials with similar latticeconstants such as GaAs/AlAs. No loss of crystalline lattice and long range order is sufferedin such interfaces. The interface is characterized by islands of height Δ and lateral extent λ.(b) High resolution cross-sectional TEM image along with schematic diagram of (411A) GaAswith a very thin (2.1 monolayer) AlAs layer in the middle. A small amount of roughness canbe observed at the interface. TEM image courtesy of S. Shimomura and S. Hiyamizu of OsakaUniversity.

energy, kd is a dimensionless parameter with values ranging from 1 to 10 in semiconductors, andT , the crystal growth temperature. Defect formation energy is in the range of an eV for mostsemiconductors.DislocationsIn contrast to point defects, line defects (called dislocations) involve a large number of atomicsites that can be connected by a line. Dislocations are produced if, for example, an extra halfplane of atoms are inserted (or taken out) of the crystal as shown in figure 1.14. Such dislocationsare called edge dislocations. Dislocations can also be created if there is a slip in the crystal sothat part of the crystal bonds are broken and reconnected with atoms after the slip. In the nitridetechnology where alternate substrates are used, dislocation densities can be quite large.

1.3. LATTICE MISMATCHED STRUCTURES 17

SiO2

SiRowsof Siatoms

Figure 1.12: The tremendous success of Si technology is due to the Si/SiO2 interface. In spiteof the very different crystal structure of Si and SiO2, the interface is extremely sharp, as shownin the TEM picture in this figure. TEM image courtesy of Bell Labs.

1.3 LATTICE MISMATCHED STRUCTURES

It is relatively easy to grow heterostructures where the overlayer lattice constant is the same orsimilar to that of the substrate. In such lattice matched epitaxy the interface quality can be veryhigh with essentially negligible interface defects and atomically abrupt interface. However oneoften needs structures where there is lattice mismatch between the overlayer and the substrate.The motivation for lattice mismatched epitaxy is two fold:

i) Incorporation of built-in strain: When a lattice mismatched semiconductor is grown on asubstrate and the thickness of the overlayer is very thin, the overlayer has a built-in strain. Thisbuilt-in strain has important effects on the electronic and optoelectronic properties of the materialand can be exploited for high performance devices. It can be exploited in nitride heterostructuresto effectively dope structures. It can also be exploited in Si/SiGe systems.

18 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

Vacancy

Self interstitial

Impurity interstitial

Substitutional

POINT DEFECTS

• Effect is localized to a few atomic sites

TYPICAL POINT DEFECTS IN CRYSTALS

Figure 1.13: A schematic showing some important point defects in a crystal.

ii) New effective substrate: High quality substrates are only available for Si, GaAs and InP(sapphire, SiC and quartz substrates are also available and used for some applications). Sincemost semiconductors are not lattice-matched to these substrates a solution that has emerged isto grow a thick overlayer on a mismatched substrate. If the conditions are right, dislocations aregenerated and eventually the overlayer forms its own substrate. This process allows a tremen-dous flexibility in semiconductor technology. Not only can it, in principle, resolve the substrateavailability problem, it also allows the possibility of growing GaAs on Si, CdTe on GaAs, GaNon SiC etc. Thus different semiconductor technologies can be integrated on the same wafer.

In figure 1.15 we show a TEM image of an InP/InAs double-barrier resonant tunneling device(DBRT). The InP barriers are 5 nm wide, enclosing a 15 nm InAs quantum dot. The InP iscoherently strained, with no dislocations created at the interfaces. The sharpness of the interfaceswas determined to be 1-3 lattice spacings.

Coherent and Incoherent StructuresConsider situation shown schematically in figure 1.16 where an overlayer with lattice constantaL is grown on a substrate with lattice constant aS . The strain between the two materials isdefined as

ε =aS − aL

aL(1.3.1)

If the lattice constant of the overlayer is maintained to be aL, it is easy to see that after every 1/εbonds between the overlayer and the substrate, either a bond is missing or an extra bond appearsas shown in figure 1.16b. In fact, there would be a row of missing or extra bonds since we havea 2-dimensional plane. These defects are the dislocations discussed earlier.

An alternative to the incoherent case is shown in figure 1.16c. Here all the atoms at the in-terface of the substrate and the overlayer are properly bonded by adjusting the in-plane lattice

1.3. LATTICE MISMATCHED STRUCTURES 19

Row of atoms have only 3 nearest neighbor bonds

Figure 1.14: A schematic showing the presence of a dislocation. This line defect is produced byadding an extra half plane of atoms.

Figure 1.15: TEM image of an InP/InAs double-barrier resonant tunneling device (DBRT) con-sisting of 5 nm InP barriers surrounding a 15 nm InAs quantum dot. The InP is coherentlystrained, with no dislocations created at the interfaces. Image courtesy of M. Bjork, Lund Uni-versity.

20 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

(a)

(b)

(c)

n bonds: substrate

n + 1 bonds: epilayer

Substrate

Overlayer

aL > aS aL < aS

GROWTH WITH DISLOCATIONS

n bonds: substrate

n–1 bonds: epilayer

DISLOCATION FREE

n~ 1ε

Figure 1.16: (a) An overlayer with one lattice constant is placed without distortion on a substratewith a different lattice constant. (b) Dislocations are generated at positions where the interfacebonding is lost. (c) The case is shown where the overlayer is distorted so that no dislocation isfree and coherent with the substrate.

constant of the overlayer to that of the substrate. This causes the overlayer to be under strainand the system has a certain amount of strain energy. This strain energy grows as the overlayerthickness increases. In the strained epitaxy, the choice between the state of the structure shownin figure 1.16b and the state shown in figure 1.16c is decided by free energy minimization con-siderations. The general observations can be summarized as follows:

For small lattice mismatch (ε < 0.03), the overlayer initially grows in perfect registry withthe substrate, as shown in figure 1.16c. However, as noted before, the strain energy will growas the overlayer thickness increases. As a result, it will eventually be favorable for the overlayer

1.4. STRAINED EPITAXY: STRAIN TENSOR 21

to generate dislocations. In simplistic theories this occurs at an overlayer thickness called thecritical thickness , dc, which is approximately given by

dc∼= aS

2|ε| (1.3.2)

where aS is the lattice constant of the substrate and ε the lattice mismatch. In reality, the point ingrowth where dislocations are generated is not so clear cut and depends upon growth conditions,surface conditions, dislocation kinetics, etc. However, one may use the criteria given by equation1.3.2 for approximately characterizing two regions of overlayer thickness for a given latticemismatch. Below critical thickness, the overlayer grows without dislocations and the film isunder strain. Under ideal conditions above critical thickness, the film has a dislocation array,and after the dislocation arrays are generated, the overlayer grows without strain with its freelattice constant.

If the strain value is greater than 0.03 one can still have strained epitaxy but the growth occursin the island mode where islands of the over-layer are formed. Such self-assembled islands arebeing used for quantum dot structures.

Epitaxy beyond the critical thickness is important to provide new effective substrates for newmaterial growth. For these applications the key issues center around ensuring that the disloca-tions generated stay near the overlayer-substrate interface and do not propagate into the overlayeras shown in figure 1.17. A great deal of work has been done to study this problem. Often thinsuperlattices in which the individual layers have alternate signs of strain are grown to “trap” or“bend” the dislocations. It is also useful to build the strain up gradually.

In recent years, the GaN material system has seen much progress in electronic and optoelec-tronic applications. Since GaN substrates are still not readily available, it is typically grown onAl2O3 (sapphire) or SiC , neither of which are closely lattice matched to GaN. The resultingmaterial is therefore highly dislocated. Many of the dislocations propagate upwards and areterminated at the surface. In figure 1.18a, we show a cross-sectional transmission electron mi-croscope image of GaN grown on sapphire. The vertical lines propagating upwards from thehighly defective interface are dislocations. Figure 1.18b is an atomic force microscope (AFM)image of the GaN surface. The black pits are dislocations that have propagated upwards. Alsoevident are the atomic steps that are typical of GaN surfaces. Such surface reconstructions weredescribed in section 1.2.5. Note that these atomic steps are always terminated by a dislocation.

In figure 1.18c, we show an AFM image of the surface of dislocation-free GaN. In contrast tothe dislocated material in figure 1.18b, there are no pits visible on the surface, and the surfacestep structure is smooth and continuous.

1.4 STRAINED EPITAXY: STRAIN TENSOR

Growth of an epitaxial layer whose lattice constant is close, but not equal, to the lattice con-stant of the substrate can result in a coherent strain. What is the strain tensor in such epitaxy?The strain tensor determines how the electronic properties are altered. If the strain is small onecan have monolayer-by-monolayer. In this case the lattice constant of the epitaxial layer in thedirections parallel to the interface is forced to be equal to the lattice constant of the substrate.

22 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

:Missing rows of atoms

Region with few dislocations

Dislocations are confined

SubstrateSubstrate

Figure 1.17: Strained epitaxy above critical thickness . The left hand side figure shows a desir-able structure in which the dislocations are confined near the overlayer-substrate interface. Onthe right hand side, the dislocations are penetrating the overlayer.

The lattice constant of the epitaxial perpendicular to the substrate will be changed by the Poissoneffect . These two cases are depicted in figure 1.16c. This type of coherently strained crystal iscalled pseudomorphic .

For layer-by-layer growth, the epitaxial semiconductor layer is biaxially strained in the planeof the substrate, by an amount ε‖, and uniaxially strained in the perpendicular direction, by anamount ε⊥. For a thick substrate, the in-plane strain of the layer is determined from the bulklattice constants of the substrate material, aS , and the layer material, aL:

e‖ =aS

aL− 1

= ε (1.4.1)

Since the layer is subjected to no stress in the perpendicular direction, the perpendicular strain,ε⊥, is simply proportional to ε‖:

ε⊥ =−ε‖σ

(1.4.2)

where the constant σ is known as Poisson’s ratio .Noting that there is no stress in the direction of growth it can be simply shown that for the

strained layer grown on a (001) substrate (for an fcc lattice)

σ =c11

2c12(1.4.3)

εxx = ε‖εyy = εxx

εzz =−2c12

c11ε‖

εxy = 0

εyz = 0

εzx = 0

1.4. STRAINED EPITAXY: STRAIN TENSOR 23

surface

Al2O3

GaN

interface

dislocations

(a)

(b) (c)

Figure 1.18: (a) Cross-sectional TEM image of GaN grown heteroepitaxially on sapphire, in-dicating the highly defective interface and the dislocations that propagate upwards. (b) AFMsurface image of the dislocated GaN , showing the atomic step structure which is typical of GaNsurfaces. The black dots are dislocations that have propagated upwards to the surface. (c) AFMsurface image of non-dislocated GaN, exhibiting a smooth and continuous step structure. Imagescourtesy of P. Fini and H. Marchand of UCSB.

24 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

while in the case of strained layer grown on a (111) substrate

σ =c11 + 2c12 + 4c44

2c11 + 4c12 − 4c44

εxx =

[2

3− 1

3

(2c11 + 4c12 − 4c44

c11 + 2c12 + 4c44

)]ε‖

εyy = εxx

εzz = εxx

εxy =

[−1

3− 1

3

(2c11 + 4c12 − 4c44

c11 + 2c12 + 4c44

)]ε‖

εyz = εxy

εzx = εyz (1.4.4)

In general, the strained epitaxy causes a distortion of the lattice and, depending upon thegrowth orientation, the distortions produce a new reduced crystal symmetry. It is importantto note that for (001) growth, the strain tensor is diagonal while for (111), and several otherdirections, the strain tensor has nondiagonal terms. The nondiagonal terms can be exploited toproduce built-in electric fields in certain heterostructures as will be discussed in the next section.

An important heterostructure system involves growth of hcp lattice-based AlGaN or InGaNon a GaN substrate along the c-axis. In this case the strain tensor is given by (aL is the substratelattice constant, aS is overlayer lattice constant)

εxx = εyy =aS

aL− 1

εzz = −2c13

c33εxx (1.4.5)

This strain is exploited to generate piezoelectric effect based interface charge as discussed inthe next chapter. Such a charge can cause effective doping in heterostructures as discussed inChapter 2. In table 1.1 we provide values of elastic constant of several important semiconductors.

1.5 TECHNOLOGY CHALLENGES

Metal and insulator (glass) technologies have been around for thousands of years. Com-pared to these semiconductor technology is relatively new. Semiconductors need to be extremely“pure” if they are to be useful. Defect densities of a percent may have minimal effect on metalsand insulators, but will ruin a semiconductor device. For most high performance devices, defectdensities of less than one part in 100 million are needed

Semiconductor substrate technology is available (i.e., bulk crystals can be grown in sufficientsize/purity) for a handful of materials. These include Si, GaAs, InP, and Ge, which are widelyavailable and SiC, Al2O3, and GaSb, etc., which are available only in small pieces (a few squarecentimeters) and are very expensive. Since most semiconductors do not have a substrate availablefrom either bulk crystal growth or another lattice matched substrate, this severely restricts the

1.6. PROBLEMS 25

Material C11(N/m2) C12(N/m2) C41(N/m2)

Si 1.66 x 1011 0.64 x 1011 0.8 x 1011

Ge 1.29 x 1011 0.48 x 1011 0.67 x 1011

GaAs 1.2 x 1011 0.54 x 1011 0.59 x 1011

C 10.76 x 1011 1.25 x 1011 5.76 x 1011

Material C13(N/m2) C33(N/m2)

GaN 10.9 x 1011 35.5 x 1011

AlN 12 x 1011 39.5 x 1011

Table 1.2: Elastic constant for some fcc and hcp based semiconductors. (For Si, Ge, GaAs see H.J. McSkimin and P. Andreatch, J. Appl. Phys., 35, 2161 (1964) and D. I. Bolef and M. Meres, J.Appl. Phys., 31, 1010 (1960). For nitrides see J. H. Edgar, Properties of III-V Nitrides, INSPEC,London (1994) and R. B. Schwarz, K. Khachaturyan, and E. R. Weber, Appl. Phys. Lett., 74,1122 (1997).)

use of a wide range of semiconductors. In table 1.3 we show an overview of some importantsubstrates and issues in semiconductor technology.

1.6 PROBLEMS

Problem 1.1 A 10.0 μm Si epitaxial layer is to be grown. The Si flux is 1014 cm−2 s−1.How long will it take to grow the film if the sticking coefficient for Si atoms is 0.95?

Problem 1.2 A Si wafer is nominally oriented along the (001) direction, but is found to becut 2◦ off, toward the (110) axis. This off axis cut produces “steps” on the surface whichare 2 monolayers high. What is the lateral spacing between the steps of the 2◦ off-axiswafer?

Problem 1.3 Conduct a literature search to find out what the lattice mismatch is betweenGaAs and AlAs at 300 K and 800 K. Calculate the mismatch between GaAs and Si at thesame temperatures.

Problem 1.4 In high purity Si crystals, defect densities can be reduced to levels of1013 cm−3. On an average, what is the spacing between defects in such crystals? Inheavily doped Si, the dopant density can approach 1019 cm−3. What is the spacingbetween defects for such heavily doped semiconductors?

26 CHAPTER 1. STRUCTURAL PROPERTIES OF SEMICONDUCTORS

Statue / ISSUESI M P O R T A N T S U B S T R A T E S

1. Silicon (Si) Mature, 12-inch diameter. Next generation

15-inch diameter.

2. Gallium Arsenide (GaAs) Mature, 6-inch diameter.

3. Indium Phosphide (InP) Mature, brittle, maximum diameter 4 inches.

4. Silicon Carbide (SiC) Developing technology, 3-inch diameter in

production. Micropipe density 1 cm-2 for

n-type and 100 cm-2 for semi-insulating.

5. Germanium (Ge) 6-inch diameter. Limited supply. Water-

soluble oxide.

6. Sapphire (Al2O3) Hydrothermal growth. 4-inch diameter

available. Low thermal conductivity.

7. Aluminum Nitride (AlN) 1-inch diameter. Early stages of

development, sublimation growth technique.

8. Gallium Nitride (GaN)

9. Indium Antimonide (InSb)

10. Zinc Oxide (ZnO)

2-inch diameter substrates by HVPE.

Dislocation density 106 cm-2.

2-inch diameter, early stages of

development.

Hydrothermal growth. 2-inch diameter

available. Dislocation density < 100 cm-2 for

n-type.

Table 1.3: A brief overview of important substrates available in semiconductor technology.

Problem 1.5 Assume that a Ga-As bond in GaAs has a bond energy of 1.0 eV. Calculatethe energy needed to cleave GaAs in the (001) and (110) planes.

Problem 1.6 Consider a hcp structure shown in the text. Prove the relation given byc/a =

√8/3 = 1.633.

Problem 1.7 Why are entropy considerations unimportant in dislocation generation?

Problem 1.8 A coherently strained quantum well laser has to made from InxGa1−xAs ona GaAs substrate. If the minimum thickness of the region is 50 A, calculate the maximum

1.7. FURTHER READING 27

composition of In that can be tolerated. Assume that the lattice constant of the alloy can belinearly interpolated from its components.

Problem 1.9 Assume that in a semiconductor alloy, the lattice constant scales as a linearweighted average. Find the composition of the InxGa1−xAs alloy that lattice matches withan InP substrate.

Problem 1.10 Calculate the critical thickness for the growth of AlAs on a GaAs substrate.

Problem 1.11 A 100 A In0.2Ga0.8As film is grown on a GaAs substrate. The film iscoherent. Calculate the strain energy per cm2 in the film.

Problem 1.12 Consider a coherently grown film of Si0.8Ge0.2 grown on a Si substrate.Calculate the thickness of the film at which the strain energy density (eV cm−2) becomesequal to the energy density arising from a square array of dislocations in the film.

Assume that the dislocations are on a planar square grid with one broken bond per spacingof a/ε where a is the film lattice constant and ε is the strain. The energy per broken bondis 1.0 eV.

1.7 FURTHER READING

• Crystal Structure

– M. M. Woolfson, An Introduction to Crystallography, Cambridge University Press(1997).

– McGraw-Hill Encyclopedia of Science and Technology, Volume 4, McGraw-Hill(1997).

– A. C. Gossard (ed.), Epitaxial Microstructures in Semiconductors and Semimetals, Volume 40, Academic Press (1994).

– G. Benedek (ed.), Point and Extended Defects in Semiconductors, Plenum Publish-ing Press (1989).

– Landolt-Bornstein, Numerical Data and Functional Relationships in Science andTechnology, (O. Madelung, M. Schultz, and H. Weiss, eds.), Springer (1985).

• Strained Structures

– J. F. Nye, Physical Properties of Crystals: Their Representation by Tensors andMatrices, Oxford University Press (1987).

– T. Ikeda, Fundamentals of Piezoelectricity, Oxford University Press (1990).

– E. Bernardini, V. Fiorentini, and D. Vanderbilt, Spontaneous Polarization, andPiezoelectric Constant of III-V Nitrides, Physical Review B, vol. 56, p. R10024(1997).

– J. H. Edgar, Properties of Group III Nitrides, INSPEC, London (1994).

Chapter 2

ELECTRONIC LEVELSIN SEMICONDUCTORS

2.1 INTRODUCTION

Semiconductor electronic and optoelectronic devices depend upon how electrons inside ma-terials behave and how they are influenced by external perturbations which may be electrical,electromagnetic, mechanical, or magnetic, etc. The simplest approach to understanding suchproperties would be to use classical physics. Based on classical physics the general problemcould be solved by using Newton’s equation

dp

dt= e (E + v × B)

where p is the electron momentum, v the velocity, and E and B are the electrical and magneticfields, respectively. Additional forces, if present, can be added on the right-hand side of the equa-tion. Although classical physics has been successful in describing many of nature’s phenomena,it fails completely when it is used to describe electrons in solids. To understand the underlyingphysical properties that form the basis of modern intelligent information devices, we need to usequantum mechanics.

According to quantum mechanics particles such as electrons behave as waves while wavessuch as electromagnetic waves behave as particles. The wave nature of particles is manifested forelectrons in solids. To the level needed in device physics, the electronic properties are describedby the Schrodinger equation . However, It turns out we can develop effective descriptions for thebehavior of electrons and then use simple classical physics. Of course to develop this effectivedescription we have to solve the Schrodinger equation. But once this description is developed wecan use Newton’s equation to understand how electrons respond to external forces. This allowsus to use simple models to describe electronic devices.

In this chapter we will review a few important outcomes of quantum mechanics. In particularwe will discuss the following:

28

2.2. PARTICLES IN AN ATTRACTIVE POTENTIAL: BOUND STATES 29

• Electronic properties in an atom: All solids are made up of atoms and the properties ofelectrons in atoms allows us to develop insight into the electronic properties of solids. We willdiscuss the hydrogen atom problem since it is the simplest atom and captures the useful physicsneeded to understand the theory of doping.

• Electrons in a quantum well: Quantum wells, both naturally occurring and artificially cre-ated in semiconductor structures are very important in modern technology. In devices such asMOSFETs, lasers, modulators etc. electrons are in quantum wells of various sizes and shapes.

• Electrons in free space and in crystalline materials: Most high performance semiconductordevices are based on high quality crystals. In these periodic structures electrons have allowedenergies that form bands separated from each other (in energy) by gaps. Almost every semicon-ductor property depends upon these bands. Once we understand the band theory, i.e propertiesof electrons in crystalline solids we can develop the effective description mentioned above anduse simple classical concepts.

• Occupation of electronic states: Quantum mechanics has very specific rules on the actualoccupation of energies allowed by Schrodinger equation. This occupation theory is central tounderstanding solid state physics and device behavior.

Once we have developed the basic quantum theory structure we will discuss properties ofvarious semiconductors and their heterostructures.

2.2 PARTICLES IN AN ATTRACTIVE POTENTIAL:BOUND STATES

We will now examine several important quantum problems that have impact on materials andphysical phenomena useful for device applications. The Schrodinger equation for electrons canbe written in as [

− �2

2m0∇2 + V (r, t)

]Ψ(r, t) = EΨ(r, t)

where m0 is the mass of the electron and V (r, t) is the potential energy. This is a differentialequation with solutions Ψ. Once the equation is solved we get a series of allowed energies andwavefunctions. Energies are allowed while others not consistent with the equation are forbidden.The band theory that forms the basis of all semiconductor devices is based on energy bands andgaps.

2.2.1 Electronic levels in a hydrogen atom

The hydrogen atom problem is of great relevance in understanding dopants in semiconductors.We will briefly summarize these findings. The hydrogen atom consists of an electron and a pro-ton interacting with the Coulombic interaction. The problem can be solved exactly and providesinsight into how electrons behave inside atoms.

Wavefunctions in the H-atom problem have the following term:

ψn�m(r, θ, φ) = Rn�(r)F�m(θ)Gm(φ)

30 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

The symbols n, �,m are the three quantum numbers describing the solution. The three quantumnumbers have the following allowed values:

principle number, n : Takes values 1, 2, 3, . . .

angular momentum number, � : Takes values 0, 1, 2, . . . n − 1

magnetic number,m : Takes values − �,−� + 1, . . . �

The principle quantum number specifies the energy of the allowed electronic levels. Theenergy eigenvalues are given by

En = − μe4

2 (4πε0)2

�2n2(2.2.1)

The spectrum is shown schematically in figure 2.1. Due to the much larger mass of the nucleusas compared with the mass of the electron, the reduced mass μ is essentially the same as theelectron mass m0. The ground state of the hydrogen atom is given by

ψ100 =1√πa3

0

e−r/a0 (2.2.2)

The parameter a0 appearing in the functions is called the Bohr radius and is given by

a0 =4πε0�

2

m0e2= 0.53 A (2.2.3)

It roughly represents the spread of the ground state.As noted earlier the dopant problem is addressed by using the potential of the H-atom

2.2.2 Electrons in a quantum well

As noted in the previous chapter, using semiconductor heterostructures it is possible to fab-ricate quantum well systems. These systems are used for high-performance devices, such astransistors, lasers and modulators. The quantum well problem can also be used to understandhow defects create trap levels.

A quantum well potential profile is shown in figure 2.2. The well (i.e., region where potentialenergy is lower) is described by a well size W = 2a as shown and a barrier height V0. Ingeneral the potential could be confining in one dimension with uniform potential in the othertwo directions (quantum well), or it could be confining in two dimensions (quantum wire) orin all three dimensions (quantum dot). As discussed later in this chapter such quantum wellsare formed in semiconductor structures and we can use the results discussed in this section tounderstand these problems.

We assume that the potential has a form

V (r) = V (x) + V (y) + V (z)

2.2. PARTICLES IN AN ATTRACTIVE POTENTIAL: BOUND STATES 31

0

116 E1

1 9 E1

1 4 E1

E1 1s

2s

3s

4s5s

= 0

E1 = –13.6 eV

A SIMPLE NON-RELATIVISTIC MODEL

FOR THE H-ATOM

Figure 2.1: Allowed energy levels of electrons in a hydrogen atom .

32 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

2a

V0V

–W2

W2

x = 00

x

Figure 2.2: Schematic of a quantum well of width 2a and infinite barrier height or barrier heightV0 .

so that the wavefunction is separable and of the form

ψ(r) = ψ(x)ψ(y)ψ(z)

We will briefly discuss the problem of the square potential well, and in section 2.10 we willuse the quantum well physics to discuss semiconductor quantum wells of importance in devices.

The simplest form of the quantum well is one where the potential is zero in the well andinfinite outside. The equation to solve then is (the wave function is non-zero only in the wellregion)

− �2

2m

d2ψ

dx2= Eψ (2.2.4)

which has the general solutions

ψ(x) = B cosnπx

2a, n odd

= A sinnπx

2a, n even (2.2.5)

The energy is

E =π2

�2n2

8ma2(2.2.6)

Note that the well size is 2a.The normalized particle wavefunctions are

ψ(x) =

√2

Wcos

nπx

W, n odd

=

√2

Wsin

nπx

W, n even (2.2.7)

2.3. ELECTRONS IN CRYSTALLINE SOLIDS 33

If the potential barrier is not infinite, we cannot assume that the wavefunction goes to zero atthe boundaries of the well. Let us define two parameters.

α =

√2mE

�2

β =

√2m(V0 − E)

�2(2.2.8)

The conditions for the allowed energy levels are given by the transcendental equations

αW

2tan

αW

2=

βW

2(2.2.9)

andαW

2cot

αW

2= −βW

2(2.2.10)

An important outcome of these solutions is that as in the H-atom case, only some energies areallowed for the electron. This result is of importance in electronic devices as will be discussedin section 2.10.

2.3 ELECTRONS IN CRYSTALLINE SOLIDS

The devices discussed in this text are made from crystalline materials. It is, therefore, impor-tant to understand the electronic properties of these materials. Let us first examine the simplerproblem of electrons in free space. It turns out that electrons in crystals can be considered tobehave as if they are in free space except they have a different “effective properties”. In thefree space problem the background potential energy is uniform in space. The time-independentequation for the background potential in a solid equal to V0 is

−�2

2m

(∂2

∂x2+

∂2

∂y2+

∂2

∂z2

)ψ(r) = (E − V0)ψ(r) (2.3.1)

A general solution of this equation is

ψ(r) =1√V

e±ik·r (2.3.2)

and the corresponding energy is

E =�

2k2

2m+ V0 (2.3.3)

where the factor 1√V

in the wavefunction occurs because we wish to have one particle per volumeV or ∫

V

d3r | ψ(r) |2 = 1 (2.3.4)

We assume that the volume V is a cube of side L. Note that if we assign the momentum of theelectron as �k the energy-momentum relation of free electrons is the same as that in classicalphysics. Later we will see that in crystalline material one can use a similar relationship exceptthe mass of the electron is modified by an effective mass.

34 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

Density of states for a three-dimensional system

We will now discuss the extremely important concept of density of states. The concept ofdensity of states is extremely powerful, and important physical properties in materials, such asoptical absorption, transport, etc., are intimately dependent upon this concept. Density of statesis the number of available electronic states per unit volume per unit energy around an energy E.If we denote the density of states by N(E), the number of states in a unit volume in an energyinterval dE around an energy E is N(E)dE.

Accounting for spin, the density of states can be shown to be (see Appendix C)

N(E) =

√2m

3/20 (E − V0)

1/2

π2�3(2.3.5)

In figure 2.4a we show the form of the three-dimensional density of states.

Density of states in sub-three-dimensional systems

The use of heterostructures has allowed one to make sub-three-dimensional-systems. In thesesystems the electron can be confined in two-dimensions (forming a quantum well) or in one-dimensional (quantum wire) and zero-dimensional (quantum dot) space. The two-dimensionaldensity of states is defined as the number of available electronic states per unit area per unit energyaround an energy E. It can be shown that the density of states for a parabolic band (for energiesgreater than V0) is (see figure 2.3b)

N(E) =m0

π�2(2.3.6)

Finally, we can consider a one-dimensional system often called a “quantum wire.” The one-dimensional density of states is defined as the number of available electronic states per unitlength per unit energy around an energy E. In a 1D system or a “quantum wire” the density ofstates is (including spin) (see figure 2.3c)

N(E) =

√2m

1/20

π�(E − V0)

−1/2 (2.3.7)

Notice that as the dimensionality of the system changes, the energy dependence of the densityof states also changes. As shown in figure 2.3, for a three-dimensional system we have (E −V0)

1/2 dependence, for a two-dimensional system we have no energy dependence, and for aone-dimensional system we have (E − V0)

−1/2 dependence.We will see later in the next section that when a particle is in a periodic potential, its wave-

function is quite similar to the free particle wavefunction. Also, the particle responds to externalforces as if it is a free particle except that its energy-momentum relation is modified by thepresence of the periodic potential. In some cases it is possible to describe the particle energy bythe relation

E =�

2k2

2m∗ + Eedge (2.3.8)

where m∗ is called the effective mass in the material and Eedge is the bandedge energy. The ef-fective mass in general summarizes the appropriate way to modify the free electron mass based

2.3. ELECTRONS IN CRYSTALLINE SOLIDS 35

N(E)

N(E)

E–1/2

1D system

E

(a)

E1/2N(E)

3D system

E

E0

2D system

E

(b)

(c)

V0

V0

V0

Figure 2.3: Energy dependence of the density of states in: (a) three-dimensional, (b) two-dimensional, and (c) one-dimensional systems.

on the physical property being characterized. Appendix C describes the various forms of effec-tive mass in detail. The expressions derived for the free electron density of states can then becarried over to describe the density of states for a particle in a crystalline material (which has aperiodic potential) by simply replacing m0 by m∗.

36 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

EXAMPLE 2.1 Calculate the density of states of electrons in a 3D system and a 2D system at an energyof 1.0 eV. Assume that the background potential is zero.

The density of states in a 3D system (including the spin of the electron) is given by (E is the energy inJoules)

N(E) =

√2(m0)

3/2E1/2

π2�3

=

√2(0.91 × 10−30 kg)(E1/2)

π2(1.05 × 10−34 J · s)3

= 1.07 × 1056E1/2 J−1 m−3

Expressing E in eV and the density of states in the commonly used units of eV−1 cm−3, we get

N(E) = 1.07 × 1056 × (1.6 × 10−19)3/2(1.0 × 10−6)E1/2

= 6.8 × 1021E1/2 eV−1 cm−3

At E = 1.0 eV we getN(E) = 6.8 × 1021 eV−1 cm−3

For a 2D system the density of states is independent of energy and is

N(E) =m0

π�2= 4.21 × 1014 eV−1 cm−2

2.3.1 Particle in a periodic potential: Bloch theorem

Band theory, which describes the properties of electrons in a periodic potential arising fromthe periodic arrangement of atoms in a crystal, is the basis for semiconductor technology.

The Schrodinger equation in the crystal[−�2

2m0∇2 + U(r)

]ψ(r) = Eψ(r) (2.3.9)

where U(r) is the background potential seen by the electrons. Due to the crystalline nature ofthe material, the potential U(r) has the same periodicity

U(r) = U(r + R)

We have noted earlier that if the background potential is V0, the electronic function in a volumeV is

ψ(r) =eik·r√

V

and the electron momentum and energy are

p = �k

E =�

2k2

2m0+ V0

2.3. ELECTRONS IN CRYSTALLINE SOLIDS 37

The wavefunction is spread in the entire sample and has equal probability (ψ∗ψ) at every pointin space. In the periodic crystal electron probability is the same in all unit cells of the crystalbecause each cell is identical. This is shown schematically in figure 2.4.

PERIODIC POTENTIAL

U(r)

Wavefuntions |ψ|2 have the same periodicity as the potential

ψ(r) = u(r)eik•r

r

r

|ψ(r)|2

Figure 2.4: A periodic potential, |ψ|2 has the same spatial periodicity as the potential.

Bloch’s theorem states the eigenfunctions of the Schrodinger equation for a periodic potentialare the product of a plane wave eik·r and a function uk(r), which has the same periodicity as theperiodic potential. Thus

ψk(r) = eik·ruk(r) (2.3.10)

is the form of the electronic function. The periodic part uk(r) has the same periodicity as thecrystal, i.e.

uk(r) = uk(r + R) (2.3.11)

The wavefunction has the property

ψk(r + R) = eik·(r+R)uk(r + R) = eik·ruk(r)eik·R

= eik·Rψk(r) (2.3.12)

To obtain the allowed energies, i.e. the band structure, computer techniques are used to solve theSchrodinger equation. One obtains a series of allowed energy bands separated by bandgaps asshown schematically in figure 2.5. Each band has an E vs. k relation Examples of such relationscalled bandstructure will be shown later in section 2.6. The product of � and the k-vector behaveslike an effective momentum for the electron inside the crystal.

The smallest k-values lie in a k-space called the Brillouin zone (see figure 2.6). If the k-valueis chosen beyond the Brillouin zone values, the energy values are simply repeated. The concept

38 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

Free states

Bou

nd s

tate

s

Isolated atoms

E1

E2

E3

E4

Evac

Free states

Evac

Crystal: Atomic spacing ~1-2 Å

}

}

}

}

}

}

Allowed energy bands

..

Bandgaps

Core bands are like those

in isolated atoms

Figure 2.5: A schematic description of allowed energy levels and energy bands in an atom andin crystalline materials.

of allowed bands of energy separated by bandgaps is central to the understanding of crystallinematerials. Near the bandedges it is usually possible to define the electron E–k relation as

E =�

2(k − ko)2

2m∗

where ko is the k-value at the bandedge and m∗ is the effective mass. The concept of an effectivemass is extremely useful, since it represents the response of the electron–crystal system to theoutside world.

k-vectorAccording to the Bloch theorem, in the perfectly periodic background potential that the crystalpresents, the electron propagates without scattering. The electronic state ∼ exp (ik · r) is anextended wave which occupies the entire crystal. To describe the response of the electron wavesto external forces one uses the wavepacket description. The equation of motion for electrons in

2.3. ELECTRONS IN CRYSTALLINE SOLIDS 39

(a)

(b)

Figure 2.6: Brillouin zone of (a) the face centered cubic lattice and (b) the hexagonal lattice.

40 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

general isdp

dt= Fext + Fint

However this is not very useful for a meaningful description of the electron because it includesthe internal forces on the electron. We need a description which does not include the evaluationof the internal forces. Using a wavepacket description of electrons as with any wave phenomenait is the wave group velocity that represents the propagation of wave energy. In the case ofa particle wave the group velocity represents the particle velocity. The group velocity of thiswavepacket is

vg =dω

dk(2.3.13)

where ω is the frequency associated with the electron of energy E; in quantum mechanics,ω = E/�:

vg =1

�

dE

dk

=1

�∇kE(k)

If we have an electric field E present, the work done on the electron during a time interval δt is

δE = −eE · vgδt (2.3.14)

We may also write, in general

δE =

(dE

dk

)δk

= �vg · δk (2.3.15)

Comparing the two equations for δE, we get

δk = −eE�

δt

giving us the relation

�dk

dt= −eE (2.3.16)

In general, we may write

�dk

dt= Fext (2.3.17)

The term �k responds to the external forces as if it is the momentum of the electron, although,as can be seen by comparing the true Newtons equation of motion, it is clear that �k containsthe effects of the internal crystal potentials and is therefore not the true electron momentum.The quantity �k is called the crystal momentum . We can, for all practical purposes, treat theelectrons as if they are free and obey the effective Newtons equation of motion. This physicalpicture is summarized in figure 2.7.

2.4. OCCUPATION OF STATES: DISTRIBUTION FUNCTION 41

–

+ + + +

+ + + +

+ + + +

Electron in a periodic potential

Bloch theorem: ψ = ukeik•r

Equation of motiondkdt = Fext

Electron behaves as if it is in free space, but with a different effective mass

E versus k relation effective mass

h

Figure 2.7: Electrons in a periodic potential can be treated as if they are in free space except thattheir energy–momentum relation is modified because of the potential. Near the bandedges theelectrons respond to the outside world as if they have an effective mass m∗. The effective masscan have a positive or negative value.

2.4 OCCUPATION OF STATES:DISTRIBUTION FUNCTION

Bandstructure calculations give us the allowed energies for the electron. How will the particlesdistribute among the allowed states? To answer this question we need to use quantum statisticalphysics. According to quantum mechanics particles (this term includes classical particles andclassical waves which are represented by particles) have an intrinsic angular momentum called

42 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

spin. The spin of particles can take a value of 0, 1/2�, �, 3/2�, etc. Particles which have inte-gral spins (in units of �) are called bosons, while those that have half-integral spins are calledfermions.

According to thermodynamics, a system with a large number of particles can be described bymacroscopic properties such as temperature, pressure, volume, etc. Under equilibrium condi-tions (no exchange of net energy with other systems) the system is described by a distributionfunction, which gives us the occupation number for any energy level. To find this occupationwe have to minimize the free energy F of the system subject to any constraints from quantummechanics (such as the Pauli exclusion principle). The following distribution functions are ob-tained for equilibrium:

• For fermions such as electrons

f(E) =1

exp[

E−EF

kBT

]+ 1

Here f(E) is the occupation function; EF is the Fermi energy and its value depends upon particledensity).

In classical physics the occupation function for electrons is

f(E) =1

exp(

E−EF

kBT

) (2.4.1)

Note that if E − EF � kBT ; i.e., f(E) � 1, the classical function approaches the quantumFermi distribution function.For completeness we note the distributed function for bosons as well.• Massless bosons (like photons)

f(E) =1

exp(

EkBT

)− 1

(2.4.2)

• Bosons with mass (this applies to electron pairs that occur in superconductors)

f(E) =1

exp(

E−μkBT

)− 1

(2.4.3)

where μ is an energy determined from the particle density.• There is a distribution function that proves to be useful in solid state devices. When solvingthe Schrodinger equation we can get more than one solution with the same energy. This is thedegeneracy gd of a state. Consider a case where a state has a degeneracy gi and can, in principle,be occupied by gd electrons. However, for dopants and defect levels, when one electron is placedin the allowed state, the next one cannot be placed because of the Coulombic repulsion. Thishappens for some states, such as those states associated with donors or acceptors, traps, etc.

2.5. METALS AND INSULATORS 43

Figure 2.8: Schematic of the Fermi function for electrons and other fermions. In general theposition of EF is dependent on temperature. The occupation probability is at 0.5 at the Fermienergy.

Thus, even though Pauli exclusion principle would allow two (or more) electrons to reside onthe state, the repulsion would not. In such cases the occupation function can be shown to be

f(E) =1

1gd

exp(

E−EF

kBT

)+ 1

(2.4.4)

In figure 2.8 we show a schematic of the Fermi function for electrons and its dependence ontemperature. It is important to note that at E = EF , f(E) = 0.5 regardless of the temperature.At zero temperature, the Fermi function becomes a step function with f(E < EF ) = 1.0 andf(E) > EF = 0.0.

2.5 METALS AND INSULATORS

Band theory shows that the allowed energy states of electrons in a crystalline material are de-scribed by a series of allowed bands separated by forbidden bandgaps. Two important situations

44 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

Vacuum energy

Conduction band

Valence band

Core level

Core level

Metal Semiconductor

Highest occupied band is partially

filled

Highest occupied band is completely filled

Work function

e

Electron affinity

eφ

χ

Eg: Bandgap

Inert bands

Figure 2.9: Electron occupation of the bands in a metal and semiconductor (or insulator). In ametal, the highest occupied band at 0 K is partially filled with electrons. In a semiconductor at0 K, the highest occupied band is completely filled with electrons and the next band is completelyempty. The separation between the two bands is the bandgap Eg .

arise when we examine the electron occupation of allowed bands. As shown in figure 2.9 wecan have a situation where an allowed band is completely filled with electrons, while the nextallowed band is separated in energy by a gap Eg and is completely empty at 0 K. In a secondcase, the highest occupied band is only half full (or partially full).

When an allowed band is completely filled with electrons, the electrons in the band cannotconduct any current. Since electrons are fermions they cannot carry any net current in a filledband since an electron can only move into an empty state. Because of this effect, when wehave a material in which a band is completely filled, while the next allowed band is separatedin energy and empty, the material has, in principle, infinite resistivity and is an insulator or asemiconductor. The material in which a band is only half full with electrons has a very lowresistivity and is a metal.

The band that is normally filled with electrons at 0 K in semiconductors is called the valenceband, while the upper unfilled band is called the conduction band . The energy difference be-tween the vacuum level and the highest occupied electronic state in a metal is called the metalwork function . The energy between the vacuum level and the bottom of the conduction band iscalled the electron affinity.

2.5. METALS AND INSULATORS 45

+

ke

kh

kElectron removed

Wavevector associated with the missing electron

Missing electron hole

Filled band Σk = 0

––

––

–– – – – –

––

––

––

–

Valence band

Electron removed

Total momentum becomes –ke hole k vector is –ke

––

––

– – – – ––

––

––

––

Figure 2.10: Illustration of the wavevector of a filled valence band with a missing electron ke.The wavevector is −ke, which is associated with the hole.

Semiconductors have zero conductivity at 0 K and quite low conductivity at finite temper-atures, but it is possible to alter their conductivity by orders of magnitude through doping orapplied electric potentials. This makes semiconductors useful for active devices.

2.5.1 Electrons and Holes

In semiconductors the valence band is full of electrons and the conduction band is emptyat 0 K. At finite temperatures some of the electrons leave the valence band and occupy theconduction band. Electrons in the conduction band can carry current. When electrons leave thevalence band there are unoccupied states. Consider the situation as shown in figure 2.10, wherean electron with momentum ke is missing from the valence band. When all of the valence bandstates are occupied, the sum of the total momentum is zero; i.e.∑

ki = 0 =∑

ki �=ke

ki + ke (2.5.1)

This result is just an indication that there are as many positive k states occupied as there arenegative ones. Now, in the situation where the electron at wavevector ke is missing, the totalwavevector is ∑

ki �=ke

ki = −ke (2.5.2)

The missing state is called a hole and the wavevector of the system −ke is attributed to it. It isimportant to note that the electron is missing from the state ke and the momentum associatedwith the hole is at −ke. The position of the hole is depicted as that of the missing electron. Butin reality the hole wavevector kh is −ke, as shown in figure 2.10 and we have

kh = −ke (2.5.3)

If an electric field is applied, all the electrons move in the direction opposite to the electric field.This results in the unoccupied state moving in the field direction. The hole thus responds as if

46 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

it has a positive charge. It therefore responds to external electric and magnetic fields E and B,respectively, according to the equation of motion

�dkh

dt= e [E + vh × B] (2.5.4)

where �kh and vh are the momentum and velocity of the hole.Thus the equation of motion of holes is that of particles with a positive charge e. The mass of

the hole has a positive value, although the electron mass in its valence band is negative. Whenwe discuss the valence band properties, we refer to holes. This is because in the valence bandonly the missing electrons or holes lead to charge transport and current flow.

2.6 BANDSTRUCTURE OF SOME IMPORTANTSEMICONDUCTORS

In this section we will examine the band structure near the band edges for several importantmaterials. To represent the bandstructure on a figure that is two-dimensional, we draw the E-kdiagram in several panels where k goes from zero to its maximum value along the (100) directionor the (111) direction, etc within the Brillouin zone. As shown in figure 2.6 for the fcc lattice,the maximum k-value along the (100) direction is 2π/a(1, 0, 0). This point is called the X-pointand there are five other equivalent points, due to the cubic symmetry of the lattice. Similarly,along the (111) direction, the maximum k-point is π/a(1, 1, 1) and seven other similar points.This point is called the L-point. Thus we commonly display the E-k diagram with k going fromthe origin (called the Γ-point) to the X-point and from the origin to the L-point.

2.6.1 Direct and indirect semiconductors

Two types of band structures arise in semiconductors- direct and indirect. The top of thevalence band of most semiconductors occurs at effective momentum equal to zero. A typicalbandstructure of a semiconductor near the top of the valence band is shown in figure 2.11. Wenotice the presence of three bands near the valence bandedge. These curves or bands are labeledI, II, and III in the figure and are called the heavy hole (HH), light hole (LH), and the split offhole bands.

The bottom of the conduction band in some semiconductors occurs at k = 0. Such semicon-ductors are called direct bandgap materials. Semiconductors, such as GaAs, InP, GaN, InN, etc.,are direct bandgap semiconductors. In other semiconductors, the bottom of the conduction banddoes not occur at the k = 0 point, but at certain other points. Such semiconductors are calledindirect semiconductors. Examples are Si, Ge, AlAs, etc.

Due to the law of momentum conservation, direct gap materials have a strong interaction withlight. Indirect gap materials have a relatively weak interaction with electrons.

When the bandedges are at k = 0 it is possible to represent the bandstructure by a simplerelation of the form

E(k) = Ec +�

2k2

2m∗ (2.6.1)

2.6. BANDSTRUCTURE OF SOME IMPORTANT SEMICONDUCTORS 47

Valence band

III

II

I

I Heavy Hole Band

II Light Hole Band

III Split-Off Band

Δ = Split-Off Energy

INDIRECT GAPDIRECT GAP

Conduction band

Conduction bandedge

Valence band

III

II

I

k = 0 k = 0

Figure 2.11: Schematic of the valence band, direct bandgap, and indirect bandgap conductionbands. The curves I, II, III in the valence band are called heavy hole, light hole, and split-offhole states, respectively.

where Ec is the conduction bandedge, and the bandstructure is a simple parabola. The equationfor the E–k relation looks very much like that of an electron in free space as noted in the previoussection.

SiliconThe most important semiconductor is silicon. Silicon has an indirect bandgap as shown in

figure 2.12. The bottom of the conduction band in Si is at point (∼ (2π/a)(0.85, 0.0); i.e., closeto the X-point. There are six degenerate X-points and, consequently, six conduction bandedgevalleys. The near bandedge bandstructure can be represented by ellipsoids of energy with simpleE vs. k relations of the form (for examples for the [100] valley)

E(k) =�

2k2x

2m∗l

+�

2(k2

y + k2z

)2m∗

t

(2.6.2)

48 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

6

5

4

3

2

1

0

–1

–2

–3

–4

Eg

(a)

EN

ER

GY

(eV

)

(b)

kz

kx (100) (010)

(001)

(010) (100)

(001)ky

Constant energy surfaces of six equivalent valleys at conduction bandedge

Γ[110] [111]

XL

SILICON

Indirect gap Eg = 1.1 eV

Direct gap 3.4 eV

Figure 2.12: (a) Bandstructure of Si. (b) Constant energy ellipsoids for the Si conduction band.There are six equivalent valley in Si at the bandedge.

where we have two masses, the longitudinal and transverse. The constant energy surfaces of Siare ellipsoids according to Eq. 2.6.2. The six surfaces are shown in figure 2.12

The longitudinal electron mass m∗l is approximately 0.98 m0, while the transverse mass is

approximately 0.19 m0.The next valley in the conduction band is the L-point valley, which is about 1.1 eV above the

bandedge. Above this is the Γ-point edge. Due to the six-fold degeneracy of the conductionbandedge, the electron transport in Si is quite poor because of the very large density of statesnear the bandedge, leading to a high scattering rate in transport.

GaAsGaAs is a direct gap material with small electron effective mass. The near bandedge bandstruc-ture of GaAs is shown in figure 2.13. The bandstructure can be represented by the relation(referenced to Ec)

E =�

2k2

2m∗ (2.6.3)

with m∗ = 0.067m0. A better relationship is the non-parabolic approximation

E(1 + αE) =�

2k2

2m∗ (2.6.4)

with α = 0.67 eV−1.For high electric field transport, it is important to note that the valleys above Γ-point are the

L-valleys. There are eight L-points, but, since half of them are connected by a reciprocal latticevector, there are four valleys. The separation ΔEΓL between the Γ- and L- minima is 0.29 eV.

2.6. BANDSTRUCTURE OF SOME IMPORTANT SEMICONDUCTORS 49

6

5

4

3

2

1

0

–1

–2

–3

–4

k

EN

ER

GY

(eV

)

Eg

GALLIUM ARSENIDE

Direct bandgapEg (T=0) = 1.53 eVEg (300 K) = 1.43 eV

[111] [100]

Figure 2.13: Bandstructure of GaAs. The bandgap at 0 K is 1.51 eV and at 300 K it is 1.43 eV.The bottom of the conduction band is at k = (0, 0, 0), i.e., the Γ-point. The upper conductionband valleys are at the L-point.

The L-valley has a much larger effective mass than the Γ-valley. For GaAs, m∗L ∼ 0.25m0. This

difference in masses is extremely important for high electric field transport as will be discussedin the next chapter.

The valence band of GaAs has the standard HH, LH, and SO bands. Due to the large spin–orbitsplitting, for most purposes the SO band does not play any role in electronic properties.

The bandstructures of Ge and AlAs, two other important semiconductors, are shown in fig-ure 2.14, along with brief comments about their important properties.

InN, GaN, and AlNThe III–V nitride family of GaN, InN, and AlN have become quite important due to progressin the ability to grow the semiconductor. These materials are typically grown with a wurtzitestructure, and have bandgaps ranging from ∼1.0 eV to over 6.0 eV. This large bangap is veryuseful for short wavelength light emitters and high power electronics. In figure 2.15 we showthe bandstructure for nitrides.

It is important to note is that the bandgap of semiconductors generally decreases as temper-ature increases. The bandgap of GaAs, for example, is 1.51 eV at T = 0K and 1.43 eV atroom temperature. In table 2.1 we show the temperature dependence of bandgaps of severalsemiconductors.

50 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

6

5

4

3

2

1

0

–1

–2

–3

–4

0.3

L [111] Γ X[100]

k

(a)

EN

ER

GY

(eV

)

GERMANIUM

Indirect bandgapEg (300 K) = 0.66 eVEg (direct) = 0.9 eV

–1

–2

–3

–4

6

5

4

3

2

1

0

L [111] Γ X[100]

k

EN

ER

GY

(eV

)

(b)

ALUMINUM ARSENIDE

Indirect bandgapEg (300 K) = 2.15 eVEg (direct) = 2.75 eV

Figure 2.14: (a) Bandstructure of Ge and AlAs.

2.7 MOBILE CARRIERS

From our brief discussion of metals and semiconductors in Section 2.5, we see that in a metalcurrent flows because of the electrons present in the highest (partially) filled band. As shownschematically in figure 2.16a. The density of such electrons is very high (∼ 1023 cm−3). In asemiconductor, in contrast, no current flows if the valence band is filled with electrons and theconduction band is empty of electrons. However, if somehow empty states or holes are createdin the valence band by removing electrons, current can flow through the holes. Similarly, ifelectrons are placed in the conduction band, these electrons can carry current. This is shownschematically in figure 2.16b. If the density of electrons in the conduction band is n and that ofholes in the valence band is p, the total mobile carrier density is n + p.

2.7.1 Mobile electrons in metals

In a metal, we have a series of filled bands and a partially filled band called the conduc-tion band. The filled bands are inert as far as electrical and optical properties of metals areconcerned. The conduction band of metals can be assumed to be described by the parabolicenergy–momentum relation

E(k) = Ec +�

2k2

2m0(2.7.1)

Note that we have used an effective mass equal to the free electrons mass. This is a reasonableapproximation for metals. The large electron density in the band “screens” out the backgroundpotential and the electron effective mass is quite close to the free space value.

2.7. MOBILE CARRIERS 51

5

0

–5

k

AL

KL

M

EN

ER

GY

(eV

)

5

0

–5

k

AL

KL

M

EN

ER

GY

(eV

)

5

0

–5

k

AL

KL

M

EN

ER

GY

(eV

)

10

k1

M K

Γ

L

H

A

k2

kz

InN

GaN

AlN

Figure 2.15: Bandstructure of InN, GaN and AlN.

The electron density in the conduction band of a metal is related to the Fermi level by therelation

n =

∫ ∞

Ec

√2m

3/20

π2�3

E1/2dE

exp(

E−EF

kBT

)+ 1

(2.7.2)

52 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

ExperimentalbandgapEG (eV)

Type of Temperature dependenceCompound bandgap 0 K 300 K of bandgap EG(T ) (eV)AlP Indirect 2.52 2.45 2.52 – 3.18 ×10−4T 2/(T + 588)AlAs Indirect 2.239 2.163 2.239 – 6.0 ×10−4T 2/(T + 408)AlSb Indirect 1.687 1.58 1.687 – 4.97 ×10−4T 2/(T + 213)GaP Indirect 2.338 2.261 2.338 – 5.771 ×10−4T 2/(T + 372)GaAs Direct 1.519 1.424 1.519 – 5.405 ×10−4T 2/(T + 204)GaSb Direct 0.810 0.726 0.810 – 3.78 ×10−4T 2/(T + 94)InP Direct 1.421 1.351 1.421 – 3.63 ×10−4T 2/(T + 162)InAs Direct 0.420 0.360 0.420 – 2.50 ×10−4T 2/(T + 75)InSb Direct 0.236 0.172 0.236 – 2.99 ×10−4T 2/(T + 140)

Table 2.1: Bandgaps of binary III–V compounds (From Casey and Panish, 1978).

This integral is particularly simple to evaluate as 0 K, since, at this temperature

1

exp(

E−EF

kBT

)+ 1

= 1 if E ≤ EF

= 0 otherwise

this gives

n =

∫ EF

EC

N(E)dE

We then have

n =

√2m

3/20

π2�3

∫ EF

EC

(E − EC)1/2

dE

=2√

2m3/20

3π2�3(EF − EC)

3/2

or

EF − EC =�

2

2m0

(3π2n

)2/3(2.7.3)

The expression is applicable to metals such as copper, gold, etc. In Table 2.2 we show theconduction band electron densities for several metals. The quantity EF , which is the highest oc-cupied energy state at 0 K, is called the Fermi energy. We can define a corresponding wavevector

2.7. MOBILE CARRIERS 53

Evac

EF

Ec

EN

ER

GY

Electrons in the conduction band can carry current

Evac

Ec

EV

EN

ER

GY

Conduction band electrons (density, n) are mobile

Holes (density, p) are mobile

Mobile carrier density = n + p

(a)

(b)

– –– –– –––– –– –– –

– –– –– ––– –– –– ––

–– –– –– –

Core electrons do not carry current

Work function

SEMICONDUCTORS

METALS

– – – – –

+ + +

EF

Figure 2.16: (a) In metals the highest occupied band is partially filled and electrons can carrycurrent. (b) A schematic showing the valence band and conduction band in a typical semicon-ductor. Only electrons in the conduction band and holes in the valence band can carry current.

kF , called the Fermi vector, and a velocity vF , called the Fermi velocity as

kF =(3π2n

)1/3

vF =

(�

m0

)(3π2n

)1/3(2.7.4)

It is important to note that even at 0 K, the velocity of the highest occupied state is vF and notzero, as would be the case if we used classical statistics. At finite temperatures, the Fermi levelis approximately given by

EF (T ) = EF (0)

[1 − π2

12

(kBT )2

(EF (0))2

](2.7.5)

where EF (T ) and EF (0) are the Fermi levels at temperatures T and 0 K, respectively. In Metalsthere is very little change in the Fermi level with temperature.

54 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

ELEMENT VALENCE DENSITY CONDUCTION (gm/cm3) ELECTRON DENSITY (1022 cm–3) Al 3 2.7 18.1

Ag 1 10.5 5.86

Au 1 19.3 5.90

Na 1 0.97 2.65

Fe 2 7.86 17.0

Zn 2 7.14 13.2

Mg 2 1.74 8.61

Ca 2 1.54 4.61

Cu 1 8.96 8.47

Cs 1 1.9 0.91

Sn 4 7.3 14.8

Table 2.2: Properties of some metals. In the case of elements that display several values ofchemical valence, one of the values has been chosen arbitrarily.

2.7. MOBILE CARRIERS 55

EXAMPLE 2.1 A particular metal has 1022 electrons per cubic centimeter. Calculate the Fermi energyand the Fermi velocity (at 0 K).

The Fermi energy is the highest occupied energy state at 0 K and is given by (measured from the con-duction bandedge)

EF =�

2

2m0

(3π2n

)2/3

=(1.05 × 10−34)2[3π2(1028)]2/3

2(0.91 × 10−30)= 2.75 × 10−19 J

= 1.72 eV

The Fermi velocity is

vF =�

m0

(3π2n

)1/3

=(1.05 × 10−34 J.s)(3π2 × 1028 m−3)1/3

0.91 × 10−30 kg= 7.52 × 105 m/s

= 7.52 × 107 cm/s

Thus, the highest energy electron has a large energy and is moving with a very large speed.

2.7.2 Electrons and holes in semiconductors

In pure semiconductors there are no mobile carriers at zero temperature. As temperature israised, electrons from the valence band are thermally excited into the conduction band, and inequilibrium there is an electron density n and an equal hole density p, as shown in figure 2.17aNote that the density of allowed states has the form

N(E) =

√2 (m∗

dos)3/2

(E − Ec)1/2

π2�3(2.7.6)

where m∗dos is the density of states mass and Ec is the conduction bandedge. A similar expression

exists for the valence band except the energy term is replaced by (Ev − E)1/2 and the density of

states exist below the valence bandedge Ev . Figure 2.17 shows a schematic view of the densityof states.

It is important to note that the density of states mass has a special term in indirect gap mate-rials. In direct gap semiconductors m∗

dos is just the effective mass for the conduction band. Inindirect gap materials it is given by (see Appendix C)

m∗dos = (m∗

1m∗2m

∗3)

1/3

where m∗1m

∗2m

∗3 are the effective masses along the three principle axes. For Si counting the six

degenerate X-valleys we have

m∗dos = 62/3

(m�m

2t

)1/3

56 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

Ec

EV

DE

NS

ITY

OF

ST

AT

ES

Pure semiconductorsn = p = ni = pi

– –

+ + +

(b)

– – – – – –

(a)

EV EcEF

Low temperatureni = pi ~ 0

DE

NS

ITY

OF

ST

AT

ES

(c)

EV EcEF

High temperature

pi ni

ENERGY

Conduction band

Valence band

–+

+++ –

––

Figure 2.17: (a) A schematic showing that electron and hole densities are equal in a pure semi-conductor. (b) Density of states and Fermi occupation function at low temperatures. (c) Densityof states and Fermi function at high temperatures when ni and pi become large.

For the valence band we can write a simple expression for a density of states masses , whichincludes the HH and LH bands

m∗dos =

(m

∗3/2hh + m

∗3/2�h

)2/3

In calculating the position of the Fermi energy, charge density, etc. we need to use the densityof states mass. In pure semiconductors, electrons in the conduction come from the valence bandand n = p = ni = pi, where ni and pi are the intrinsic carrier concentrations. In general the

2.7. MOBILE CARRIERS 57

electron density in the conduction band is

n =

∫ ∞

Ec

Ne(E)f(E)dE

n =1

2π2

(2m∗

e

�2

)3/2 ∫ ∞

Ec

(E − Ec)1/2dE

exp (E−EF

kBT ) + 1(2.7.7)

For small values of n (non-degenerate statistics where we can ignore the unity in the Fermifunction) we get

n = Nc exp [(EF − Ec) /kBT ] (2.7.8)

where the effective density of states Nc is given by

Nc = 2

(m∗

ekBT

2π�2

)3/2

A similar derivation for hole density gives

p = Nv exp [(Ev − EF ) /kBT ] (2.7.9)

where the effective density of states Nv is given by

Nv = 2

(m∗

hkBT

2π�2

)3/2

We also obtain

np = 4

(kBT

2π�2

)3

(m∗em

∗h)

3/2exp (−Eg/kBT ) (2.7.10)

Notice that within our low carrier density approximation, the product np is independent of theposition of the Fermi level and is dependent only on the temperature and intrinsic properties ofthe semiconductor. This is the law of mass action. If n increases, p must decrease, and viceversa. For the intrinsic case n = ni = p = pi, we have from the square root of the equationabove

ni = pi = 2

(kBT

2π�2

)3/2

(m∗em

∗h)

3/4exp (−Eg/2kBT )

EFi =Ec + Ev

2+

3

4kBT ln (m∗

h/m∗e) (2.7.11)

Thus the Fermi level of an intrinsic material lies close to the midgap.In Table 2.3 we show the effective densities and intrinsic carrier concentrations in Si, Ge, and

GaAs The values given are those accepted from experiments. These values are lower than theones we get by using the equations derived in this section. The reason for this difference is dueto inaccuracies in carrier masses and the approximate nature of the analytical expressions.

We note that the carrier concentration increases exponentially as the bandgap decreases. Re-sults for the intrinsic carrier concentrations for Si, Ge, GaAs, and GaN are shown in figure 2.18.

58 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

CONDUCTION BAND VALENCE BAND INTRINSIC CARRIER

MATERIAL EFFECTIVE DENSITY (NC) EFFECTIVE DENSITY (NV) CONCENTRATION (ni = pi)

Si (300 K) 2.78 x 1019 cm–3 9.84 x 1018 cm–3 1.5 x 1010 cm–3

Ge (300 K) 1.04 x 1019 cm–3 6.0 x 1018 cm–3 2.33 x 1013 cm–3

GaAs (300 K) 4.45 x 1017 cm–3 7.72 x 1018 cm–3 1.84 x 106 cm–3

Table 2.3: Effective densities and intrinsic carrier concentrations of Si, Ge, and GaAs. Thenumbers for intrinsic carrier densities are the accepted values even though they are smaller thanthe values obtained by using the equations derived in the text.

In electronic devices where current has to be modulated by some means, the concentration ofintrinsic carriers is fixed by the temperature and therefore is detrimental to device performance.Once the intrinsic carrier concentration increases to ∼ 1015 cm−3, the material becomes unsuit-able for electronic devices, due to the high leakage current arising from the intrinsic carriers.A growing interest in high-bandgap semiconductors, such as diamond (C), SiC, etc., is partlydue to the potential applications of these materials for high-temperature devices where, due totheir larger gap, the intrinsic carrier concentration remains low up to very high temperatures.For GaN the background defect density usually does not allow one to reach theoretical intrinsiccarrier densities.

EXAMPLE 2.2 Calculate the effective density of states for the conduction and valence bands of GaAs andSi at 300 K. Let us start with the GaAs conduction-band case. The effective density of states is

Nc = 2

(m∗

ekBT

2π�2

)3/2

Note that at 300 K, kBT = 26 meV = 4 × 10−21 J.

Nc = 2

(0.067 × 0.91 × 10−30 (kg) × 4.16 × 10−21 (J)

2 × 3.1416 × (1.05 × 10−34 (Js))2

)3/2

m−3

= 4.45 × 1023 m−3 = 4.45 × 1017 cm−3

In silicon, the density of states mass is to be used in the effective density of states. This is given by

m∗

dos = 62/3(0.98 × 0.19 × 0.19)1/3 m0 = 1.08 m0

2.7. MOBILE CARRIERS 59

1017

1016

1015

1014

1013

1012

1011

1010

109

108

107

106

1000 500 200 100 27 0 –20T (˚C)

0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

1000/T (K–1)

Ge

Si

GaA s

INT

RIN

SIC

CA

RR

IER

DE

NS

ITY

ni (c

m–3

)

GaN

105

104

Lowest measured unintentional carrier

concentration in GaN.

Figure 2.18: Intrinsic carrier densities of Ge, Si, GaAs, and GaN as a function of reciprocaltemperature. Currently, the lowest measured unintentional background density in GaN at roomtemperature is around 1× 1015 cm−3, indicating that the electronic properties are dominated bydefects (either extrinsic or intrinsic point defects).

60 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

The effective density of states becomes

Nc = 2

(m∗

doskBT

2π�2

)3/2

= 2

(1.06 × 0.91 × 10−30 (kg) × 4.16 × 10−21 (J)

2 × 3.1416 × (1.05 × 10−34 (Js))2

)3/2

m−3

= 2.78 × 1025 m−3 = 2.78 × 1019 cm−3

We can see the large difference in the effective density between Si and GaAs.In the case of the valence band, we have the heavy hole and light hole bands, both of which contribute

to the effective density. The effective density is

Nv = 2(m

3/2

hh + m3/2

�h

)(kBT

2π�2

)3/2

For GaAs we use mhh = 0.45m0, m�h = 0.08m0 and for Si we use mhh = 0.5m0, m�h = 0.15m0, toget

Nv(GaAs) = 7.72 × 1018cm−3

Nv(Si) = 9.84 × 1018cm−3

2.8 DOPING OF SEMICONDUCTORS

To avoid leakage current in the ‘OFF’ state, semiconductor devices operate at temperatureswhere the intrinsic carrier density is small (

<∼ 1015 cm−3). To introduce electrons and holes in asemiconductor the material is doped with dopants. The electrons (holes) created by the dopantsare used in device design.

Donors are dopants which can donate an electron to the conduction band and acceptors aredopants which can accept an electron from the valence band and thus create a hole. The donoratom replaces a host atom in the crystal and contains one (or more) extra electrons in its outershell. The donor atom could be a pentavalent atom in Si or a Si atom on a Ga site in GaAs.Focusing on the pentavalent atom in Si, four of the valence electrons of the donor atom behaveas they would in a Si atom; the remaining fifth electron now sees a positively charged ion towhich it is attracted, as shown in figure 2.19. The ion has a charge of unity and the attraction issimply Coulombic suppressed by the dielectric constant of the material. The problem is now thatof the hydrogen atom case, except that the electron mass is the effective mass at the bandedge.The attractive potential is

U(r) =−e2

4πεr(2.8.1)

where ε is the dielectric constant of the semiconductor; i.e., the product of ε0 and the relativedielectric constant. In this simplification the properties of the dopant atom can be describedby a simple hydrogen-like model, where the electron mass is simply the effective mass at thebandedge.

2.8. DOPING OF SEMICONDUCTORS 61

Silicon host atom

Pentavalentdonor impurity

= +

= Silicon-like Electron-ion+

All 4 outer electrons go into the valence band

EC

EV

— —

— —

— —

— —

— — —

— —

——

—

—+

—

Figure 2.19: A schematic showing the approach we can take to understand donors in semicon-ductors. The donor problem is treated as the host atom problem, together with a Coulombicinteraction term.

We have seen that electrons in the crystal can be represented by an effective mass near thebandedge. We get the effective mass equation for the donor level which has an energy for Ed of[−�

2

2m∗e

∇2 − e2

4πεr

]Fc(r) = (Ed − Ec)Fc(r) (2.8.2)

where m∗e is the conduction bandedge mass and Ed − Ec is the impurity energy with respect to

the conduction bandedge Ec levels.This equation is now essentially the same as that of an electron in the hydrogen atom problem.

The only difference is that the electron mass is m∗ and the Coulombic potential is reduced byε0/ε.

The energy solutions for this problem are

Ed = Ec − e4m∗e

2(4πε)2�2

1

n2, n = 1, 2, ... (2.8.3)

A series of energy levels are produced, with the ground state energy level being at

Ed = Ec − e4m∗e

2(4πε)2�2

= Ec − 13.6

(m∗

mo

)(εo

ε

)2

eV (2.8.4)

62 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

Si

A sPositiveion

E xcess electron

: Donor levelEdEc+

E

Ev V alenceband

Conductionband

A rsenic (A s) atom donates one electron to the conduction band to

produce an n-type silicon

Si

Si

Si

Si

Si

Si

–

Figure 2.20: A schematic of doping of Si with arsenic (or other group V dopant). A donor levelis produced below the conduction bandedge.

Note that in the hydrogen atom problem the electron levels are measured from the vacuum energylevel which is taken as E = 0. In the donor problem, the energy level is measured from thebandedge. Figure 2.20 shows the energy level associated with a donor impurity.

The wavefunction of the ground state is as in the hydrogen atom problem

Fc(r) =1√πa3

e−r/a (2.8.5)

where a is the donor Bohr radius and is given by

a =(4πε)�2

m∗ee

2= 0.53

(ε/ε0

m∗e/m0

)A (2.8.6)

For most semiconductors the donor energies are a few meVs below the conduction bandedgeand the Bohr radius is ∼100 A.

Note that donors are defect levels, which are neutral when an electron occupies the defectlevel and positively charged when unoccupied. Acceptors are neutral when empty and negativelycharged when occupied by an electron. The acceptor levels are produced when impurities, whichhave a similar core potential as the atoms in the host lattice, but have one less electron in theoutermost shell, are introduced into the crystal.

As shown in figure 2.21 the acceptor impurity potential could now be considered to be equiv-alent to a host atom potential, together with the Coulombic potential of a negatively chargedparticle. The “hole” (i.e., the absence of an electron in the valence band) can then bind to the ac-ceptor potential. The effective mass equation can again be used, since only the top of the valenceband contributes to the acceptor level. The valence band problem is considerably more complex

2.8. DOPING OF SEMICONDUCTORS 63

and requires the solution of multiband effective mass theory. However, the acceptor level can bereasonably predicted by using the heavy hole mass. Due to the larger hole mass, acceptor levelsare usually deeper in the bandgap than donor levels.

Population of dopant levelsThe presence of a dopant impurity creates a bound level Ed (or Ea) near the conduction (or va-lence) bandedge. If the extra electron associated with the donor occupies the donor level, it doesnot contribute to the mobile carrier density. The purpose of doping is to create a mobile electronor hole. When the electron associated with a donor (or a hole associated with an acceptor) is inthe conduction (or valence) band, the dopant is said to be ionized. To calculate densities of elec-trons and holes at finite temperatures in doped semiconductors we note that carrier densities theelectrons will be redistributed, but their numbers will be conserved and will satisfy the followingequality resulting from charge neutrality

(n − ni) + nd = Nd (2.8.7)

(p − pi) + pa = Na (2.8.8)

or

n + nd = Nd − Na + p + pa (2.8.9)

where

n = total free electrons in the conduction band

nd = electrons bound to the donors

p = total free holes in the valence band

pa = holes bound to the acceptors

The number density of electrons attached to the donors has been derived in equation 2.4.4 andis given by

nd

Nd=

1

12 exp

(Ed−EF

kBT

)+ 1

(2.8.10)

The factor 12 essentially arises from the fact that there are two states an electron can occupy at a

donor site corresponding to the two spin-states.The probability of a hole being trapped to an acceptor level is given by

pa

Na=

1

14 exp

(EF −Ea

kBT

)+ 1

(2.8.11)

The factor of 14 comes about because of the presence of the two bands, light hole, heavy hole,

and the two spin-states.To find the fraction of donors or acceptors that are ionized, we have to use a computer pro-

gram in which the position of the Fermi level is adjusted so that the charge neutrality conditiongiven Eq. 2.8.9 is satisfied. Once EF is known, we can calculate the electron or hole densitiesin the conduction and valence bands. For doped systems, it is useful to use the Joyce–Dixon

64 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

Si

BNegative B ion

Hole

One electron taken from the valence band to complete the

bonding of the boron atom hole

Si

Si

Si

Si

Si

Si

+

–

A cceptor levelEa

Eg

E

0: V alence band

Conductionband

Figure 2.21: Boron has only three valence electrons. It can complete its four fold tetrahedralbonds only by taking an electron from an Si–Si bond, leaving behind a hole in the silicon valenceband. The positive hole is then available for conduction.

approximation, which gives the relation between the Fermi level and the free carrier concentra-tion. This approximation is more accurate than the Boltzmann approximation. According to theJoyce–Dixon approximation , we have

EF = Ec + kBT

[ln

n

Nc+

1√8

n

Nc

]= Ev − kBT

[ln

p

Nv+

1√8

p

Nv

](2.8.12)

This relation can be used to obtain the Fermi level if n is specified. Or else it can be used toobtain n if EF is known by solving for n iteratively. If the term (n/

√8 Nc) is ignored, the result

corresponds to the Boltzmann approximation.If we examine the mobile carrier density dependence upon temperature, there are three regimes,

as shown in figure 2.22 for an n−type material. At low temperatures, the electrons coming fromthe donors are attached to the donors and occupy the impurity levels Ed. Thus there is no con-tribution to the mobile carrier density from the dopants. This regime is called the carrier freezeout regime. At higher temperatures, the dopants ionize until most of them are ionized out over atemperature regime, the mobile carrier is essentially equal to the dopant density and independentof temperature. This is the saturation regime and semiconductor devices are operated in thisregime. At very high temperatures, the intrinsic carrier density overwhelms the dopant densityand the material acts as an intrinsic material.

In figure 2.23 we show experimentally measured properties of Mg in GaN (Mg acts as adeep acceptor in GaN). When the temperature is not extremely high, the hole concentration ismuch less than the effective acceptor concentration NA −ND, since deep acceptors are not fullyionized at lower temperatures.

2.9. DOPING IN POLAR MATERIALS 65

Intrinsic range

Si

Nd = 1015cm–3

1000 300 200 100 75 50500

1710

10

10

10

10

16

15

14

13

0 4 8 12 16 20

Saturation range

Freeze-outrange

1000/T (K–1)

ni

ELE

CT

RO

ND

EN

SIT

Yn

(cm

–3)

TEMPERATURE (K)

Nd = 1016cm–2

Figure 2.22: Electron density as a function of temperature for a Si sample with donor impurityconcentration of 1015 cm−3.

2.9 DOPING IN POLAR MATERIALS

Semiconductors such as GaN, In, and AlN are called polar materials since they can have netpolarization due to a shift in the cation and anion sublattices. In unstrained zinc-blende structuresthe cation and anion sublattices are arranged in such a way that there is no net polarization inthe material. However, in the wurtzite crystal (like InN, GaN, AlN) the arrangement of thecation and anion sublattices can be such that there is a relative movement from the ideal wurtziteposition to produce a “spontaneous polarization” in the crystal which becomes very importantfor heterostructures. This effect is illustrated in figure 2.24. Also given in table 2.4 are the valuesof the spontaneous polarization which is aligned along the c-axis of the crystal.

In addition to spontaneous polarization is another phenomena which can lead to polarization inthe material. Strain can cause a relative shift between the cation and anion sublattices and createnet polarization in the material. This is the piezoelectric effect. In figure 2.25 we show howthe movement of rows can cause polarization effect by looking at the structural arrangements ofatoms in barium titanate.

66 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

(b)

(c)

0 1 2 3 4 5 6 7 8 9 10 111012

1013

1014

1015

1016

1017

1018

1019

1020

A B C

Hol

e C

once

ntra

tion

(cm

-3)

1000/T (1/K)

0 1 2 3 4 5 6 7 81014

1015

1016

1017

1018

1019

1020

D E F

Hol

e C

once

ntra

tion

(cm

-3)

1000/T (1/K)

100 1000

10-1

100

101

102

A B C D E F

Mob

ility

(cm

2 /Vs)

Temperature (K)

Cp2Mg flow

Sample Growth sccm nmol/min ΔEA (meV) NA (cm-3) ND (cm-3)

A 990206PB 15 24.4 190 1.8×1019 1.1×1018

B 990206PA 26 42.3 174 4.6×1019 3.0×1018

C 990205PD 47 76.5 152 1.4×1020 1.2×1019

D 980901PA 83 135 118 2.2×1020 4.1×1019

E 990205PC 140 228 112 8.6×1019 2.7×1019

F 980901PE 263 428 165 7.6×1018 5.0×1018

(a)

Figure 2.23: Measured properties of a deep acceptor: Mg doping of GaN. (a) Doping parametersfor six different samples. (b) Hole concentration as a function of temperature. Notice that for allthese samples, when the temperature is not extremely high, the hole concentration is much lessthan the effective acceptor concentration NA − ND, since deep acceptors are not fully ionizedat lower temperatures. (c) Hole mobility as a function of temperature. Figures are from the PhDdissertation of Peter Kozodoy, UCSB.

2.9. DOPING IN POLAR MATERIALS 67

C

a

Figure 2.24: The wurtzite crystal structure unit cell. In the ideal wurtzite structure the c lattice

constant is related to the a lattice constant by the relation c = 2√

23a. However, when the cation-

anion bond lengths cause a deviation from this relationship a net spontaneous polarization iscreated.

Polar Charge at Heterointerfaces

If there is a net movement of one sublattice against each other, a polarization field is set up.This results in a positive and negative polar charge. Under most conditions the polar charge onthe free surfaces is neutralized by charges present in the atmosphere. This causes depolarizationof the material. If, however, a heterostructure is synthesized and the two materials forming thestructure have different values for the polarization, there is a net polar charge (and polarization)at the interface as shown in figure 2.30. In semiconductors this polar charge can cause a built-inelectric field

E =P

ε(2.9.1)

The interface charge PA−PB and the built-in interface field (see figure 2.26) can be exploited indevice design since for most applications this fixed polar charge can act as dopant (see figure 2.27and figure 2.28).

68 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

Ba++ Ti4+

Displacement of positive charges with respect to negative chargesferroelectric effect

(b)

Ba++

O– –

Ti4+

Cube corners: Ba++

Cube face centers: O– –

Cube center: Ti4+

(a)

Figure 2.25: The structure of a typical perovskite crystal illustrated by examining barium titanate.(b) The movement of the ions leads to a ferroelectric effect.

A

–

+

– – – – –

+ + + + +– – – – – –

+ + + + + +– – – – – –

+ + + + + +– – – – – –

B

Polarization PA

Interface charge density = PA – PB

Polarization PB

Figure 2.26: A schematic showing how interface charge density can be produced at heterointer-faces of two polar materials.

For example, in AlGaN/GaN HFETs , a fixed sheet charge is formed at the heterointerfacedue to the the piezoelectric polarization in the strained AlGaN, and the discontinuity in thespontaneous polarization at the interface (see figure 2.27). To screen the net positive chargeat the AlGaN/GaN junction, a 2DEG is formed. The same effect can also be used to create abulk three-dimensional electron slab, as shown in figure 2.28. This is achieved by grading fromGaN to AlGaN, thus spreading the polarization-induced charge over the graded region. Thepolarization-induced carrier density, ρπ , is given by the equation ρπ = ∇ · P; here P is the totalpolarization in the material. Since the AlGaN composition and polarization are shown to be well-approximated by Vegard’s law, any desired channel charge profile can be obtained by choosing

2.9. DOPING IN POLAR MATERIALS 69

ZINC BLENDE

Material e14 (C/m2)

AlAs –0.23

GaAs –0.16

GaSb –0.13

GaP –0.10

InAs –0.05

InP –0.04

WURTZITE (c-axis growth)

Material e31 (C/m2) e33 (C/m2) Psp (C/m2)

AlN –0.6 1.46 –0.081

GaN –0.49 0.73 –0.029

InN –0.57 0.97 –0.032

Table 2.4: Piezoelectric constants in some important semiconductors. For the nitrides the spon-taneous polarization values are also given. (Data for zinc-blende material from S. Adachi, J.Appl. Phys. vol. 58, R1 (1985). For nitrides see E. Bernardini, V. Fiorentini, and D. Vanderbilt,Phys. Rev. B vol. 56, R10024 (1997).)

the appropriate grading scheme. This polarization induced channel charge can be modulated bya gate in a structure called a polarization-doped FET or PolFET can be used to tailor the gm-Vgs

profile of the PolFET. This is analogous to impurity doped MESFETs, where the gm-Vgs profileis modified by dopant profile design. In figure 2.29, we show experimentally measured electricalcharacteristics of doped GaN, GaN 2DEG structures, and GaN 3DEG structures.

Piezoelectric EffectAs noted above, when a structure is under strain a net polarization can arise—a phenomenoncalled piezoelectric effect. The value of the polar charge induced by strain depends upon thestrain tensor. In the previous section we have discussed the nature of the strain tensor in strainedepitaxy (i.e., in the coherent growth regime).

Nitride heterostructures have polarization charges at interfaces because of strain related piezo-electric effect as well as from spontaneous polarization. For growth along (0001) orientation thestrain tensor for coherently strained wurtzite crystals is given in Chapter 1. The piezoelectricpolarization is related to the strain tensor by the following relation

Ppz = e33εzz + e31(εxx + εyy) (2.9.2)

Piezoelectric effect is also present in zinc blende structures. However, the piezoelectric effectonly occurs when the strain tensor has off-diagonal components. The polarization values aregiven by

Px = e14εyz

Py = e14εxz

Pz = e14εxy (2.9.3)

70 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

(a)

(b)

Su

rfa

ce

Do

no

rs

GaN

2DEG

0 200 400 600 800 1000 1200-4

-3

-2

-1

0

1

2

Energ

y (

eV

)

Distance (Angstrom)

Ec Ev Ef

Ec Ev Ef

AlXGa1-XN

ΔP

SP

+ P

PE

ΔP

SP

+ P

PE

Figure 2.27: Mobile 2-dimensional sheet of electrons induced by polarization fields in an Al-GaN/GaN heterostructure. (a) Charge distribution and (b) band diagram for the structure.

As can be seen from the discussion of the previous section the strain tensor is diagonal for growthalong (001) direction. As a result there is no piezoelectric effect. However for other orientations,notably for (111) growth there is a strong piezoelectric effect.

2.9. DOPING IN POLAR MATERIALS 71

(a) (b)

20 40 600

1x1018

2x1018

3x1018C

harg

e (c

m-3)

Distance (nm)

30%

20 40 60 800

2x1018

4x1018

Cha

rge

(cm

-3)

Distance (nm)

20 40 60 800

2x1019

4x1019

6x1019

8x1019

1x1020

Cha

rge

(cm

-3)

Distance (nm)

Al C

om

p

Al C

om

p

Al C

om

p

HEMT Linear Grading Parabolic Grade

(c)

Figure 2.28: A 3-dimensional charge distribution can be induced in polar materials via bandgapgrading. (a) 2-dimensional charge distribution induced via an abrupt interface. (b) Linear gradeand (c) parabolic grade result in the displayed 3-dimensional charge distributions. (Figure cour-tesy S. Rajan, UCSB)

Piezoelectric effect can be exploited to create interface charge densities as high as 1013 cm−2

in materials. In Table 2.4 we provide the values of piezoelectric constants for some semicon-ductors. In addition to the polarization induced by strain, the cation and anion sublattices arespontaneously displaced with respect to each other producing an additional polarization. Forheterostructures the difference of the spontaneous polarization appears at the interfaces, as notedearlier. In Chapter 1 we have provided the values of spontaneous polarization for AlN, GaN, andInN.

EXAMPLE 2.5 A thin film of Al0.3Ga0.7N is grown coherently on a GaN substrate. Calculate the polarcharge density and electric field at the interface.

The lattice constant of Al0.3Ga0.7N is given by Vegard’s law

aall = 0.3aAlN + 0.7aGaN = 3.111 A

The strain tensor isεxx = 0.006

Using the elastic constant values from Chapter 1

εzz = −0.6 × 0.006 = 0.0036

The piezoelectric effect induced polar charge then becomes

Ppz = 0.0097 C/m2

72 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

Figure 2.29: Measured electrical characteristics as a function of temperature for three differentGaN samples. The sample with the lowest sheet charge is doped with Si (a shallow donor inGaN) to generate mobile electrons. In the sample with the highest sheet charge, carriers aregenerated by grading AlGaN from 0% Al to 30% Al, resulting in a 3-dimensional electron dis-tribution (as in figure 2.28b and c). In the third sample, a 2DEG is generated in an AlGaN/GaNheterostructure (as in figure 2.28a). While the charge in the Si-doped sample decreases as tem-perature is decrease (carrier freeze-out), the charge in the other two samples remains constant.Figures courtesy of D. Jena, University of Notre Dame.

This corresponds to a density of 6.06 × 1012 cm−2 electronic charges.In addition to the piezoelectric charge the spontaneous polarization charge is

Psp = 0.3(0.089) + 0.7(0.029) − 0.029 = 0.018 C/m2

which corresponds to a density of 1.125 × 1013 cm−2 charges. The total charge (fixed) arising at theinterface is the sum of the two charges.

2.10. TAILORING ELECTRONIC PROPERTIES 73

2.10 TAILORING ELECTRONIC PROPERTIES

In many applications we need bandgaps or carrier properties that are not available in naturallyoccurring materials. It is possible to tailor electronic properties by using alloys and quantumwells.

2.10.1 Electronic properties of alloys

Alloys are made from combinations of two or more materials and can be exploited to createnew bandgaps or lattice constants. In Chapter 1 we have discussed how the lattice constant ofalloys changes with composition. To the first order the electronic properties are also given by asimilar relation. Consider an alloy AxB1−x made from materials A with bandstructure given byEA(k) and B with bandstructure given by EB(k). The bandstructure of the alloy is then givenby

Eall(k) = xEA(k) + (1 − x)EB(k) (2.10.1)

Note that the energy averaging is done at the same k value. If we make an alloy from a directand an indirect material, one does not simply average the bandgaps to get the alloy bandgap.Instead the bandgaps at the same k values are averaged and the bandgap is then given by thelowest energy difference between the conduction and valence energies.

Based on the equation above the effective mass of the alloy is to be averaged as

1

m∗all

=x

m∗A

+(1 − x)

m∗B

(2.10.2)

It is important to note that alloys have inherent disorder since they have random arrangementsof atoms. This leads to disorder related scattering discussed in the next chapter.

2.10.2 Electronic properties of quantum wells

Quantum wells offer a very useful approach to bandstructure tailoring. In Section 2.2 we havediscussed electronic properties in quantum wells. In quantum wells electrons behave as if theyare in a 2-dimensional space and acquire properties that are especially useful for many electronicand optoelectronic applications.

When two semiconductors with different bandgaps (and chemical compositions) form an in-terface, We need to know how does the conduction band (valence band) on one material lineup with the other materials bands? This information is usually obtained through experiments.There are three possible scenarios as shown in figure 2.30. In type I structures the layer bandgapmaterial “surrounds” the bandgap of the small gap material. In quantum wells made from suchmaterials, both electrons and holes are confined in the same physical quantum well. Most elec-tronic and optoelectronic devices are based on type I lineup. In type II lineup the conductionband of material A is below that of the material B, but the valence band of A is above thatof B as shown. In quantum wells made from such materials the electrons and holes are con-fined in spatially different quantum wells. These structures are useful for applications in thelong wavelength regime, since their “effective” bandgap can be very small. Finally, in type III

74 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

TYPE I

HETEROSTRUCTURE

AB

TYPE II

HETEROSTRUCTURE

BROKEN GAP TYPE III

HETEROSTRUCTURE

BB

AABandgap

Figure 2.30: Various possible bandedge lineups in semiconductors A and B.

heterostructures, both the conduction and valence band edges of material A are above the con-duction band edge of material B. In figure 2.31 we show bandlineups for a number of differentmaterial systems.

In figure 2.32 we show a schematic of a type I quantum well made from a smaller bandgapmaterial B sandwiched between a large bandgap material A. To understand the electronic prop-erties of the quantum well we use the effective mass approach and the discussion of Section 2.2.The key difference in semiconductor quantum wells is that we need to use the effective massinstead of the free electron mass.

The confinement of electrons and holes by quantum wells alters the electronic properties ofthe system. This has important consequences for optical properties and optoelectronic devices.In an infinite quantum well the confined energies are

En =π2

�2n2

2m∗W 2(2.10.3)

The energy of the electron bands are then

E = En +�

2k2‖

2m∗ (2.10.4)

The two-dimensional quantum well structure thus creates electron energies that can be describedby subbands (n = 1, 2, 3 · · · ). The subbands for the conduction band and valence band areshown schematically in figure 2.33.

2.10. TAILORING ELECTRONIC PROPERTIES 75

SiGe

SiCSiO2

GaNAlNInN

GaAsInAsInP

ZnOZnOZnSAlPGaPAlAsAlSbGaSbInSbCdS

ZnSeCdSeZnTeCdTeH2O

Si3N4

TB2O5

BaTiO3

550-BaTiO3

BaZrO3

SrTiO3

SrTiOSrO

ZrO2

HfO2

Al2O3

Y2O3

ZrSiO4

PrO3

a-Si

-10 -9 -8 -7 -6 -5 -4 -3 -2 -1 0

Band Alignment

eV

Mat

eria

l

Figure 2.31: Bandedge lineups in a variety of materials.

If the barrier potential Vc is not infinite, the wavefunction decays exponentially into the barrierregion, and is a sine or cosine function in the well. By matching the wavefunction and itsderivative at the boundaries one can show that the energy and the wavefunctions are given by thesolution to the transcendental equations (see Section 2.2)

α tanαW

2= β

α cotαW

2= −β (2.10.5)

where

α =

√2m∗E

�2

β =

√2m∗(Vc − E)

�2

76 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

∞

E2

E1

V(z)∞

∞∞

quantum well

Valence band

POSITION z

Conduction band

quantum well

EN

ER

GY

Barrier materialWell

material

W

V0

Barrier material

Figure 2.32: A schematic of a quantum well formed for the electron and holes in a heterostruc-ture.

These equations can be solved numerically. The solutions give the energy levels E1, E2, E3

. . . and the wavefunctions, f1(z), f2(z), f3(z), · · · .Each level E1, E2, etc., is actually a subband due to the electron energy in the x–y plane. As

shown in figure 2.33 we have a series of subbands in the conduction and valence band. In thevalence band we have a subband series originating from heavy holes and another one originatingfrom light holes.

The subband structure has important consequences for the optical and transport properties ofheterostructures. An important manifestation of this subband structure is the density of statesof the electronic bands. The density of states figures importantly in both electrical and opticalproperties of any system. In Section 2.3 we have discussed how dimensionality alters the densityof states.

2.10. TAILORING ELECTRONIC PROPERTIES 77

The density of states in a quantum well is

• Conduction band

N(E) =∑

i

m∗

π�2θ(E − Ei) (2.10.6)

where θ is the heavyside step function (unity if E > Ei; zero otherwise) and Ei are the subbandenergy levels.• Valence band

N(E) =∑

i

2∑j=1

m∗j

π�2θ(Eij − E) (2.10.7)

where i represents the subbands for the heavy hole (j = 1) and light holes (j = 2). The densityof states is shown in figure 2.33 and has a staircase-like shape.

The differences between the density of states in a quantum well and a three-dimensional semi-conductor is one of the important reasons why quantum wells are useful for optoelectronic de-vices. The key difference is that the density of states in a quantum well is large and finite at theeffective bandedges (lowest conduction subband and highest valence subband). As a result thecarrier distribution is highest at the bandedges.

The relationship between the electron or hole density (areal density for 2D systems) and theFermi level is different from that in three-dimensional systems because the density of statesfunction is different. The 2D electron density in a single subband starting at energy Ee

1 is

n =m∗

e

π�2

∫ ∞

Ee1

dE

exp(

E−EF

kBT

)+ 1

=m∗

ekBT

π�2

[ln

{1 + exp

(EF − Ee

1

kBT

)}]or EF = Ee

1 + kBT ln

[exp

(nπ�

2

m∗ekBT

)− 1

](2.10.8)

If more than one subband is occupied we can add their contribution similarly. For the holedensity we have (considering both the HH and LH ground state subbands)

p =m∗

hh

π�2

∫ −∞

Ehh1

dE

exp(

EF −EkBT

)+ 1

+m∗

�h

π�2

∫ −∞

E�h1

dE

exp(

EF −EkBT

)+ 1

(2.10.9)

where m∗hh and m∗

�h are the in-plane density of states masses of the HH and LH subbands. Wethen have

p =m∗

hhkBT

π�2

[ln

{1 + exp

(Ehh1 − EFp)

kBT

}]+

m∗�hkBT

π�2

[ln

{1 + exp

(E�h1 − EFp)

kBT

}](2.10.10)

If Ehh1 − E�h

1 > kBT

78 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

E2

Ec (bulk)

–W/2 +W/20

z

E1

E2

E1

k11

E = h2k// + E2

2m*

E nergy

Parabolic two-dimensional subbands

ΔEc

E = h2k// + E1

2m*

E1(HH)E1(L H)E2(HH)E2(L H)

L ight hole subbands

Heavy hole subbands

V alence band

Conduction band

Ev (bulk)

Den

sity

of

stat

es

E ffective gap

Well gap

Quantum well E vs k11

2

2

Figure 2.33: Schematic of density of states in a 3–, 2– and 1–dimensional system . The subbandstructure is shown.

2.10. TAILORING ELECTRONIC PROPERTIES 79

The occupation of the light hole subband can be ignored.In many electronic devices used for information processing, a quantum well with a “triangu-

lar” shape is produced. The potential for electrons may be written in the form

V (x) = ∞ x < 0

= eEx x > 0 (2.10.11)

The potential energy of the particle is of the form

V (x) = Fx + constant (2.10.12)

where F is the force on the particle (say, an electron) and has a value eE . We choose theconstant in the potential energy to be such that at x = 0, V (x) = Ex as shown in figure 2.34.The solutions to this problem are the Airy functions

Φ(ξ) =1√π

∫ ∞

0

cos

(u3

3+ uξ

)du (2.10.13)

with a normalized solutionψ(ξ) = AΦ(ξ) (2.10.14)

The normalization constant can be shown to have the value

A =(2m)1/3

π1/2E 16 �2/3

(2.10.15)

The Airy functions have the following asymptotic behavior:

Φ(ξ) ∼ 1

2(ξ)−1/4 exp

(−2ξ3/2

3

), ξ > 0

Φ(ξ) ∼ | ξ |−1/4 sin

(2 | ξ |3/2

3+

π

4

), ξ < 0 (2.10.16)

Note that at x = 0 the second form is to be used, since ξ < 0.The solutions for the energy levels turn out to be:

En =

(�

2

2m

)1/3 (3

2πE

)2/3 (n − 1

4

)2/3

, n = 1, 2, . . . (2.10.17)

As shown in figure 2.35, in electronic devices such as a MOSFET or a MODFET the deviceconsists of an insulator-semiconductor junction. Electrons are injected at the interface on thesemiconductor side by a controlling electrode (the gate). The free charge causes a bending ofthe semiconductor band to produce an approximately triangular quantum well, as shown. Thetriangular quantum well is defined by an electric field Es which is related to the areal chargedensity by Gauss’s law

Es =ens

εs(2.10.18)

As a result of the confinement, quantized energy levels are formed in the triangular well.Approximate positions of these levels can be obtained from the results given above.

80 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

x

Semiconductor

Insulator

Device channe l with free carriers

E2

E1

–

– –– –

V(x) = Interface electric field Es =

enS

TRIANGULAR QUANTUM WELL FORMED IN ELECTRONIC DEVICES

eEsx

εs

Figure 2.34: A schematic of free electrons (conduction electrons) in a semiconductor deviceconfined to an approximately triangular quantum well.

2.11 STRAINED HETEROSTRUCTURES

As noted in chapter 1 it is now possible to incorporate strain into an epitaxial film. In fact,strain of a few percent can be built-in simply by growing a film on a mismatched substrate. ne ofthe most important strained heterostructure is the SiGe/Si structure. This system is compatiblewith Si based technology since it uses Si substrates. Due the modifications in the bandstructurehigh performance SiGe electronic devices can be made. Other important strained structures areInGaAs grown on GaAs or InP substrates and the AlGaN/GaN structure.

Once the strain tensor is known, we are ready to apply the deformation potential theory tocalculate the effects of strain on various eigenstates in the Brillouin zone. The strain perturbationHamiltonian is defined and its effects are calculated in the simple first order perturbation theory.In general we have

Hαβε =

∑ij

Dαβij εij (2.11.1)

where Dij is the deformation potential operator which transforms under symmetry operations asa second rank tensor. Dαβ

ij are the matrix elements of Dij .

2.11. STRAINED HETEROSTRUCTURES 81

The built in strain causes several different effects on electronic properties: i) It can lift thedegeneracies or band edges; ii) it can change the bandgap; iii) it can alter effective masses.To calculate the effect of strain one uses perturbation theory using equation 2.11.1. we willsummarize the relevant equations for a direct gap conduction band, an indirect gap X-valleyconduction bandedge and for the valence bands.

Case 1: Let us first examine how strain influences the bottom of the non degenerate Γ′2 state

which represents the conduction bandedge of direct bandgap semiconductors. This state is ans-type state and has the full cubic symmetry associated with it. The effect of the strain is toproduce a shift in energy.

δE(000) = Hε

= Dxx(εxx + εyy + εzz) (2.11.2)

Conventionally we writeDxx = Ξ

(000)d (2.11.3)

where Ξ(000)d represents the dilation deformation potential for the conduction band (000) valley.

Case 2: In this next case we will examine indirect gap materials like Si which have the con-duction bandedge along the (100) and equivalent directions. The bandedges are shifted accordingto the following equations.

δE(100) = Ξ(100)d (εxx + εyy + εzz) + Ξ(100)

u εxx (2.11.4)

By symmetry we can write

δE(010) = Ξ(100)d (εxx + εyy + εzz) + Ξ(100)

u εyy (2.11.5)

δE(001) = Ξ(100)d (εxx + εyy + εzz) + Ξ(100)

u εzz (2.11.6)

We note that if the strain tensor is such that the diagonal elements are unequal (as is the case instrained epitaxy), the strain will split the degeneracy of the six valleys in Si. This occurs in theSiGe/Si structures so that the 6-fold degenerate valleys split into 2-fold and 4-fold valleys. Theamount of splitting will be given later in this section.

Case 3: The triple degenerate states describing the valence bandedge.The valence band states are defined (near the bandedge) by primarily px, py , pz (denoted

by x,y,z) basis states. We have already discussed the strain tensor in epitaxial growth. For(001) growth which has been the main growth direction studied because of its compatibility withtechnology of processing we have

εxx = εyy = ε

εzz = −2c12

c11ε (2.11.7)

The effects of the strain can be shown to be like heavy hole and light hole degeneracy at thevalence bandedge. This also causes the hole mass to become smaller. For the InyGa1−yAs

82 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

system the separation between the HH and LH state is given by δ = −5.966ε eV. The effectof strain on bandstructure for both conduction band and valence band states is illustrated byexamining the direct bandgap material InxGa1−xAs grown on GaAs and the indirect bandgapmaterial GexSi1−x alloy grown on Si. For direct bandgap materials conduction bands, the straintensor only moves the position of the bandedge and has a rather small effect on the carrier mass.

TENSILE STRAIN IN

GROWTH PLANE

UNSTRAINED COMPRESSIVE STRAIN IN

GROWTH PLANE

Light hole

Heavy hole

LH

HH

LH

HH

Figure 2.35: Effect of strain on bandedges of a direct bandgap material. Due to the epitaxialstrain, the valence band degeneracy is lifted.

In figure 2.35 we show a schematic of how strain in a layer grown along the (001) directioninfluences the bandedges in a direct gap semiconductor. The conduction bandedge moves up ordown with respect to its unstrained position as discussed earlier, but since it is a non-degeneratestate there is no splitting. The valence bandedge is degenerate in the unstrained system. This de-generacy is lifted by quantum confinement even in an unstrained quantum well, but the splittingproduced by quantum confinement is usually small (∼ 10–15 meV). Under biaxial compressivestrain the bandgap of the material increases and the HH and LH degeneracy is lifted. The split-ting can easily approach 100 meV making strain an important resource to alter valence banddensity of states. Under biaxial compressive strain the HH state is above the LH state, whileunder biaxial tensile strain the LH state is above the HH state, as shown in figure 2.35.

In the case of the indirect bandgap Si1−xGex alloy grown on Si, the conduction band also issignificantly affected according to equation 2.11.4 through equation 2.11.6. For (001) growththere is splitting in the 6 equivalent valleys.The results on the bandedge states are shown infigure 2.36. Note that the biaxial compressive strain causes a lowering of the four-fold in-planevalleys below the 2 two-fold out of plane valleys. We see that the bandgap of SiGe falls rapidlyas Ge is added to Si. This makes the SiGe very useful for Si/SiGe heterostructure devices suchas heterojunction bipolar transistors. the splitting of the HH, LH and SO bands also cause asharp reduction in the density of states mass near the bandedge. The splitting of the conductionbandedge valleys also reduces the conduction band density of states in SiGe.

2.11. STRAINED HETEROSTRUCTURES 83

1.5

1.0

0.5

0.0

–0.50.0 0.2 0.4 0.6 0.8

Ge MOLE FRACTION (x)

BA

ND

ED

GE (

eV) [001] 6-fold degenerate unstrained

SiGe conduction band

Bands when SiGe is strained by Si substrate

[100][010]

HHLH

SH

Figure 2.36: Epitaxial strain induced splittings of the conduction band and valence band as afunction of alloy composition for Si1−xGex grown on (001) Si. UCB: unstrained conductionband, HH: heavy hole, LH: light hole, SH: split-off hole.

0.5

0.4

0.3

0.2

0.1

0.0–2.0 –1.0 0.0 1.0 2.0

m* /

m0

ε(%)

Figure 2.37: Change in the density of states mass at the valence bandedges as a function of strainfor the Al0.3Ga0.7As/InGaAs system.

84 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

2.12 DEFECT STATES IN SOLIDS

The band theory discussed in this chapter is valid only for perfect crystals. Even in good-quality crystals there are defects, which break the periodicity of the structure. Typical defects incrystalline materials are: (i) defects in the structure arise from missing atoms (vacancies), atomsat the wrong sites, unintended impurities, etc. (ii) We may also have dislocations at surfaces of acrystal the arrangement of atoms does not have the same periodicity as in the bulk. (iii) We couldalso have absorbed atoms or molecules at the surface; disordered solids such as amorphous orpolycrystalline materials.

Defects and surface states

In figure 2.38 we show a schematic of a perfectly periodic material and one with a defect. Adeep potential region indicates the region of defect. In the case of the periodic system we haveseen the electrons see a bandedge and are described by simple a effective mass equations nearthe bandedge. There are no allowed states in the bandgap region. In the case of a defect the deeplevel causes new electronic states, which can have energies in the bandgap.

Bound state trapped near the grain boundary

Perfectly periodic material Defect in a material

ATOMIC

POTENTIALS

ψ ψ

Schematic of electron states in a perfect crystal

Schematic of a defect

r"free" states

r

Defect

(a) (b)

ATOMIC

POTENTIALS

Figure 2.38: A schematic of the structural and electronic properties of (a) crystals and of (b) amaterial with a defect.

2.12. LOCALIZED STATES IN SOLIDS 85

Ev Ec

Valence band

Perfect structure

ELECTRON ENERGY

DE

NSI

TY

OF

STA

TE

S

(a)

Ev Ec

Structure with Defects

ELECTRON ENERGY

DE

NSI

TY

OF

STA

TE

S

(b)

Defect states}

Conduction band

Valence band Conduction band

No bandgap states

Figure 2.39: Schematic of density of states (a) in a perfectly periodic solid and (b) in a materialwith defects. The presence of bangap states influences semiconductor devices.

86 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

The key difference between electronic states in the perfect crystal and a non-perfect crystal isrelated to the wavefunction. In the periodic state, the electron state is extended over the entiresystem, as shown in figure 2.38a. This reflects the fact that the electron can propagate from oneregion to another. In the case of a defect a bandgap state may be created with an associatedwavefunction that is spatially localized near the defect region, as shown in figure 2.38b. Whenan electron is occupying such a localized state its transport (mobility, diffusion) properties areseriously affected. Localized electrons cannot move across the material as easily.

In figure 2.39 we show a comparison of the density of states in a perfectly periodic and of adefect-containing material. In the case of the perfect material we have a well-defined bandgap,while in the presence of defects we have bandgap states. Electrons can be trapped into thebandgap states (hence these states are also called traps).

2.13 TECHNOLOGY ISSUES

We have examined some of the driving forces behind some of the technologies. The useof alloys and heterostructures adds a tremendous versatility to the available parameter space toexploit. Semiconductor alloys are already an integral part of many advanced technology systems.Consider the following examples.

• The HgCdTe alloy is the most important high-performance imaging material for longwavelength applications (10 – 14 μm). These applications include night vision, seeingthrough fog, thermal imaging of the human body parts for medical applications, and ahost of special purpose applications involving thermal tracking.

• The AlGaAs alloy is an important ingredient in GaAs/AlGaAs heterostructure deviceswhich drive a multitude of technologies including microwave circuits operating up to100 GHz, lasers for local area networks, and compact disc players.

• InGaAs and InGaAsP alloy systems are active ingredients of MMICs operating above100 GHz and long-haul optical communication lasers.

While alloys are important ingredients of many technologies, it must be emphasized againthat alloys are not perfectly periodic structures. This results in random potential fluctuationswhich leads to an important scattering mechanism that limits certain performances. For example,the low temperature low field mobility is severely affected by alloy scattering as is the excitonline width of optical modulators. The growth and fabrication issues in alloy systems are alsosometimes serious due to miscibility gaps that may be present.

2.14 PROBLEMS

Problem 2.1 Plot the conduction band and valence band density of states in Si and GaAsfrom the bandedges to 0.5 eV into the bands. Use the units eV−1 cm−3. Use the following

2.14. PROBLEMS 87

data:

Si : m∗1 = m∗

� = 0.98 m0

m∗2 = m∗

3 = m∗t = 0.19 m0

m∗hh = 0.49 m0

m∗�h = 0.16 m0

GaAs : m∗e = m∗

dos = 0.067 m0

m∗hh = 0.45 m0

m∗�h = 0.08 m0

The wavevector of a conduction band electron in GaAs is k =(0.1, 0.1, 0.0) A−1. Calculate the energy of the electron measured from the conductionbandedge.

Problem 2.2 Calculate the lattice constant, bandgap, and electron effective mass of thealloy InxGa1−xAs as a function of composition from x = 0 to x = 1.

Problem 2.3 Calculate the effective density of states at the conduction and valence bandsof Si GaAs, and GaN at 77 K, 300 K, and 500 K.

Problem 2.4 Estimate the intrinsic carrier concentration of diamond at 700 K. You canassume that the carrier masses are similar to those in Si. Compare the results with thosefor GaAs, Si, SiC and GaN.

Problem 2.5 Estimate the change in intrinsic carrier concentration per K change intemperature for InAs, Si, and GaAs at near room temperature.

Problem 2.6 Calculate the Fermi energy and Fermi velocity for the following metals: Ag,Au, Ca, Cs, Cu, Na.

Problem 2.7 Calculate the change in the Fermi level as temperature changes from 0 to1000 K for Al and Cu.

Problem 2.8 Consider a donor an energy ED from the conduction band as shown infigure 2.40. If the density of the donor device is ND(cm−3) derive a relationship for theposition of the fermi level as a function of temperature in terms of NC and NV. Plot thefermi level as a function of temperature for the case ND = NA= NV. Physically explainyour result. Repeat for the case of a donor and an acceptor of densities ND and NA

respectively. What will be the dependence of the fermi level on temperature if (i) ND =NA, (ii) ND >NA, and (iii) ND < NA. Explain.

Problem 2.9 Consider a slab of GaAs that is doped n-type with 1017cm−3.

1. Consider the case where there is a surface donor state 0.5 eV from the conductionband. What is the fermi level at the surface as the density of this level is increasedfrom 1010cm−2 to 1014cm−2?

88 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

EC

EV

ED

ECED

EV

EA

Figure 2.40: Figure for problem 2.8.

2. Solve the previous part for the case with only an acceptor state 0.5 eV from theconduction band.

3. Assume now that there are two defect levels of equal density, one donor-like and theother acceptor-like, at the surface. The acceptor state is 0.3 eV from the conductionband edge and the donor state is 0.5 eV from the conduction band edge. How doesthe fermi level pinning at the surface change as the areal density of each of thesestates is kept equal and increased from 1010cm−2 to 1014cm−2?

4. Now the positions of the defect levels are changed. The acceptor state is 0.5 eV fromthe conduction band edge and the donor state is 0.3 eV from the conduction bandedge. How does the fermi level pinning at the surface change as the density of eachof these states is kept equal and increased from 1010cm−2 to 1014cm−2?

5. Metals X and Y are now evaporated on the surface with 1013cm−2 donor states at 0.5eV from the conduction band. Find the position of the fermi level at the surface formetal X(Φms = 0.3eV ) and metal Y(Φms = 0.7eV ).

6. Repeat part 5 but with acceptor states this time, assuming they have the same energylevel and areal density.

Draw band diagrams to explain your solutions.

Problem 2.10 Assume a pn junction with an acceptor close to the valence band edge, sothat the acceptors are fully ionized at 300K. Assume NA = ND = 1018cm−3. What is thebuilt-in voltage of the junction? Now, the choice of acceptor is changed such that only1/10th of the acceptors are ionized.

1. What is the acceptor level relative to the valence band?

2. What is the new built-in voltage of the diode. Make reasonable approximationswhich should be justified.

3. Draw a band diagram of the system showing the acceptor level and the Fermi level.

Problem 2.11 Using Vegard’s law for the lattice constant of an alloy (i.e., the latticeconstant is the weighted average) find the bandgaps of alloys made in InAs, InP, GaAs,GaP which can be lattice matched to InP.

2.14. PROBLEMS 89

Problem 2.12 For long-haul optical communication, the optical transmission losses in afiber dictate that the optical beam must have a wavelength of either 1.3 μm or 1.55 μm.Which alloy combinations lattice matched to InP have a bandgap corresponding to thesewavelengths?

Problem 2.13 Calculate the composition of HgxCd1−xTe which can be used for a nightvision detector with bandgap corresponding to a photon energy of 0.1 eV. Bandgap ofCdTe is 1.6 eV and that of HgTe is −0.3 eV at low temperatures around 4 K.

Problem 2.14 In the In0.53Ga0.47As/InP system, 40% of the bandgap discontinuity is inthe conduction band. Calculate the conduction and valence band discontinuities. Calculatethe effective bandgap of a 100 A quantum well. Use the infinite potential approximationand the finite potential approximation and compare the results.

Problem 2.15 In an n-type Si crystal the doping changes abruptly from ND = 1015 toND = 1017. Make a qualitative sketch of the band diagram. Calculate

1. the built-in potential at the n+/n− interface, in eV. Also calculate how much of theband-bending occurs on each side of the junction,

2. the electric field at the n+/n− interface and

3. the electron concentration at the n+/n− interface.Assume T = 300K.

Problem 2.16 Calculate the first and second subband energy levels for the conductionband in a GaAs/Al0.3Ga0.7As quantum well as a function of well size. Assume that thebarrier height is 0.18 eV.

Problem 2.17 Calculate the width of a GaAs/AlGaAs quantum well structure in which theeffective bandgap is 1.6 eV. The effective bandgap is given by

Eeffg = Eg(GaAs) + Ee

1 + Eh1

where Eg (GaAs) is the bandgap of GaAs (= 1.5 eV) and Ee1 and Eh

1 are the ground stateenergies in the conduction and valence band quantum wells. Assume thatm∗

e = 0.067 m0,m∗hh = 0.45 m0. The barrier heights for the conduction and valence

band well is 0.2 eV and 0.13 eV, respectively.

Problem 2.18 Assume that a particular defect in silicon can be represented by athree-dimensional quantum well of depth 1.5 eV (with reference to the conductionbandedge). Calculate the position of the ground state of the trap level if the defectdimensions are 5 A× 5 A× 5 A. The electron effective mass is 0.26 m0.

Problem 2.19 A defect level in silicon produces a level at 0.5 eV below the conductionband. Estimate the potential depth of the defect if the defect dimension is 5 A× 5 A×5 A.The electron mass is 0.25 m0.

90 CHAPTER 2. ELECTRONIC LEVELS IN SEMICONDUCTORS

Problem 2.20 In an n-type Si crystal the doping changes abruptly from ND = 1015 toND = 1017. Make a qualitative sketch of the band diagram. Calculate(a) the built-in potential at the n+/n− interface, in eV. Also calculate how much of theband-bending occurs on each side of the junction,(b) the electric field at the n+/n− interface and(c) the electron concentration at the n+/n− interface.Assume T = 300K.

Problem 2.21 Consider a schottky barrier formed between Al(sφM = 4.1eV ) andGaAs(qχ = 4.04eV ). Consider that the surface has both acceptor and donor states in equalconcentration, 1.0 eV and 0.6 eV from the conduction band respectively. Assume that theconcentrations are equal (measured in cm−2). Assume a thin insulator (δA thick) betweenthe metal and the semiconductor to help set-up the problem. Calculate the barrier height asa function of the density of states Dscm

−2. Solve the problem for both n and p typesemiconductors doped at 1017cm−3. Plot.Note: The problem is solve by balancing charges in the system.

2.15 FURTHER READING

• General bandstructure

– H.C. Casey Jr. and M.B. Panish, Heterostructure Lasers, Part A, “Fundamental Prin-ciples,” Part B, “Materials and Operating Characteristics,” Academic Press, NewYork (1978).

– R.E. Hummel, Electronic Properties of Materials–An Introduction for Engineers,Springer Verlag, New York (1985).

– Landolt-Bornstein, Numerical Date and Functional Relationship in Science andTechnology, Vol. 22, Eds. O. Madelung, M. Schulz, and H. Weiss, Springer-Verlog,New York (1987).

– K. Seeger, Semiconductor Physics: An Introduction, Springer, Berlin (1985).

– H.F. Wolf, Semiconductors, Wiley-Interscience, New York (1971).

• Bandstructure modification

– A.G. Milnes and D.L. Feucht, Heterojunctions and Metal Semiconductor Junctions,Academic Press, New York (1972).

– For a simple discussion of electrons in quantum wells any book on basic quantummechanics is adequate. An example is L. Schiff, Quantum Mechanics, McGraw-Hill,New York (1968).

– J. Singh, Electronic and Optoelectronic Properties of Semiconductor Structures, Cam-bridge University Press (2003).

2.15. FURTHER READING 91

• Intrinsic and extrinsic carriers

– J.S. Blakemore, Electron. Commun., 29, 131 (1952).

– J.S. Blakemore, Semiconductor Statistics, Pergamon Press, New York (1962) reprintedby Dover, New York (1988).

– K. Seeger, Semiconductor Physics: An Introduction, Springer Verlag, Berlin (1985)

Chapter 3

CHARGE TRANSPORTIN MATERIALS

3.1 INTRODUCTION

Electronic devices rely on transport of electrons (holes) in materials. This transport occurseither under the influence of an electric field or carrier concentration gradients. In this chapterwe will examine how electrical current flows occur in materials. The charges in a solid canbe loosely classified as fixed and mobile. When an external perturbation is applied (e.g., anelectric field) the mobile charges can move from one point in space to another. In particularthey can move from one contact on a device to another. The fixed charge, however, can only bedisturbed slightly from its equilibrium position, but cannot move over the length of a device. Asshown in figure 3.1 both fixed charges and mobile charges play an important role in the physicsof semiconductors. Essentially all electronic devices such as field effect transistors, bipolartransistors, diodes, as well as optoelectronic devices, such as lasers and detectors depend uponfree or mobile charges. Mobile charges are the electrons in the conduction band and holes in thevalence band for semiconductors and insulators. As we have discussed in the previous chapter,in metals the mobile charges are the electrons in the conduction band.

Fixed charges in materials also play an important role in devices, even though they cannotparticipate in current flow. Small movements in the position of the fixed charges are responsiblefor the dielectric response of solids. The fixed charges are also responsible for polarizationeffects, which are exploited for devices, such as sensors and detectors.

Mobile carriers respond to electric fields and carrier concentration gradients. Electrons andholes also combine with each other. In this chapter we will examine the physical processes thatform the basis of electronic devices

92

3.2. CHARGE TRANSPORT: AN OVERVIEW 93

FIXED CHARGES

• Ions and tightly bound electrons

Important in dielectric response, polarization

effects

MOBILE CHARGES

• Electrons in the conduction band and holes

in the valence band

Important for current flow electronic and

optoelectronic devices

CHARGES IN SOLIDS

Figure 3.1: An overview of fixed and mobile charges in solids and their impact on physicalphenomena. Semiconductor devices are dependent upon mobile electrons and holes.

3.2 CHARGE TRANSPORT: AN OVERVIEW

Before discussing issues in free carrier (or mobile carrier) transport we remind the reader ofthe nature of electronic states in solids in figure 3.2. As noted in chapter 2, in the case of theperfect crystal we see that in the conduction and valence bands the electronic states are “free,”.There are no allowed energy levels in the bandgap (density of states is zero in the bandgap, asshown). In the case of a crystal with defects we still have the free states in the conductionand the valence bands, but we also have defect-related allowed states in the bandgap region, asshown in figure 3.2b. In these states (trap states) electrons are not free to move.

We will first provide a simple overview of how electrons respond to applied electric fields. Infigure 3.3 we show a schematic of how electrons (holes) move through a sample when an electricfield is applied. In figure 3.3a we show the situation in a good-quality crystalline material. Theelectron moves under the electric field force, but suffers a number of scattering processes. Thescattering occurs due to various imperfections, such as defects and vibrations of atoms (due tothermal energy). The relation between the electron velocity or distance traveled and appliedfield is complex. However at low fields the relation can be described by a simple relation. Ifwe examine the distance versus time trajectory of a typical electron we observe that the electronshows a path as shown in figure 3.3. On average the electron trajectory is described by

d = vt

v = μE (3.2.1)

where d is the distance traveled in time t. The velocity v is proportional to the electric field

94 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Ev Ec

Valence band

Perfect structure

ELECTRON ENERGY

DE

NSI

TY

OF

STA

TE

S

(a)

Ev Ec

Structure with Defects

ELECTRON ENERGY

DE

NSI

TY

OF

STA

TE

S

(b)

Defect levels}

Conduction band

Valence band Conduction band

Noallowed states

Figure 3.2: A schematic of the nature of electronic states in solids: (a) for a perfect crystal, (b)for a crystal with defects.

applied through μ, the mobility. When the electric field in large the relationship between velocityand applied field is not so simple and will be discussed later.

3.3 TRANSPORT AND SCATTERING

The problem of transport involves non-equilibrium physics. We need to find the distributionfunction for electrons in energy and momentum space under an applied field or under carrier con-centration gradients. We know that under equilibrium the electron (hole) distribution in energy(or momentum) is given by the Fermi–Dirac distribution

f(E) = f◦(E) =1

exp(

E−EF

kBT

)+ 1

E = Ei +�

2k2

2m∗

where Ei is the bandedge.

3.3. TRANSPORT AND SCATTERING 95

Crystalline Solid

–

–

E -field

E lectron

T IME

Free electron path

DIS

TA

NC

E d = vtv = μE

Mobility VE

=

Figure 3.3: A typical electron trajectory in a sample and the distance versus time profile.

We can see that in the absence of any applied electric field, the occupation of a state withmomentum +�k is the same as that of a −�k state. Thus there is net cancellation of momentaand there is no net current flow. The distribution function in momentum space is shown schemat-ically in figure 3.4a. The question we would like to answer is the following: If an electric fieldis applied, what happens to the free electrons (holes)? When a field is applied the electron dis-tribution will shift, as shown schematically in figure 3.4b, and there will be a net momentum ofthe electrons. This will cause current to flow. If the crystal is rigid and perfect, according to theBloch theorem the electron states are described by

ψk(r, t) = uk exp i(k · r − ωt) (3.3.1)

where ω = E/� is the electron wave frequency. There is no scattering of the electron in theperfect system. Also, if an electric field E is applied, the electron behaves as a “free” spaceelectron would, obeying the equation of the motion

�dk

dt= Fext = −eE (3.3.2)

According to this equation the electron will behave just as in classical physics (in absence ofscattering) except the electron will gain energy according to the appropriate bandstructure rela-tion.

In a real material, there are always imperfections which cause scattering of electrons so that theequation of motion of electrons is not given by equation 3.3.2. A conceptual picture of electrontransport can be developed where the electron moves in space for some time, then scatters and

96 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

–k 0 +k

f 0(k)

=

Σ = 0k

f(k) = f(–k)

Σ f(k) = 0

–k 0 +k

f(k)

(a)

(b)

-field

= 0Assymetric Function

f 0(k) f 0(-k)

f 0(k)

-Field = 0Symmetric Function

E

E

E

Figure 3.4: A schematic of the electron momentum distribution function in (a) equilibrium wheref(k) = f(−k) and (b) in the presence of an electric field.

then again moves in space and again scatters. The process is shown schematically in figure 3.5.The average behavior of the ensemble of electrons will then represent the transport properties ofthe electron.

3.3.1 Quantum Mechanics and Scattering of electrons

As noted above in absence of scattering the electron transport is very simple to understand.However, scattering dominates transport in semiconductor devices. The scattering problem insolids is treated by using the perturbation theory in quantum mechanics. The electron problemis formally represented by

HΦ = EΦ (3.3.3)

where H is the full hamiltonian (potential energy + kinetic energy operator) of the problem andthe electron states are denoted by Φ. This hamiltonian is, in our case, the sum of the hamiltonian

3.3. TRANSPORT AND SCATTERING 97

Collision

Free flight

Free flight

Collision

Collision

Collision

E

ZZ = 0

Free flight

CARRIER TRANSPORT IN SEMICONDUCTORS

Figure 3.5: Schematic view of an electron as it moves under an electric field in a semiconductor.The electron suffers a scattering as it moves. In between scattering the electron moves accordingto the “free” electron equation of motion.

of the perfect crystal Ho and the energy V corresponding to the imperfection causing scattering.Thus

H = Ho + V (3.3.4)

The problemHoψ = Eψ (3.3.5)

just gives us the bandstructure of the semiconductor which has been discussed in chapter 2. Inthe perturbation theory, we use the approach that the effect of the perturbation V is to causescattering of the electron from one perfect crystalline state to another. This theory works well ifthe perturbation is small. The effect of the scattering is shown schematically in figure 3.6. Therate of scattering for an electron initially in state i to a state f in the presence of a perturbationof the form

V (r, t) = V (r) exp (iωt) (3.3.6)

is given by the Fermi golden rule

Wif =2π

�| Mij |2 δ(Ei ± �ω − Ef ) (3.3.7)

where the various quantities in the equation represent the following:

98 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

How strongly V(r) couples the initial and final states

How many final states there are to scatter into

SCATTERING RATE

Initial electron Final electron

SCATTERING POTENTIAL

V(r)

k'k

+

Figure 3.6: Scattering of an electron initially with momentum �k from a scattering potentialV (r). The final momentum is �k′. The scattering process is assumed to be instantaneous.

• | Mij |2: The quantity is called the matrix element of the scattering and is given by

Mij =

∫ψ∗

fV (r)ψid3r (3.3.8)

The matrix element tells us how the potential couples the initial and the final state. A strongercoupling causes a higher rate of scattering.

• δ(Ei ± �ω − Ef ) :This δ-function is simply a representative of energy conservation. Theprocess where

Ef = Ei + �ω (3.3.9)

is called absorption, while the process

Ef = Ei − �ω (3.3.10)

3.3. TRANSPORT AND SCATTERING 99

is called emission. Thus, both absorption or emission of energy can occur if the perturbation hasa time dependence exp(iωt). If the potential is time independent (defects of various kinds), thescattering is elastic (Ei = Ef ).

The dominant scattering of carriers involves lattice vibrations resulting from thermal energy.Carriers may scatter from various crystal imperfections including dopants and other point de-fects, alloy disorder, and interface imperfections.

Phonon scatteringIn chapter 1, we discussed the crystalline structure in which atoms were at fixed periodic po-

sitions. In reality, the atoms in the crystal are vibrating around their mean positions. Theselattice vibrations are represented by “particles” in quantum mechanics and are called phonons.The properties of the lattice vibrations are represented by the relation between the vibration am-plitude, u, frequency, ω, and the wavevector q. The vibration of a particular atom, i, is givenby

ui(q) = uoi exp i(q · r − ωt) (3.3.11)

which represents an oscillation with quantum energy �ω. In a semiconductor there are two kindsof atoms in a basis. This results in a typical ω vs. k relation shown in figure 3.7. Although theresults are for GaAs, they are typical of all compound semiconductors. We notice two kinds oflattice vibrations, denoted by acoustic and optical. Additionally, there are two transverse andone longitudinal modes of vibration for each kind of vibration. The acoustic branch can becharacterized by vibrations where the two atoms in the basis of a unit cell vibrate with the samesign of the amplitude as shown in figure 3.7b. In optical vibrations, the two atoms with opposingamplitudes are shown.

As noted above, in quantum mechanics lattice vibrations are treated as particles carrying en-ergy �ω. According to the discussion on Bose-Einstein statistics in chapter 2, the phonon occu-pation is given by

nω =1

exp(

�ωkBT

)− 1

(3.3.12)

According to quantum mechanics, the total energy contained in the vibration is given by

Eω = (nω +1

2)�ω (3.3.13)

Note that even if there are no phonons in a particular mode, there is a finite “zero point” energy12�ω in the mode. This is important since even if n = 0 one can have scattering processes.

The vibrations of the atoms produce three kinds of potential disturbances that result in thescattering of electrons. A schematic of the potential disturbance created by the vibrating atomsis shown in figure 3.8. In a simple physical picture, we can imagine the lattice vibrations causingspatial and temporal fluctuations in the conduction and valence band energies. The electrons(holes) then scatter from these disturbances. The acoustic phonons produce a strain field in thecrystal and the electrons see a disturbance which produces a potential of the form

VAP = D∂u

∂x(3.3.14)

100 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Optical mode

Acoustical mode

k

k

16

14

12

10

6

8

4

2

0

0.06

0.05

0.04

0.03

0.02

0.01

00 1.0[100]

TO

LO

GaAs

LA

TA

FRE

QU

EN

CY

v(1

012

Hz)

REDUCED WAVE NUMBER k/Kmax

EN

ER

GY

(eV

)

(a)

(b)

The two atoms on the unit cell vibrate in opposing motion.

The two atoms in the unit cell vibrate along the same direction.

– –

––

– –

– –

Figure 3.7: (a) Typical frequency-wavenumber relations of a semiconductor (GaAs in this case).(b) The displacement of atoms in the optical and acoustic branches of the vibrations is shown.The motion of the atoms is shown for small k vibrations.

where D is called a deformation potential (units are eV) and ∂u∂x is the amplitude gradient of the

atomic vibrations.The optical phonons produce a potential disturbance, which is proportional to the atomic

vibration amplitude, since in the optical vibrations the two atoms in the basis vibrate opposing

3.3. TRANSPORT AND SCATTERING 101

Atomicdisplacement

Bandedgepositions

EC

r

EV

LATTICE VIBRATIONS

BANDEDGE VIBRATIONS

Figure 3.8: A schematic showing the effect of atomic displacement due to lattice vibrations onbandedge energy levels in real space.

each otherVop = Dou (3.3.15)

where Do (units are eV/cm) is the optical deformation potential.In compound semiconductors the two atoms on the basis are different and there is an effective

positive and negative charge e∗ on each atom. When optical vibrations take place, the effectivedipole in the unit cell vibrates, causing polarization fields from which the electron scatters. Thisscattering, called polar optical phonon scattering, has a scattering potential of the form

Vpo ∼ e∗u (3.3.16)

Each material has its own effective charge which is related to the ionicity of the material.By using the Fermi golden rule we can calculate the scattering rates of electrons due to latticevibrations. The acoustic acoustic phonon scattering rate for an electron with energy Ek to anyother state is given by

Wac(Ek) =2πD2kBTN(Ek)

�ρv2s

(3.3.17)

where N(Ek) is the electron density of states, ρ is the density of the semiconductor, vs is thesound velocity and T is the temperature.

In materials like GaAs, the dominant optical phonon scattering is polar optical phonon scatter-ing, and the scattering rate is given by (assuming the bandstructure is defined by a non-parabolic

102 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

band; ε∞ and εs are the high frequency and static dielectric constants of the semiconductor,while εo is the free space dielectric constant)

W (k) =e2m∗1/2ωo

4π√

2�

(εo

ε∞− εo

εs

)1 + 2αE′

γ1/2(E)Fo(E,E′)

×{

n(ωo) absorptionn(ωo) + 1 emission

}. (3.3.18)

where

E′ = E + �ωo for absorption

= E − �ωo for emission

γ(E) = E(1 + αE)

Fo(E,E′) = C−1

(A ln

∣∣∣∣γ1/2(E) + γ1/2(E′)γ1/2(E) − γ1/2(E′)

∣∣∣∣ + B

)A = [2(1 + αE)(1 + αE′) + α {γ(E) + γ(E′)}]2B = −2αγ1/2(E)γ1/2(E′)

= × [4(1 + αE)(1 + αE′) + α {γ(E) + γ(E′)}] aC = 4(1 + αE)(1 + αE′)(1 + 2αE)(1 + 2αE′)

It is important to examine typical values of scattering rates from these processes. The values forGaAs are shown in figure 3.9. Note that the phonon emission process can start only after theelectron has energy equal to the phonon energy. Optical phonon scattering is the most importantscattering mechanism for high-field or high-temperature transport of electrons. The emission rateis stronger than the absorption rate by the rate n(ω0p + 1) to n(ω0). Optical phonon emission isthe dominant mechanism for electrons to lose energy they gain from the electric field.

Ionized impurity scattering

An important scattering mechanism is due to ionized dopants. The scattering potential isCoulombic in nature, except that the potential is suppressed by screening effects due to freecarriers. The screening is due to the presence of the other free electrons or holes, which forma cloud around the ion. There are several models for the ionized impurity scattering potential.A good approximation for the potential seen by electrons in a semiconductor is given by thescreened Coulombic potential

V (r) =e2

ε

e−λr

r(3.3.19)

where

λ2 =ne2

εkBT(3.3.20)

3.3. TRANSPORT AND SCATTERING 103

8.0

7.0

6.0

5.0

4.0

3.0

2.0

1.0

0.00.00 0.10 0.20 0.30 0.40 0.50 0.60 0.70 0.80 0.90 1.00

Polar optical phonon emission

Polar optical phonon absorption

Acoustic phonon scattering

SCA

TT

ER

ING

RA

TE (

1012

s–1 )

ENERGY (eV)

10.0

9.0GaAs EXAMPLE

hωop = 36 meV threshold

Figure 3.9: Scattering rates due to acoustic and optical phonons for GaAs electrons at roomtemperature.

with n the free electron density. The scattering rate for an electron with energy Ek and momen-tum �k can be shown to be

W (k) = 4πF

(2k

λ

)2 [1

1 + (λ/2k)2

]F =

1

�

(e2

ε

)2N(Ek)

32k4NI (3.3.21)

where NI is the ionized impurity density. Note that ionized impurities (and the scattering pro-cesses discussed here) do not alter the spin of the electron. Thus N(E) is the density of stateswithout counting the spin degeneracy i.e it is half the usual density of states.

104 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Alloy scattering

Alloys are made from combinations of two or more materials. Since atoms on the lattice arearranged randomly there is random potential fluctuation which causes scattering. The scatteringrate for an alloy AxB1−x is found to be

Wtot =2π

�

(3π2

16V0

)U2

all N(Ek)[x (1 − x)2 + (1 − x) x2

]a =

3π3

8�V0 U2

all N(Ek) x (1 − x) (3.3.22)

Here Uall is the potential difference between A type and B type potentials (see Appendix B), V0

is the volume of the unit cell in the lattice and N(E) is the density of states without countingspin degeneracy.

While the phonon and impurity scattering are the dominant scattering processes for most trans-port problems, electron–electron scattering, electron–hole scattering, and alloy potential scatter-ing, etc., can also play an important role.

Example 3.1 Calculate the ratio of the polar optical phonon emission rate to theabsorption rate for GaAs and GaN at 300K.

The optical phonon energies in GaAs and GaN are 36 meV and 90 meV respectively. If theelectron energies are below these values, there is no phonon emission. The phononoccupation number in GaAs at 300 K is 0.33 and in GaN is 0.032. Thus above threshold,the emission to absorption ratios are approximately 4:1 and 32:1 respectively.

3.4 TRANSPORT UNDER AN ELECTRIC FIELD

The problem of finding the distribution function of electrons under an electric field is quitecomplicated. Two important approaches to understanding transport in semiconductors are thesolution of the transport equation using numerical methods and the Monte Carlo method usingcomputer simulations. We will summarize the results of such theories by examining the driftvelocity versus electric field relations in semiconductors.

3.4.1 Velocity–electric field relations in semiconductors

When an electron distribution is subjected to an electric field, the electrons tend to move inthe field direction (opposite to the field E and gain velocity from the field. However, becauseof imperfections in the crystal potential, they suffer scattering. A steady state is establishedin which the electrons have some net drift velocity in the field direction. The response of theelectrons to the field can be represented by a velocity–field relation. We will briefly discuss thevelocity-field relationships at low electric fields and moderately high electric fields.

3.4. TRANSPORT UNDER AN ELECTRIC FIELD 105

Low field response: mobilityAt low electric fields, the macroscopic transport properties of the material (mobility, conductiv-ity) can be related to the microscopic properties (scattering rate or relaxation time) by simple ar-guments. We will not solve the Boltzmann transport equation, but we will use simple conceptualarguments to understand this relationship. In this approach we make the following assumptions:

(i) The electrons in the semiconductor do not interact with each other. This approximation iscalled the independent electron approximation.(ii) Electrons suffer collisions from various scattering sources and the time τsc describes themean time between successive collisions.(iii) The electrons move according to the free electron equation

�dk

dt= eE (3.4.1)

in between collisions. After a collision, the electrons lose all their excess energy (on the average)so that the electron gas is essentially at thermal equilibrium. This assumption is really valid onlyat very low electric fields.

According to these assumptions, immediately after a collision the electron velocity is thesame as that given by the thermal equilibrium conditions. This average velocity is thus zero aftercollisions. The electron gains a velocity in between collisions; i.e., only for the time τsc.

This average velocity gain is then that of an electron with mass m∗, traveling in a field E , fora time τsc

vavg = −eEτsc

m∗ = vd (3.4.2)

where vd is the drift velocity . The current density is now

J = −neevd =ne2τsc

m∗ E (3.4.3)

Comparing this with the Ohm’s law result for conductivity σ

J = σE (3.4.4)

we have

σ =ne2τsc

m∗ (3.4.5)

The resistivity of the semiconductor is simply the inverse of the conductivity. From the definitionof mobility μ, for electrons

vd = μE (3.4.6)

we haveμ =

eτsc

m∗ (3.4.7)

If both electrons and holes are present, the conductivity of the material becomes

σ = neμn + peμp (3.4.8)

106 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Bandgap Mobility at 300 K(eV) (cm2/V-s)

Semiconductor 300 K 0 K Elec. HolesC 5.47 5.48 1800 1200GaN 3.4 3.5 1400 350Ge 0.66 0.74 3900 1900Si 1.12 1.17 1500 450α-SiC 3.00 3.30 400 50GaSb 0.72 0.81 5000 850GaAs 1.42 1.52 8500 400GaP 2.26 2.34 110 75InSb 0.17 0.23 80000 1250InAs 0.36 0.42 33000 460InP 1.35 1.42 4600 150CdTe 1.48 1.61 1050 100PbTe 0.31 0.19 6000 4000In0.53Ga0.47As 0.8 0.88 11000 400

Table 3.1: Bandgaps along with electron and hole mobilities in several semiconductors. Proper-ties of large bandgap materials (C, GaN, SiC) are continuously changing (mobility is improving),due to progress in crystal growth. Zero temperature bandgap is extrapolated.

where μn and μp are the electron and hole mobilities and n and p are their densities.Notice that the mobility has an explicit 1

m∗ dependence in it. Additionally τsc also decreaseswith m∗. Thus the mobility has a strong dependence on the carrier mass. In table 3.1 we showthe mobilities of several important semiconductors at room temperature. The results are shownfor pure materials. If the semiconductors are doped, the mobility decreases. Note that Ge hasthe best hole mobility among all semiconductors.

The scattering rate (or inverse of scattering time) due to ionized impurity scattering is

1

〈〈τ〉〉 = Ni1

128√

2π

(Ze2

ε

)21

m∗1/2 (kBT )3/2

×

⎡⎢⎣ln

(1 +

(24m∗kBT

�2λ2

)2)

− 1

1 +(

�2λ2

8m∗kBT

)2

⎤⎥⎦ (3.4.9)

The mobility limited from ionized impurity scattering is

μ =e〈〈τ〉〉m∗

The mobility limited by ionized dopant has the special feature that it decreases with temper-ature (μ ∼ T 3/2). This temperature dependence is quite unique to ionized impurity scattering.

3.4. TRANSPORT UNDER AN ELECTRIC FIELD 107

One can understand this behavior physically by saying that at higher temperatures, the electronsare traveling faster and are less affected by the ionized impurities.

After doing the proper ensemble averaging the relaxation time for the alloy scattering is

1

〈〈τ〉〉 =3π3

8�V0U

2allx(1 − x)

m∗3/2(kBT )1/2

√2π2�3

1

0.75(3.4.10)

according to which the mobility due to alloy scattering is

μ0 ∝ T−1/2

The temperature dependence of mobility is in contrast to the situation for the ionized impurityscattering. The value of Uall is usually in the range of 1.0 eV.

Example 3.2 Consider a semiconductor with effective mass m∗ = 0.26 m0. The opticalphonon energy is 50 meV. The carrier scattering relaxation time is 10−13 sec at 300 K.Calculate the electric field at which the electron can emit optical phonons on the average.

In this problem we have to remember that an electron can emit an optical phonon only ifits energy is equal to (or greater than) the phonon energy. According to the transporttheory, the average energy of the electrons is (vd is the drift velocity)

E =3

2kBT +

1

2m∗v2

d

In our case, this has to be 50 meV at 300 K. Since kBT ∼ 26 meV at 300 K, we have

1

2m∗v2

d = 50 − 39 = 11 meV

or

v2d =

2 × (11 × 10−3 × 1.6 × 10−19 J)

(0.91 × 10−30 × 0.26 kg)

vd = 1.22 × 105 m/s

vd =eτEm∗

Substituting for vd, we get (for the average electrons) for the electric field

E =(0.26 × 0.91 × 10−30 kg)(1.22 × 105 m/s)

(4.8 × 10−10 esu)(1013 s)

= 18.04 kV/cm

The results discussed correspond approximately to silicon. Of course, since thedistribution function has a spread, electrons start emitting optical phonons at a field lowerthan the one calculated above for the average electron.

108 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Example 3.3 The mobility of electrons in pure GaAs at 300 K is 8500 cm2/V·s. Calculatethe relaxation time. If the GaAs sample is doped at Nd = 1017 cm−3, the mobilitydecreases to 5000 cm2/V·s. Calculate the relaxation time due to ionized impurityscattering.

The relaxation time is related to the mobility by

τ (1)sc =

m∗μe

=(0.067 × 0.91 × 10−30 kg)(8500 × 10−4 m2/V · s)

1.6 × 10−19 C

= 3.24 × 10−13 s

If the ionized impurities are present, the time is

τ (2)sc =

m∗μe

= 1.9 × 10−13 s

The total scattering rate is the sum of individual scattering rates. Since the scattering rateis inverse of scattering time we find that (this is called Mathieson’s rule) theimpurity-related time τ

(imp)sc is given by

1

τ(2)sc

=1

τ(1)sc

+1

τ(imp)sc

which givesτ (imp)sc = 4.6 × 10−13s

Example 3.4 The mobility of electrons in pure silicon at 300 K is 1500 cm2/Vs. Calculatethe time between scattering events using the conductivity effective mass.

The conductivity mass for indirect semiconductors, such as Si, is given by (see AppendixC)

m∗σ = 3

(2

m∗t

+1

m∗�

)−1

= 3

(2

0.19mo+

1

0.98mo

)−1

= 0.26mo

The scattering time is then

τsc =μm∗

σ

e=

(0.26 × 0.91 × 10−30)(1500 × 10−4)

1.6 × 10−19

= 2.2 × 10−13 s

Example 3.5 Consider two semiconductor samples, one Si and one GaAs. Both materialsare doped n-type at Nd = 1017 cm−3. Assume 50 % of the donors are ionized at 300 K.Calculate the conductivity of the samples. Compare this conductivity to the conductivityof undoped samples.

3.4. TRANSPORT UNDER AN ELECTRIC FIELD 109

You may assume the following values:

μn(Si) = 1000 cm2/V · sμp(Si) = 350 cm2/V · s

μn(GaAs) = 8000 cm2/V · sμp(GaAs) = 400 cm2/V · s

In the doped semiconductors, the electron density is (50 % of 1017 cm−3)

nn0 = 5 × 1016 cm−3

and hole density can be found from

pn0 =n2

i

nn0

For silicon we have

pn0 =2.25 × 1020

5 × 1016= 4.5 × 103 cm−3

which is negligible for the conductivity calculation.

The conductivity isσn = nn0eμn + pn0eμp = 8 (Ω cm)−1

In the case of undoped silicon we get (n = ni = p = 1.5 × 1010 cm−3)

σundoped = nieμn + pieμp = 3.24 × 10−6 (Ω cm)−1

For GaAs we get

σn = 5 × 1016 × 1.6 × 10−19 × 8000 = 64 (Ω cm)−1

For undoped GaAs we get (ni = 1.84 × 106 cm−3)

σundoped = nieμn + pieμp = 2.47 × 10−9 (Ω cm)−1

You can see the very large difference in the conductivities of the doped and undopedsamples. Also there is a large difference between GaAs and Si.

Example 3.6 Consider a semiconductor in equilibrium in which the position of the Fermilevel can be placed anywhere within the bandgap.

What is the maximum and minimum conductivity for Si and GaAs at 300 K? You can usethe data given in the problem above.

The maximum carrier density occurs when the Fermi level coincides with the conductionbandedge if Nc > Nv or with the valence bandedge if Nv > Nc. If Nc > Nv; theBoltzmann approximation gives

nmax = Nc

110 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

while if Nv > Nc we getpmax = Nv

This gives us for the maximum density: i) for Si, 2.78 × 1019 cm−3 ii) for GaAs,7.72 × 1018 cm−3. Based on these numbers we can calculate the maximum conductivity:

For Si

σmax = 2.78 × 1019 × 1.6 × 10−19 × 1000 = 4.45 × 103 (Ω cm)−1

For GaAs

σmax = 7.72 × 1018 × 1.6 × 10−19 × 400 = 4.9 × 102 (Ω cm)−1

To find the minimum conductivity we need to find the minima of the expression

σ = neμn + peμp

=n2

i

peμn + peμp

To find the minimum we take the derivative with respect to p and equate the result to zero.This gives

p = ni

√μn

μp

This then gives for the minimum conductivity

σmin = nie[μn

√μp

μn+ μp

√μn

μp]

For Si this gives upon plugging in numbers

σmin = 2.8 × 10−6 (Ω cm)−1

and for GaAsσmin = 1.05 × 10−9 (Ω cm)−1

Note that these values are lower than the values we get in the the previous problem for theundoped cases. This example shows the tremendous variation in conductivity that can beobtained in a semiconductor.

High field transport: velocity–field relations

In most electronic devices a significant portion of the electronic transport occurs under strongelectric fields. This is especially true of field effect transistors. At such high fields (∼ 1−500 kV/cm) the electrons get “hot” and acquire a high average energy. The extra energy comesdue to the strong electric fields. The drift velocities are also quite high. The description of

3.4. TRANSPORT UNDER AN ELECTRIC FIELD 111

electrons at such high electric fields is quite complex and requires either numerical techniquesor computer simulations. We will only summarize the results.

At high electric field as the carriers gain energy from the field they suffer greater rates ofscattering, i.e., τsc decreases. The mobility thus starts to decrease. It is usual to representthe response of the carriers to the electric field by velocity–field relations. There are severalimportant regimes in the velocity-field relation. At lower fields the relation is linear as discussedabove. As electrons (holes) gain enough energy to emit optical phonons the scattering ratesincrease and the differential mobility starts to decrease as shown in figure 3.10. The relation isno longer linear.

In the case of direct gap materials an interesting phenomena occurs that leads to negativedifferential relation as shown in figure 3.10. As carriers gain energy comparable to the inter-valley separation in the conduction band they get scattered out of the low mass lower energyvalley to higher mass upper valley. As a result the velocity drops as can be seen for GaAs andInP in Figure 3. 10. The negative differential mobility (resistance) is exploited by microwavedevices such as Gunn diodes to generate microwave power.

At very high fields the drift velocity becomes saturated; i.e., becomes independent of theelectric field. This occurs because the scattering rates increase as the field increases so that theelectrons gain energy from the field but their net velocity does not change. The drift velocity forcarriers in most materials saturates to a value of ∼ 107 cm/s. The fact that the velocity saturatesis very important in understanding current flow in semiconductor devices.

It is important to note that the concept of velocity-field relation is valid if the fields are chang-ing slowly over distances comparable the electron mean free path. This is the case in devices thatare longer than a micron or so. For sub-micron devices electrons can move without scatteringfor a some distance. In this case the transport is called ballistic transport and is described by theNewton’s equation without scattering,

m∗ dx

dt= eF (3.4.11)

For short distances electrons can display overshoot effects i.e they can have velocities larger thanwhat may be expected from a steady state velocity-field relation. For light mass semiconductorssuch as GaAs and InGaAs velocity overshoot effects dominate modern devices.

Example 3.7 The mobility of electrons in a semiconductor decreases as the electric fieldis increased. This is because the scattering rate increases as electrons become hotter due tothe applied field. Calculate the relaxation time of electrons in silicon at 1 kV/cm and100 kV/cm at 300 K.

The velocity of the silicon electrons at 1 kV/cm and 100 kV/cm is approximately 1.4 ×106 cm s and 1.0 × 107 cm/s, respectively, from the v-F curves given in figure 3.10. Themobilities are then

μ(1 kV/cm) =v

E = 1400 cm2/V · sμ(100 kV/cm) = 100 cm2/V · s

112 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

102

ELECTRIC FIELD (V/cm)

CA

RR

IER

DR

IFT

VE

LO

CIT

Y (

cm/s

)

103 104 105 106105

106

107

108

GaAs

Si

InP

Electrons

Holes

Figure 3.10: Velocity–field relations for several semiconductors at 300 K.

The corresponding relaxation times are

τsc(1 kV/cm) =(0.26 × 0.91 × 10−30 kg)(1400 × 10−4 m2/V)

1.6 × 10−19 C= 2.1 × 10−13 s

τsc(100 kV/cm) =(0.26 × 0.91 × 10−30)(100 × 10−4)

1.6 × 10−19= 1.48 × 10−14 s

Thus the scattering rate has dramatically increased at the higher field.

Example 3.8 The average electric field in a particular 0.1 μm GaAs device is 50 kV/cm.Calculate the transit time of an electron through the device (a) if the transport is ballistic;(b) if the saturation velocity value of 107 cm/s is used.

For ballistic transport the transit time is

τtr =

√2L

a

with the acceleration, a given by

a =eEm∗

3.4. TRANSPORT UNDER AN ELECTRIC FIELD 113

This gives a transit time of 0.123 ps.

The transit time, if the saturation velocity (which is the correct velocity value) is used, is

τtr =L

v=

1 × 10−5

107= 1 ps

This example shows that in short channel devices, ballistic effects can be very strong.

Very high field transport: breakdown phenomena

When the electric field becomes extremely high (∼ 100 kV cm−1), the semiconductor suffersa “breakdown” in which the current has a “runaway” behavior. The breakdown occurs due to car-rier multiplication, which arises from the two sources discussed below. By carrier multiplicationwe mean that the number of electrons and holes that can participate in current flow increases. Ofcourse, the total number of electrons is always conserved.

Avalanche breakdown

In the transport considered in the previous subsections, the electron (hole) remains in thesame band during the transport. At very high electric fields, this does not hold true. In theimpact ionization process shown schematically in figure 3.11, an electron, which is “very hot”(i.e., has a very high energy due to the applied field) scatters with an electron in the valenceband via Coulombic interaction, and knocks it into the conduction band. The initial electronmust provide enough energy to bring the valence-band electron up into the conduction band.Thus the initial electron should have energy slightly larger than the bandgap (measured from theconduction-band minimum). In the final state we now have two electrons in the conduction bandand one hole in the valence band. Thus the number of current carrying charges have multiplied,and the process is often called avalanching. Note that the same could happen to “hot holes” andthus could then trigger the avalanche.

Once avalanching starts, the carrier density in a device changes as

dn(z)

dz= αimpn (3.4.12)

where n is the carrier density and αimp represents the average rate of ionization per unit distance.The coefficients αimp for electrons and βimp for holes depend upon the bandgap of the material

in a very strong manner. This is because, as discussed above, the process can start only if theinitial electron has a kinetic energy equal to a certain threshold (roughly equal to the bandgap).This is achieved for lower electric fields in narrow gap materials.

If the electric field is constant so that αimp is constant, the number of times an initial electronwill suffer impact ionization after traveling a distance x is

n(x) = exp (αimpz) (3.4.13)

A critical breakdown field Ecrit is defined where αimp or βimp approaches 104 cm−1. Whenαimp (βimp) approaches 104 cm−1, there is about one impact ionization when a carrier travels

114 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Initial state has one electron

Final state has two electrons + one hole

Conduction band

Valence band+

––

–

Figure 3.11: How carriers multiply. The impact ionization process where a high energyconduction-band electron scatters from a valence-band electron, producing two conduction-bandelectrons and a hole.

a distance of one micron. Values of the critical field are given for several semiconductors intable 3.2. The avalanche process places an important limitation on the power output of devices.Once the process starts, the current rapidly increases due to carrier multiplication and the controlover the device is lost.1 The push for high-power devices is one of the reasons for research inlarge gap semiconductor devices. It must be noted that in certain devices, such as avalanchephotodetectors, the process is exploited for high gain detection. The process is also exploited inspecial microwave devices.

Band-to-band tunneling breakdown

In quantum mechanics electrons behave as waves and one of the outcomes of this is that elec-trons can tunnel through regions where classically they are forbidden. Thus they can penetrateregions where the potential energy is larger than their total energy. This process is described bythe tunneling theory. This theory is invoked to understand another phenomenon responsible forhigh field breakdown. Consider a semiconductor under a strong field, as shown in figure 3.12a.At strong electric fields, the electrons in the valence band can tunnel into an unoccupied state inthe conduction band. As the electron tunnels, it sees the potential profile shown in figure 3.12b.

1An analytical treatment of the avalanche breakdown process of a p − n junction is presented in section 4.7

3.4. TRANSPORT UNDER AN ELECTRIC FIELD 115

Material B andga reakdown electric(eV ) field (V/cm)

GaAs 1.43 4 x 105

Ge 0.664 105

InP 1.34

Si 1.1 3 x 105

In0.53Ga0.47As 0.8 2 x 105

C 5.5 107

SiC 2.9 2-3 x 106

SiO2 9 –107

Si3N4 5 –107

GaN 3.4 2 x 106

p B

Table 3.2: Breakdown electric fields in some materials.

The tunneling probability through the triangular barrier is given by

T = exp

(−4

√2m∗E3/2

g

3e�E

)(3.4.14)

where E is the electric field in the semiconductor.In narrow bandgap materials this band-to-band tunneling or Zener tunneling can be very im-

portant. It is the basis of the Zener diode, where the current is essentially zero until the band-to-band tunneling starts and the current increases very sharply. A tunneling probability of ∼ 10−6

is necessary to start the breakdown process.

Example 3.9 Calculate the band-to-band tunneling probability in GaAs and InAs at anapplied electric field of 2 × 105 V/cm.

116 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Ec

Ev –x1

x2 Ec

Ev

–x10 x 2

x

(a)

(b)

Available empty states (holes) in valence band

Electrons in conduction band

Eg

– – – – – – – – –+ + + + + +

Tunnel barrier

Figure 3.12: (a) A schematic showing the band profile for a p–n junction. An electron in theconduction band can tunnel into an unoccupied state in the valence band or vice versa. (b) Thepotential profile seen by the electron during the tunneling process.

The exponent for the tunneling probability is (m∗(GaAs) = 0.065 m0; m∗(InAs)∼ 0.02 m0; Eg(GaAs) = 1.5 eV; Eg(InAs) = 0.4 eV) for GaAs

− 4 × (2 × 0.065 × 0.91 × 10−30 kg)1/2(1.5 × 1.6 × 10−19 J)3/2

3 × (1.6 × 10−19 C)(1.05 × 10−34 Js)(2 × 107 V/m)

= −160

The tunneling probability is exp(−160) ∼= 0. For InAs the exponent turns out to be −12.5and the tunneling probability is

T = exp (−12.5) = 3.7 × 10−6

In InAs the band-to-band tunneling will start becoming very important if the field is∼ 2 × 105 V/cm.

3.5. SOME IMPORTANT ISSUES IN TRANSPORT 117

3.5 SOME IMPORTANT ISSUES IN TRANSPORT

We will discuss some important issues in transport and how bandgap, carrier masses, devicelength, etc. influence transport. We note that in absence of collisions, electron transport is givenby the modified Newton’s expression

�dk

dt= eE (3.5.1)

which (for the simple parabolic band)

E(k) =�

2k2

2m∗ (3.5.2)

Of course, in reality, as we have discussed earlier, scattering modifies this simple picture. Infigure 3.13(a) we show a schematic of carrier velocity as a function of electric field in steadystate for electrons in a direct bandgap material (solid line) and electrons in indirect bandgap ma-terials (dashed line) or holes (dashed line), the negative resistance region arises due to electronstransferring from a low mass direct gap valley to high mass indirect valley.As indicated on the figure, at low fields the important scattering mechanisms are acoustic phononscattering, ionized impurity scattering, and optical phonon absorption. There is not much opticalphonon emission since electron energies are small compared to optical phonon energy. At highfields, the optical phonon emission dominates. As a result of the different mechanisms dominat-ing scattering at low and high fields, when temperature is lowered, low field mobility is greatlyenhanced (since phonon occupation is lower) but there is not much change in high field velocity.

velo

city

Electric Field

Optical phononemission

Acous

tic ph

onons

Optical p

hono

n abs

orpt

ion

Impu

rity S

catte

ring

Direct gap electronsHoles, electrons indirect gap

0

(a)

Low mass valley High mass valley

velo

city

Distance

High Field

0

Ballistic transport(overshoot effect)

Low Field

(b)

Figure 3.13: a) A schematic of how different scattering mechanisms dominate in various regionsof electric field; under steady state field conditions. b) non-steady state transport velocity versusdistance profile. The electron sees a step in field profile at the origin. At high fields, velocityovershoot effects occur.

118 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Elec t ron Energy (eV)

GaN

GaAs

InGaAs

Figure 3.14: Scattering rates in InGaAs, GaAs, and GaN in 2-dimensional HFET channels

In figure 3.13b we show how an electron evolves with distance (or time) when electrons comeinto a high field region. The important point to note is that electrons take time to scatter and dur-ing that initial time (∼ picoseconds or smaller) travel ballistically according to equation equation3.5.1 As a result of ballistic transport, electrons can exhibit overshoot effect of high fields whereelectron velocity can be larger than what is expected from steady state velocity. This effect isquite dominant in materials such as InGaAs and GaAs where scattering times are long. Toillustrate some of the points mentioned above, we examine electron transport in In0.53Ga0.47As,GaAs, and GaN. Transport in Si falls in between GaAs and GaN in terms of scattering rates. Infigure 3.14 we show scattering rates in these three materials in 2-dimensional HFET channels(not in bulk). We note that for low electron energies there is a great difference in the scatteringrates between the materials. At higher energies the relative difference is smaller. In table 3.3 weshow some of the important scattering mechanisms. The rates are given for low electron ener-gies and higher energies. In figure 3.15 we show the temperature dependence of scattering rateversus energy for InGaAs and GaN. materials. The rates drop quite dramatically at small elec-tron energies due to phonon occupation number becoming small. Later when we examine deviceproperties in chapter 8 we will see how the issues disscus in long and short channel devices.

3.6 CARRIER TRANSPORT BY DIFFUSION

Semiconductor devices fall into two broad categories: majority carrier devices and minoritycarrier devices. In the majority carrier devices, current flow is dominated by electric field drivencurrent. In minority carrier devices current flow is dominated by diffusion effects. Whenever

3.6. CARRIER TRANSPORT BY DIFFUSION 119

a) b)

Figure 3.15: Temperature dependence of scattering rates in 2DEGs for (a) InGaAs and (b) GaN

Table 1: Scattering Comparison

Point A B

GaN GaAs InGaAs GaN GaAs InGaAs

Energy (eV) 0.2 0.2 0.2 0.8 0.8 0.8

Optical phonon emission 8.85x 1013 6.60x 1012 6.33x 1012 8.95x 1013 6.35x 1012 7.00x 1012

Optical phonon absorption 3.48x 1012 1.79x 1012 2.08x 1012 2.88x 1012 1.61x 1012 2.11x 1012

acoustic Phonon 1.50x 1012 3.44x 1011 1.64x 1011 3.23x 1012 9.06x 1011 5.69x 1011

Alloy scattering 0.0 0.0 9.56x 1010 0.0 0.0 4.23x 1011

ionized impurity 1.47x 1013 7.41x 1012 6.41x 1012 8.47x 1012 5.11x 1012 5.08x 1012

dislocation 2.33x 1012 7.35x 108 4.90x 108 2.33x 1012 7.35x 108 4.90x 108

Nonequivalent intervalley

emission(Γ–L)0.0 0.0 0.0 0.0 3.42x 1013 1.23x 1013

Nonequivalent intervalley

absorption(Γ–L)0.0 0.0 0.0 0.0 1.15x 1013 5.46x 1012

Total (s- 1 ) 1.11x 1014 1.61x 1013 1.51x 1013 1.06x 1014 5.97x 1013 3.30x 1013

Table 3.3: Scattering rate mechanisms in InGaAs, GaAs, and GaN 2-DEG channels

there is a gradient in the concentration of a species of mobile particles, the particles diffuse fromthe regions of high concentration to the regions of low concentration. As the mobile chargesmove they suffer random collisions, as discussed in the previous section. The collision processcan be described by the mean free path � and the mean collision time τsc. The mean free pathis the average distance the electron (hole) travels between successive collisions. In between thecollisions the electrons move randomly, with equal probability of moving in any direction (thereis no electric field). We are interested in finding out how the electrons move (diffuse) when thereis a concentration gradient in space.

120 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

nR

xo– xo

x

xo+

nL

L R

mean free path

CA

RR

IER

CO

NC

EN

TR

AT

ION

Figure 3.16: The concentration profile of electrons as a function of space. The terms nL, nR, L,and R are defined in the text. The distance � is the mean free path for electrons; i.e., the distancethey travel between collisions.

In figure 3.16 is shown a concentration profile n(x, t) of electrons at time t,. We are goingto calculate the electron flux φ(x, t) across a plane x = xo at any instant of time. Consider aregion of space a mean free path � to each side of xo, from which electrons can come across thex = xo boundary in time τsc. Electrons from regions further away will suffer collisions that willrandomly change their direction. Since in the two regions labeled L and R in figure 3.16, theelectrons move randomly, half of the electrons in region L will go across x = xo to the right andhalf in the region R will go across x = xo to the left in time τsc. The flux to the right is

φn(x, t) =(nL − nR)�

2τsc(3.6.1)

where nL and nR are the average carrier densities in the two regions. Since the two regions Land R are separated by the distance �, we can write

nL − nR∼= −dn

dx· � (3.6.2)

The total flux is

φn(x, t) = − �2

2τsc

dn(x, t)

dx= −Dn

dn(x, t)

dx(3.6.3)

3.6. CARRIER TRANSPORT BY DIFFUSION 121

where Dn is called the diffusion coefficient of the electron system and depends upon the scatter-ing processes that control � and the τsc. Since the mean free path is essentially vthτsc, where vth

is the mean thermal speed, the diffusion coefficient depends upon the temperature as well. In asimilar manner, the hole diffusion coefficient gives the hole flux due to a hole density gradient

φp(x, t) = −Dpdp(x, t)

dx(3.6.4)

The electron and hole flux causes current to flow in the structure This current is given by

Jtot(diff) = Jn(diff) + Jp(diff)

= eDndn(x, t)

dx− eDp

dp(x, t)

dx(3.6.5)

Note that the electron charge is −e while the hole charge is e. While both electrons and holesmove in the direction of lower concentration of electrons and holes respectively, the currents theycarry are opposite, since electrons are negatively charged, while holes are positively charged.

3.6.1 Drift and diffusion transport: Einstein’s relation

In case both electric field and carrier concentration gradients are present, the current is givenby

Jn(x) = eμnn(x)E(x) + eDndn(x)

dx

Jp(x) = eμpp(x)E(x) − eDpdp(x)

dx(3.6.6)

The diffusion and drift processes are linked by scattering processes. We will now establishan important relationship between mobility and diffusion coefficients. Consider a case where auniform electric field is applied, as shown in figure 3.17a. The potential energy associated withthe field is shown in figure 3.17b. There is a positive potential on the left-hand side in relation tothe right-hand side. For a uniform electric field the potential energy is

U(x) = U(0) − eEx (3.6.7)

The applied force is related to the potential energy by

Force = −∇U(x) (3.6.8)

Thus, since the electron charge −e is negative, the bands bend as shown in figure 3.17c accordingto the relation

Ec(x) = Ec(0) + eEx (3.6.9)

Thus, if a positive potential is applied to the left of the material and a negative to the right, theenergy bands will be lower on the left-hand side, as shown in figure 3.17c. The electrons driftdownhill in the energy band picture and thus opposite to the field.

122 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

E lectric field E (x)

Position in space, x

UNIFOR M E L E CT R IC FIE L D

(a)

+ve

–ve

0

U(x)

E nergy band, Ec, Ev

Ec

EFi

Ev

x

(b)

x

(c)

POT E NT IA L E NE R GY PR OFIL E

E NE R GY B A ND PR OFIL E

Figure 3.17: (a) Electric field profile in a semiconductor. (b) Plot of the potential energy associ-ated with the electric field. (c) Electron energy band profile. The negative charge of the electroncauses the energy band profile to have the opposite sign to the potential energy profile.

To find the relation between diffusion parameters and drift parameters (i.e. between D andμ) we assume that the system is in equilibrium and the total electron and hole currents are

3.6. CARRIER TRANSPORT BY DIFFUSION 123

individually zero and we have from equation 3.6.6 for the electrons

E(x) = −Dn

μn

1

n(x)

dn(x)

dx(3.6.10)

To obtain the derivative of carrier concentration, we write n(x) in terms of the intrinsic Fermilevel, EFi, which serves as a reference level, and the Fermi level in the semiconductor, EF (x).If we assume that the electron distribution is given by the Boltzmann distribution we have

n(x) = ni exp

{−

(EFi − EF (x)

kBT

)}(3.6.11)

This givesdn(x)

dx=

n(x)

kBT

(−dEFi

dx+

dEF

dx

)(3.6.12)

At equilibrium, the Fermi level cannot vary spatially, otherwise the probability of findingelectrons along a constant energy position will vary along the semiconductor. This would causeelectrons at a given energy in a region where the probability is low to move to the same energyin a region where the probability is high. Since this is not allowed by definition of equilibriumconditions, i.e. no current is flowing, the Fermi level has to be uniform in space at equilibrium,or

dEF

dx= 0 (3.6.13)

We then have from equation 3.6.10 and equation 3.6.12

Dn

μn=

kBT

e

using

E(x) =1

e

dEFi

dx

This relation is known as the Einstein relation with an analogous relation for the holes. As we cansee from table 3.4 which lists the mobilities and diffusion coefficients for a few semiconductorsat room temperature, the Einstein relation is quite accurate.

Example 3.10 Use the velocity–field relations for electrons in silicon to obtain thediffusion coefficient at an electric field of 1 kV/cm and 10 kV/cm at 300 K.

According to the v-E relations given in figure 3.10, the velocity of electrons in silicon is ∼1.4 × 106 cm/s and ∼ 7 × 106 cm/s at 1 kV/cm and 10 kV/cm. Using the Einsteinrelation, we have for the diffusion coefficient

D =μkBT

e=

vkBT

eE

124 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Dn Dp μn μp

(cm2/s) (cm2/s) (cm2/V • s) (cm2/V • s)

Ge 100 50 3900 1900 Si 35 12.5 1350 480 GaAs 220 10 8500 400

Table 3.4: Low field mobility and diffusion coefficients for several semiconductors at roomtemperature. The Einstein relation is satisfied quite well.

This gives

D(1kV/ cm−1) =(1.4 × 104m/s)(0.026 × 1.6 × 10−19 J)

(1.6 × 10−19 C)(105 V/m−1

)

= 3.64 × 10−3 m2/s = 36.4 cm2/s

D(10kV/ cm−1) =(7 × 104 m/s)(0.026 × 1.6 × 10−19 J)

(1.6 × 10−19 C)(106 Vm−1)

= 1.82 × 10−3 m2/s = 18.2 cm2/s

The diffusion coefficient decreases with the field because of the higher scattering rate athigher fields.

3.7 CHARGE INJECTION AND QUASI-FERMI LEVELS

In semiconductor devices the electron and hole distributions are usually not under equilibrium.electric fields and optical energy causes electron densities and velocities to be different from theequilibrium values. If electrons and holes are injected into a semiconductor, either by externalcontacts or by optical excitation, the question arises: What kind of distribution function describesthe electron and hole occupation? We know that in equilibrium the electron and hole occupationis represented by the Fermi function. It is possible to describe the non-equilibrium distributionby using the concept of quasi-equilibrium

3.7.1 Non-equilibrium Distributions

Under equilibrium conditions, electrons in the conduction band and holes in the valence bandare in equilibrium with each other. Under non-equilibrium conditions it is often reasonable toassume that electrons are in equilibrium in the conduction band, while holes are in equilibriumin the valence band. In this case, the quasi-equilibrium electron and holes can be represented byan electron Fermi function fe (with electron Fermi level) and a hole Fermi function fh (with a

3.8. CARRIER GENERATION AND RECOMBINATION 125

different hole Fermi level). We then have

n =

∫ ∞

Ec

Ne(E)fe(E)dE (3.7.1)

p =

∫ Ev

−∞Nh(E)fh(E)dE (3.7.2)

where

fe(E) =1

exp (E−EF n

kBT ) + 1(3.7.3)

and

fh(E) = 1 − fv(E) = 1 − 1

exp (E−EF p

kBT ) + 1

=1

exp (EF p−E

kBT ) + 1(3.7.4)

Each band is described by its own Fermi level, EFn and EFp. At equilibrium EFn = EFp.If excess electrons and holes are injected into the semiconductor, the electron Fermi level EFn

moves toward the conduction band, while the hole Fermi level EFp moves toward the valenceband. This is shown schematically in figure 3.18. By defining separate Fermi levels for theelectrons and holes, one can study the properties of excess carriers using the same relationshipbetween Fermi level and carrier density as we developed for the equilibrium problem. Thus, inthe Boltzmann approximation we have

n = Nc exp

[(EFn − Ec)

kBT

]p = Nv exp

[(Ev − EFp)

kBT

](3.7.5)

For high carrier densities, we have the more accurate Joyce-Dixon approximation:

EFn − Ec = kBT

[�n

n

Nc+

n√8Nc

]Ev − EFp = kBT

[�n

p

Nv+

p√8Nv

](3.7.6)

3.8 CARRIER GENERATION AND RECOMBINATION

In this section we will examine how mobile carrier densities change when temperature ischanged or light shines on a semiconductor: The electron may start out in the valence band, then

126 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

– – – –

+ +

Ec

Equilibrium Fermi level for an n-type material

Ev

Excess electron injection

Excess electron and hole injection

EF

(a)

– – – –

+ +

Ec

Ev

EFp

(b)

EFn

– – –

– – – –

+ +

Ec

Ev

EFp

(c)

EFn

– – –

+ + + + +

EFn moves towards Ec

EFn moves towards Ec

EFp moves towards Ev

Figure 3.18: (a) Schematic of an equilibrium Fermi level position in an n−type semiconductor.(b) The positions of the quasi-Fermi levels for the case where excess electrons are injected in theconduction band. (c) The position of the quasi-Fermi levels when excess electrons and holes areinjected.

jump to the conduction band, then fall into a trap, etc. On a microscopic level there are generationrecombination processes occurring in a material which cause electrons to jump between valenceband, conduction band and trap states, as shown in figure 3.19.

3.8. CARRIER GENERATION AND RECOMBINATION 127

– – – – – – –

Ec Band to bandelectron-hole generation

Ev + – –

–

– – ––

– – – – – –

– donor ionization: free electron + ionized donor

– – –

–

– ––

++

–– – – – – –

Band to bandelectron-hole recombination

– – – – – –+

–

– – – – – –

electron recombination with a donor

–

– – –

–

– ––

++

Figure 3.19: A schematic of carrier generation and recombination. Processes involving band toband transitions are shown along with processes involving dopant or other impurity levels.

At equilibrium, thermal energy is responsible for exciting electrons from the valence band tothe conduction band. Such a generation process is called thermal generation. We can also seethat if electrons are continuously excited up from the valence band into the conduction band,there will be a build-up of free carriers. In order to reach an equilibrium concentration there hasto be carrier recombination as well. Under steady state conditions we have

G = R (3.8.1)

where G is the generation rate and R is the carrier recombination rate.In figure 3.19 we show a schematic description of carrier generation and recombination. Free

carriers can be generated if an electron leaves the valence-band and goes to the conduction-band. They can also be generated if electrons leave a donor and go into the conduction-band.

128 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

+

Absorption

Photon

ABSORPTION

(a) (b)

Photon

EMISSION

“Vertical”in k

–

Emission

–

MOMENTUM CONSERVATION LAW

Figure 3.20: Band-to-band absorption in semiconductors. Momentum conservation ensures thatonly vertical transitions are allowed during absorption and emission.

An electron from the valence-band going to an acceptor causes a hole to be generated. Reverseprocesses can also occur.

One of the most important mechanisms for carrier generation and recombination is absorptionof light and emission of light.

3.8.1 Optical Absorption and Emission in Semiconductors

According to quantum mechanics, electromagnetic radiation is made up of particles calledphotons, each carrying an energy �ω. The particle nature of E-M waves is manifested in semi-conductor devices. When light shines on a semiconductor it can cause an electron in the valenceband to go into the conduction band. This process generates electron-hole pairs. It is also pos-sible for an electron and a hole to recombine and emit light. The most important optoelectronicinteraction in semiconductors as far as devices are concerned is the band-to-band transitionshown in figure 3.20. In the photon absorption process, a photon scatters an electron in thevalence band, causing the electron to go into the conduction band. In the reverse process theelectron in the conduction band recombines with a hole in the valence band to generate a photon.These two processes are of obvious importance for light-detection and light-emission devices.

3.8. CARRIER GENERATION AND RECOMBINATION 129

These processes are controlled by the conservation laws.

• Conservation of energy: In the absorption and emission process we have for the initial andfinal energies of the electrons Ei and Ef

absorption : Ef = Ei + �ω (3.8.2)

emission : Ef = Ei − �ω (3.8.3)

where �ω is the photon energy. Since the minimum energy difference between the conductionand valence band states is the bandgap Eg , the photon energy must be larger than the bandgap.

• Conservation of momentum: In addition to the energy conservation, one also needs toconserve the effective momentum �k for the electrons and the photon system. The photon kph

value is given by

kph =2π

λ(3.8.4)

The k-value of photons with energies equal to the bandgaps of typical semiconductors ∼ 10−4 A,which is essentially zero compared to the k-values for electrons. Thus k-conservation ensuresthat the initial and final electrons have the same k-value. Thus for optical processes onlytransitions which are“vertical” in k are allowed in the bandstructure picture, as shown in fig-ure 3.20.

Because of k-conservation, in semiconductors where the valence band and conduction band-edges are at the same k = 0 value (the direct semiconductors), the optical transitions are quitestrong. In indirect materials like Si, Ge, etc. the optical transitions are very weak near thebandedges because they require the help of lattice vibrations to satisfy k-conservation.

Electromagnetic waves traveling through a medium like a semiconductor are described byMaxwell’s equations which show that the waves have a form given by the electric field vectordependence

E = Eo exp{

iω(nrz

c− t

)}exp

(−αz

2

)(3.8.5)

Here z is the propagation direction, ω the frequency, nr the refractive index, and α the absorptioncoefficient of the medium. As the E-M wave propagates through a material, its intensity decaysas

I(z) = I(0) exp {−αz} (3.8.6)

In figure 3.21 we show the absorption coefficient of some direct and indirect bandgap semi-conductors. Note that for indirect gap semiconductors the absorption coefficient is weak near thebandedge but once the photon energy is large enough to cause direct (vertical in k) transitions,the absorption coefficient increases.

When a photon is absorbed it creates an electron and a hole. If Pop is the optical power densityof light impinging on a semiconductor, the photon flux is

Φ =Pop

�ω

130 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

100.2 0.6 1.4 1.81

106

105

104

103

102

0.711.53 2

PHOTON ENERGY (eV)

WAVELENGTH (μm)

AB

SO

RP

TIO

NC

OE

FF

ICIE

NT (

cm–1

)

GaP

InP

GaAs

In0.53Ga0.47As

Si

Figure 3.21: Absorption coefficient of some direct and indirect gap semiconductors. For thedirect gap material, the absorption coefficient is very strong once the photon energy exceeds thebandgap. For indirect materials the absorption coefficient is small near the bandedge, but oncethe photon energy is more than the direct gap, the absorption coefficient increases rapidly.

and the electron-hole pair generation rate is

RG = αΦ =αPop

�ω(3.8.7)

Under equilibrium conditions, electron occupation in the valence band is close to unity whilethe occupation in the conduction band is close to zero. Assuming this is the case the absorptioncoefficient for direct gap materials is

α(�ω) =πe2

�

2nrcεom0

(2p2

cv

m0

)Ncv(�ω)

�ω· 2

3(3.8.8)

Here nr is the refractive index of the material, pcv is the momentum matrix element for thescattering process, c is the speed of light in vacuumand Ncv is the joint density of states for the

3.8. CARRIER GENERATION AND RECOMBINATION 131

electron-hole system and is

Ncv(E) =

√2(m∗

r)3/2(E − Eg)

1/2

π2�3(3.8.9)

If we express the energy in eV, and the absorption coefficient in cm−1for most direct gap semi-conductors the absorption coefficient is approximately

α(�ω) ∼ 5.6 × 104 (�ω − Eg)1/2

�ωcm−1 (3.8.10)

For indirect gap materials the absorption coefficient is an order of magnitude smaller than theresult given above since in first order transitions momentum is not conserved. Thus for materialslike Si and Ge near bandedge absorption is weak.If there are electrons in the conduction band andholes in the valence band they can recombine to emit photons. If the occupation of an electronstate is unity and the occupation of the corresponding hole state is also unity the recombinationrate is given by

Wem =1

τ0=

e2nr

6πεom0c3�2

(2p2

cv

m0

)�ω (3.8.11)

Using typical values of the momentum matrix element pcv for direct gap materials the result is

Wem =1

τ0= 109Eg s−1 (3.8.12)

When electrons and holes are injected into the conduction and valence bands of a semiconductor,they recombine with each other. In general the occupation of electrons and holes is given bythe quasi-Fermi levels. Theemission rateor the electron-hole recombination rate is (units arecm−3s−1)

Rspon =1

τo

∫d(�ω)Ncv{fe(Ee)}{fh(Eh)} (3.8.13)

The spontaneous recombination rate is quite important for both electronic and optoelectronicdevices. It is important to examine the rate for several important cases. We will give results forthe electron hole recombination for the following cases: i) Minority carrier injection: If n � pand the sample is heavily doped, we can assume that fe(Ee) is close to unity. We then have forthe rate at which holes will recombine with electrons,

Rspon∼= 1

τo

∫d(�ω)Ncvfh(Eh) ∼= 1

τo

∫d(�ω)Nhfh(Eh)

(m∗

r

m∗h

)3/2

∼= 1

τo

(m∗

r

m∗h

)3/2

p (3.8.14)

Thus the recombination rate is proportional to the minority carrier density (holes in this case).ii) Strong injection: This case is important when a high density of both electrons and holes isinjected and we can assume that both fe and fh are step functions with values 1 or zero. We getfor this case

Rspon =n

τo=

p

τo(3.8.15)

132 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

iii) Weak injection: In this case we can use the Boltzmann distribution to describe the Fermifunctions. We have

fe ·fh ∼= exp

{− (Ec − EFn)

kBT

}exp

{− (EFp − Ev)

kBT

}· exp

{− (�ω − Eg)

kBT

}(3.8.16)

The spontaneous emission rate now becomes

Rspon =1

2τo

(2π�

2m∗r

kBTm∗em

∗h

)3/2

np (3.8.17)

If we write the total charge as equilibrium charge plus excess charge,

n = no + Δn; p = po + Δn (3.8.18)

we have for the excess carrier recombination (note that at equilibrium the rates ofrecombinationand generation are equal)

Rspon∼= 1

2τo

(2π�

2m∗r

kBTm∗em

∗h

)3/2

(Δnpo + Δpno) (3.8.19)

If Δn = Δp, we can define the rate of a single excess carrier recombination as

1

τr=

Rspon

Δn=

1

2τo

(2π�

2m∗r

kBTm∗em

∗h

)(no + po) (3.8.20)

At low injection τr is much larger than τo, since at low injection, electrons have a low probabilityto find a hole with which to recombine. iv) Inversion condition: Another useful approximationoccurs when the electron and hole densities are such that fe + fh = 1. This is the condition forinversion when the emission and absorption coefficients become equal. If we assume in this casefe ∼ fh = 1/2, we get the approximate relation

Rspon∼= n

4τo

∼= p

4τo(3.8.21)

The recombination lifetime is approximately 4τo in this case. This is a useful result to estimatethe threshold current of semiconductor lasers.

Example 3.11 Optical radiation with a power density of 1.0 kW/cm2 impinges on GaAs.The photon energy is 1.5 eV and the absorption coefficient is 3 × 103 cm−1. Calculate thecarrier generation rate at the surface of the sample. If the e − h recombination time is 1 ns,calculate the steady state excess carrier density.

At the surface the carrier generation rate is

G(0) =(3 × 103 cm−1)(103 W cm−2)

(1.5 × 1.6 × 10−19 J)

= 1.25 × 1025 cm−3s−1

The excess carrier density is

δn = δp = 1.25 × 1025 × 10−9 = 1.25 × 1016 cm−3

3.8. CARRIER GENERATION AND RECOMBINATION 133

3.8.2 Schockley Read Hall Statistics

Semiconductor behavior is determined primarily by controlled impurities. Shallow impuritiesgive rise to dopants, while deep impurities give rise to traps. In either case, the occupancy of allstates, whether in the bands or the gap, is determined by the occupancy function.

(a)Electron capture

Before After

(a)Electron capture

Before After

(b)Electron emission

Before After

(b)Electron emission

(b)Electron emission

Before After

(c)Hole capture

Before After

(c)Hole capture

(c)Hole capture

Before After

(d)Hole emission

Before After

(d)Hole emission

Before After

Figure 3.22: Exchanges with the conduction band are dealt as electron capture and emission,whereas exchanges with the valence band are considered hole capture and emission. The arrowsindicate electron transitions

In equilibrium, the occupancy function for these states may be written:

f =1

1 + exp ((Et − Ef ) /kBT )(3.8.22)

where Et is the trap energy and Ef is the Fermi energy. For non-equilibrium a quasi-fermi levelshould be used, which in general applies to each set of states separately e.g. the conduction band,valence band, and each group of traps separately. Each process shown in figure 3.22 has a rate,r.

ra ∝ n · Nt (1 − f) (3.8.23)

where n is the concentration of available electrons and the Nt (1 − f) term represents the con-centration of empty traps. To calculate the proportionality constant, we recognize that electronsmust be in the vicinity of the trap to be captured. We call this region σn cm−2, a capture crosssection as shown in figure 3.23.

The numbers of electrons that sweep past a trap in every second are contained in the volumedefined by:

V = σn · vth (3.8.24)

with units of cm3/s where vth is the thermal velocity of the electron. Those electrons containedin the volume described by this product in a given unit of time will be captured by the trap.

Consider an electron as shown in figure 3.24, vth cms away from the trap position, x0. After1 second the electron will be at x0, and therefore in the capture cross section of the trap. Anyelectron vth +ΔL2 cms away will, after 1 second still be ΔL2 away (case 2) from x0 and hencenot be captured. All electrons closer than vth cms away (as for case 3 of the electron ΔL3 cms

134 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

σn [cm-2]

Trap

Figure 3.23: Picture of the capture cross section

Case 1

vthx0

Case 2 ΔL2

ΔL2

ΔL3

ΔL3

Path in the absence of trap

Figure 3.24: Electrons within the “volume” above will be captured by the trap

closer) would have intersected the capture cross section and be captured. Hence all electronsin the volume V = σn · vth will be captured each second by available empty traps. Thus thenumber of electrons available to be captured per second is

nσnvth (3.8.25)

and recalling the concentration of available empty traps is Nt (1 − f), then the rate, ra can bewritten:

ra = vthσnnNt (1 − f) (3.8.26)

OR, the proportionality constant is σnvth (for the rate of electron capture)

vth =

√2E

m∗ =

√2 · 3kBT

2m∗ (3.8.27)

3.8. CARRIER GENERATION AND RECOMBINATION 135

where E is thermal energy, 3/2kBT in three dimensions. Thus

vth =

√3kBT

m∗ 107cm/sec (3.8.28)

For the electron emission process, b,rb = enNtf (3.8.29)

where en is the emission rate from the trap and Ntf is the concentration of occupied traps. Thecapture rate for holes, process c, will be analogous to process a with the difference that holes arecaptured by occupied traps.

rc = vthσppNtf

Finally, the emission of holes has a rate:

rd = epNt (1 − f) (3.8.30)

where ep is the emission probability for holes. The next step is to determine the emission proba-bilities en and ep. In general this is a very difficult problem since, f is known only in equilibrium.So first consider the equilibrium values of en, and ep. In equilibrium transition rates into and outof the conduction band must be equal, or ra = rb. Inserting

n = Nc exp (− (EC − EF ) /kBT ) = ni exp ((EF − Ei) /kBT ) (3.8.31)

into ra = rb leads to:

en = vthσnni exp ((Et − Ei) /kBT ) (3.8.32)

oren = vthσnNC exp (− (EC − Et) /kBT ) (3.8.33)

Thus the emission probability of electrons into the conduction band rises exponentially as thetrap gets closer to EC which we expect intuitively. From rc = rd and

p = NV exp [− (Ef − EV ) /kBT ]

ep = vthσpNV exp (− (EV − Et) /kBT )

= vthσpni exp (+ (Ei − Et) /kBT )

In non-equilibrium (the case of most interest) f is unknown and has to be calculated. To doso, rate equations are solved. Assume that non-equilibrium is generated by optical excitationresulting in a generation rate of GL electron-hole pairs/second. We also assume that the emissionrates, en, and ep are not a function of illumination and the same as that calculated at equilibrium.

In steady state, the concentration of electrons, nn and holes, pn in an n−type semiconductoris not a function of time and from figure 3.25 we get:

dnn

dt= GL − (ra − rb) = 0 (3.8.34)

dPn

dt= GL − (rc − rd) = 0 (3.8.35)

∴ ra − rb = rc − rd (3.8.36)

136 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

GL

ra rb

rc rd

Figure 3.25: Possible Recombination processes

or the net capture rate of electrons = net capture rate of holes. This leads us to:

vthσnnNt [1 − f(Et)] − vthni exp (Et−i/kBT ) Ntf(Et) =

vthσppNtf − vthσpni exp [(Ei − Et) /kBT ] Nt [1 − f(Et)]

Since we are in non-equilibrium, f (Et), the distribution function for the traps has to be cal-culated from the above equation, where we have substituted for ra through rd,

f (Et) =σnn + σpni exp (Ei−t/kBT )

σn [n + ni exp (Et−i/kBT )] + σp [p + n · exp (Ei−t/kBT )](3.8.37)

where for compactness we have used the notation: Ei−t = Ei − Et and vice versa. Re-substituting to find a net rate of recombination:

U = ra − rb = rc − rd (3.8.38)

leads to:

U =σpσnvthNt

(pn − n2

i

)σn [n + ni exp (Et−i/kBT )] + σp [p + ni exp (Ei−t/kBT )]

(3.8.39)

Let us now consider some special cases:

1. for σn = σp = σ

U = σvthNtpn − n2

i

n + p + 2ni cosh (Et−i/kBT )(3.8.40)

2. for σn = σp = σp and when Et = Ei

U =1

τ

pn − n2i

n + p + 2ni(3.8.41)

We see clearly that pn−n2i is the driving force for recombination. We can also see that n+p+2ni

is a resistance to recombination term, which is minimized when n + p is minimized. For lowlevel injection, we assume that nn � pn and

nn � ni exp ((Et − Ei) /kBT ) (3.8.42)

3.9. CURRENT CONTINUITY 137

as ET ∼ Ei for efficient recombination. Then the recombination rate becomes:

U =σpσnvthNt

σnnn

[nnpn − n2

i

](3.8.43)

= σpvthNt

[pn − n2

i /nn

](3.8.44)

= σpvthNt [pn − pn0] (3.8.45)

U =Δpn

τp(3.8.46)

where the minority carrier lifetime, τp is defined as

1

τp= σpvthNt (3.8.47)

Here the rate limiting step is the capture of the minority carrier. This is also achieved by recog-nizing the hole capture rate, rc is the dominant step. In an n−type semiconductor, since EF isclose to the conduction band and f(ET ) → 1 which makes ra and rd both negligible. Typicalvalues of σ are 10−15 − 10−16cm−2.

Generation occurs when n2i � pn. From equation 3.8.39

U = − σpσnvthNtn2i

σn [n + ni exp (Et−i/kBT )] + σp [p + ni exp (Ei−t/kBT )]

= − σpσnvthNtni

σn exp (Et−i/kBT ) + σpni exp (Ei−t/kBT )

For the case σn = σp = σ

U = − σvthNtni

2 cosh (Et−i/kBT )(3.8.48)

Thus, generation rate peaks when the trap energy is at mid-gap:

U = −ni

2τ(3.8.49)

when Ei → Et the lifetime

τ =1

σvthNT

3.9 CURRENT CONTINUITY(The law of conservationof electrons and holes separately)

In the previous sections we have considered several elements of non-equilibrium phenomenain semiconductors. These include drift and diffusion, carrier generation and recombination.

138 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

If we consider a volume of space in which charge transport and recombination is taking place,we have the simple equality (see figure 3.26a) As a result of consideration of particle current,

Net Rate of particle flow = Particle flow rate due to current −Particle loss rate due to recombination + Particle gain due to generation.

Let us now collect the various terms in this continuity equation. If δn is the excess carrier densityin the region, the recombination rate R in the volume A ·Δx shown in figure 3.26 may be writtenapproximately as

R =δn

τn· A · Δx (3.9.1)

where τn is the electron recombination time per excess particle due to both the radiative and thenonradiative components. The particle flow rate into the same volume due to the current Jn isgiven by the difference of particle current coming into the region and the particle current leavingthe region, [

Jn(x)

(−e)− Jn(x + Δx)

(−e)

]A ∼= 1

e

∂Jn(x)

∂xΔx · A (3.9.2)

If G is the generation rate per unit volume, the generation rate in the volume A · Δx is GAΔx.The rate of electron build up in the volume A · Δx is then

A · Δx

[∂n(x, t)

∂t≡ ∂δn

∂t=

1

e

∂Jn(x)

∂x− δn

τn

](3.9.3)

where δn/τn is U = G − R, the net recombination rate of electrons. We have similar terms forholes, collecting the various terms we have, for the electrons and holes, the continuity equations(note the sign difference in the particle current density for electrons and holes)

∂δn

∂t=

1

e

∂Jn(x)

∂x− δn

τn(3.9.4)

∂δp

∂t= −1

e

∂Jp(x)

∂x− δp

τp(3.9.5)

Using these expressions, the the diffusion currents are

Jn(diff) = eDn∂δn

∂x(3.9.6)

Jp(diff) = −eDp∂δp

∂x(3.9.7)

We get

∂δn

∂t= Dn

∂2δn

∂x2− δn

τn(3.9.8)

∂δp

∂t= Dp

∂2δp

∂x2− δp

τp(3.9.9)

3.9. CURRENT CONTINUITY 139

Jn(x+Jn(x)

x x+Δx)

Δ

Δ

xR= recombination rate

x

Area A

Loss Gain

(a)

(b)

Particle current is conserved

IN OUT

RecombinationLoss

Generation Gain

in volume

Δx

Figure 3.26: (a) A conceptual description of the continuity equation. (b) Geometry used todevelop the current continuity equation.

the time dependent continuity equation for electrons and holes, valid separately. These equationswill be used when we discuss the transient time responses of the p-n diodes and bipolar transis-tors. These equations are also used to study the steady-state charge profile in these devices. Insteady state we have (the time derivative is zero)

d2δn

dx2=

δn

Dnτn=

δn

L2n

(3.9.10)

d2δp

dx2=

δp

Dpτp=

δp

L2p

(3.9.11)

140 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

δn(0)

δn(x=L)

δn(x)

Lx

0

Carrier injection

Figure 3.27: Electrons are injected at x = 0 into a sample. At x = 0, a fixed carrier concentrationis maintained. The figure shows how the excess carriers decay into the semiconductor.

where Ln(Lp) defined as Dnτn(Dpτp) are called the diffusion lengths We will see below thatthe diffusion length represents the distance an electron (hole) will travel before it recombineswith a hole (electron). Let us examine the schematic of the equation derived above. Considerthe case where an excess electron density δn(0) is maintained at the semiconductor at x = 0, asshown in figure 3.27. At some point L in the semiconductor the excess carrier density is fixed atδ(L). We are interested in finding out how the excess density varies with position. The generalsolution of the second-order differential equation 3.9.11 is

δn(x) = A1ex/Ln + A2e

−x/Ln

Using the boundary conditions at x = 0 and x = L, we find that the coefficients A1 and A2 are

A1 =δn(L) − δn(0)e−L/Ln

eL/Ln − e−L/Ln

A2 =δn(0)eL/Ln − δn(L)

eL/Ln − e−L/Ln(3.9.12)

3.9. CURRENT CONTINUITY 141

This gives for the excess carrier concentration

δn(x) =δn(0) sinh

(L−xLn

)+ δn(L) sinh

(x

Ln

)sinh

(L

Ln

) (3.9.13)

There are two important cases that occur in bipolar devices, we will examine them here:(i) L � Ln and δn(L) = 0: In this case the semiconductor sample is much longer than Ln. Thishappens in the case of the long p-n diode , which will be discussed in chapter 4 For this case wehave

δnp(x) = δnp(0)e−x/Ln (3.9.14)

Thus the carrier density simply decays exponentially into the semiconductor.(ii) L � Ln: This case is very important in discussing the operation of bipolar transistors andnarrow p-n diodes . Using the small x expansion for sinh(x)

sinh(x) = x +x3

3!+

x5

5!+ . . .

and retaining only the first-order terms we get

δnp(x) = δnp(0) − x [δnp(0) − δnp(L)]

L(3.9.15)

i.e., in this case the carrier density goes linearly from one boundary value to the other.Note that once the carrier density is known the diffusion current can be simply obtained by

taking its derivative.Let us examine the case where excess carriers are injected into a thick semiconductor sample.

As the excess carriers diffuse away into the semiconductor they recombine. The diffusion lengthLn represents the distance over which the injected carrier density falls to 1/e of its original value.It also represents the average distance an electron will diffuse before it recombines with a hole.This can be seen as follows.

The probability that an electron survives up to point x without recombination is, from equation3.9.15,

δnp(x)

δnp(0)= e−x/Ln (3.9.16)

The probability that it recombines in a distance Δx is

δnp(x) − δnp(x + Δx)

δnp(x)= − Δx

δnp(x)

dδnp(x)

dx=

1

LnΔx (3.9.17)

where we have expanded δnp(x + Δx) in terms of δnp(x) and the first derivative of δnp. Thusthe probability that the electron survives up to a point x and then recombines is

P (x)Δx =1

Lne−x/LnΔx (3.9.18)

142 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Thus the average distance an electron can move and then recombine is

< x > =

∫ ∞

o

xP (x)dx =

∫ ∞

0

xe−x/Ln

Lndx

= Ln (3.9.19)

This average distance (=√

Dnτn) depends upon the recombination time and the diffusion con-stant in the material. In the derivations of this section, we used a simple form of recombinationrate

R =δnp

τn(3.9.20)

where τn is given in terms of the radiative and nonradiative rates as

1

τn=

1

τr+

1

τnr(3.9.21)

The simple δnp/τn form is valid, for example, for minority carrier recombination (p � n).These equations are therefore used widely to discuss minority carrier injection.

3.10 PROBLEMS

Problem 3.1 The electron mobility of Si at 300 K is 1400 cm2/V·s. Calculate the meanfree path and the energy gained in a mean free path at an electric field of 1 kV/cm. Assumethat the mean free path = vth · τsc, where vth is the thermal velocity of the electron (vth ∼2.0 × 107 cm/s).

Problem 3.2 The mobility of electrons in the material InAs is ∼ 35,000 cm2/V·s at 300Kcompared to a mobility of 1400 cm2/V·s for silicon. Calculate the scattering times in thetwo semiconductors. The electron masses are 0.02 m0 and 0.26 m0 for InAs and Si,respectively.

Problem 3.3 Calculate the ionized impurity limited mobility (ND = 1016 cm−3;1017 cm−3) in GaAs from 77 K to 300 K.

Problem 3.4 If the measured room temperature mobility of electrons in GaAs dopedn-type at 5 × 1017 cm−3 is 3500 cm2V−1 s−1 calculate the relaxation time for phononscattering.

Problem 3.5 Calculate the alloy scattering limited mobility in In0.53Ga0.47As as afunction of temperature from 77 K to 400 K. Assume an alloy scattering potential of1.0 eV.

Problem 3.6 The velocity of electrons in silicon remains ∼1 × 107 cm s−1 between50 kVcm−1 and 200 kVcm−1. Estimate the scattering times at these two electric fields.

3.10. PROBLEMS 143

Problem 3.7 The power output of a device depends upon the maximum voltage that thedevice can tolerate before impact-ionization-generated carriers become significant (say10% excess carriers). Consider a device of length L, over which a potential V dropsuniformly. What is the maximum voltage that can be tolerated by an Si and a diamonddevice for L = 2 μm and L = 0.5 μm? Use the values of the critical fields given in thischapter.

Problem 3.8 The electron concentration in a Si sample is given by

n(x) = n(0) exp(−x/Ln); x > 0

with n(0) = 1018 cm−3 and Ln = 3.0 μm. Calculate the diffusion current density as afunction of position if Dn=35 cm2/s.

Problem 3.9 Consider a GaAs sample doped n-type at 1016 cm−3 on which anexperiment is done. At time t = 0 an external stimulus introduces excess electrons at apoint x = 0. The excess charge is detected at x = 10.0 μm in the absence of any appliedfield after 2.5 × 10−9 s.Use this information to answer the following:• What is the diffusion coefficient of electrons?• How much time will electrons travel (by drift) 1.0 μm under an applied field of1.0 kV/cm? Assume that the velocity–field relation is linear.• What is the conductivity of this sample? Assume that the electron effective mass is0.067 m0.

Problem 3.10 In a p-type GaAs doped at Na = 1018 cm−3, electrons are injected toproduce a minority carrier concentration of 1016 cm−3. What is the rate of photonemission assuming that all e-h recombination is due to photon emission ? What is theoptical output power? The photon energy is �ω = 1.41 eV and the radiative lifetime is1.0 ns.

Problem 3.11 Calculate the electron carrier density needed to push the electron Fermilevel to the conduction bandedge in GaAs. Also calculate the hole density needed to pushthe hole Fermi level to the valence bandedge. Calculate the results for 300 K and 77 K.

Problem 3.12 A photodetector uses pure silicon as its active region. Calculate the darkconductivity of the detector (i.e., conductivity when no light is shining on the detector).Light with intensity 10−3 W/cm2 shines on the device. Calculate the conductivity inpresence of light.

μn = 1000 cm2/V · sμp = 400 cm2/V · sα = 103 cm−1

τr = 10−7 s

144 CHAPTER 3. CHARGE TRANSPORT IN MATERIALS

Problem 3.13 Electrons are injected into a p−typesilicon sample at 300 K. Theelectron-hole radiative lifetime is 1 ensuremathμs. The sample also has midgap traps witha cross-section of 10−15 cm−2and a density of 1016 cm−3. Calculate the diffusion lengthfor the electrons if the diffusion coefficient is 30 cm2s−1.

Problem 3.14 Assume that silicon has a midgap impurity level with a cross-section of10−14 cm2. The radiative lifetime is given to be 1 ensuremathμsat 300 K. Calculate themaximum impurity concentration that will ensure that τr < τnr.

Problem 3.15 When holes are injected into an n−typeohmic contact, they decay within afew hundred angstroms. Thus one can assume that the minority charge density goes to zeroat an ohmic contact. Discuss the underlying physical reasons for this boundary condition.

Problem 3.16 Electrons are injected into p−typeGaAs at 300 K. The radiative lifetime forthe electrons is 2 ns. The material has 1015 impurities with a cross-section of 10−14 cm2.Calculate the distance the injected minority charge will travel before 50% of the electronsrecombine with holes. The diffusion coefficient is 100 cm2/s.

Problem 3.17 Electrons are injected into p−typesilicon at x = 0. Calculate the fraction ofelectrons that recombine within a distance L where L is given by (a) 0.5 μm, (b) 1.0 μm,and (c) 10.0 μm. The diffusion coefficient is 30 cm2s−1and the minority carrier lifetime is10−7s.

Problem 3.18 Consider a Si sample of length L. The diffusion coefficient for electrons is25 cm2s−1 and the electron lifetime is 0.01 μs. An excess electron concentration ismaintained at x = 0 and x = L. The excess concentrations are:

δn(x = 0) = 2.0 × 1018 cm−3; δn(x = L) = −1.0 × 1014 cm−3

Calculate and plot the excess electron distribution from x = 0 to x = L. Do thecalculations for the following values of L:

L = 10.0 μm

L = 5.0 μm

L = 1.0 μm

L = 0.5 μm

Note that the excess electron distribution starts out being nonlinear in space for the longstructure, but becomes linear between the two boundary values for the short structure.

Problem 3.19 An experiment is carried out at 300 K on n-type Si doped at Nd = 1017

cm−3. The conductivity is found to be 10.0 (Ω cm)−1.

When light with a certain intensity shines on the material the conductivity changes to 11.0(Ω cm)−1. The light is turned off at time 0 and it is found that at time 1.0 μs theconductivity is 10.5 (Ω cm)−1. The light-induced excess conductivity is found to decay as

δσ = δσ(0) exp

(− t

τ

)

3.11. FURTHER READING 145

where τ is the carrier lifetime. Calculate the following:• What fraction of the donors is ionized?• What is the diffusion length of holes in this material?

Use the following data:

μn = 1100 cm2/V · s : μp = 400 cm2/V · s

Problem 3.20 Calculate the area density of surface states that would lead to surfacegeneration rate of a fully depleted surface to equal twice the generation rate in the surfacedepletion region. Consider the states to be characterized by a capture cross-section of10−15cm2 and the thermal velocity to be 107 cm

s . Assume the surface depletion region tobe 1μm wide and the time constant τ0 = 1μs.

3.11 FURTHER READING

• Transport in crystalline materials

– M. Lundstrom, Fundamentals of Carrier Transport (Modular Series on Solid StateDevices), eds. by G.W, Neudeck and R.F. Pierret, Addison-Wesley, Reading, MA,vol. X (1990).

– J. Singh, Modern Physics for Engineers, Wiley-Interscience, New York (1999).

– K. Seeger, Semiconductor Physics, Springer Verlag, New York (1985).

– J. Singh, Electronic and Optoelectronic Properties of Semiconductors, CambridgeUniversity Press (2003).

• Transport in disordered materials

– N.F. Mott and E.A. Davis, Electronic Processes in Non-Crystalline Materials, Claren-den Press, Oxford (1971).

– A.J. Moulson and J.M. Herbert, Electroceramics: Materials, Properties, andApplications, Chapman & Hall (1992).

Chapter 4

JUNCTIONS INSEMICONDUCTORS: P-NDIODES

4.1 Introduction

In the introduction to this textbook we examined how semiconductor devices are driving mod-ern information technology. Cell phones, computer, internet, etc. all depend upon devices thatwill be discussed in the next several chapters. Semiconductor diodes (and Schottky diodes) dis-cussed in this and the next chapter have rectifying properties. p-n diodes can be used as detectorsand light emitters. Devices such as field effect and bipolar transistors are used for amplificationand signal generation. They can also be used in digital technology as ON/OFF switches.

Semiconductor devices operate on the basis of the basic principle that the conducting andoptical properties of semiconductors can be altered easily and rapidly. One way this can bedone is through the use of junctions between dissimilar materials. Junctions can form betweenn−type and p−type materials, between materials with different bandgaps, and between metalsand semiconductors. In this chapter we will discuss the p-n junction.

4.2 P-N JUNCTION IN EQUILIBRIUM

The p-n junction is one of the most important junctions in solid-state electronics. The junctionis used as a device in applications such as rectifiers, waveform shapers, variable capacitors,lasers, detectors, etc. The key ingredient of the bipolar transistor, which is one of the mostimportant electronic devices is a p-n junction,. To understand how a p-n junction operates weneed to know: i) What are the carrier distributions for electrons and holes in the material? ii)What are the physical processes responsible for current flow in the structure?

146

4.2. P -N JUNCTION IN EQUILIBRIUM 147

Let us start with p- and n-type semiconductors without forming a junction as shown in fig-ure 4.1(a). The electron affinity eχ, defined as the energy difference between the conductionband and vacuum level, is shown along with the work function (eφsp or eφsn). The work func-tion represents the energy required to remove an electron from the semiconductor to the “free”vacuum level and is the difference between the vacuum level and the Fermi level.

Let us now examine what happens when the p- and n-type materials are made to form ajunction. In the absence of any applied bias, there is no net current in the system and the Fermilevel is uniform throughout the structure. In figure 4.1(b) we show a schematic of the banddiagram of a p-n junction.

Majority carriers near the interface on both sides diffuse across the junction (holes from p sideand electrons from n side), as a result of the difference in electron and hole densities across thejunction. Most of the electrons which diffuse to the p-side recombine with holes, and most of theholes which diffuse to the n-side recombine with electrons. As a result, a region is formed nearthe junction that has been depleted of mobile carriers. An electric field exists in this depletionregion that sweeps out any electrons and holes that enter the region.

Three regions can be identified as seen in figure 4.1(b):i) The p-type region where the material is neutral and the bands are flat. The density of

acceptors exactly balances the density of holes (assuming that all of the acceptors are ionized);ii) The n-type region away from the junction where again the material is neutral and the

density of immobile donors exactly balances the free electron density. Again we assume that allof the donors are ionized. In general the majority carrier (holes in the p-region and electronsin the n-region) densities are equal to the density of ionized dopants as long as minority carrierdensities are negligible.

iii) Around the junction there is a depletion region where the bands are bent and a field existsthat sweeps the mobile carriers, leaving behind negatively charged acceptors in the p-region andpositively charged donors in the n-region. The depletion region extends a distance Wp in thep-region and a distance Wn in the n-region.

Due to the field in the depletion region electrons or holes which enter the depletion region areswept away. Thus, once equilibrium is established, a drift current exists that counterbalances thediffusion current. Let us calculate the width of the depletion region, and the electric field. Toobtain analytical results we make some simplifying assumptions:

i) The junction is uniformly doped.ii) The mobile charge density in the depletion region is not zero, but it is much smaller than

the background dopant density. To solve the Poisson equation we will assume that the mobilecarrier density is essentially zero, the depletion approximation.

The various current flow terms in the diode are as follows: the electron drift current andelectron diffusion current as well as the hole drift and hole diffusion current, as shown in fig-ure 4.2(b). When there is no applied bias, these currents cancel each other individually. Let usconsider these current components. The hole current density is

Jp(x) = e

⎡⎢⎢⎣μpp(x)E(x)︸ ︷︷ ︸drift

−Dpdp(x)

dx︸ ︷︷ ︸diffusion

⎤⎥⎥⎦ = 0 (4.2.1)

148 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

⇓

+

+

eχ

Evac

EFn

Junction formation

(a)

Electrons

Fermi level is flat

W p Wn

Holes

p-type n-type

(b)

Evac

Evac

Evac

Ev

Ev

Ev

Ec

Ec

EcEc

Ev

EFp

eφsn

eφsp

eχ

Depletion of mobile charge

–+

– – – – –+

– – – – ––

+++++++++

–

+ + + + + + + +

–––––– –

Diffusion of electrons

Diffusion

Drift

–––––––

+

++++

– – –Drift

+++++++

Electron density, nnHole density, pn

Hole density, ppElectron density, np

––––––– –––

+ +

Figure 4.1: Forming a p-n junction (a) The p- and n-type regions before junction formation.The electron affinity eχ and work functions eφsp and eφsn are shown along with the Fermilevels. (b) A schematic of the junction and the band profile showing the vacuum level and thesemiconductor bands.

4.2. P -N JUNCTION IN EQUILIBRIUM 149

Neutral p-region Neutral n-region

negativelychargedregion

positivelychargedregion

Wp 0 Wn

(a)

E E lectric field direction

Diffusion particle flow Diffusion current flow

Drift particle flow Drift current flow

Diffusion particle flow Diffusion current flow

Drift particle flow Drift current flow

Holes

E lectrons {

{

(b)

+ + +

+ + +

+ + +– – –

– – –

– – –

Figure 4.2: (a) Region of a p-n junction without bias, showing the neutral and depletion ar-eas. (b) A schematic showing various current and particle flow components in the p-n diode atequilibrium.

The ratio of μp and Dp is given by the Einstein relation

μp

Dp=

e

kBT(4.2.2)

Since the Fermi level is uniform in the structure as we go from the p-side to the n-side, as shownin figure 4.3. As a result of bringing the p and n type semiconductors, a built-in voltage, Vbi,isproduced between the n−side and the p−side of the structure. As indicated in figure 4.3, thebuilt-in voltage is given by

eVbi = Eg − (Ec − EF )n − (EF − Ev)p

150 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

where the subscripts n and p refer to the n-side and p-side of the device. Using the Boltzmannapproximation for the Fermi level (see equation 2.4.4)

(Ec − EF )n = −kBT ln(nno

Nc)

where nno is the electron density on the n-side of the device. Assuming that all of the donorsare ionized,

nno = Nd

Similarly,

(EF − Ev)p = −kBT ln(pp0

Nv)

where ppo is the hole density on the p-side and is given by

pp = Na

This gives the built-in voltage

eVbi = Eg + kBT ln(nn0pp0

NcNv)

Using the relation for intrinsic carrier density

n2i = NcNv exp

(− Eg

kBT

)we get

Vbi =kBT

eln(

nn0pp0

n2i

) (4.2.3)

If nn0 and np0 are the electron densities in the n-type and p-type regions, the law of mass action(i.e., the product np is constant) tells us that

nn0pn0 = np0pp0 = n2i (4.2.4)

This gives for the built-in potential, Vbi = Vn − Vp (figure 4.3)

Vbi =kBT

eln

pp0

pn0(4.2.5)

or

Vbi =kBT

eln

nn0

np0(4.2.6)

We have the following equivalent expressions:

pp0

pn0= exp (eVbi/kBT ) =

nn0

np0(4.2.7)

4.2. P -N JUNCTION IN EQUILIBRIUM 151

p n

–Wp 0

pp

Structure

Vp

Potential profile

Electron band profile

pn

nnnp

Wn

Hole density

Electron density

Vn

Ec

Ev

Ev

EcEF

eVbi

Vbi

Eg

Figure 4.3: A schematic showing the p-n diode and the potential and band profiles. The voltageVbi is the built-in potential at equilibrium.

In this relation Vbi is the built-in voltage in the absence of any external bias. Under the approxi-mations discussed later, a similar relation holds when an external bias V is applied to alter Vbi toVbi −V , and will be used when we calculate the effect of external potentials on the current flow.

We need to solve the Poisson equation to calculate the width of the depletion region for thediode under no applied bias. The calculation in the presence of a bias V will follow the sameapproach and Vbi will simply be replaced by Vbi−V , the total potential across the junction. Notethat we have the equality

A WpNa = A WnNd (4.2.8)

where A is the cross-section of the p-n structure and Na and Nd are the uniform doping densitiesfor the acceptors and donors.

152 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

The Poisson equation in the depletion approximation for various regions is

d2V (x)

dx2= 0 −∞ < x < −Wp (4.2.9)

d2V (x)

dx2=

eNa

ε− Wp < x < 0 (4.2.10)

d2V (x)

dx2= −eNd

ε0 < x < Wn (4.2.11)

d2V (x)

dx2= 0 Wn < x < ∞ (4.2.12)

Solving these equations gives the electric field in the p-side of the depletion region

E(x) = −dV

dx= −eNax

ε− eNaWp

ε− Wp < x < 0 (4.2.13)

The electric field reaches a peak value at x = 0. The potential is given by integrating the field,

V (x) =eNax2

2ε+

eNaWpx

ε+

eNaW 2p

2ε+ Vp − Wp < x < 0 (4.2.14)

For the n-side of the depletion region and n-side of the neutral region, we use the conditions

V (x) = Vn Wn < x < ∞E(x) = 0 (4.2.15)

where Vn is the potential at the neutral n-side. The electric field and potential on the n-side isfound to be

E(x) =eNdx

ε− eNdWn

ε0 < x < Wn (4.2.16)

V (x) = −eNdx2

2ε+

eNdWnx

ε− eNdW

2n

2ε+ Vn 0 < x < Wn (4.2.17)

The potential difference between points −Wp and 0 is

V (0) − V (−Wp) =eNaW 2

p

2ε(4.2.18)

Similarly,

V (Wn) − V (0) =eNdW

2n

2ε(4.2.19)

Thus the built-in potential is

V (Wn) − V (−Wp) = Vbi =eNdW

2n

2ε+

eNaW 2p

2ε(4.2.20)

4.2. P -N JUNCTION IN EQUILIBRIUM 153

Please note that in the above equation, and throughout this chapter, the p−type semiconductor(the semiconductor on the left hand side) is the reference electrode. In the case of the MOSFETas we will see in chapter 9 a different reference is used. As noted earlier charge neutrality givesus

NdWn = NaWp (4.2.21)

and we get

Wp(Vbi) =

{2εVbi

e

[Nd

Na(Na + Nd)

]}1/2

(4.2.22)

Wn(Vbi) =

{2εVbi

e

[Na

Nd(Na + Nd)

]}1/2

(4.2.23)

W (Vbi) =

[2εVbi

e

(Na + Nd

NaNd

)]1/2

(4.2.24)

The expressions derived above can be extended to find the electric fields, potential, anddepletion widths for arbitrary values of Vp and Vn under certain approximations. Thus we canuse these equations directly when the diode is under external bias V , by simply replacing Vbi byVbi - V .

In figure 4.4 we show the charge and electric field profile. The electric field is nonuniform inthe depletion region, peaking at the junction with a peak value.

Em = −eNdWn

ε= −eNaWp

ε(4.2.25)

The sign of the field simply reflects the fact that in our study the field points toward thenegative x-axis. It is important to note that if Na � Nd, the depletion width Wp is much smallerthan Wn. Thus a very strong field exists over a very narrow region in the heavily doped side ofthe junction. In such junctions (p+n or n+p) the depletion region exists primarily on the lightlydoped side.

Example 4.1 A diode is fabricated on an n-type (Nd = 1016 cm−3) silicon substrate, onwhich a p-type region doped to 1018 cm−3 is created. Calculate the Fermi level positionsin the p- and n-regions, determine the contact potential in the diode, and calculate thedepletion widths on the p- and n-side. Using the effective density of states relations, wehave (Nc = 2.8 ×1019 cm−3; Nv = 1 ×1019 cm−3at 300 K)

EFn = Ec + kBT lnnn0

Nc

= Ec − (0.026 eV) × 7.937

= Ec − 0.206 eV

EFp = Ev − kBT lnpp0

Nv

= Ev + (0.026 eV) × 2.3

= Ev + 0.06 eV

154 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

0

p-type n-type

Structure

Charge density

–Wp

Wn

m

Electric field

Wn

Charge neutrality in the depletion region:WpNa = WnNd

–Wp Wn

–Wp

+ + ++ + ++ + +

– – –– – –– – –

0

0

Electric field peaks at the junction

x

x

E

Figure 4.4: The p-n structure, with the charge and the electric field profile in the depletion region.The electric field peaks at the junction as shown.

4.3. CURRENT FLOW: P-N DIODE UNDER BIAS 155

The built-in potential is given by

eVbi = Eg − 0.06 − 0.206 eV

= 1.1 − 0.06 − 0.206

= 0.834 eV

The depletion width on the p-side is given by

Wp(Vbi) =

{2εVbi

e

[Nd

Na(Na + Nd)

]}1/2

∼={

2 × (11.9 × 8.84 × 10−12 F/m) × 0.834 (volts)

(1.6 × 10−19 C)

× 1022 m−3

1024 m−3 × (1.01 × 1024 m−3)

}1/2

= 3.2 × 10−9 m = 32 A

The depletion width on the n-side is 100 times longer:

Wn(Vo) = 0.32 μm

4.3 P-N DIODE UNDER BIAS

We have noted that in the absence of an applied bias, even though there is no current flowingin the diode, there are drift and diffusion currents that flow and exactly cancel each other. In thepresence of the applied bias, the balance between the drift and diffusion currents is disturbed anda net current will flow. Under the following simplifying assumptions, one can use the formalismof the previous section to study the biased diode. These approximations are found to be validunder usual diode operating conditions.• We assume that the change in carrier densities is small so that we can use the concept of quasi-equilibrium. The diode is made up of quasi-neutral regions and the depletion region. In thedepletion region, the electron and hole distributions are essentially described by a Boltzmanndistribution and that the concept of a quasi-Fermi level (see section 3.7 and section 4.5.2) isvalid for electrons and holes. The quasi-Fermi levels for the electrons and holes extend from thequasi-neutral regions as shown in figure 4.5.• The external potential drops mainly across the depletion region because the major barrier tocurrent flow is the p-n junction dipole.

The key to the p-n diode operation is that a bias applied across the diode can shrink or increasethe barrier seen by electrons and holes. This is shown schematically in figure 4.5. When aforward bias Vf is applied, the p-side is at a positive potential with respect to the n-side. In thereverse bias case, the p-side is at a negative potential −Vr with respect to the n-side.

In the forward bias case, the potential difference between the n- and p-side is (applied biasV = Vf )

VTot = Vbi − V = Vbi − Vf (4.3.1)

156 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

p n p pn n

Vf

EQUILIBRIUM FORWARD BIAS REVERSE BIAS

(a)

(b)

(c)

eVf

Vr

Vbi – Vf Vbi + VrVbi

Vp

Vn

EFn EFp

EFnEFp

EFp

EFn

eVr

Depletion region

}

EFn

EFpEFp

EFn

Figure 4.5: A schematic showing (a) the biasing of a p-n diode in the equilibrium, forward, andreverse bias cases; (b) the energy band profiles. In forward bias, the potential across the junctiondecreases, while in reverse bias it increases. The quasi-Fermi levels are shown in the depletionregion.

while for the reverse bias case it is (the applied potential V is negative, V = −Vr, where Vr hasa positive value)

VTot = Vbi − V = Vbi + Vr (4.3.2)

Under the approximations given above, the equations for electric field profile, potential profile,and depletion widths we calculated in the previous section are directly applicable except that Vbi

is replaced by VTot. Thus the depletion width and the peak electric field at the junction decreaseunder forward bias, while they increase under reverse bias, as can be seen from equation 4.2.24and 4.2.25 if Vbi is replaced by VTot.

4.3. CURRENT FLOW: P-N DIODE UNDER BIAS 157

4.3.1 Drift and Diffusion Currents in the Biased Diode

The p-n diode characteristics are dominated by minority carrier flow i.e. electrons enteringthe p-side and holes entering from the p-side. When the diode is forward biased the barrier thatelectrons (holes) need to overcome to enter the p-side (n-side) from the n-side (p-side) decreases.This allows a higher minority charge injection. In reverse bias, the minority carrier injection issuppressed. This is shown schematically in figure 4.6. The presence of the bias increases ordecreases the electric field in the depletion region. However, under moderate external bias, theelectric field in the depletion region is always higher than the field for carrier velocity saturation(E >

∼10kV cm−1) for most semiconductors. Thus the change in electric field does not alter thedrift part of the electron or hole current in the depletion region and the magnitude is determinedby the rate of supply of minority carriers by diffusion from the bulk to the depletion region aswill be described in section 4.5. When no bias is applied we have

pp0

pn0= exp (eVbi/kBT ) (4.3.3)

In the presence of the applied bias, under the assumptions of quasi-equilibrium, we get

p(−Wp)

p(Wn)= exp (e(Vbi − V )/kBT ) ∼= pp0

p(Wn)(4.3.4)

We have assumed that the injection of mobile carriers is small (low-level injection) so that themajority carrier densities are essentially unchanged because of injection, i.e., p(−Wp) = pp0.Taking the ratio of the two equations

pn(Wn)

pn0= exp (eV/kBT ) (4.3.5)

This equation suggests that the hole minority carrier density at the edge of the n-side depletionregion can be increased or decreased dramatically by applying a bias.

A similar consideration gives, for the electrons injected as a function of applied bias,

np(−Wp)

np0= exp (eV/kBT ) (4.3.6)

From these equation we can see that the excess carriers created due to injection across the deple-tion regions are

Δpn = p(Wn) − pn = pn0( exp (eV/kBT ) − 1) (4.3.7)

Δnp = np(−Wp) − npo = npo( exp (eV/kBT ) − 1) (4.3.8)

The excess minority carriers that are introduced will decay into the majority region due torecombination with the majority carriers. For long diodes, the decay is simply given by the ap-propriate diffusion lengths (Lp for holes, Ln for electrons). Using results derived in section 3.9,

δp(x) = Δpn exp ((−(x − Wn)/Lp))

= pn0 [ exp (eV/kBT ) − 1] · exp [−(x − Wn)/Lp] (4.3.9)

158 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

–––––––––––––––

}

}

Electron density in thep-side depletion edge

EFp

EFn

+++++++++++

++++++

+

++

++

(a)

––

––– –– –– –– ––––

+++++++

++++++++++

+

EFp

EFn

(c)

V

––

––– –– –– –– ––––

+++++++

++++++++++

+

EFpEFn

V

(b)

++

++

++

++

Fraction of electrons able tobe injected into the p-side

Electron density versusenergy on the n-sidedepletion edge

Zero bias:Diffusion current= drift current

Fraction of holes able tobe injected into the n-side

Fraction of electrons able tobe injected into the p-side

Forward bias:Diffusion current>> drift current

Fraction of holes able tobe injected into the n-side

Negligible density of holesable to cross the barrier

Negligible density of electronsable to cross the barrier

Reverse bias:Diffusion current ~ 0

Figure 4.6: A schematic of the minority and majority charge distribution in the n- and p-sides.The minority carrier injection (electrons from n-side to p-side or holes from p-side to n-side) iscontrolled by the applied bias as shown.

4.3. CURRENT FLOW: P-N DIODE UNDER BIAS 159

for x > Wn

δnp(x) = Δnpo exp ((x + Wp)/Ln)= npo [ exp (eV/kBT ) − 1] exp [(x + Wp)/Ln]

(4.3.10)⎧⎨⎩x < −Wp

x is negativeWp is positive

⎫⎬⎭ .

Holes are injected into the n-side and the value of this diffusion current is

Ip(x) = −eADpd(δp(x))

dx= eA

Dp

Lp(δp(x)) x > Wn (4.3.11)

The hole current injected into the n-side is given by the hole current at x = Wn (after using thevalue of δp(x = Wn) from equation 4.3.9)

Ip(Wn) = eADp

Lppn ( exp (eV/kBT ) − 1) (4.3.12)

Using similar arguments, the total electron current injected across the depletion region into thep-side region is given by

In(−Wp) =eADn

Lnnpo ( exp (eV/kBT ) − 1) (4.3.13)

In this section we will assume that the diode is ideal which essentially means there is no e-hrecombination within the depletion region. In the next section we will discuss the case whererecombination occurs for a real diode. For the ideal diode the total current can be simply obtainedby adding the hole current injected across Wn and electron current injected across −Wp, whichis clear from figure 4.7c. The sum of the electron and hole currents in the depletion region,I = Ip + In is given by Ip(Wn) + In(−Wp) as the currents do not change in the depletionregion due to the assumption of no generation - recombination. The diode current is therefore

I(V ) = Ip(Wn) + In(−Wp)

= eA

[Dp

Lppn0 +

Dn

Lnnpo

]( exp (eV/kBT ) − 1)

I(V ) = Io ( exp (eV/kBT ) − 1) (4.3.14)

This is the diode equation. Under reverse bias, the current simply goes toward the value −Io,where Io is the prefactor of the diode equation.

Io = eA

(Dppn0

Lp+

Dnnpo

Ln

)(4.3.15)

Notice that the diode current increases rapidly when a forward bias is applied and has a smallvalue at negative bias. This gives the diode its rectification properties.

160 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

4.3.2 Minority and Majority Currents in the p-n Diode

The p-n diode is a bipolar device in which electrons and holes both carry current. To obtainthe diode current we have simply added the electron current and hole current injection acrossthe depletion region. This current was evaluated at its peak value at the edges of the depletionregion. The diffusion current decreases rapidly in the majority region because of recombination.As the holes recombine with electrons in the n-region, an equal number of electrons are injectedinto the region. These electrons provide a drift current in the n-side to exactly balance the holecurrent that is lost through recombination. Let us consider the hole diffusion current in the n-typeregion. This current is, from equation 4.3.11, using the value of δp(x) from equation 4.3.10,

Ip(x) = e ADp

Lppn0 exp

(−x − Wn

Lp

)[exp

(eV

kBT

)− 1

]x > Wn

We have also seen that the total current is

I = e A

(Dp

Lppn0 +

Dn

Lnnpo

)[exp

(eV

kBT

)− 1

](4.3.16)

Thus the electron current in the n-type region is

In(x) = I − Ip(x) (for x > Wn)

= eA

{Dp

Lppn0

[1 − exp

(−x − Wn

Lp

)]+

Dn

Lnnp0

}[exp

(eV

kBT

)− 1

]As the hole current decreases from Wn into the n-side, the electron current increases correspondinglyto maintain a constant current. A similar situation exists on the p-side region. As the electroninjection current decays, the hole current compensates. The electron and hole currents flowingin the diode have a behavior shown schematically in figure 4.7.

The rectifying properties of a diode are shown in figure 4.8. The reverse current saturatesto a value Io given by equation 4.3.15. Since this value is quite small, the diode is essentiallynonconducting. On the other hand, when a positive bias is applied, the diode current increasesexponentially and the diode becomes strongly conducting. The forward bias voltage at whichthe diode current density becomes significant (∼ 103 A·cm−2) is called the cut-in voltage. Thisvoltage is ∼ 0.8V for Si diodes and ∼ 1.2 V for GaAs diodes. The cut-in voltage is approximately80 % of the material bandgap.

4.3.3 Narrow Diode Current

In the discussion for the diode current we have assumed the n and p-sides have lengths thatare much greater than the minority carrier diffusion lengths. Often this is not the case. Thisis true for high speed diodes and for p-n junctions in bipolar transistors. In this such case we

4.3. CURRENT FLOW: P-N DIODE UNDER BIAS 161

np

W p 0 Wn

n(x) p(x)

np pn

Depletion Region

minority charge

(a)

(b)

(c)

np + np

pn + pn

Total current

Electron current

Electron current

position

(minority) Hole current

(minority)

Hole current

δn(x) = n(x) np δp(x) = p(x) pn

+ ++ ++ ++ ++ +

x

x

Figure 4.7: (a) A schematic showing the p-n structure under forward bias. (b) The minoritycarrier distribution (c) Minority and majority current.

162 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

p n

V

I

I

I

VIo

Diode symbol

Reverse current due

to drift current in the

depletion region

Forward-bias current

dominated by minority

carrier injection

Figure 4.8: Rectifying I-V current of the p-n diode.

cannot assume that the injected excess minority carrier density will simply decay exponentiallyas exp {− (x − Wn) /Lp} (for holes). In fact, for the narrow diode one has to consider the ohmicboundary conditions where at the contacts the excess minority carrier density goes to zero.

In figure 4.9 we show a case where the diode extends a distance Wln and Wln as shown in then- and p-sides. We know from section 3.9 if the diode is narrow the injected minority carrierconcentration goes from its value at the depletion edge toward zero at the contact in a linearmanner. The hole current injected across Wn becomes (note that δpn(W�n) = 0)

Ip(Wn) = −eADpd(δp(x))

dx= −eADp

[δpn(Wn) − δpn(W�n)

W�n − Wn

]=

−eADp

W�n − Wnpn

[exp

(eV

kBT

)− 1

](4.3.17)

A similar expression results in this linear approximation for the electron distribution. The neteffect is that the prefactor of the diode current changes (i.e., the term Ln or Lp in the denominatoris replaced by a smaller term (W�n − Wn) or (|W�p − Wp|). The prefactor becomes

Io = eA

[Dppn0

(W�n − Wn)+

Dnnp0

(|W�p − Wp|)]

(4.3.18)

The narrow diode therefore has a higher saturation current than a long diode. The advantage ofthe narrow diode lies in its superior time-dependent response—a topic we will consider later.

4.4. REAL DIODES:DEFECTS AND CARRIER GENERATION 163

–W p 0

Ohmiccontact

Ohmiccontact

Injected charge

δnp(x)

–Wp W nWn

δpn(x)

–W p –Wp Wn W n0

p-side n-side

(a)

(b)

Linear decay of minority charge

Figure 4.9: (a) A schematic of the narrow p-n diode with ohmic contacts at the boundaries. (b)The injected charge distribution.

4.4 REAL DIODES: CONSEQUENCES OF DEFECTS ANDCARRIER GENERATION

In the discussion so far we have assumed the diode we are dealing with is ideal, i.e., there areno defects and associated bandgap states that may lead to trapping, recombination, or generationterms. In section 3.7 we discussed the effects of bandgap states produced by defects. In a realdiode, a number of sources may lead to bandgap states. The states may arise if the materialquality is not very pure so that there are chemical impurities present. Let us assume that thedensity of such deep level states is Nt. We will assume that the deep level is at the center of thebandgap.

We learned in chapter 3 in the SRH analysis that under the approximation of:

1. σ = σn = σp and

2. Et = Ei, and

3. en, ep, σn, σp are unperturbed in non-equilibrium

164 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

np

+

+

+

0 wn-wp

In

Ip

IR

IG

Figure 4.10: Qualitative diagram of all current components flowing in a p-n diode.

We get

U =1

τ· pn − n2

i

n + p + 2ni(4.4.1)

where

τ =1

σvthNt

and pn− n2i = driving force for recombination and n + p + 2ni = resistance to recombination.

This applies to any semiconductor with or without band bending. Note that the values of n and pare functions of band bending, photon flux, etc. Also, note that U is maximized for a certain levelof perturbation when the denominator is minimized. As electrons and holes enter the depletionregion, one possible way they can cross the region without overcoming the potential barrier is torecombine with each other. This leads to an additional flow of charged particles. This current,called the generation-recombination current, must be added to the current calculated so far. Infigure 4.10 we show a qualitative diagram of all current components flowing in the diode.

4.4.1 Generation-Recombination Currents

To calculate the recombination currents in a diode, the Sah-Noyce-Shockley current, JSNS ,we consider a forward biased diode shown in figure 4.11b. Under a forward bias of V , theproduct of np is a constant across the depletion layer and is

np = n2i exp

(eV

kBT

)This is easily seen by recognizing that

n(x) = nn0 exp

(−eψ′(x)

kBT

)(4.4.2)

4.4. REAL DIODES:DEFECTS AND CARRIER GENERATION 165

EV

EFp

ECEFnEip

Ein

ψ (x)

ψ ’(x)

EV

EF

EC

EF

Eip

Ein

(a)

(b)

Figure 4.11: Band diagram of a p-n junction (a) in equilibrium and (b) under forward bias

p(x) = pp0 exp

(−eψ(x)

kBT

)(4.4.3)

Note that ψ(x) is the voltage measured downwards from Eip and ψ′(x) is measured upwardsfrom Ein and that

n(x) · p(x) = nn0 pp0 exp

[−e(ψ′(x) + ψ(x))

kBT

]ψ(x) + ψ′(x) = Vbi + V (4.4.4)

Therefore,

n(x) · p(x) = nn0pn0 exp

(eV

kBT

)or

n(x) · p(x) = n2i exp

(eV

kBT

)(4.4.5)

166 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

X = 0

xψ

ψ

xTowards nTowards p

Maximum Recombination Plane

Figure 4.12: The maximum recombination plane is where the recombination is peaked withinthe depletion region

Under steady state bias of V the term n + p + 2ni is minimized when n = p. The value of xwhere this occurs is chosen to be zero. This is the maximum recombination plane (MRP).

n(0) = p(0) = ni exp

(eV

2kBT

)(4.4.6)

If we move away from the MRP, the electron and hole concentrations change proportionally tothe term

exp

(±eψ(x)

kBT

)as shown in figure 4.12, Where

n(x) = n(0) exp

(eψ(x)

kBT

)and p(x) = p(0) exp

(−eψ(x)

kBT

)Assuming the distance x is small so that we can assume the electric field is constant for purposesof the analysis to be E = E(0). Then ψ = ±Ex and therefore,

U =1

τ· pn − n2

i

n + p + 2ni=

1

τ· n2

i exp (eV /kBT ) − n2i

n(0) exp (eψ/kBT ) + p(0) exp (−eψ/kBT ) + 2ni

Neglecting n2i in the numerator and 2ni in the denominator we get

U =1

τ· ni exp (eV /2kBT )

2 cosh(eEx/kBT )(4.4.7)

4.4. REAL DIODES:DEFECTS AND CARRIER GENERATION 167

U

X = 0

Figure 4.13: Schematic of the net recombination rate as a function of distance from the MRP

To calculate the total recombination current we need to integrate over the volume of the depletionregion. Since the recombination rate curve is highly peaked about x = 0, the MRP, as shown infigure 4.13, the following approximations remain valid.

1. Linearizing the potential ψ = ±Ex since only small values of x contribute to the integral.

2.∫ Wn

−Wp→ ∫

∞

Therefore,

ISNS = IR = eA

∫U(x)dx (4.4.8)

Making these substitutions and solving equation 4.4.8, we find:

IR =eniA

2τexp

(eV

2kBT

)∫ +∞

−∞

dx

cosh [eE(0)x/kBT ](4.4.9)

=eniA

2τ· πkBT

eE(0)exp

(eV

2kBT

)(4.4.10)

=I◦GR exp

(eV

2kBT

)(4.4.11)

At zero applied bias, a generation current of IG balances out the recombination current.

168 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

The generation-recombination current therefore has an exponential dependence on the voltageas well, but the exponent is different. The generation-recombination current is

IGR = IR − IG = IR − IR(V = 0)

= I◦GR

[exp

(eV

2kBT

)− 1

](4.4.12)

where V is small so that the MRP is assumed constant.The total device current now becomes

I = Io

[exp

(eV

kBT

)− 1

]+ I◦GR

[exp

(eV

2kBT

)− 1

]or

I ∼= IS

[exp

(eV

nkBT

)− 1

](4.4.13)

= IS

[exp

(V

n· e

kBT

)− 1

]where n is called the diode ideality factor or the voltage partitioning factor because the factor of 2in equation 4.4.12 is a consequence of recombination occurring at the maximum recombinationplane. The prefactor Io

GR can be much larger than Io for real devices. Thus at low appliedvoltages the diode current is often dominated by the second term. However, as the applied biasincreases, the diffusion current starts to dominate. We thus have two regions in the forward I-Vcharacteristics of the diode, as shown in figure 4.14. One of the reasons it is experimentallydifficult to measure an IV curve with an ideality factor of 2 is because the MRP is actuallychanging with applied bias.

In figure 4.15, we show the effects that material defects can have on the diode current char-acteristics. We can see that defects such as threading dislocations can cause large undesirablereverse leakage currents that are not predicted by the ideal diode characteristics calculated in thissection.

Example 4.2 Consider the p-n diodes examined in problem 4.12. In that example, thediode prefactor was calculated assuming that there is no recombination in the depletionregion. Calculate the effect of the generation-recombination current assuming a lifetime of10−6 s.

The prefactor of the generation-recombination current is

IoGR =

eAni

2τ

πkBT

eE(0)

At zero applied bias, we know that the MRP occurs where pp0e− ψ(x)

kBT = ni. This allows

4.4. REAL DIODES:DEFECTS AND CARRIER GENERATION 169

((

Region 1

Region 2

HIGH INJECTION

REGION

• Dominated by generation- recombination

• Diode behaves like an ohmic resistor

FORWARD BIAS, V (volt)

Region 3

CU

RR

EN

T I

(A

)

10–3

10–6

10–9

10–12

10–150.2 0.4 0.6 0.8

VD rS

I =

eVkBT

exp –1

( eV2kBT

exp –1(

Figure 4.14: A log plot of the diode current in forward bias. At low biases, the recombinationeffects are quite pronounced, while at higher biases the slope becomes closer to unity. At stillhigher biases the behavior becomes more ohmic.

us to solve for ψ(x) and thus E(0). This gives

I◦GR =

(1.6 × 10−19 C

) (10−3 cm2

) (1.5 × 1010 cm−3

)2 (10−6 s)

· (3.14) (.026V )

(3.2 × 104 V/cm)

= 3.0 × 10−12 A

and

IGR = IoGR

[exp

(eV

2kBT

)− 1

]We can see that the generation-recombination prefactor is much larger than the prefactordue to the diffusion term. Thus the reverse current will be dominated by thegeneration-recombination effects.

In forward bias, the diffusion current is initially much smaller than thegeneration-recombination term. However, at higher forward bias the diffusion current willstart to dominate. For example, we see that at a forward bias of 0.2 V, the diffusion currentis 2.2 × 10−11 A, while the generation-recombination current is 1.65 × 10−10 A. At a

170 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

N-contactP-contact

Diode ondislocated

GaN

Diode onLEO GaN

p-GaN

n-GaN

SiO2 mask LEO GaN

Dislocated GaN

2μm GaN

10-13

10-12

10-11

10-10

10-9

10-8

10-7

-50 -40 -30 -20 -10 0

50100150200250

10-6

10-5

10-4

10-3

10-2

10-1

Curr

ent (A

)

Voltage (V)

Temperature (C)C

urr

ent D

ensi

ty (

A / c

m2)

(a)

(b)

(c)

(d)

Figure 4.15: Effects of threading dislocations on reverse leakage current in p-n diodes. GaNp-n diodes were fabricated on the same wafer, some of them being placed on areas with highdislocation density, and some placed in areas with virtually no dislocations. The fabricationprocess is shown in (a) - (c). Current characteristics for a number of diodes are shown in (d).We see that the reverse leakage current in the devices on dislocated material is 3-4 orders ofmagnitude higher than that of devices on non-dislocated material, indicating that the dislocationsprovide a leakage path for current to travel. Figures taken from the PhD dissertation of PeterKozodoy, UCSB.

4.4. REAL DIODES:DEFECTS AND CARRIER GENERATION 171

forward bias of 0.6 V, the diffusion current is 1.07 × 10−4 A, while thegeneration-recombination current is 8.45 × 10−7 A.

Example 4.3 Consider a long p-n diode on silicon with the following parameters:

n-side doping = 1017 cm−3

p-side doping = 1017 cm−3

Minority carrier lifetime τn = τp = 10−7 s

Electron diffusion constant = 30 cm2/s

Hole diffusion constant = 10 cm2/s

Diode area = 10−4 cm2

Carrier lifetime in the depletion region = 10−8 s

Calculate the diode current at a forward bias of 0.5 V and 0.6 V at 300 K. What is theideality factor of the diode in this range?

For this diode structure we have the following:

np = 2.25 × 103 cm−3

pn = 2.25 × 103 cm−3

Ln = 17.32 μm

Lp = 10.0 μm

Vbi = 0.817V

The prefactor in the ideal diode equation is

I0 = eA

(Dppn

Lp+

Dnnp

Ln

)= 9.83 × 10−16

The prefactor to the recombination-generation current is

I0GR =

eAni

2τ· πkBT

eE(0)

where τ is the lifetime in the depletion region.

The E(0) at a forward bias of 0.5 V is found to be

E(0) = 6.94 × 104 V/cm

The E(0) at a forward bias of 0.6 V is found to be

E(0) = 5.74 × 104 V/cm

172 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

The prefactors to the recombination-generation current is

I0GR(0.5 V) = 1.4 × 10−11 A

I0GR(0.6 V) = 1.7 × 10−11 A

The current is now

I(0.5 V) = 9.83 × 10−16 exp

(0.5

0.026

)+ 1.4 × 10−11 exp

(0.5

0.052

)= 4.33 × 10−7 A

and

I(0.6 V) = 9.83 × 10−16 exp

(0.6

0.026

)+ 1.7 × 10−11 exp

(0.6

0.052

)= 1.21 × 10−5 A

We can write the diode current as

I ∼= IS exp

(eV

nkBT

)Thus

I(V2)

I(V1)∼= exp

(e(V2 − V1)

nkBT

)Using this relation, we find that

n ∼= 1.15

4.5 Reverse Bias Characteristics

The case for reverse bias is very different. Here the application of bias increases barriers.The only carriers that can flow are those that can diffuse to the depletion region and are sweptacross by the field; these are minority carriers, holes in the n-region and electrons in the p-region(figure 4.16).

4.5.1 First Observation

Since we are only dealing with minority carrier currents we know that minority carrier drift canbe neglected, hence only minority carrier diffusion is relevant. To calculate diffusion currents weneed to know the charge profile. Charge profiles are obtained by solving the continuity equationas shown in chapter 3. We assume that the large electric field in the reverse biased p-n junctionsweeps minority carriers away from the edge of the junction. Using the Schockley BoundaryConditions:

np (−Wp) = 0 And pn (+Wn) = 0

4.5. REVERSE BIAS CHARACTERISTICS 173

np0 pn0Wp Wn

Pn(x)np(x)

VR

x =wn

+ x

x =-wp x=0

- x

Figure 4.16: Here the minority carriers are electrons injected from the p-region to the n-region(opposite to the forward-biased case)

We also know that the minority carrier concentration in the bulk is np0 (p−type) and pn0

(n−type). Therefore, the shape of the curve will be qualitatively as shown (figure 4.16) re-ducing from the bulk value to zero at the depletion region edge. We now consider the flow ofminority holes. The charge distribution is obtained by solving:

Dpd2pn

dx2+ Gth − R = 0 (4.5.1)

Where Gth is the generation due to thermal emission of carriers, and R is the recombinationrate for excess carriers. The process of carrier recombination is driven by excess carriers. Thisdependence may be written as: (where αr is a material-dependent rate constant).

R = npαr =pn

τp(4.5.2)

where in a p-type semiconductor τp = 1αrn . Clearly, in an intrinsic semiconductor without

excess minority carriers the expressions for R and Gth become equivalent - expressing the equi-librium of the system:

Gth − R = 0

174 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

orGth = αrn

2i

In non equilibrium recognizing that Gth is a function of temperature and invariant under injection

Gth − R = αrn2i − αrnp =

pn0 − pn

τp(4.5.3)

Therefore, from equation 4.5.1

Dpd2pn

dx2+

pn0 − pn

τp= 0 (4.5.4)

Note that the second term in this sum is a generation term because pn < pn0 for all x > Wn.This is natural because both generation and recombination are mechanisms by which the systemreturns to its equilibrium value. When the minority carrier concentration is above the equilibriumminority carrier value then recombination dominates and when the minority carrier concentrationis less than that at equilibrium, then generation dominates. Again, using Δpn (x − Wn) =pn0 − pn (x − Wn), we have

X=0 LpLn

np

+

+

Figure 4.17: Minority carriers generated within a diffusion length of the depletion region enterand are swept away.

Dpd2Δpn (x)

dx2+

Δpn (x)

τp= 0 (4.5.5)

and,

Δpn (x − Wn) = C1 exp

(+

x − Wn

Lp

)+ C2 exp

(−x − Wn

Lp

)(4.5.6)

Where we know that:⎧⎪⎨⎪⎩C1 = 0 for physical reasons,

Δpn (x − Wn) → 0 x − Wn = ∞,

Δpn (x − Wn) → pn0 − pn(0) = pn0 x − Wn = 0.

4.5. REVERSE BIAS CHARACTERISTICS 175

∴ Δpn (x − Wn) = pn0 exp

(−x − Wn

Lp

)which can be rewritten for x ≥ Wn

pn (x) = pn0

[1 − exp

(−x − Wn

Lp

)](4.5.7)

which implies that the flux of holes entering the depletion region is

Jp(Wn) = eDpdpn(Wn)

dx= e

Dp

Lppn0

and similarly, Jn = eDn

Ln·np0. Assuming no generation in the depletion region, the net current

flowing is:

Js = e

(Dp

pn0

Lp+ Dn

np0

Ln

)(4.5.8)

This result is remarkable because we get the same answer if we took the forward bias equation(valid only in forward bias) and arbitrarily allowed V to be large and negative (for reverse bias)-i.e.

J = Js [ exp (qV/kT ) − 1] (4.5.9)

if V is large and negative, JR = −JS which is the answer we derived in equation 4.5.8. Thiscan be understood as follows. As shown in figure 4.17 any minority carrier electrons generatedwithin a diffusion length of the n depletion edge can diffuse to the edge of the junction and beswept away. Minority electrons generated well beyond a length Ln will recombine with holesresulting in the equilibrium concentration, np0. Similarly holes generated within Lp, a diffusionlength, of the depletion region edge could diffuse into the depletion region. It is important tonote (from the first term of equation 4.5.8) that the slope of the minority carrier profile at thedepletion region edge :

slope =pn0

Lp=

difference from bulk value

Lp(4.5.10)

This is always true when recombination and generation dominate. Recall that even in forwardbias (shown in figure 4.18) the slope of the carrier profile is again

difference from bulk value

Lp=

Δpn(Wn)

Lp(4.5.11)

4.5.2 Quasi Fermi Levels

The Quasi Fermi Level is a very useful concept as it accurately represents the occupancy ofstates of the system that it refers to. It is important to recognize that semiconductor devicesare composed of several interacting systems. For example, the conduction band containing freeelectrons, the valence band containing free holes and trap states in the gap have an occupancy,

176 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

Minority carrier concentration

Pn=0

pn0

slope

Pn=0

Slope

( )1/

0 −=Δ kBTeV

nn epp

Figure 4.18: left: Reverse bias minority carrier concentration. right: Forward bias minoritycarrier concentration

with each set of traps constituting a separate system. Each of these systems will be representedby their own quasi Fermi level, EFn for the electrons, EFp for the holes and EFTi for the trapsof energy ETi. If thermal energy is the only energy source determining the occupancy of thedifferent states and the systems are all freely interacting then of course all the quasi Fermi levelsmerge into the Fermi level of the system at equilibrium. We have also seen in figure 4.5 thatthe quasi Fermi levels vary across a device in non-equilibrium. The variation of the Fermi levelis determined by the current flow in the system and the interaction of the various systems. Letus look at the variation of EFn and EFp in the case of a forward biased diode in figure 4.5c.The electron quasi Fermi level is determined by the electron concentration point by point and isdetermined by the level set by the reservoir of electrons which is the n−type layer. The largeelectron concentration in the n−type layer ensures that only a small gradient in EFn can sus-tain current of relevant magnitudes and hence is pictured flat in the bulk. The same applies forEFp on the p−side. As electrons and holes flow across the depletion region the quasi Fermilevels remain almost flat because the length of the depletion region is very small allowing largegradients to be present to satisfy needed current flow with low absolute values of ΔEFn andΔEFp. In the depletion region, since there is no recombination assumed, the electron concen-tration is determined by the n−region and the hole concentration by the p−region, and in bothinstances substantially by the thermal supply as given by the Boltzmann distribution as shownin figure 4.6. However, in the bulk regions the electrons and holes recombine and hence the EFn

in the p−region decreases in a manner determined by the recombination rate and not the Boltz-mann tail of the majority electrons. In the case of reverse bias (figure 4.5c) the injected electronsand holes are sourced as thermally generated minority carriers in the bulk regions and sweptacross the junction to constitute the reverse saturation current. The quasi-femi levels reflect thechange in the minority carrier concentration in the bulk regions on the application of the reversebias. The minority carrier electron concentration at the edge of the depletion region of the p-sideunder zero bias is nn0 exp (−eVbi/kBT ) or np0. On application of the reverse bias of Vr, theelectron concentration at the junction edge supplied by thermionic emission from the n-side is

4.6. HIGH-VOLTAGE EFFECTS IN DIODES 177

given by nno exp (−e(Vbi − Vr)/kBT ) or np0 exp (eVr/kBT ), but since Vr is negative this isvery small. The linear decrease in the value of EFn from the p−bulk to the edge of the junc-tion reflects the exponential decrease in the carrier concentration because of diffusion toward thejunction as shown in equation 4.5.7. The reader should be aware that this picture reflects the caseof no velocity saturation of either electrons or holes in the materials. If that happens, the electronconcentration at the edge of the junction cannot decrease arbitrarily and the problem has to besolved such that the carriers allow current to be continuous through the structure and is left tothe reader as an exercise.

4.6 HIGH-VOLTAGE EFFECTS IN DIODES

In deriving the current-voltage relation we have made two important assumptions: i) the excesscarrier density injected across the depletion region is small compared to the majority chargedensity; ii) the reverse current saturates since it is due to the carriers drifting across the depletionregion and is limited by the diffusive flux of minority carriers to the junction.

4.6.1 Forward Bias: High Injection Region

We have so far assumed that the injection density of minority carriers was low so that thevoltage all dropped across the depletion region. However, as the forward bias is increased, theinjection level increases and eventually the injected minority carrier density becomes comparableto the majority carrier density. When this happens, an increasingly larger fraction of the externalbias drops across the undepleted region. The diode current will then saturate, as shown as Region3 in figure 4.14. The minority carriers transport is not only due to diffusion, but also due to theelectric field that is now present in the undepleted region. As the forward bias increases, thedevices start to behave like a resistor, where the current-voltage relation is given by a simplelinear expression. The current is now controlled by the resistance of the n- and p-type regions aswell as the contact resistance.

4.6.2 Reverse Bias: Impact Ionization

We have noticed that under reverse bias conditions the electric field across the depletion regionincreases. As a result electrons and holes forming the reverse current can acquire very highenergies. Once this excess energy reaches the value of the bandgap we can have impact ionizationas discussed in chapter 3. The final result is that one initial electron can create two electrons inthe conduction band and one hole in the valence band. This results in current multiplication andthe initial current reverse bias Io becomes

I′

o = M(V )Io (4.6.1)

here M is a factor that depends upon the impact ionization rate which we now derive.

178 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

4.7 Avalanche Breakdown in a p-n junction

Consider a p − i − n junction where the applied voltage is such that the electric field on theintrinsic region which is a constant is assumed to be large enough to saturate the electron andhole velocities. We assume in our analysis that vse = vsh = vs. As is shown schematicallyin figure 4.19, a few lucky electrons (minority carriers) injected from the p-side into the highfield region can gain enough kinetic energy (> Eg) to collide with the lattice creating electron-hole pairs. This process is called impact ionization. These electrons and holes accelerate againleading to more collisions and further generation. The same applies to holes injected from then−side. To analyze the resultant current due to impact ionization one solves the continuityequation for electrons and holes:

∂n

∂t=

1

e

∂Jn

∂x+ Gn(e) + Gh(e) (4.7.1)

where Gn(e) = the rate of generation of secondary electrons by accelerated electrons = αnn(x)vs,where α(cm−1), the ionization coefficient of electrons, is the number of electron-hole pairsgenerated per electron per cm, and n(x)(cm−3) is the local concentration of electrons, and vs

(cm/s) is the saturated electron velocity. The ionization coefficient is much less than 1 becauseonly lucky electrons create electron-hole pairs and the above equation assumes that all elec-trons are participating in the process. Gh(e) is the rate of generation of secondary electrons byaccelerated holes:

Gh(e) = αp · p(x) · vs (4.7.2)

where αp is the ionization coefficient for holes. p(x)(cm−3

)= local concentration of holes. vs

is the saturated hole velocity. Assuming αn = αp = α and that α �= f(E), the latter being agood approximation in a p − i − n structure,

∂n

∂t=

1

e

∂n

∂x+ α (n(x)vs + p(x)vs) = 0 (4.7.3)

in steady state which we now consider. The impact ionization process causes the electron currentto increase from its reverse saturation value,

Jn0 = −eDn

Lnnp0 (4.7.4)

to a larger value at the p-side. The same is true for holes as shown in figure 4.20. To solve thesteady state continuity equation we also note that

Jn(x) = −en(x)vs (4.7.5)

andJp(x) = ep(x) (−vs) = −ep(x)vs (4.7.6)

which gives∂Jn

∂x− α (envs + epvs) = 0 (4.7.7)

4.7. AVALANCHE BREAKDOWN IN A P-N JUNCTION 179

p i n

*

**

Figure 4.19: Band diagram for a p − i − n diode showing the avalanche ionization and mul-tiplication process where an injected minority carrier causes generation of electron-hole pairsthrough impact ionization. Multiple ionization events may be caused by a single carrier. Thestar represents a collision which generates an electron-hole pair.

or∂Jn

∂x= α (Jp + Jn) = αJTotal (4.7.8)

Integrating over the length of the multiplication region, wa, we get∫dJn = JTotal

∫ wa

0

α dx (4.7.9)

Jn (wa) − Jn(0) = JTotal

∫ wa

0

α dx (4.7.10)

RecognizingJn (wa) = JTotal − Jp0 (4.7.11)

and J(0) = Jn0, one gets

JTotal − JP0 − Jn0 = JTotal

∫ wa

0

α dx (4.7.12)

180 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

Jp

Jn0 Jp0

Jn

JTotal

wa

Figure 4.20: Majority and minority currents in a reverse-biased p − i − n junction

Defining a multiplication factor, M ,

M =JTotal

Jp0 + Jn0=

JTotal

Js(4.7.13)

the equation reduces to:

1 − 1

M=

∫ wa

0

α dx (4.7.14)

or

M =

[1 −

∫ wa

0

α dx

]−1

(4.7.15)

Breakdown is defined as the case where JTotal → ∞ or M → ∞. This condition is achievedwhen

1 −∫ wa

0

α dx → 0 (4.7.16)

or ∫ wa

0

α dx → 1 (4.7.17)

We recognize that α is a f(E) in general. In the case of a constant α, the breakdown conditionreduces to

α · wa → 1

which represents the case of every electron (hole) injected into the high field region generatingan electron-hole pair before exiting. This process is self-sustaining.

4.7.1 Reverse Bias: Zener Breakdown

Impact ionization or avalanche breakdown is one mechanism for breakdown in diodes. Thereis another one that can be important for narrow gap diodes or heavily doped diodes. This mech-anism is due to the quantum-mechanical process of tunneling. The tunneling process, allows

4.7. AVALANCHE BREAKDOWN IN A P-N JUNCTION 181

J

V

Total

Ideal

M ∞

Figure 4.21: Current-Voltage characteristics for a p − i − n diode in avalanche breakdownshowing the ideal (non-avalanche) case as well as the limit where M becomes large.

electrons in the valence band to tunnel into the conduction band and vice versa. Electrons tun-neling through the diode do not have to go over the barrier and as a result the diode reversecurrent can increase dramatically.

To examine how tunneling occurs let us examine the band profile in a reverse-biased p-njunction. Assume that the diode is heavily doped so that the Fermi level on the n-side and theFermi level on the p-side are in the conduction and valence bands, respectively. The heavydoping ensures that electrons in the conduction band can tunnel into “available” empty states inthe valence band. A typical electron sees a potential barrier between points x2 and x1, as shownin figure 4.22b. The tunneling probability is given under such conditions by

T ≈ exp

(−4

√2m∗E3/2

g

3e�E

)(4.7.18)

where Eg is the bandgap of the semiconductor, m∗ is the reduced mass of the electron-holesystem, and E is the field.

There is a special class of diodes called Zener diodes where tunneling is exploited. Thedepletion width can be controlled by the doping density. If the junction is made from heavilydoped materials, the Zener tunneling can start at a reverse bias of Vz , which could be as low asa few tenths of a volt. The voltage across the junction is then clamped at Vz , and the current iscontrolled by the external circuit as shown in figure 4.23. This clamping property provides a veryuseful application for the Zener diodes. If Vz is breakdown voltage (due to impact ionization or

182 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

E c

E vEc

Ev

E

Eg

–x1 0X

Potential energy

(a)

(b)

Forbidden gap

–x 2

EFp

EFn

Figure 4.22: (a) A schematic showing the band diagram for a reverse-biased p-n junction alongwith how an electron in the valence band can tunnel into an unoccupied state in the conductionband.(b) The potential barrier seen by the electron during the tunneling process.

Zener breakdown), the current for reverse bias voltages greater than Vz is

I =|V − Vz|

RL(4.7.19)

Example 4.4 A silicon p+n diode has a doping of Na = 1019 cm−3, Nd = 1016 cm−3.Calculate the 300 K breakdown voltage of this diode. If a diode with the same ε/Nd valuewere to be made from diamond, calculate the breakdown voltage.

The critical fields of silicon and diamond are (at a doping of 1016 cm−3) ∼ 4 × 105 V/cmand 107 V/cm. The breakdown voltage is

VBD(Si) =ε(Ecrit)

2

2eNd=

(11.9)(8.85 × 10−14F/cm)(4 × 105 V/cm)2

2(1.6 × 10−19 C)(1016 cm−3)= 51.7 V

4.8. DIODE APPLICATIONS: AN OVERVIEW 183

(Zener diode)

p n

Vo

I

I

V

Forward current

Reverse saturation current

Vout = VzReversecurrent = (Vo – Vz)/RL

VzRL

Figure 4.23: (a) Tunneling breakdown effect in the reverse-biased p-n diode for a voltage-clamping circuit. The circuit is thus very useful as a voltage regulator and zener diode circuitsymbol.

The breakdown for diamond is

VBD(C) = 51.7 ×(

107

4 × 105

)2

= 32.3 kV!

One can see the tremendous potential of diamond for high-power applications where thedevice must operate under high applied potentials. At present, however, diamond-baseddiodes are not commercially available.

4.8 DIODE APPLICATIONS: AN OVERVIEW

4.8.1 Applications of p-n diodes

The p-n junction (or the Schottky diode) is the fundamental building block of semiconductordevices. The applications are based on certain properties of the junction

I. The injection of electron-hole pairs to generate light via recombination (eg. LEDs andLASERs)

II. The separation of electron-hole pairs at the junction to constitute a current source (eg.solar cell)

III. The temperature dependence of the I-V characteristic (eg. a temperature sensor)

IV. The non-linear nature of the I-V characteristic (eg. frequency multipliers and mixers)

V. The device as a switch (eg. rectifiers, inverters, power supplies etc)

184 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

DIODE

PROPERTIES

CURRENT

SOURCE

NON-LINEAR I-V

AND C-V

EMISSION

AND

ABSORPTION

SWITCH

• SOLAR CELL• PHOTODETECTOR• TRANSISTOR

• MULTIPLIERS• POWER DETECTORS• TUNING CAPACITORS

• LEDs• LASERs• MODULATORS

• RECTIFIERS• POWER CONDITIONING• LEVEL SHIFTERS

Table 4.1: Some important applications of semiconductor diodes in electronics and optoelec-tronics.

We now go through these applications briefly to help explain how these properties are har-nessed. The goal is not to provide full details but to elucidate methodology. The diode has manyuses when employed as a current source. The diode when operated under reverse bias has theproperties of a current source (infinite output resistance or equivalently a constant current withvoltage). Consider figure 4.24. If a current source is available which can be controlled then it canform the basis of several critical and valuable applications. If large changes in the current sourcecan be effected by a small change in input voltage, ΔVin) then the resultant change in outputvoltage, ΔVout, could be large if the current is delivered to a large load resistance. The resultantvoltage gain , ΔVout/ΔVin, forms the basis of transistor operation and explains why the outputof a transistor is always represented by a current source. If the current source can be controlledby incident photons, then the resultant current is basis of the operation of a photodetector or asolar cell. The transistor is described in detail in later chapters and we describe the solar cell andphotodetector below.

4.8.2 The Solar Cell and Photodetector

Consider a reverse biased diode which is subjected to illumination with photons with energylarger than the bandgap.

Generation Currents: p-n Junctions Illuminated With Light

For a reverse biased junction, equation 4.3.15 can be understood as follows. Any minoritycarrier electrons generated within a diffusion length of the depletion edge can diffuse to the edge

4.8. DIODE APPLICATIONS: AN OVERVIEW 185

RL

Variable current source controlled

by light, voltage, etc.

I

V

III

III IV

PHOTODETECTOR SOLAR CELL

Figure 4.24: Simple circuit diagram (left) and current-voltage (I − V ) plot showing regimes ofoperation for a p − n diode under illumination. When operated in quadrant III, the device actsas a photodetector, whereas in quadrant IV it behaves as a solar cell

of the junction and be swept away. Minority electrons generated well beyond a length Ln willrecombine with holes resulting in the equilibrium concentration, np0. Similarly holes generatedwithin, Lp, a diffusion length, of the depletion region edge will be swept into the depletionregion.

In the event that there is light shining on the p-n junction, as shown in figure 4.25a, then thecharge profile is perturbed in the following manner. Far in the bulk region, an excess minoritycarrier concentration is generated, where Δnp = GLτn and Δpn = GLτp. This is shown infigure 4.25b. The new equation to be solved for reverse saturation current differs from the onepreviously used in that a light generation term is added.

Dpd2p

dx2+ Gth − R + GL = 0 (4.8.1)

or

Dpd2p

dx2+

pn0 − pn

τp+ GL = 0 (4.8.2)

with boundary conditions similar to before.

pn(∞) = pn0 + τpGL (4.8.3)

pn(Wn) = 0 (4.8.4)

Solving these equations, we get

pn(x) = (pn0 + τpGL)

[1 − exp

(−x − Wn

Lp

)](4.8.5)

186 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

np

0 wn-wp

pn0np0

0 Wn-Wp

x

LpLn

ΔpnΔnp

(a)

(b)

V

J

GL=0

increasing GL

(c)

Figure 4.25: (a) Schematic diagram of a reverse-biased p-n junction illuminated with light. (b)Minority carrier profile in the structure. (c) Reverse bias current increases as the light intensityis increased.

4.8. DIODE APPLICATIONS: AN OVERVIEW 187

A similar set of equations for electrons gives us the following expression for np(x) in the neutralp-region:

np(x) = (np0 + τnGL)

[1 − exp

(x + Wp

Ln

)](4.8.6)

The slope of the charge profile at the edge of the depletion region is

dpn(Wn)

dx=

pn0 + τpGL

Lp(4.8.7)

Therefore

Jp(x = Wn) = eDp

(pn0 + τpGL

Lp

)(4.8.8)

Similarly,

Jn(x = Wp) = eDn

(np0 + τnGL

Ln

)(4.8.9)

The reverse saturation current JR is then given by

JR = e

[Dn

np,bulk

Ln+ Dp

pn,bulk

Lp

](4.8.10)

where np,bulk(pn,bulk) is the minority carrier concentration in the bulk in non-equilibrium (steadystate). Here np,bulk = np0 + τnGL. By changing the slope of the minority profile at the edgeof the junction, such as by shining light on the diode, it is possible to control the reverse cur-rent across the diode. This is shown schematically in figure 4.25c. Controlling and monitoringthe current flowing across a reverse bias diode forms the basis of a large number of devices,including photodetectors and bipolar transistors. As the incident light intensity is enhanced, orequivalently the electron-hole pair generation rate is increased, the reverse current increases asis shown schematically in figure 4.24, where the I − V plane is demarcated into four quadrants.The photodetector operation is in the third quadrant. Notice here that the current and voltagehave the same sign (negative) and hence the device dissipates power (a positive product of cur-rent and voltage). However, if a positive voltage is applied to the diode while light is incident onthe junction then the sign of the current is negative and the sign of the voltage across the diodeis positive. This results in a negative product of current and voltage or the diode is a source ofpower and not a dissipater of power. This is the regime of operation of the solar cell and is inthe fourth quadrant of the I − V plane. The current characteristic is best analyzed by employingthe rule that the current through the diode is always the sum of forward and reverse currents. Inthe absence of any energy source (other than thermal) carriers contributing to both forward andreverse currents are generated thermally (either by the thermal ionization of dopants, or band-to-band generation). At zero bias these currents balance each other. In a solar cell under opticalexcitation the forward current is unchanged and continues to be provided by the thermal injectionof carriers across the junction (as has been described before) whereas the reverse current changesdramatically and is carried dominantly by photo-generated carriers. This is the reason why thenet current is not zero at zero applied bias in an illuminated solar cell. This current is called

188 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

p n

RL

Isc

ID

I = Isc - ID

G

RLIsc

ID I = Isc - ID

D LV IR=

Figure 4.26: Equivalent circuit of a solar cell

the short circuit current, Isc. The forward voltage increases the forward thermionic/diffusioncurrents exponentially as given by the diode law whereas the reverse current remains a constantwith the net current being given by

J · A = I = If − Ir = Is

[exp

(eV

kBT

)− 1

]− Isc (4.8.11)

4.8. DIODE APPLICATIONS: AN OVERVIEW 189

In a solar cell configuration the forward bias is not explicitly applied across the cell. It isgenerated by the flow of the current across the load (which may be the resistance of a light bulbfor instance). This is shown schematically in figure 4.26 along with the equivalent circuit of thesolar cell. The total cell current goes to zero at a voltage, Voc, termed the open circuit voltage,when the forward diode current is equal and opposite to the generated current. From equation4.8.11

Voc =kBT

eln

(Isc

Is+ 1

)To obtain the maximum power from a cell it is desirable to have the largest product of voltageand current possible in the fourth quadrant of the I−V plane. The maximum power point is thatbias at which the maximum power is available from the cell, or, is the bias at which the largestrectangle can be accommodated within the I-V curve. The power at any bias point is given bythe IV product

P = I · V = (Isc − ID) · V =

[Isc − Is exp

(eV

kBT

)]· V

and the maximum power point is obtained by maximizing the product. This is left as an exercise.The maximum power is also alternately represented by

P = VocIsc · F

where F is the defined as the Fill Factor of the cell. Hence to get the maximum power from a cellit is desirable to obtain the largest Voc and Isc possible which is best achieved by using a tandemcell which comprise of a series connection of cells with different bandgaps that maximize solarabsorption (while maintaining a large open circuit voltage) coupled with concentrator lenses thatmaximize input photon intensity.

4.8.3 The uses of diode non-linearity (Mixers, Multipliers, Power Detec-tors)

A mixer is a frequency translation device that translates an input signal band of frequencies toa different band of output frequencies. There are two main uses of the mixer: down conversionand up conversion. Down conversion, used in receivers, takes a higher input RF frequency andshifts it down to a lower frequency where the channel selection can be performed and interferingsignals can be filtered out. Up conversion takes a lower frequency band limited signal and shiftsit to a higher frequency. This is typically the transmitter application.

A mixer does not really “mix” or sum signals; it multiplies them. For example, the analogmultiplier performs the frequency translation function:

A = A sin ω1t B = B sin ω2t

(A sin ω1t)(B sin ω2t) = (AB/2) [cos(ω1 − ω2)t − cos(ω1 + ω2)t] (4.8.12)

Note that both sum and difference frequencies are obtained by the multiplication of the two

190 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

A

B

AB(Signal)

(Local Oscillator)

(Output to load)

Figure 4.27: Mixer symbol. A represents the signal input; B the reference input.

input sinusoidal signals as shown in equation 4.8.12. One of these is the input signal (A) whoseamplitude and phase generally vary with time. The other input (B) is a reference signal, locallygenerated, called the local oscillator, normally with fixed amplitude and phase. With the idealanalog multiplication process shown in figure 4.27, no harmonics or spurious signals are pro-duced. Also, there is no feed through of A or B to the output. But, in reality, mixers alwaysproduce many spurious outputs that consist of harmonics of A and B and additional mixingproducts mω1 ± nω2, where m and n are integers. A “good” mixer is designed such that itsuppresses these spurious outputs and provides a highly linear amplitude and phase relationshipbetween signal input (A) and the output.

The forward I-V characteristic of the diode can be represented by a series expansion. Forexample, in the case of a simple exponential diode characteristic, equation 4.8.13 can representthe current voltage characteristic. Coefficients ai will vary with DC bias, series resistance, andthe shape of the I − V characteristic.

ID = IS

[exp

(eVD

kBT )

)− 1

] IS

[a1VD +

1

2a2V

2D +

1

6a3V

3D + . . .

](4.8.13)

VRF + VLO − VD − IS

(a1VD +

1

2a2V

2o

)(RS + RL) = 0

Vo(t) = IS(a1VD +1

2a2V

2D)RL

a2V2D sin2 ωt = a2V

2D [1 − cos 2ωt] (4.8.14)

Now, suppose that two inputs are summed as shown in figure 4.27 and the diode current producesan output Vo(t) across resistor RL. One input VRF is the signal; the other VLO is the referencelocal oscillator. The diode voltage, VD, can be found using the series approximation equation4.8.13, and the output voltage, Vo(t), is calculated from the diode current ID. If only first andsecond order terms are used, a quadratic equation is easily solved.

While only the outputs shown in equation 4.8.12 are desired, the mixer output will also containa DC term, RF and LO feed through, and terms at all harmonics of the RF and LO frequencies.Only the second-order product term produces the desired outputs. It can be seen in equation

4.8. DIODE APPLICATIONS: AN OVERVIEW 191

4.8.14 that the second-order nonlinearity also produces a second harmonic and a DC term. Thesecond harmonic generation is the property used in frequency multipliers. Also, the DC termamplitude is proportional to the square of the input voltage, hence input power. This is theprinciple of operation of diode power detectors.

4.8.4 Power Devices

A DC-to-DC converter is a module that accepts a DC input voltage and produces a DC outputvoltage typically at a different voltage level or of different polarity. These modules have becomeubiquitous in modern electronic systems. For example, laptops use them to convert the mainspower supply voltage to the battery voltage (18 V), which in turn is converted to the supplyvoltage for the computing electronics (1.5-3.5 V) and the voltage for the display (voltage variabledepending on type of display). All are different! In addition, DC-to-DC converters are used toprovide bus isolation, power bus regulation, etc. There are several topologies to achieve thedesired conversion and we will briefly discuss a Buck or Step- Down Converter to appreciate thefunctional requirements of the transistor switch and diode that this employed. As in most powerconversion circuits it is imperative to not have current flow with a large voltage across dissipativeelements such as transistor switches. This will cause power dissipation and excessive heating inthe circuit. To reduce the voltage across a switch while it is conducting, an inductor is typicallyemployed in circuits. Furthermore a capacitor is used at the output to stabilize the output voltagethrough the switching cycle. In the Buck/Step-Down circuit (figure 4.28), an input transistor isturned on causing the input voltage Vin (which has to be stepped-down) to appear at one end ofthe inductor while the other remains at the output. This voltage will cause the inductor current torise, storing energy as magnetic flux. During this process the diode is reverse biased and turnedoff and the current flows through the transistor and the inductor to the output capacitor and load.When the transistor is turned off, the current through the inductor will continue flowing but nowbe forced through the diode causing the diode to turn on. This process is called free-wheeling.The voltages Vx and Vo will follow standard L and C charging/discharging relationships asshown in figure 4.28.

Figure 4.28 shows schematically the change in the current and voltage across the inductor overa switching cycle of the transistor. From the relation

Vx − Vo = Ldi

dt(4.8.15)

the change of current satisfies

if − ii =

∫ON

(Vx − Vo) dt +

∫OFF

(Vx − Vo) dt (4.8.16)

where ii and if are the currents through the inductor at the beginning and the end of a cycle.For steady state operation it is required that the current at the start and end of a period T be thesame. To get a ’simple relation’ between voltages we assume ’no voltage drop across transistoror diode’ while ON and a perfect switch change. Thus during the ON time Vx = Vin and in the

192 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

VinVO

Input Output

C

LVx IL

Time

Vx

Inductor

current

T

ton toff

(a)

(b)

Figure 4.28: (a)Buck converter schematic (b) Voltage and current changes

OFF time Vx = 0. Thus in steady state

if − ii = 0 =

∫ tON

0

(Vin − Vo) dt +

∫ tON+tOFF

tON

(−Vo) dt (4.8.17)

which gives(Vin − Vo) tON − VotOFF = 0 (4.8.18)

orVo

Vin=

tON

T(4.8.19)

Using D as the “duty cycle” gives

D =tON

T(4.8.20)

the voltage relationship becomes Vo = DVin. Since the circuit is ’lossless’ and the inputand output powers must match on the average VoIo = VinIin . This requires the diode to

4.9. LIGHT EMITTING DIODE (LED) 193

have no voltage drop in the forward direction and no leakage current in the reverse direction.In the presence of a reverse leakage current Irev , additional loss of IrevVin occurs in the free-wheeling diode when the transistor is ON; and if the forward diode drop is non- negligible,IoVdiode will be lost in the diode when the transistor is OFF. Both these losses are importantsince in the first case Vin is large and in the second Io is large. It is imperative that in theseapplications the device behave as a nearly- perfect diode with Vdiode and Irev both being assmall as possible. Furthermore, the diode should switch off faster than the transistor, to reducetransient dissipation in it. Schottky diodes which are unipolar and have short switching times areemerging as preferred diodes in free-wheeling applications.

One of the most important applications is in the area of optoelectronic devices. Essentiallyall the semiconductor devices catering to optoelectronics use the diode concept. These includedetectors, avalanche photodetectors, optical modulators, as well as light-emitting diodes andsemiconductor lasers. In this section we discuss the operation of the light emitting diode

4.9 Light emitting diode (LED)

The simplicity of the light-emitting diode (LED) makes it a very attractive device for displayand communication applications. The basic LED is a p-n junction that is forward biased toinject electrons and holes into the p- and n-sides respectively. The injected minority chargerecombines with the majority charge in the depletion region or the neutral region. In directband semiconductors, this recombination leads to light emission since radiative recombinationdominates in high-quality materials. In indirect gap materials, the light emission efficiency isquite poor and most of the recombination paths are nonradiative, which generates heat ratherthan light. In the following section we will examine the important issues that govern the LEDoperation.

We will briefly outline some of the important considerations in choosing a semiconductor forLEDs or laser diodes.

4.9.1 Emission Energy

The light emitted from the device is very close to the semiconductor bandgap, since the in-jected electrons and holes are described by quasi-Fermi distribution functions. The desire for aparticular emission energy may arise from a number of motivations. In figure 4.29 we show theresponse of the human eye to radiation of different wavelengths. Also shown are the bandgapsof some semiconductors. If a color display is to be produced that is to be seen by people, one hasto choose an appropriate semiconductor. Very often one has to choose an alloy, since there is agreater flexibility in the bandgap range available. In figure 4.30 we show the loss characteristicsof an optical fiber. As can be seen, the loss is least at 1.55 μm and 1.3 μm. If optical communi-cation sources are desired, one must choose materials that can emit at these wavelengths. Thisis especially true if the communication is long haul, i.e., over hundreds or even thousands ofkilometers. InP-based materials are used for these applications. Materials like GaAs that emit at0.8 μm can still be used for local area networks (LANs), which involve communicating withina building or local areas. The area of displays and lighting is filled dominantly by GaN-based

194 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

InSb PbS Ge Si GaAs CdSe GaP CdS SiC GaN ZnS

GaAs1-yPyHgCdTe

Infrared Red Green Violet Ultraviolet

Orange Yellow Blue

λ (µm)

Human eye repsonse

Eg (eV)

0.0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 1.8 2.0 2.2 2.4 2.6 2.8 3.0 3.2 3.4 3.6

6.0 3.0 2.0 1.5 1.0 0.9 0.8 0.7 0.6 0.5 0.45 0.4 0.35

CdTe

Figure 4.29: The bandgap and cutoff wavelengths for several semiconductors. The semiconduc-tor bandgaps range from 0 (for Hg0.84Cd0.15Te) to well above 3 eV, providing versatile detectionsystems.

materials using InGaN as the emission region for blue and green and GaAs-based AlGaInP forthe red region.

Substrate Availability:

Almost all optoelectronic light sources depend upon epitaxial crystal growth techniques wherea thin active layer (a few microns) is grown on a substrate (which is ∼ 200 μm). The availabil-ity of a high-quality substrate is extremely important in epitaxial technology. If a substrate thatlattice-matches to the active device layer is not available, the device layer may have dislocationsand other defects in it. These can seriously hurt device performance. One of the most importantopto-electronic materials for LEDs that has emerged lately is GaN. In spite of the lack of a nativesubstrate, GaN-based LEDs grown on either sapphire or SiC have become multi-billion dollarindustry. The reason is that the InGaN quantum well which is used as the emission region hasfluctuations which cause local energy minima for electron and holes. Thus radiative recombi-nation is encouraged within this region and diffusion to and non-radiative recombination at adislocation minimized. This is shown schematically in figure 4.31. Furthermore, the dislocationpropagation and generation of dislocation sin GaN is very high because of the high bond energiesin the material. This eliminates one of the failure mechanisms in conventional LEDs and lasers,that of generation and propagation of dislocations caused by absorption of emitted the photonenergy. The important substrates that are available for conventional light-emitting technology

4.9. LIGHT EMITTING DIODE (LED) 195

0.6 0.8 1.0 1.2 1.4 1.6 1.8 2.0

100

50

20

10

5

2

1

0.5

0.2

0.1

0.05

–OH absorption peaks

Infrared absorption tail from lattice transitions

Rayleigh scattering

FIB

ER

AT

TE

NU

AT

ION

(dB

km

–1)

WAVELENGTHS, MICRONS

1.55 μm loss ~ 0.2 dB/km1.3 μm loss ~ 0.5 dB/km

Figure 4.30: Optical attenuation vs. wavelength for an optical fiber. Primary loss mechanismsare identified as absorption and scattering.

(which do not benefit from the above mentioned advantages of GaN and InGaN) are GaAs andInP. A few semiconductors and their alloys can match these substrates. The lattice constant of analloy is the weighted mean of the lattice constants of the individual components, i.e., the latticeconstant of the alloy AxB1−x is

aall = xaA + (1 − x)aB (4.9.1)

where aA and aB are the lattice constants of A and B. Semiconductors that cannot lattice-matchwith GaAs or InP have an uphill battle for technological success. The crystal grower must learnthe difficult task of growing the semiconductor on a mismatched substrate without allowingdislocations to propagate into the active region.

Important semiconductor materials exploited in optoelectronics are the alloy GaxAl1−xAs,and AlGaInP which is a quaternary material which is lattice-matched very well to GaAs sub-strates; In0.53Ga0.47As and In0.52Al0.48As, which are lattice-matched to InP; InGaAsP, whosecomposition can be tailored to match with InP and can emit at 1.55 μm; and GaAsP, which hasa wide range of bandgaps available.

196 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

hv

Substrate

p

n

hv

Substrate

p

n

hvhv

Dislocations

(a) (b)

Figure 4.31: (a) e-h diffuse to dislocations and recombine. (b) In the presence of energy fluctu-ations such as in the InGaN the electrons recombine efficiently.

In general, the electron-hole recombination process can occur by radiative and nonradiativechannels. Under the condition of minority carrier recombination or high injection recombination,as shown in section 3.8.1and section 3.8.2, one can define a lifetime for carrier recombination. Ifτr and τnr are the radiative and nonradiative lifetimes, the total recombination time is (for, say,an electron)

1

τn=

1

τr+

1

τnr(4.9.2)

The internal quantum efficiency for the radiative processes is then defined as

ηQr =1τr

1τr

+ 1τnr

=1

1 + τr

τnr

(4.9.3)

In high-quality direct gap semiconductors, the internal efficiency is usually close to unity. Inindirect materials the efficiency is of the order of 10−2 to 10−3.

Before starting the discussion of light emission, let us remind ourselves of some importantdefinitions and symbols used in this chapter:

Iph : photon current = number of photons passing a cross-section/second.

Jph : photon current density = number of photons passing a unit area/second.

Pop : optical power intensity = energy carried by photons per second per area.

4.9. LIGHT EMITTING DIODE (LED) 197

EC

EF

EV

Eg Emission

tQW

Figure 4.32: Band diagram of a single quantum-well LED with the advantages of increased car-rier density, enhanced confinement and reduced probability of re-absorption of emitted photonsin bulk layers.

4.9.2 Carrier Injection and Spontaneous Emission

The LED is essentially a forward-biased p-n diode, with a quantum well emission region asshown in figure 4.32. The reason for using a quantum well is to (i) increase the electrons andhole density in the recombination region increasing the direct recombination rate and leadingto higher light output, (ii) having an emission region that is lower in energy that the injection(cladding) regions which allows the generated photons to escape without being re-absorbed in theinjection regions, (iii) minimizing the overflow of electrons into the cladding regions where theinjected carriers either recombine non-radiatively or generate light of an undesired wavelength.The current flow in a p-n junction was discussed in detail earlier in this chapter.The basis ofthat derivation was that electrons and holes are injected across the junction and recombine eitherin the bulk(long base case) or at contacts (short base case). Neither of those conditions applyto an LED. Here the current flow occurs via recombination in the quantum well. The turn-onvoltage of the LED is therefore given by the bandgap of the emission region and is not explicitlyrelated to the built-in voltage of the p-n junction. An example of this is an InGaN LED grownwithin GaN p-and n regions. The built-in voltage of this device is close to the bandgap of GaN(3.4V) though the turn-on voltage is 2.8V close to the emission energy of the photons. Thecurrent flow mechanism is shown in figure 4.33. The current is given by J = e · Rspon whereRspon is the spontaneous recombination rate in the well. The efficiency of the process is the

198 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

EC

EFp

EV

hvEFn

Jparasitic

(recombination

in junction)

Jn parasitic injection

Jp parasitic injection

J = Jparasitic + eRspon tQW

Figure 4.33: Current flow mechanisms in a LED.

ratio of the current generating photons of the desired wavelength to the total current. The currentcalculated for the p-n junction in the earlier sections are the wasted currents in the LED as theycalculate currents in the bulk and due to non-radiative centers. What remains to be calculated isthe spontaneous recombination rate Rspon.a

As discussed in section 3.8.1, the radiative process is “vertical,” i.e., the k-value of the elec-tron and that of the hole are the same in the conduction and valence bands, respectively. Fromfigure 4.34 we see that the photon energy and the electron and hole energies are related by

�ω − Eg =�

2k2

2

[1

m∗e

+1

m∗h

]=

�2k2

2m∗r

(4.9.4)

where m∗r is the reduced mass for the e-h system.

If an electron is available in a state k and a hole is also available in the state k (i.e., if the Fermifunctions for the electrons and holes satisfy fe(k) = fh(k) = 1), the radiative recombination rateis found to be

Wem ∼ 1.5 × 109�ω [eV s−1] (4.9.5)

4.9. LIGHT EMITTING DIODE (LED) 199

CONDUCTION

BAND

VALENCE

BAND

Eg

Ec

Ev

k

h2k2

2m*

h2k2

2m*

hω

e

h

Figure 4.34: A schematic of the E-k diagram for the conduction and valence bands. Opticaltransitions are vertical; i.e., the k-vector of the electron in the valence band and in the conductionband is the same.

and the recombination time becomes (�ω is expressed in electron volts)

τo =0.67

�ω[eV]ns (4.9.6)

The recombination time discussed above is the shortest possible spontaneous emission timesince we have assumed that the electron has a unit probability of finding a hole with the samek-value.

When carriers are injected into the semiconductors, the occupation probabilities for the elec-tron and hole states are given by the appropriate quasi-Fermi levels. The emitted photons leavethe device volume so that the photon density never becomes high in the e-h recombination re-gion. In a laser diode the situation is different, as we shall see later. The photon emission rate isgiven by integrating the emission rate Wem over all the electron-hole pairs after introducing theappropriate Fermi functions.

200 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

There are several important limits of the spontaneous rate:

i. In the case where the electron and hole densities n and p are small (non degenerate case),the Fermi functions have a Boltzmann form (exp(−E/kBT )). The recombination rate isfound to be

Rspon =1

2τo

(2π�

2m∗r

kBTm∗em

∗h

)3/2

np (4.9.7)

The rate of photon emission depends upon the product of the electron and hole densities.If we define the lifetime of a single electron injected into a lightly doped (p = Na ≤1017cm−3) p-type region with hole density p, it would be given from equation 4.9.7 by

Rspon

n=

1

τr=

1

2τo

(2π�

2m∗r

kBTm∗em

∗h

)3/2

p (4.9.8)

The time τr in this regime is very long (hundreds of nanoseconds), as shown in figure 4.35,and becomes smaller as p increases.

ii. In the case where electrons are injected into a heavily doped p-region (or holes are injectedinto a heavily doped n-region), the function fh(fe) can be assumed to be unity. Thespontaneous emission rate is

Rspon ∼ 1

τo

(m∗

r

m∗h

)3/2

n (4.9.9)

for electron concentration n injected into a heavily doped p-type region and

Rspon ∼ 1

τo

(m∗

r

m∗e

)3/2

p (4.9.10)

for hole injection into a heavily doped n-type region.

The minority carrier lifetimes (i.e., n/Rspon) play a very important role not only in LEDsbut also in diodes and bipolar devices. In this regime the lifetime of a single electron (hole)is independent of the holes (electrons) present since there is always a unity probability thatthe electron (hole) will find a hole (electron). The lifetime is now essentially τo, as shownin figure 4.35.

iii. Another important regime is that of high injection, where n = p is so high that one canassume fe = fh = 1 in the integral for the spontaneous emission rate. The spontaneousemission rate is

Rspon ∼ n

τo∼ p

τo(4.9.11)

and the radiative lifetime (n/Rspon = p/Rspon) is τo.

4.9. LIGHT EMITTING DIODE (LED) 201

10–5

10–6

10–7

10–8

10–9

10–101014 1015 1016 1017 1018

Nd (for holes injected into an n-type semiconductor)

n = p (for excess electron-hole pairs injected into a region)

RA

DIA

TIV

EL

IFE

TIM

E (

τ r)(

s) Typical carrier densities for laser

operation

Low injection regime

τ o

Carrier occupation is degenerate fe = fh = 1

Semiconductor GaAs Temperature is 300 K

1019cm–3

Figure 4.35: Radiative lifetimes of electrons or holes in a direct gap semiconductor as a functionof doping or excess charge. The figure gives the lifetimes of a minority charge (a hole) injectedinto an n-type material. The figure also gives the lifetime behavior of electron-hole recombina-tion when excess electrons and holes are injected into a material as a function of excess carrierconcentration.

iv. A regime that is quite important for laser operation is one where sufficient electrons andholes are injected into the semiconductor to cause “inversion.” As will be discussed later,this occurs if fe + fh ≥ 1. If we make the approximation fe ∼ fh = 1/2 for all theelectrons and holes at inversion, we get the relation

Rspon ∼ n

4τo(4.9.12)

or the radiative lifetime at inversion is

τ ∼ τo

4(4.9.13)

This value is a reasonable estimate for the spontaneous emission rate in lasers near thresh-old.

202 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

The radiative recombination depends upon the radiative lifetime τr and the non-radiative lifetimeτnr. To improve the efficiency of photon emission one needs a value of τr as small as possibleand τnr as large as possible. To increase τnr one must reduce the material defect density. Thisincludes improving surface and interface qualities.

The LED current is then given by

J = eRspontQW + J0 exp

[e(Vbi − Vturnon)

)kBT

]+ JSNS

The parasitic currents are the second and third terms in the expression. The second term repre-sents current injected over the barrier and the third term the current recombining at the maximumrecombination plane.

Example 4.5 Calculate the e-h recombination time when an excess electron and holedensity of 1015cm−3 is injected into a GaAs sample at room temperature.

Since 1015 cm−3 or 1021 m−3 is a very low level of injection, the recombination time isgiven by equation 4.9.8 as

1

τr=

1

2τo

(2π�

2m∗r

kBTm∗em

∗h

)3/2

p

=1

2τo

(2π�

2

kBTm∗e + m∗

h

)3/2

p

Using τo = 0.6 ns and kBT = 0.026 eV, we get for m∗e = 0.067 mo,m

∗h = 0.45 mo,

1

τr=

1021 m−3

2 × (0.6 × 10−9 s)

[2 × 3.1416 × (1.05 × 10−34 Js)2

(0.026 × 1.6 × 10−19 J) × (0.517 × 9.1 × 10−31 kg)

]3/2

τr = 5.7 × 10−6s ∼= 9.5 × 103τo

We see from this example that at low injection levels, the carrier lifetime can be very long.Physically, this occurs because at such a low injection level, the electron has a very smallprobability of finding a hole to recombine with.

Example 4.6 In two n+p GaAs LEDs, n+ � p so that the electron injection efficiency is100% for both diodes. If the nonradiative recombination time is 10−7s, calculate the300 K internal radiative efficiency for the diodes when the doping in the p-region for thetwo diodes is 1016 cm−3 and 5 × 1017 cm−3.

When the p-type doping is 1016 cm−3, the hole density is low and the e-h recombinationtime for the injected electrons is given by equation 4.9.8 as

1

τr=

1

2τo

(2π�

2m∗r

kBTm∗em

∗h

)3/2

p

4.9. LIGHT EMITTING DIODE (LED) 203

From the previous example, we can see that for p equal to 1016 cm−3, we have (in theprevious example the value of p was ten times smaller)

τr = 5.7 × 10−7 s

In the case where the p-doping is high, the recombination time is given by the high-densitylimit (see equation 4.9.10) as

1

τr=

Rspon

n=

1

τo

(m∗

r

m∗h

)3/2

τr =τo

0.05∼ 20τo ∼ 12 ns

For the low-doping case, the internal quantum efficiency for the diode is

ηQr =1

1 + τr

tnr

=1

1 + (5.7)= 0.15

For the more heavily doped p-region diode, we have

ηQr =1

1 + 10−7

20×10−9

= 0.83

Thus there is an increase in the internal efficiency as the p doping is increased.

Example 4.7 Consider a GaAs p-n diode with the following parameters at 300 K:

Electron diffusion coefficient, Dn = 30 cm2/V · sHole diffusion coefficient, Dp = 15 cm2/V · sp-side doping, Na = 5 × 1016 cm−3

n-side doping, Nd = 5 × 1017 cm−3

Electron minority carrier lifetime, τn = 10−8 sHole minority carrier lifetime, τp = 10−7 s

Calculate the injection efficiency of the LED assuming no recombination due to traps.

The intrinsic carrier concentration in GaAs at 300 K is 1.84 × 106 cm−3. This gives

np =n2

i

Na=

(1.84 × 106)2

5 × 1016= 6.8 × 10−5 cm−3

pn =n2

i

Nd=

(1.84 × 106)2

5 × 1017= 6.8 × 10−6 cm−3

The diffusion lengths are

Ln =√

Dnτn =[(30)(10−8)

]1/2= 5.47 μm

Lp =√

Dpτp =[(15)(10−7)

]1/2= 12.25 μm

204 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

The injection efficiency is now (assuming no recombination via traps)

γinj =

eDnnpo

Ln

eDnnpo

Ln+

eDppno

Lp

= 0.98

Example 4.8 Consider the p-n+ diode of the previous example. The diode is forwardbiased with a forward-bias potential of 1 V. If the radiative recombination efficiency ηQr =0.5, calculate the photon flux and optical power generated by the LED. The diode area is1 mm2.

The electron current injected into the p-region will be responsible for the photongeneration. This current is

In =AeDnnpo

Ln

[exp

(eV

kBT

)− 1

]=

(10−2 cm2)(1.6 × 10−19 C)(30 cm2/s)(6.8 × 10−5 cm−3)

5.47 × 10−4 cm

[exp

(1

0.026

)− 1

]= 0.30 mA

The photons generated per second are

Iph =In

e· ηQr =

(0.30 × 10−3 A)(0.5)

1.6 × 10−19 C

= 9.38 × 1014 s−1

Each photon has an energy of 1.41 eV (= bandgap of GaAs). The optical power is thus

Power = (9.38 × 1014 s−1)(1.41)(1.6 × 10−19 J)

= 0.21 mW

4.10 PROBLEMS

• Section 4.2

Problem 4.1 Why does the potential in a p-n diode fall mainly across the depletion regionand not across the neutral region?

Problem 4.2 An abrupt GaAs p-n diode has Na = 1017 cm−3 and Nd = 1015 cm−3.(a) Calculate the Fermi level positions at 300 K in the p and n regions.(b) Draw the equilibrium band diagram and determine the contact potential Vbi.

Problem 4.3 Consider an Si p-n diode doped at Na = 1017 cm−3;Nd = 5 × 1017 cm−3

at 300 K. Plot the band profile in the neutral and depletion region. Also, plot the electronand hole concentration from the p- to the n-sides of equilibrium. How good is thedepletion approximation?

4.10. PROBLEMS 205

Problem 4.4 Consider the sample discussed in problem 4.2. The diode has a diameter of50 μm. Also calculate the charge in the depletion regions and plot the electric field profilein the diode.

Problem 4.5 An abrupt silicon p-n diode at 300 K has a doping ofNa = 1018 cm−3, Nd = 1015 cm−3. Calculate the built-in potential and the depletionwidths in the n and p regions.

Problem 4.6 A Ge p-n diode has Na = 5 × 1017 cm−3 and Nd = 1017 cm−3. Calculatethe built-in voltage at 300 K. At what temperature does the built-in voltage decrease by1%?

Problem 4.7 Consider a p-n junction with NA = ND = 1017cm−3. When thecapacitance is measured to be twice the value expected.The reason is an unintentional interfacial dipole between the p and n layers.

1. What is the magnitude of the dipole moment?

2. Draw the band diagrams of the ideal p-n junction and the non-ideal one. Include theelectric field profiles and depletion region widths.

Assume that the dipole is supported by negative and positive charges separated by a verysmall distance, δ.

• Section 4.3

Problem 4.8 Explain, using physical arguments, why the reverse current in a p-n diodedoes not change with bias (before breakdown). Would this be the case if the electrons andholes had a constant mobility independent of the electric field?

Problem 4.9 The diode of problem 4.3 is subjected to bias values of: (a) Vf = 0.1 V; (b)Vf = 0.5 V; (c) Vr = 1.0V; (d) Vr = 5.0 V. Calculate the depletion widths and the maximumfield Fm under these biases.

Problem 4.10 Consider a p+n Si diode with Na = 1018 cm−3 and Nd = 1016 cm−3. Thehole diffusion coefficient in the n-side is 10 cm2/s and τp = 10−7 s. The device area is10−4 cm2. Calculate the reverse saturation current and the forward current at a forwardbias of 0.8 V at 300 K.

Problem 4.11 Consider a p+n silicon diode with area 10−4 cm2. The doping is given byNa = 1018 cm−3 and Nd = 1017 cm−3. Plot the 300 K values of the electron and holecurrents In and Ip at a forward bias of 0.8 V. Assume τn = τp = 1 μs and neglectrecombination effects. Dn = 20 cm2/s and Dp = 10 cm2/s.

Problem 4.12 A GaAs LED has a doping profile of Na = 1017 cm−3, Nd = 1018 cm−3 at300 K. The minority carrier time is τn = 10−8 s; τp = 5 × 10−9 s. The electron diffusioncoefficient is 100 cm2 s−1 while that of the holes is 20 cm2 s−1. Calculate the ratio of theelectron-injected current (across the junction) to the total current.

206 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

Problem 4.13 The diode of problem 4.12 has an area of 1 mm2 and is operated at aforward bias of 1.2 V. Assume that 50% of the minority carriers injected recombine withthe majority charge to produce photons. Calculate the rate of the photon generation in then- and p-side of the diode.

Problem 4.14 Consider a GaAs p-n diode with a doping profile of Na = 1016 cm−3,Nd = 1017 cm−3 at 300 K. The minority carrier lifetimes are τn = 10−7 s; τp = 10−8 s.The electron and hole diffusion coefficients are 150 cm2/s and 24 cm2/s, respectively.Calculate and plot the minority carrier density in the quasi-neutral n and p regions at aforward bias of 1.0 V.

Problem 4.15 Consider a p-n diode made from InAs at 300 K. The doping isNa = 1016 cm−3 = Nd. Calculate the saturation current density if the electron and holedensity of states masses are 0.02mo and 0.4mo, respectively. Compare this value with thatof a silicon p-n diode doped at the same levels. The diffusion coefficients areDn = 800 cm2/s; Dp = 30 cm2/s. The carrier lifetimes are τn = τp = 10−8s for InAs.For the silicon diode use the values Dn = 30 cm2/s; Dp = 10 cm2/s; τn = τp = 10−7s.

Problem 4.16 Consider a p-n diode in which the doping is linearly graded. The doping isgiven by

Nd − Na = Gx

so that the doping is p-type at x < 0 and n-type at x > 0. Show that the electric fieldprofile is given by

E(x) =e

2εG

[x2 −

(W

2

)2]

where W is the depletion width, given by

W =

[12ε (Vbi − V )

eG

]1/3

Problem 4.17 A silicon diode is being used as a thermometer by operating it at a fixedforward-bias current. The voltage is then a measure of the temperature. At 300 K, thediode voltage is found to be 0.6 V. How much will the voltage change if the temperaturechanges by 1 K?

Problem 4.18 Compare the dark currents (i.e., reverse saturation current) in p-n diodesfabricated from GaAs, Si, Ge, and In0.53Ga0.47As. Assume that all the diodes are doped atNd = Na = 1018 cm−3. The material parameters are (300 K):

GaAs : τn = τp = 10−8 s; Dn = 100 cm2/s; Dp = 20 cm2/s

Si : τn = τp = 10−7 s; Dn = 30 cm2/s; Dp = 15 cm2/s

Ge : τn = τp = 10−7 s; Dn = 50 cm2/s; Dp = 30 cm2/s

When p-n diodes are used as light detectors, the dark current is a noise source.

4.10. PROBLEMS 207

Problem 4.19 When we derived the law of the junction, we assumed that the electron andhole quasi-fermi levels were constant across the depletion region. Inherent in thisassumption is another assumption, that the electron and hole mobilities are high enoughthat most reasonable current densities can be provided by a minimum change in thequasi-fermi level across the depletion edge, or ΔEFn is small. Jn = qμnnΔEF n

Δx What ifthis were not true and I had a p-n junction made of a semiconductor where the holemobility was very low? Assuming no recombination in the junction calculate and plot thehole concentration at the edge of the depletion region as a fuction of bias for μp = 10 cm2

V sand compare to the the value obtained from the law of the junction. State yourassumptions.

Problem 4.20 Consider the GaAs diode shown in figure 4.36, where the n-type region hasa small width WN << LP while the p-region is thick.

1. Plot the minority and majority carrier and currents distributions in the n and p regionsof this diode.

2. Now the diode is illuminated leading to an optical generation of 1020cm−3s−1. Plotthe carrier distributions and currents in the n and p regions. Calculate the current inthe diode under forward bias and reverse bias voltages of 0.5 V and −1 Vrespectively. Both sides are doped at 1017cm−3. Assume that there are ohmiccontacts on both sides, and that they have infinite recombination velocities.

WN

n p

WP

Figure 4.36: Figure for problem 4.20.

• Section 4.4

Problem 4.21 Consider a Si p-n diode at 300 K. Plot the I-V characteristics of the diodebetween a forward bias of 1.0 V and a reverse bias of 5.0 V. Consider the following casesfor the impurity-assisted electron-hole recombination time in the depletion region: (a)

208 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

1.0 μs; (b) 10.0 ns; and (c) 1.0 ns. Use the following parameters:

A = 10−3 cm2

Na = Nd = 1018 cm−3

τn = τp = 10−7 s

Dn = 25 cm2/s

Dp = 6 cm2/s

Problem 4.22 Consider a GaAs p-n diode with Na = 1017 cm−3, Nd = 1017 cm−3. Thediode area is 10−3 cm2 and the minority carrier mobilities are (at 300 K)μn = 3000 cm2/V·s; μp = 200 cm2/V·s. The electron-hole recombination times are10−8s (τp = τn = τ). Calculate the diode current at a reverse bias of 5 V. Plot the diodeforward-bias current including generation-recombination current between 0.1 V and 1.0 V.

Problem 4.23 A long base GaAs abrupt p-n junction diode has an area of 10−3 cm2,Na = 1018 cm−3, Nd = 1017 cm−3, τp = τn = 10−8 s, Dp = 6 cm2 s−1 andDn = 100 cm2 s−1. Calculate the 300 K diode current at a forward bias of 0.3 V and areverse bias of 5 V. The electron-hole recombination time in the depletion regions is 10−7s.

Problem 4.24 Two different processes are used to fabricate a Si p-n diode. The firstprocess results in a electron-hole recombination time via impurities in the depletion regionof 10−7 s while the second one gives a time of 10−9 s. Calculate the diode ideality factorsfor the two cases near a forward bias of 0.9 V. Use the following parameters:

Na = Nd = 1018 cm−3

τn = τp = 10−7 s

Dn = 25 cm2/s

Dp = 8 cm2/s

Problem 4.25 Consider a Si diode with the following parameters:

A = 10−3 cm2

Na = Nd = 1018 cm−3

τn = τp = 10−7 s

Dn = 25 cm2/s

Dp = 8 cm2/s

The length of the n- and p-sides are 1.0 μm each and the electron-hole impurity-assistedrecombination time in the depletion region is 10−8 s. Plot the I-V relation of the diodefrom −5.0 V to 1.0 V. Compare the results for the case where a long diode is made fromthe same material technology.

4.10. PROBLEMS 209

Figure 4.37: Diode for problem 4.28.

Problem 4.26 Consider a GaAS p-n junction with NA = ND = 1017cm−3. Assume amid-gap trap in the material that causes the minority carrier lifetime to be 0.1ns. Calculateand plot the electron and hole currents (including the recombination current) in thedepletion region. Explain the features on the graph.

Problem 4.27 Consider a Si p-n junction biased as a solar cell. Light falls on this solarcell leading to optical generation GOP = 1020/s. What is the optically generatedcurrent(IOP ) for the diode? What is the open-circuit voltage(VOC )? Plot the minoritycarrier profiles when the voltage across the junction is VOC , VOC/2 and 0. Considergeneration in the depletion region. Use τp = τn = 10−6s, μn = μp = 1000cm2/V.s andND = NA = 1017.

Problem 4.28 Consider the diode in figure 4.37. A sheet of acceptors of areal density QA

is placed in an intrinsic region of GaAs such that it is at a distance L1 from one n+ regionand L2 from another.(a) Calculate an expression for the potential across the structure in terms of QA, L1, L2,ND and other material parameters of GaAs.(b) Sketch the band diagram for the case where L1 = 0.1 μm, L2 = 0.2 μm, QA =5 × 1011cm−2 and ND = NC . What will the turn-on voltage of the diode be in eachdirection?(c) Calculate the maximum value of QA, QA,MAX that gives the highest turn-on voltage ineach direction/polarity.(d) If I now set QA=2QA,MAX , what will the turn-on voltage of the diode be? Explainwhat happens.

Problem 4.29 Consider a p-i-n junction in AlInAs (Eg = 1.4 eV, ni = 107 cm−2) that isgrown by MOCVD. To prevent the acceptor atoms from diffusing, the temperature of

210 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

Figure 4.38: Diode for problem 4.29.

growth is dropped after growth of the p-layer is completed. The growth is then completedwith an i-layer of thickness Wi and the subsequent n-layer, as shown in figure 4.19. Whenthe capacitance of the diode is measured, it is determined that the diode is actually a p-njunction and not the p-i-n that was designed. The reason is that while waiting for thetemperature to drop after growth of the p-layer, oxygen (a donor) incorporated withdensity qσ cm −2 at the p-i interface, (see figure 4.19).(a) Derive the relation between the doping densities, Wi, and qσ so that the measurementis explained. Assume NA = ND for simplicity.(b) Next, calculate a numerical value for Wi. Assume NA = ND = 1017 cm−3 andqσ = 5 × 1011 cm−2.

• Section 4.5

Problem 4.30 The critical field for breakdown of silicon is 4 ×105 V/cm. Calculate then-side doping of an abrupt p+n diode that allows one to have a breakdown voltage of 30 V.

Problem 4.31 Consider an abrupt p+n GaAs diode at 300 K with a doping ofNd = 1016 cm−3. Calculate the breakdown voltage. Repeat the calculation for a similarlydoped p+n diode made from diamond. Use Appendix B for the data you may need.

Problem 4.32 What is the width of the potential barrier seen by electrons duringband-to-band tunneling in an applied field of 5 × 105 V/cm in GaAs, Si andIn0.53Ga0.47As (Eg = 0.8 V)?

Problem 4.33 Consider an Si p-n diode with Na = 1018 cm−3;Nd = 1018 cm−3.Assume that the diode will break down by Zener tunneling if the peak field reaches106 V/cm. Calculate the reverse bias at which the diode will break down.

Problem 4.34 Punch through diode: For junction diodes that have to operate at highreverse biases, one needs a very thick depletion region. However, in forward-biasconditions this region is undepleted and leads to a series resistance. One uses a p+-n-n+

4.11. DESIGN PROBLEMS 211

structure in such cases. The width of the n-region is smaller than the depletion regionwidth at breakdown.

Consider two Si p+-n-n+ diodes with the n region having a doping of 1014 cm−3. In onecase the n-region is 150 μm long while in the other case it is 80 μm. What are thereverse-bias voltages that the diodes can tolerate before punch through occurs?

• Section 4.8

Problem 4.35 Consider a Si p-n junction where the p and n regions are much shorter thanthe diffusion length. Assume that the doping on both sides is 1017cm−3. Usemp = mn = 1000 cm2

V s , NA = ND = 1017cm−3 and that the neutral region width on eachside is Wn = Wp = 0.1μm Use Eg = 1.1eV,NC = NV = 1019cm−3 and tGEN = 1μs.

1. What is the reverse current in the this diode when no light shines on it? Assume alarge reverse bias, qV >> kT , and room temperature.

2. Now, light incident on the devide leads to an optical EHP generation rateGOP = 1022cm−3s−1. What is the reverse current in the diode? Assume roomtemperature, as before.

3. Now, the temperature of the diode is reduced with the light left on. At whattemperature will the reverse current be equal to that calculated in the first part of theproblem?

4.11 DESIGN PROBLEMS

Problem 4.1 Consider a Si long diode that must be able to operate up to a reverse bias of10 V. The maximum electric field that the diode can tolerate anywhere within the structureis 5 × 105 V/cm. Design the diode so that the reverse current is as small as possible withinthe given specifications. Assume that Na = Nd. What is the doping density you will use?

Problem 4.2 Consider a Si short p-n diode with the following parameters:

n-side length = 2.0 × 10−4 cm

p-side length = 2.0 × 10−4 cm

n-side doping = 1017 cm−3

p-side doping = 1017 cm−3

minority carrier lifetime τn = τp = 10−7 s

electron diffusion constant = 25 cm2/s

hole diffusion constant = 10 cm2/s

diode area = 10−3 cm2

Calculate the diode current (assuming that the diode is non-ideal) at a forward bias of 0.1V and at 0.7 V at 300 K. What are the diode ideality factors near the two biasing values?

212 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

Problem 4.3 Give a short discussion on why the reverse-bias current in an ideal p-n diodehas no voltage dependence. Discuss also the voltage dependence of the reverse-biascurrent in a non-ideal diode (i.e., a diode with defects).

Problem 4.4 Consider a Si short (or narrow) p-n diode with the following parameters:

n-side thickness = 3.0 μ/m

p-side thickness = 4.0 μ/m

n-side doping = 1018 cm−3

p-side doping = 1018 cm−3

minority carrier lifetime τn = τp = 10−7 s

electron diffusion constant = 30 cm2/s

hole diffusion constant = 10 cm2/s

diode area = 10−4 cm2/s

Calculate the diode current at a forward bias of 0.5 V at 300 K. Also calculate the totalexcess hole charge (in coulombs) injected into the n-side (from Wn to the diode n-sidecontact) at this biasing.

Problem 4.5 Consider a Si long p-n diode with the following parameters:

n-side doping = 1018 cm−3

p-side doping = 1018 cm−3

minority carrier lifetime τn = τp = 10−7 s

electron diffusion constant = 30 cm2/s

hole diffusion constant = 10 cm2/s

diode area = 10−4 cm2/s

Calculate the diode current at a forward bias of 1.0 V at 300 K.

An electron comes from the p-side into the depletion region and is swept away by the fieldto the n-side. Estimate the time it takes the electron to cross the depletion region at zeroapplied bias and a reverse bias of 1.0 volt.

Problem 4.6 Consider a Si long p-n diode with the following parameters:

n-side doping = 1017 cm−3

p-side doping = 1017 cm−3

minority carrier lifetime τn = τp = 10−7 s

electron diffusion constant = 30 cm2/s

hole diffusion constant = 10 cm2/s

diode area = 10−4 cm2

carrier lifetime in the depletion region = 10−8 s

4.11. DESIGN PROBLEMS 213

Calculate the diode current at a forward bias of 0.5 V and 0.6 V at 300 K. What is theideality factor of the diode in this range?

Problem 4.7 Consider a narrow diode with the same parameters as given above. Calculatethe total electron- and hole-injected charge in the n- and p- sides at a forward bias of 0.4 V.The widths of the n- and p-sides are both 1.0 μm.

Problem 4.8 Discuss how a p-n diode can be used as a temperature sensor. Assuming anideal Si p-n diode, calculate the value of x and y where

x =1

Io

dIo

dT, y =

1

I

dI

dT

In real diodes the value of x and y is smaller than what is expected for an ideal diode.Discuss the reason for this.

Problem 4.9 Assume that a Si diode suffers Zener breakdown at a field of 2×105 V/cm ifboth n- and p-sides are doped above 1018 cm−3. Design a diode that suffers Zenerbreakdown at a reverse bias of 5 V. Draw the I-V characteristics for this diode assumingreasonable material parameters.

Problem 4.10 Consider a 20 μm diameter p-n diode fabricated in silicon. The donordensity is 1016 cm−3 and the acceptor density is 1018 cm−3. Calculate the following inthis diode at 300 K: i) The depletion widths and the electric field profile under reversebiases of 0, 2, 5, and 10 V, and under a forward bias of 0.5 V. ii) What are the charges inthe depletion region for these biases?

Problem 4.11 Consider the diode discussed in design problem 4.10. Calculate the averagefield in the depletion region at the four reverse-bias values considered. Calculate thevelocity of the electrons at these average fields using the velocity-field results given inchapter 3 What can be said about the change in the drift components of the diode currentwith the change in bias?

Problem 4.12 Consider an ideal diode model for a silicon p-n diode withNd = 1016 cm−3 and Na = 1018 cm−3. The diode area is 10−3 cm2.

The transport properties of the diode are given by the following values at 300 K:

n − side

{μp = 300 cm2 V−1 s−1; μn = 1300 cm2 V−1 s−1

Dp = 7.8 cm2 s−1; Dn = 33 cm2 s−1

p − side

{μp = 100 cm2 V−1 s−1; μn = 280 cm2 V−1 s−1

Dp = 2.6 cm2 s−1; Dn = 7.3 cm2 s−1

(Note that the mobility is a lot lower in the heavily doped p-side because of the increasedionized impurity scattering.) Assume that τn = τp = 10−6 s. Calculate the diode current.

214 CHAPTER 4. JUNCTIONS IN SEMICONDUCTORS: P-N DIODES

Problem 4.13 We will define a p-n diode to be “turned on” when the current densityreaches 103 A/cm2 (this is an approximate criterion). Calculate the turn-on or cut-involtage for a GaAs and a Si p-n diode with following parameters (same for both diodes):

Nd = Na = 1017 cm−3

τn = τp = 10−8 s

Use table 3.1 to determine diffusion coefficients. Assume that the diodes are long and T =300 K.

Problem 4.14 An important use of a forward-biased p-n diode is as an emitter in a bipolartransistor. In the emitter it is desirable that the current be injected via only one kind ofcharge. The diode efficiency is thus defined as (Jn is the current density carried byelectron injection into the p-side)

γinj =Jn

JTot=

1

1 + Jp/Jn

Consider a GaAs p-n diode with the following parameters:

Electron diffusion coefficient, Dn = 30 cm2/sHole diffusion coefficient, Dp = 15 cm2/sp-side doping, Na = 5 × 1016 cm−3

n-side doping, Nd = 5 × 1017 cm−3

Electron minority carrier time, τn = 10−8 sHole minority carrier time, τp = 10−7 s

Calculate the diode injection efficiency (this is called the emitter efficiency in a bipolartransistor).

Problem 4.15 Consider the p-n diode in problem 4.12. In that problem we examined theprefactor of the diode current using the long diode conditions. Calculate the prefactor forthe case of a short diode in which both the n- and p-side widths are 5.0 μm.

4.12 FURTHER READING

• General

– M. S. Tyagi, Introduction to Semiconductor Materials and Devices (John Wiley andSons, New York, 1991).

– B. G. Streetman and S. Banerjee, Solid State Electronic Devices (Prentice-Hall, En-glewood Cliffs, NJ, 1999).

– G. W. Neudeck, “Modular Series on Solid State Devices,” Vol. 11, The P-N JunctionDiode, (Addison-Wesley, Reading, MA, 1983).

4.12. FURTHER READING 215

– R. S. Muller and T. I. Kamins, Device Electronics for Integrated Circuits (John Wileyand Sons, New York, 1986).

• Diode Breakdown

– M. H. Lee and S. M. Sze, “Orientation Dependence of Breakdown Voltage in GaAs,”Solid State Electronics 23, 1007 (1980).

– S. M. Sze, Physics of Semiconductor Devices (John Wiley and Sons, New York,1981).

– S. M. Sze and G. Gibbons, Applied Physics Letters 8, 112 (1986).

• Temporal Response of Diodes

– R. H. Kingston, “Switching Time in Junction Diodes and Junction Transistors,” Proc.IRE 42, 829 (1954).

– M. S. Tyagi, Introduction to Semiconductor Materials and Devices (John Wiley andSons, New York, 1991).

– D. A. Neamen, Semiconductor Physics and Devices: Basic Principles (Irwin, Home-wood, IL, 1992).

Chapter 5

SEMICONDUCTOR JUNCTIONS

5.1 INTRODUCTION

The discussions in chapter 4 suggest that when two different materials form a junction (e.g.n−type and p−type semiconductors) interacting electrical effects arise. We have seen howthe p-n diode has nonlinear I-V characteristics and tunable C-V characteristics. We can formjunctions between metals and semiconductors, between semiconductors with different gaps etc.These junctions also have special properties useful for devices. Metals by themselves are neces-sary to connect the semiconductors to the “outside world” of voltage sources and circuits. Theyare also able to produce rectifying junctions. Insulators are also an integral part of electronics.These materials provide an isolation between two regions of a device, can be used for bandstruc-ture tailoring, can be used as capacitors, etc. In this chapter we will examine some importantproperties of a variety of junctions.

5.2 METAL INTERCONNECTS

Metals form an important part of semiconductor technology. As shown in figure 5.1, they areused as interconnects (i.e. low resistance conductors), they form Schottky barriers and Ohmiccontacts, and they form gates in field effect transistors. We have discussed in section 2.7 thatdue to the high density of mobile electrons, the resistivity of metals is very low. In table 5.1 weshow the resistivities of some important metals used in electronics. In semiconductor circuits,interconnects provide pathways through which charge travels from one point to another. Whilethese interconnects are obviously passive elements of the circuit they are extremely importantand play a role in circuit performance. The metal strips making up the interconnect must be ableto carry adequate current and make good contact with the devices. Interconnects are depositedon insulators and touch the active devices only through windows that are opened at select points.Aluminum is a commonly used interconnect material. In bulk, Al is a good conductor, withresistivity of 2.7×10−6 Ω − cm. In thin-film form, the resistivity can be up to a factor of 20

216

5.2. METAL INTERCONNECTS 217

Element Work function, φm (volt)

Ag, silver 4.26

Al, aluminum 4.28

Au, gold 5.1

Cr, chromium 4.5

Mo, molybdenum 4.6

Ni, nickel 5.15

Pd, palladium 5.12

Pt, platinum 5.65

Ti, titanium 4.33

W, tungsten 4.55

ELECTRON AFFINITY OF SOME SEMICONDUCTORS

Element Electron affinity, χ (volt)

Ge, germanium 4.13

Si, silicon 4.01

GaAs, gallium arsenide 4.07

AlAs, aluminum arsenide 3.5

MATERIAL RESISTIVITY

(μΩ-cm)

Aluminum (Al)

Bulk 2.7

Thin Film 0.2-0.3

Alloys, Δρ

per %Si +0.7%Si

per %Cu +0.3%Cu

Titanium (Ti) 40.0

Tungsten (W) 5.6

Ti-W 15-50

Gold (Au) 2.44

Silver (Ag) 1.59

Copper (Cu) 1.77

Platinum (Pt) 10.0

Silicides

PtSi 28-35

NiS2 50

WORK FUNCTIONS OF SOME METALS

Table 5.1: Resistivities of some metals used in solid state electronics

lower, allowing the thin interconnect film to carry very high current densities, of the order of(∼ 106 Acm−2).

Example 5.1 In this example we will study some important concepts in thin-film resistors,which form an important part of semiconductor device technology. The resistors are oftenmade from polysilicon that is appropriately doped. In thin-film technology it is usual todefine sheet resistance instead of the resistance of the material. Consider, as shown infigure 5.1b, a material of length L, width W , and depth D. The resistance of the material is

R =ρL

WD=

ρL

A(5.2.1)

As we have discussed in chapter 3, the resistivity ρ is given by

ρ =1

neμ(5.2.2)

218 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

R =

Cross-sectional area, A

LρA

R esistivity = ρ

LW

D

L

Sheet resistance = R W R L

WR =

(b )

ME T A L S IN SE MICONDUCT OR T E CHNOL OGY

Interconnects to provide low resistance paths for current

Schottky barriers to provide non-linear I -V response

Ohmic contacts to provide low resistance paths to inject electrons and holes into semiconductors

(a)

(c)

Figure 5.1: (a) Metals serve three important functions in semiconductor technology. (b) A resis-tor of dimensions L × W × D. (c) Representation of the resistors in terms of sheet resistance.

where n is the free carrier density and μ is the mobility of the carriers (the equation can bemodified for a p-type material).

The sheet resistance is a measure of the characteristics of a uniform sheet of film. It isdefined as ohms per square, as shown in figure 5.1c, and is related to the film resistance by

R� = RW

L(5.2.3)

5.3. METAL SEMICONDUCTOR JUNCTION: SCHOTTKY BARRIER 219

5.3 METAL SEMICONDUCTOR JUNCTION:SCHOTTKY BARRIER

The metal-semiconductor junction can result in a junction that has non-linear diode charac-teristics similar to those of the p-n diode except that for many applications it has a much fasterresponse since carrier transport is unipolar. Such a junction is called a Schottky barrier diode.

5.3.1 Schottky Barrier Height

The working of the Schottky diode depends upon how the metal-semiconductor junction be-haves in response to external bias. Let us pursue the approximation we used for the p-n junctionand examine the band profile of a metal and a semiconductor. A metal semiconductor structureis shown in figure 5.2a. In figure 5.2b and figure 5.2c the band profiles of a metal and a semi-conductor are shown. Figure 5.2b shows that the band profile and Fermi level positions whenthe metal is away from the semiconductor. In figure 5.2c the metal and the semiconductor are incontact. The Fermi level EFm in the metal lies in the band, as shown. Also shown is the workfunction eφm. In the semiconductor, we show the vacuum level along with the position of theFermi level EFs in the semiconductor, the electron affinity, and the work function.

We will assume an ideal surface for the semiconductor in the first calculation. Later we willexamine the effect of surface defects. We will assume that φm > φs so that the Fermi level in themetal is at a lower position than in the semiconductor. This condition leads to an n−type Schot-tky barrier. When the junction between the two systems is formed, the Fermi levels should lineup at the junction and remain flat in the absence of any current, as shown in figure 5.2c. At thejunction, the vacuum energy levels of the metal side and semiconductor side must be the same.To ensure the continuity of the vacuum level and align the Fermi levels. Electrons move outfrom the semiconductor side to the metal side. Note that since the metal side has an enormouselectron density, the metal Fermi level or the band profile does not change when a small fractionof electrons are added or taken out. As electrons move to the metal side, they leave behind pos-itively charged fixed dopants, and a dipole region is produced in the same way as for the p-ndiode.

In the ideal Schottky barrier with no bandgap defect levels, the height of the barrier at thesemiconductor-metal junction (figure 5.2c), is defined as the difference between the semicon-ductor conduction band at the junction and the metal Fermi level. This barrier is given by (seefigure 5.2c)

eφb = eφm − eχs (5.3.1)

The electrons coming from the semiconductor into the metal face a barrier denoted by eVbi

as shown in figure 5.2c. The potential eVbi is called the built-in potential of the junction and isgiven by

eVbi = −(eφm − eφs) (5.3.2)

It is possible to have a barrier for hole transport if φm < φs. In figure 5.3 we show the case ofa metal-p-type semiconductor junction where we choose a metal so that φm < φs. In this case,at equilibrium the electrons are injected from the metal to the semiconductor, causing a negative

220 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

SCHOTTKY METAL n Si p Si n GaAs

Aluminum, Al 0.7 0.8

Titanium, Ti 0.5 0.61

Tungsten, W 0.67

Gold, Au 0.79 0.25 0.9

Silver, Ag 0.88

Platinum, Pt 0.86

PtSi 0.85 0.2

NiSi2 0.7 0.45

Table 5.2: Schottky barrier heights (in volts) for several metals on n- and p-type semiconductors.

charge on the semiconductor side. The bands are bent once again and a barrier is created for holetransport. The height of the barrier seen by the holes in the semiconductor is

eVbi = eφs − eφm (5.3.3)

The Schottky barrier height for n- or p-type semiconductors depends upon the metal andthe semiconductor properties. This is true for an ideal case. It is found experimentally thatthe Schottky barrier height is often independent of the metal employed, as can be seen fromtable 5.2 This can be understood qualitatively in terms of a model based upon non ideal surfaces.In this model the metal-semiconductor interface has a distribution of interface states that mayarise from the presence of chemical defects from exposure to air or broken bonds, etc. We haveseen in chapter 3 that defects can create bandgap states in a semiconductor. Surface defectscan create ∼ 1013 cm−2defects if there is 1 in 10 defects at the surface. Surface defects leadto a distribution of electronic levels in the bandgap at the interface, as shown in figure 5.4. Thedistribution may be characterized by a neutral level φo having the property that states below it areneutral if filled and above it are neutral if empty. If the density of bandgap states near φo is verylarge, then addition or depletion of electrons to the semiconductor can not alter the Fermi levelposition at the surface without large changes in surface charges (beyond the numbers demandedby charge neutrality considerations). Thus, the Fermi level is said to be pinned. In this case, asshown in figure 5.4, the Schottky barrier height is

eφb = Eg − eφo (5.3.4)

5.3. METAL SEMICONDUCTOR JUNCTION: SCHOTTKY BARRIER 221

n-type or p-typesemiconductor

Metal

≈ ≈

φm > φs n-type

EcEFs

n-semiconductorMetal

EFm

(a)

Vacuum energy

Ev

METAL-SEMICONDUCTOR JUNCTION AT EQUILIBRIUM

eφseχs

eφm

(b)

(c)

EcEFs

Ev

EFm

eφm – eφs = eVbi

W

eφbeφm

eχsVacuum energy

Figure 5.2: (a) A schematic of a metal-semiconductor junction. (b) The various important energylevels in the metal and the semiconductor with respect to the vacuum level. (c) The junctionpotential produced when the metal and semiconductor are brought together. Due to the built-inpotential at the junction, a depletion region of width W is created.

222 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

≈ ≈

p-typeSemiconductor

Metal

Evac

p-semiconductor

Metal

(a)

(b)

eφs

Ecs

EFsEvs

EFm

Ec

EFsEv

eφs – eφm = eVbieφb

eχseφm

W

++++++++

Figure 5.3: A schematic of the ideal p-type Schottky barrier formation. (a) The positions of theenergy levels in the metal and the semiconductor; (b) the junction potential and the depletionwidth.

and is almost independent of the metal used. The model discussed above provides a qualitativeunderstanding of the Schottky barrier heights. However, the detailed mechanism of the interfacestate formation and Fermi level pinning is quite complex. In table 5.2 we show Schottky barrierheights for some common metal-semiconductor combinations. In some materials such as GaNand AlGaN,the surface retains its ideal behavior and the Schottky barrier is indeed controlled bythe metal work function.

5.3. METAL SEMICONDUCTOR JUNCTION: SCHOTTKY BARRIER 223

EFm

eφb = Eg – eφο

EFsEc

Ev

eφο

Defect levels in the bandgap

Figure 5.4: Interface states at a real metal-semiconductor interface. A neutral level φo is definedso that the interface states above φo are neutral if they are empty and those below φo.

5.3.2 Capacitance Voltage Characteristics

Once the Schottky barrier height is known, the electric field profile, depletion width, depletioncapacitance, etc., can be evaluated the same way we obtained the values for the p-n junction. Theproblem for a Schottky barrier on an n-type material is identical to that for the abrupt p+n diode,since there is no depletion on the metal side. One again makes the depletion approximation; i.e.,there is no mobile charge in the depletion region and the semiconductor is neutral outside thedepletion region. Then the solution of the Poisson equation gives the depletion width W for anexternal voltage applied to the metal V

W =

[2ε(Vbi − V )

eNd

]1/2

(5.3.5)

Here Nd is the doping of the n-type semiconductor. Note that there is no depletion on the metalside because of the high electron density there. The potential V is the applied potential, whichis positive for forward bias and negative for reverse bias.

5.3.3 Current Flow across a Schottky Barrier: Thermionic Emission

Consider the Schottky barrier band diagram shown on figure 5.5 at zero bias.The Schottky barrier between a metal and semiconductor is shown in equilibrium (at zero

bias) with the electron distribution shown on the right

224 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

EFm

eVbieφ B

x

z

y

n

n(E-EC)

ECEFs

Figure 5.5: Schottky Barrier in equilibrium

Also shown is the electron distribution:

n (E − EC) = 2f (E − EC) · N (E − EC) (5.3.6)

similar to the case of a p−n junction, the factor of 2 in accounting for electron spin. Thermionicemission assumes that all electrons in the semiconductor with kinetic energy in the +z directiongreater than eVbi (Ez > eVbi) and kz > 0, are capable of surmounting the barrier and con-tributing to current flow from the semiconductor to the metal, Js→m. Note that the total kineticenergy E − EC = Ex + Ey + Ez . At thermal equilibrium the current from the metal to thesemiconductor, Jm→s, will be equal in magnitude and opposite in sign to Js→m, making the netcurrent zero. To calculate Js→m one needs to sum the current carried by every allowed electron:

Js→m = e∑

n (E − Ec) · vz (5.3.7)

for Ez > eVbi and vz > 0. The methodology employed is to calculate the number of electronsat energy E in a volume of k-space (dk)3, multiply the number with the electron velocity in thedirection along the barrier, and sum or integrate over energy. Assuming a crystal of length L,periodic boundary conditions yield allowed k values given by

k = 2πN (5.3.8)

where N is an integer and the separation between allowed k’s is Δk = 2π/L. The number ofelectrons in a volume element dkx, dky, dkz is therefore

dN = 2f (E − EC)dkxdkydkz

Δk3(5.3.9)

Assuming (E − EC) � EF and writing E − EF = E − EC + EC − EF gives

dN = 2 exp

(−((E − EC) + (EC − EF ))

kBT

)dkxdkydkz

Δk3(5.3.10)

5.3. METAL SEMICONDUCTOR JUNCTION: SCHOTTKY BARRIER 225

The current density contributed by these electrons is

Jz = −evzdN

L3(5.3.11)

if kz > 0 and Ez > eVbi. Note that all values of Ex and Ey are allowed as they represent motionin the x − y plane which is not constrained by the barrier in the +z direction. Note that

(Ex − EC) =�

2k2x

2m∗ (5.3.12)

with similar relationships for (Ey − EC) and (Ez − EC). Also employing the condition (Ez − Ec) >eVbi yields a minimum value of

kmin =

√eVbi

(2m∗

�2

)(5.3.13)

Also,

vz =�kz

m∗ (5.3.14)

Therefore,

Jz =−e

(2π)3

∫ +∞

−∞dkx

∫ +∞

−∞dky

∫ +∞

kmin

�kz

m∗ dkz ·

2 exp [− (Ex + Ey + Ez) /kBT ] · exp [− (EC − EF ) /kBT ] exp

(EC

kBT

)

= − 2e

(2π)3

∫x

·∫

y

·∫

z

exp

(−EC − EF

kBT

)(5.3.15)

where ∫x

=

∫y

=

∫ ∞

−∞exp

(�

2k2x

2m∗kBT

)dkx =

√2πm∗kBT

�(5.3.16)

and ∫z

=

∫ ∞

kmin

exp

(−�

2k2z

kBT

)· �kz

m∗ · dkz (5.3.17)

=kBT

�exp

(−�2k2

min/kBT)

=kBT

�exp

(−eVbi

kBT

)(5.3.18)

Therefore,

Jz =4π

(2π�)3 · em∗k2

BT 2 exp

(− (eVbi + (EC − EF ))

kBT

)(5.3.19)

or

Jz = A∗ · T 2 exp

(−eφB

kBT

)= Js→m (V = 0) (5.3.20)

226 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

where

A∗ =4πem∗k2

B

2π�3= 120 A cm−2 K−2 × m∗

m0(5.3.21)

is the Richardson constant and φB = Vbi + (EC − EF ), the barrier seen by electrons in themetal of the Schottky barrier height. We have calculated Js→m at V = 0. The analysis can beeasily extended to a forward bias of VF , the only change being replacing the barrier, Vbi by thenew barrier Vbi − VF . This changes Iz to

Iz =kBT

�exp

(− eVbi

kBT

)· exp

(eVF

kBT

)(5.3.22)

or

Js→m (V = VF ) = Js→m (V = 0) · exp

(eVF

kBT

)(5.3.23)

Since the current flow from the metal to the semiconductor is unchanged:

J (V = VF ) = Js→m (V = VF ) − Jm→s (V = VF ) (5.3.24)

= A∗T 2 exp

(−qφB

kBT

)[exp

(eVF

kBT

)− 1

](5.3.25)

Example 5.2 In a W-n-type Si Schottky barrier the semiconductor has a doping of 1016

cm−3 and an area of 10−3 cm2.(a) Calculate the 300 K diode current at a forward bias of 0.3 V.(b) Consider an Si p+ − n junction diode with the same area with doping ofNa = 1019 cm−3 and Nd = 1016 cm−3, and τp = τn = 10−6 s. At what forward bias willthe p-n diode have the same current as the Schottky diode? Dp = 10.5 cm2/s.

From table 5.2 the Schottky barrier of W on Si is 0.67 V. Using an effective Richardsonconstant of 110 A cm−2K−1, we get for the reverse saturation current

Is = (10−3 cm2) × (110 A cm−2K−2) × (300K)2 exp

(−0.67(eV)

0.026(eV)

)= 6.37 × 10−8 A

For a forward bias of 0.3 V, the current becomes (neglecting 1 in comparison toexp (0.3/0.026))

I = 6.37 × 10−8A exp(0.3/0.026)

= 6.53 × 10−3 A

In the case of the p-n diode, we need to know the appropriate diffusion coefficients andlengths. The diffusion coefficient is 10.5 cm2/s, and using a value of τp = 10−6s we getLp = 3.24 × 10−3 cm. Using the results for the abrupt p+ − n junction, we get for the

5.3. METAL SEMICONDUCTOR JUNCTION: SCHOTTKY BARRIER 227

saturation current (pn = 2.2 × 104 cm−3) (note that the saturation current is essentiallydue to hole injection into the n-side for a p+-n diode)

Io = (10−3 cm2) × (1.6 × 10−19 C) × (10.5 cm2/s−1)

(3.24 × 10−3 cm)× (2.25 × 104 cm−3)

= 1.17 × 10−14 A

This is an extremely small value of the current. At 0.3 V, the diode current becomes

I = Is exp

(eV

kBT

)= 1.2 × 10−9 A

a value which is almost six orders of magnitude smaller than the value in the Schottkydiode. For the p-n diode to have the same current that the Schottky diode has at 0.3 V, thevoltage required is 0.71 V.

This example highlights the important differences between Schottky and junction diodes.The Schottky diode turns on (i.e., the current is ∼1 mA) at 0.3 V while the p-n diode turnson at closer to 0.7 V.

5.3.4 Comparison of Schottky and p-n diodes

Both the p − n diode and the Schottky diode can be used for rectification and non-linearI − V response. One may ask which provides superior performance. The answer depends uponspecific applications. The questions of turn on voltage, speed needed, reverse leakage, etc. areimportant in deciding whether a p − n diode or Schottky diode should be used. The Schottkydiodes have a number of important advantages over p − n diodes. Some of these are listed infigure 5.6. The temperature dependence of the Schottky barrier current is quite weak comparedto that of a p-n diode. This is because in a p-n diode, the currents are controlled by the diffusioncurrent of minority carriers, which in turn depends on minority carrier concentration that has arather strong temperature dependence.

The fact that the Schottky barrier is a majority carrier device gives it a tremendous advantageover p-n diodes in terms of the device speed. Device speed is no longer dependent upon ex-tracting minority charge via diffusion or recombination. By making small devices, the RC timeconstant of a Schottky barrier can approach a few picoseconds, which is orders of magnitudefaster than that of p-n diodes.

Another important advantage of the Schottky diode is the fact that there is essentially norecombination in the depletion region and the ideality factor is very close to unity. In p-n diodes,there is significant recombination in the depletion region and ideality factors range from 1.2 to2.0.

The main disadvantage of Schottky diodes is a higher reverse current density. The thermionic-emission-controlled prefactor gives a current density in the range of ∼ 10−7 Acm−2, which isthree to four orders of magnitude higher than that of the p − n diode. Thus for a given appliedbias, the Schottky barrier has much higher current than the p−n diode. As a result the Schottkydiode is preferred as a low-voltage high-current rectifier. Since, the reverse current in a Schottky

228 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

SCHOT T K Y DIODEp-n DIODE

R everse current is very low

Forward current due to minority carrier injection from n- and p-sides

Switching speed controlled byrecombination (elimination) of minority injected carriers

Ideality factor in I -V characteristics ~ 1.2-2.0 due to recombination in depletion region

R everse current is relatively large

Device very fast: switching speed controlled by thermalization of “hot” injected electrons across the barrier ~ few picoseconds

Forward current due to majorityinjection from the semiconductor

E ssentially no recombination in depletion region ideality factor ~ 1.0

T he cut-in voltage is quite smallForward bias needed to make the device conducting (the cut-in voltage) is large

Figure 5.6: A comparison of some pros and cons of the p-n diode and the Schottky diode.

barrier is also quite large, which is a disadvantage for many applications. Another issue istechnology related. The Schottky barrier quality depends critically on the surface quality, theprocessing steps are quite critical. For many semiconductors, it is not possible to have a goodSchottky contact since the contact is very “leaky” due to defects. For such materials, the onlyway to have rectification is by using a p-n junction.

5.4. METAL SEMICONDUCTOR JUNCTIONS FOR OHMIC CONTACTS 229

––– –

–––

– – –

OHMIC CONTACT

Electrons tunnel through narrow depletion region

n+

Regionn-type

Semiconductor

Met

al

Ec–EF

Ev

– – – –I

V

Figure 5.7: Current-voltage characteristics of an ohmic contact along with the band diagrams ofmetal -n+-n contact. The heavy doping reduces the depletion width to such an extent that theelectrons can tunnel through the spiked barrier easily in either direction.

5.4 METAL SEMICONDUCTOR JUNCTIONSFOR OHMIC CONTACTS

In our discussion on p−n diodes and Schottky diodes we have discussed how a bias is appliedacross the device to cause current flow. It is important to ask how a connection is made from apower supply to the semiconductor. How do electrons or holes flow into and out of a semicon-ductor? There is a large barrier (the work function) that restricts the flow of electrons. We havealso seen from the previous section that at least in some cases a metal-semiconductor junctionalso provides a barrier to flow of electrons. However, it is possible to create metal-semiconductorjunctions that have a linear non-rectifying I-V characteristic, as shown in figure 5.7. Such junc-tions or contacts are called ohmic contacts.

There are two possibilities for creating ohmic contacts. In the previous section, to producea Schottky barrier on an n−type semiconductor, we needed (for the ideal surface) a metalwith a work function larger than that of the semiconductor. Thus, in principle, if we use ametal with a work function smaller than the semiconductor, one should have no built-in barrier.However, this approach is not often useful in practice because the Fermi level at the surface ofreal semiconductors is pinned because of the high interface density in the gap.

The Schottky barrier discussed earlier can be altered to create an ohmic contact. This is donethrough heavy doping and use of tunneling to get large current across the interface. Let us saywe have a built-in potential barrier, Vbi. The depletion width on the semiconductor side is

W =

[2εVbi

eNd

]1/2

(5.4.1)

Now if near the interface region the semiconductor is heavily doped, the depletion width couldbe made extremely narrow. In fact, it can be made so narrow that even though there is a potential

230 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

barrier, the electrons can tunnel through the barrier with ease, as shown in figure 5.7. The qualityof an ohmic contact is usually defined through the resistance R of the contact over a certain areaA. The normalized resistance is called the specific contact resistance rc and is given by

rc = R · A (5.4.2)

Under conditions of heavy doping where the transport is by tunneling, the specific contactresistance has the following dependence for tunneling, probability T , through a triangular bar-rier):

ln (rc) ∝ 1

�n(T )∝ (Vbi)

3/2

F(5.4.3)

where the field is

E =Vbi

W∝ (Vbi)

1/2 (Nd)1/2 (5.4.4)

Thus,

�n (rc) ∝ Vbi

∝ 1√Nd

(5.4.5)

The resistance can be reduced by using a low Schottky barrier height and doping as heavilyas possible. The predicted dependence of the contact resistance on the doping density is, indeed,observed experimentally. It is observed from experiments that it is usually more difficult to obtaincontacts with p−type semiconductors with low resistance. This is due to the difficulty in p-doping. It is also due to the fact that in many materials the relatively high effective mass of holes,leads to reduced tunneling currents. Also, in the case of many wide bandgap semiconductorssuch as GaN, the barrier heights between available metals and the valence band is much greaterthan that of the conduction band.

5.5 INSULATOR-SEMICONDUCTOR JUNCTIONS

In chapter 2 we have called materials with large bandgaps insulators. Usually these materialsdon’t have high crystalline quality and are difficult to dope. These materials have very highresistivity and are used to isolate regions to prevent current flow. Most insulator-semiconductorcombinations involve structures that are not lattice-matched. In most cases the insulator andthe semiconductor do not even share the same basic lattice type. In this section we will brieflyreview a few such combinations. Important issues in these junctions are listed in figure 5.8. Thekey issues here revolve around producing an interface with very low density of trapping statesand low interface leakage.

5.5.1 Insulator-Silicon

The most important junction in solid state electronics is the SiO2-Si system. In spite of thesevere mismatch between SiO2 structure and Si structure, the interface quality is quite good.

5.5. INSULATOR-SEMICONDUCTOR JUNCTIONS 231

Insulator

Semiconductor

Interface defectsInterface roughness

Substrate

{

Figure 5.8: Insulator-semiconductor junctions are dominated by interface quality and defectlevels in insulators.

Midgap interface density as low as 1010 eV−1 cm−2can be readily obtained. The ability toproduce such high-quality interfaces is responsible for the remarkable success of the metal-oxide-silicon (MOS) devices. Due to the low interface densities, there is very little trapping ofelectrons (holes) at the interface so that high-speed switching can be predictably used. In has tobe recognized though that the interface is still rough with islands with a height of 5 A over lateralextents of ∼50 A. Typical electron mobility in Si MOSFETs is ∼600 cm2/(V · s) compared toa mobility of ∼1100 cm2/(V · s) (300 K) for bulk pure Si. We will discuss the MOS structurein detail in chapter 9.

Silicon nitride (Si3N4) is another important film that forms modest-quality junctions with Si.Silicon nitride can be used in a metal-insulator-semiconductor device in Si technology, but itsapplications are limited. The film is used more as a mask for oxidation of the Si film. It alsomakes a good material for passivation of finished devices. Silicon oxy-nitride on the other handforms high-quality interfaces with silicon and can be used in FETs.

Although not an insulator or a metal, we include polycrystalline silicon (“poly”) in this chapterbecause of its importance in Si technology. Polysilicon can be deposited by the pyrolysis (heat-induced decomposition) of silane:

SiH4 −→ Si + 2H2 (5.5.1)

Depending upon the deposition temperature, micro crystallites of different grain sizes areproduced. Typical grain size is ∼ 0.1 μm.

Poly films can be doped to low resistivity to produce useful conductors for a number ofapplications. Poly is often used as a gate of an MOS transistor, as a resistor, or as a link betweena metal and the Si substrate to ensure an ohmic contact.

232 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

5.6 SEMICONDUCTOR HETEROJUNCTIONS

A growing number of modern devices are based on semiconductor heterojunctions, or junc-tions formed between two different materials. Modern bipolar transistors employ a p-n het-erojunction in order to improve the emitter injection efficiency (see chapter 7), while in HFETtechnology a heterojunction is used to form a high mobility channel (see chapter 8). In thissection we discuss the properties of p-n heterojunctions. Specifically, we will focus on the junc-tion formed between an n-type wide bandgap material (such as AlGaAs) and a p-type narrowerbandgap material (such as GaAs).

5.6.1 Abrupt p-n heterojunction

Electrostatics

To construct a band diagram for an abrupt p-n heterojunction, we proceed in the same manneras for the p-n homojunction. We begin with two separate materials (figure 5.9a) and considerwhat the equilibrium conditions must be when a junction is formed between them (figure 5.9b).In figure 5.9a, the material on the left (material 1) is n-type and has a wide bandgap, whilethe material on the right (material 2) is p-type and has a narrower bandgap. The doping in thep-type material is much higher than that of the n-type material (this is the typical emitter-basestructure in a III-V npn heterojunction bipolar transistor). The two materials have differentelectron affinities (χ1 and χ2), bandgaps (Eg1 and Eg2), and dielectric constants (ε1 and ε2).

Figure 5.9b shows a band diagram of the system once a junction is formed between the twomaterials. Since the materials have different bandgaps, there must exist a discontinuity in theconduction band (ΔEc) and/or the valence band (ΔEv) at the interface . The difference in thebandgap between the two materials is equal to the sum of the conduction band and valence banddiscontinuities, or

ΔEg = Eg1 − Eg2 = ΔEc + ΔEv (5.6.1)

By examination of figure 5.9, it is tempting to assume that ΔEc is simply the difference inthe electron affinities of the two materials. However, there also exist dipole charges at the het-erointerface which cause a shift in the relative band discontinuities. These dipole charges resultfrom the locally different atomic and electronic structures of the two materials at the heterointer-face as compared to their bulk atomic structure. While electron affinity rules accurately predictdiscontinuities in a limited number of material systems in which these dipole effects are small,in most heterostructures these dipole charges are significant and must be accounted for. Bandline-ups for a number of materials were shown in figure 2.31.

Similar to the case of a p-n homojunction, when the p- and n-type semiconductors are broughttogether, a built-in voltage, Vbi, is produced between the two sides of the structure. The built-involtage is equal to the sum of the band bending on the n-side (Vd1) and the bend bending on thep-side (Vd2). By examination of figure 5.9, the built-in voltage can be shown to be

eVbi = eVd1 + eVd2 = Eg2 − (EF − Ev)p − (Ec − EF )n + ΔEc

where the subscripts n and p refer to the n-side and p-side of the device. Comparing this ex-pression to that of the p-n homojunction , we see that the only difference is the additional ΔEc

5.6. SEMICONDUCTOR HETEROJUNCTIONS 233

Ec

eVd1

0 W-W pn

eVd2

Ev

EF

ΔEc

ΔEv

eΧ1 eΧ2

Eg1Eg2

Ec1

EF1

Ev1

Evac

Ec2

EF2Ev2

(a) (b)

Figure 5.9: (a) Band line-ups of two distinct materials prior to the formation of a junction. (b)Band diagram of a heterojunction formed between the two materials.

term. Making the same substitutions for (EF − Ev)p and (Ec − EF )n as we made in the p-nhomojunction case gives us the built-in potential as

Vbi =1

e(ΔEc + Eg2) − kBT

e�n

[Nc1Nv2

n1p2

](5.6.2)

where Nc1 is the conduction band density of states in material 1, Nv2 is the valence band den-sity of states in material 2, n1 = Nd1 is the electron concentration in material 1 (assuming fullionization), and p2 = Na2 is the hole concentration in material 2 (also assuming full ionization).

The depletion region width W (Vbi) and the electric field profile in the depletion region canbe found in the same way as for a p-n homojunction, except that ε1 �= ε2, so the electric fieldis not continuous at the material interface. The charge density and electric field profiles in thestructure are shown in figure 5.10. Gauss’ Law states that the displacement field D = εE (E isthe electric field) must be continuous at the interface. This gives the relationship

ε1E1,m = ε2E2,m (5.6.3)

where E1,m is the maximum electric field in material 1 and E2,m is the maximum electric fieldin material 2 (see figure 5.10).

234 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

0 W-W pn

1,m

2,m

+++

+++

+++

+++

+++

+++

+++

+++

(b)

(a)

E

EE

Figure 5.10: (a) Space-charge density and (b) electric field profiles in an n-p heterostructure.

To find E1,m, E2,m, Wn, and Wp, the following equations, along with equation 5.6.3, can beused:

NdWn = NaWp (5.6.4)

E1,m

Wn=

qNd

ε1and

E2,m

Wp=

qNa

ε2(5.6.5)

Vbi = area under E =1

2[WnE1,m + WpE2,m] = Vd1 + Vd2 (5.6.6)

These are essentially the same set of equations used to derive Wn, Wp, and E for a p-n homo-junction . Equation 5.6.4 is our charge neutrality condition, and equation 5.6.5 and equation5.6.6 result from solving Poisson’s equation.

From these equations, we obtain the following set of relationships:

Wp(Vbi) =

{2ε1ε2Vbi

e

[Nd

Na(Naε2 + Ndε1)

]}1/2

(5.6.7)

Wn(Vbi) =

{2ε1ε2Vbi

e

[Na

Nd(Naε2 + Ndε1)

]}1/2

(5.6.8)

W (Vbi) = Wp(Vbi) + Wn(Vbi) =[W 2

n(Vbi) + W 2p (Vbi) + 2Wn(Vbi)Wp(Vbi)

]1/2

5.6. SEMICONDUCTOR HETEROJUNCTIONS 235

W (Vbi) =

[2ε1ε2Vbi

e

([Na + Nd]

2

NaNd [Naε2 + Ndε1]

)]1/2

(5.6.9)

E1,m =eNdWn

ε1(5.6.10)

E2,m =eNaWp

ε2(5.6.11)

We can also solve for the band bending on either side of the junction Vd1 and Vd2:

Vd1 =1

2WnE1,m =

eNdW2n

2ε1(5.6.12)

Vd2 =1

2WpE2,m =

eNaW 2p

2ε2(5.6.13)

Current flow in abrupt p-n heterostructure

In a p-n homojunction, the ratio of current carried by electrons to current carried by holesIn/Ip can be made large by making Nd larger than Na. However, in bipolar transistor technol-ogy, it is desirable to have Na be large while simultaneously maintaining a large value of In/Ip.This can only be achieved by employing a p-n heterostructure. We will now calculate the currentcharacteristics of a p-n heterojunction and show how the ratio In/Ip can be controlled.

In figure 5.11a, we show the band diagram of the p-n heterostructure from figure 5.9b underforward bias. In determining the current characteristics of this structure, we make the followingassumptions:

1. The electron and hole components of the current can each be described by thermionicemission, similar to the treatment given in section 5.3.3 for the electron current in ann-type Schottky barrier. The barrier to hole injection from the p side to the n side islabeled eφBh in figure 5.11a, and the barrier to electron injection from the n side to the pside is labeled eφBe. The electron current In ∝ exp[−eφBe/kBT ], and the hole currentIp ∝ exp[−eφBh/kBT ].

2. The downwards notch in the conduction band immediately to the right of the junction doesnot capture electrons or in any way affect the electron current.

The general idea behind the use of heterostructures is that we would like to increase the barrierthat holes must overcome φBh relative to the barrier that electrons must overcome φBe. In p-nhomojunctions, φBe = φBh = Vbi − VF . In p-n heterojunctions, these barriers are no longerequal.

236 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

Ec

eΦBe

0 W-W pn

eVd2

Ev

EFp

ΔEc

ΔEv

eVF

eΦBh

EFn

Ec

eΦBe

0 W-W pn

eVd2

Ev

EFpeVF

eΦBh

EFn

(a) (b)

notch graded region

Figure 5.11: Band diagrams of (a) a forward biased abrupt p-n junction and (b) a forward biasedgraded p-n junction

Referring to figure 5.11a, for an abrupt p-n heterojunction, the barriers to hole injection (φBp)and to electron injection (φBn) are given by

eφBh = Eg1 − (EF − Ev)p − (Ec − EF )n − eVF (5.6.14)

eφBe = e(Vd1 − VF ) (5.6.15)

= Eg2 − (EF − Ev)p − (Ec − EF )n − eVF − eVd2 + ΔEc (5.6.16)

Since we are assuming Na >> Nd, the term eVd2 in the expression for φBe is small and can beomitted. The difference in the two barriers is given by

eφBh − eφBe = Eg1 − Eg2 − ΔEc = ΔEv (5.6.17)

The ratio of electron current to hole current in a p-n homojunction is given by(In

Ip

)hom

=DnNdLp

DpNaLn(5.6.18)

In the p-n homojunction, the barrier seen by electrons is the same as that seen by holes, andthe only means of controlling this ratio is through doping. In an abrupt p-n heterojunction withnegligible barrier discontinuity at the conduction band edge, the barrier seen by electrons is

5.6. SEMICONDUCTOR HETEROJUNCTIONS 237

smaller than that seen by holes by an amount ΔEv , and so the corresponding ratio of electroncurrent to hole current becomes(

In

Ip

)het

=DnNdLp

DpNaLnexp

(ΔEv

kBT

)(5.6.19)

We can see that even if Na is kept high, the ratio of electron current to hole current in a hetero-junction can still be kept large, even for a relatively modest bandgap discontinuity.

5.6.2 Graded p-n heterojunction

Although the abrupt p-n heterostructure discussed in the previous section did result in anincrease in the barrier to hole injection, the notch in the conduction band at the interface alsocaused an undesirable increase in the barrier to electron injection. While the net effect was stillan increase in the ratio In/Ip, eliminating this notch further increases In/Ip to a value(

In

Ip

)=

DnNdLp

DpNaLnexp

(ΔEg

kBT

)(5.6.20)

In order to reduce this notch, the bandgap of the p material can be graded upwards from thejunction, as shown in figure 5.11b. For example, in an n-AlGaAs/p-GaAs graded heterostructure,the n material is GaAs at the junction and is graded to the final AlGaAs composition over a shortdistance. The final shape of the notch depends on the length and profile of the grade; longergrading typically gives a smaller notch. However, it is important that the grade is contained wellwithin the depletion region. If the grade ends outside the depletion region, then the barrier seenby holes decreases, thus reducing the benefits of the heterojunction. Note that the barrier to holesin both abrupt and graded heterojunctions is the same. It is just the barrier for electron flow thatis reduced in the graded structures, allowing for the increased ratio of In/Ip.

Example 5.3 Designing a p-n heterojunction gradeConsider four different n-p+ Al0.3Ga0.7As/GaAs heterojunctions with ND = 1017 andNA = 5 × 1018. The AlGaAs in these junctions is graded from x = 0 to x = 0.3 overXGrade = 0(abrupt), XGrade = 100A, XGrade = 300A, and XGrade = 1μ. Calculateand plot the energy band diagrams for the above four cases.

Assume the dielectric constant of AlGaAs to be the same as that of GaAs.Eg = 1.8 eV for Al0.3Ga0.7As, and Eg = 1.4 eV for GaAs. ΔEg = 0.374 eV,ΔEC = 0.237 eV, and ΔEV = 0.137 eV. On the AlGaAs emitter side, far away from thejunction,

φn = EC − EF = kBT ln

(NC

n

)= 0.0323 eV (5.6.21)

Since the the p-GaAs is degenerately doped, Joyce-Dixon statistics must be applied:

φp = EV − EF =

238 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

Figure 5.12: Solutions to example 5.3

kBT

[ln

(p

NV

)+ A1

p

NV+ A2

(p

NV

)2]

= 0.011 eV

The solutions are plotted in figure 5.12.

5.6.3 Quasi-electric fields

In a homogeneous semiconductor, the separation between the conduction and valence bands iseverywhere equal to the semiconductor bandgap. Any electric field applied to the material there-fore results in an equal slope in the conduction and valence bands, as indicated in figure 5.13a.When a hole or electron is placed in this structure, a force of magnitude eE will act on the par-ticle. The magnitude of the force is equal to the slope of the bands and is the same for bothelectrons and holes. However, the direction of the force is opposite for the two particles.

5.6. SEMICONDUCTOR HETEROJUNCTIONS 239

Ec

Ev

+

Fe = -e

Fh = +e

(a)

Ec

Ev

+

Fe = 0

Fh = +e

(b)

Ec

Ev

+

Fh = +e

(c)

Fe = -e

E

E

Eh

Eh

Ee

Figure 5.13: (a) Band diagram when an electric field is applied to a homogeneous semiconductor.(b) Quasi-field causes a force on holes but not on electrons. (c) Quasi-field in which electronsand holes feel a force in the same direction.

An interesting phenomenon arises in semiconductors with graded bandgaps, such as the bipo-lar transistor emitter-base structure shown in figure 5.11b. In the graded region, the bandgapis not constant, so the slopes in the conduction and valence bands are no longer equal. Hencethe forces acting on electrons and holes in this region are no longer equal in magnitude. It is ingeneral possible for a force to act on only one type of carrier, as shown in figure 5.13b, or forforces to act in the same direction for both electrons and holes, as in figure 5.13c. Such behavior

240 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

cannot be achieved by pure electric fields in homogeneous materials. These fields, which werefirst described by Herbert Kroemer in 1957, are therefore referred to as quasi-electric fields.

In a given material, the total field acting on a hole or an electron is always the sum of theapplied field and the quasi field, or

Ee,tot = Eapp + Ee,quasi (5.6.22)

Eh,tot = Eapp + Eh,quasi (5.6.23)

The applied field, which results from applying a voltage difference between the ends of thematerial, will always be the same for both electrons and holes, but the quasi field could bedifferent for both. The band profiles in figure 5.13b and figure 5.13c can therefore be achievedin a number of different ways. For example, the profile in figure 5.13b could be achieved in thefollowing two ways:

1. An undoped (intrinsic) material with a graded composition and zero applied electric fieldtypically results in the profile in figure 5.13c. If an electric field Eapp = −Ee,quasi is thenapplied to this material, the resulting profile will be the one shown in figure 5.13b.

2. A uniformly doped n-type material with a graded composition and zero applied electricfield will also result in the profile in figure 5.13b. In this case, the doping ensures thatthe separation between the conduction band and the Fermi level remains approximatelyconstant. Notice that the resulting quasi-electric field in this structure acts only on minoritycarriers.

Quasi-electric fields provide engineers with additional tools that can be exploited in devicedesign. They have proven to be very useful in decreasing transit times in devices that rely onminority carrier transport. For example, in bipolar technology, a highly doped graded base layeris often used to speed up the transport of minority carriers from the emitter to the collector. Fora base with uniform bandgap, minority carriers injected from the emitter must diffuse acrossthe base, a process that is generally slow. By using a highly doped graded base to generate aquasi-electric field, such as was described in the second example above, minority carriers can beswept across much more quickly, thus reducing the base transit time and improving the deviceRF performance.

5.7 PROBLEMS

Temperature is 300 K unless stated otherwise.

• Section 5.2

Problem 5.1 A 2 μm thick ×10 μm Al interconnect is used in a semiconductor chip. Ifthe length of a particular interconnect is 1 cm, calculate the resistance of the line. Usetable 5.1 for the resistivity data.

5.7. PROBLEMS 241

Problem 5.2 If a current density of 105 A/cm2 flows in the interconnect of problem 5.1 to,calculate the potential drop.

Problem 5.3 Use the resistivity of Al and Cu given in table 5.1 and use the Drude model(chapter 1) to calculate the mobility of electrons in these two materials.

Problem 5.4 Discuss why in the analysis of the conductivity of metals we do not considerhole conductivity.

• Section 5.3

Problem 5.5 Assume the ideal Schottky barrier model with no interface states for ann-type Si with Nd = 1016 cm−3. The metal work function is 4.5 eV and the Si electronaffinity is 4 eV. Calculate the Schottky barrier height, built-in voltage, and depletion widthat no external bias.

Problem 5.6 A Schottky barrier is formed between Al and n-type silicon with a doping of1016 cm−3. Calculate the theoretical barrier if there are no surface states. Compare thiswith the actual barrier height. Use the data in the text.

Problem 5.7 Assume that at the surface of GaAs, 50% of all bonds are “defective” andlead to a uniform distribution of states in the bandgap. Each defective bond contributesone bandgap state. What is the two-dimensional density of bandgap states (units ofeV−1cm−2)? Assume that the neutral level φo is at midgap. Approximately how muchwill the Fermi level shift if a total charge density of 1012 cm−2 is injected into the surfacestates? This example gives an idea of “Fermi level pinning”.

Problem 5.8 The capacitance of a Pt-n-type GaAs Schottky diode is given by

1

(C(μF ))2 = 1.0 × 105 − 2.0 × 105 V

The diode area is 0.1 cm2. Calculate the built-in voltage Vbi, the barrier height, and thedoping concentration.

Problem 5.9 Calculate the mean thermal speed of electrons in Si and GaAs at 77 K and300 K. m∗

Si = 0.3mo;m∗GaAs = 0.067mo.

Problem 5.10 Calculate the saturation current density in an Au Schottky diode madefrom n-type GaAs at 300 K. Use the Schottky barrier height values given in table 5.2.

Problem 5.11 Consider an Au n-type GaAs Schottky diode with 50 μm diameter. Plotthe current voltage characteristics for the diode between a reverse voltage of 2 V and aforward voltage of 0.5 V.

Problem 5.12 Calculate and plot the I-V characteristics of a Schottky barrier diodebetween W and n-type Si doped at 5 × 1016 cm−3 at 300 K. The junction area is 1 mm2.Plot the results from a forward current of 0 to 100 mA.

242 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

Problem 5.13 In some narrow-bandgap semiconductors, it is difficult to obtain a goodSchottky barrier (with low reverse current) due to the very small barrier height. Consideran n-type InGaAs sample. Describe, on physical bases, how the “effective” Schottkybarrier height can be increased by incorporating a thin p-type doped region near thesurface region.

Problem 5.14 In the text, when we discussed the current flow in a Schottky barrier, weassumed that the current was due to thermionic emission only. This is based on classicalphysics where it is assumed that only particles with energy greater than a barrier can passthrough. Consider a W -n-type GaAs Schottky barrier in which the Schottky barriertriangular potential is described by a field of 105 V/cm. The Schottky barrier height is 0.8V. Calculate the tunneling probability through the triangular barrier as a function ofelectron energy from E = 0.4 eV to E = 0.8 eV. The tunneling current increases theSchottky reverse current above the value obtained by thermionic current considerations.

Problem 5.15 Consider an Al-n-type Si Schottky diode. The semiconductor is doped at1016 cm3. Also consider a p-n diode made from Si with the following parameters (thediode is ideal):

Nd = Na = 1018 cm−3

Dn = 25 cm2/s

Dp = 8 cm2/s

τn = τp = 10 ns

Calculate the turn-on voltages for the Schottky and p-n diode. Assume that the currentdensity has to reach 105 A/cm2 for the diode to be turned on.

Problem 5.16 An important problem in very high-speed transistors (to be discussed inchapter 8) based on the InAlAs/InGaAs system is the reliability of the Schottky barrier.Consider a Schottky barrier formed on an InAlAs doped n-type at 1016 cm−3. Calculatethe saturation current density if the Schottky barrier height is (i) 0.7 V; (ii) 0.6 V at 300 K.

The mass of the electrons in InAlAs is 0.08 mo. The Richardson constant has a value

R∗ = 120

(m∗

mo

)= 9.6A cm−2K−2

The saturation current density then becomes

Js (φb = 0.7 V) = R∗T 2 exp

[−

(eφb

kBT

)]= 1.8 × 10−6 A/cm

2

Js(φb = 0.6 V) = 8.2 × 10−5 A/cm2

Thus the current density varies by a very large value depending upon the Schottky barriervalue. The Schottky barrier height depends upon the metal-semiconductor interface

5.7. PROBLEMS 243

quality and can be easily affected by fabrication steps. In a p-n diode, on the other hand,the built-in voltage is fixed by doping and is more controllable.

Problem 5.17 A metal-i-GaN-n-GaN Schottky junction is shown in the figure 5.14 (a)below. Fixed positive and negative polarization charges across the GaN create a 2DEG inthis structure. The metal semiconductor barrier height φB is 0.5 eV. Assume that thei-GaN layer is 50 nm thick, and that the relative dielectric constant of AlGaN is 10.

1. Draw the equilibrium band diagram. Also draw the band diagram for a reverse biasof 10V.

2. Now, a phantom material (see figure 5.14(b)) with a high dielectric constant of 100and thickness of 50 nm is inserted between the gate and the GaN layer. Draw theband diagram at equilibrium and at a reverse bias of 10 V across the junction.Assume that the barrier height on this material is the same as in the case of GaN, andthat the bands of this material align perfectly with GaN.

3. The tunneling probability across a barrier of the form in figure 5.14 (c) is given by

P = e− 4π

√2md(E

3/20 −E

3/21 )

2(E0−E1)h

Use the above expression to estimate the ratio between the tunneling probabilities forthe cases in part (a) and (b) at equilibrium, and when a reverse bias of 10 V isapplied.

i - GaN

n - GaN

Metal

i - GaN

n - GaN

Metal

Phantom Material

EC

E1

E0

A B C

Figure 5.14: Figure for problem 5.17.

• Section 5.4

Problem 5.18 A gold contact is deposited on GaAs doped at Nd = 5 × 20 cm−3.Calculate the tunneling probability of the electrons to go into the semiconductor.

Problem 5.19 A metal with a work function of 4.2 V is deposited on an n-type siliconsemiconductor with an electron affinity of 4.0 V. Assume that there are no interface states.Calculate the doping density for which there is no space charge region at zero applied bias.

244 CHAPTER 5. SEMICONDUCTOR JUNCTIONS

Problem 5.20 To fabricate very high-quality ohmic contacts on a large-bandgap materialone often deposits a heavily doped low-bandgap material. For example, to make an n-typeohmic contact on GaAs, one may deposit n+InAs. Discuss why this would help toimprove the resistance of the contact.

Problem 5.21 Consider a W -n Si Schottky barrier on silicon doped at 1018 and1020 cm−3. Calculate the tunneling probability of electrons for electrons with energiesnear the conduction band in the two doping cases.

• Section 5.5

Problem 5.22 A (001) Si-SiO2 interface has ∼ 1011 cm−2 interface states. Assume thateach state corresponds to one defective bond at the interface. Calculate the fraction ofdefective bonds for the interface.

Problem 5.23 Calculate the sheet resistance of a 0.5 μm thick poly film doped n-type at1019 cm−3. This film is used to form a resistor of width 20 μm and length 0.1 cm.Calculate the resistance of the contact if the electron mobility is 150 cm2/V·s.

• Section 5.6

Problem 5.24 The measured value of ΔEC for the AlGaAs/GaAs system isapproximately 0.6ΔEG. However, electron affinity rules predict a different value forΔEC . Show, using band diagrams and potential profiles, that an interfacial dipole presentat the AlGaAs/GaAs interface can explain this. Discuss both n-AlGaAs/n-GaAs andn-AlGaAs/p-GaAs junctions.

Problem 5.25 Consider four different n-p+ Al0.3Ga0.7As/GaAs heterojunctions withND = 1017 and NA = 5 × 1018. The AlGaAs in these junctions is graded from x = 0 tox = 0.3 over XGrade = 0 (abrupt), XGrade = 100 A, XGrade = 300 A, andXGrade = 1 μm.(a) Calculate and plot the energy band diagrams for the above four cases.(b) When a forward bias is applied, how will the minority carrier current ratioIn−GaAs/Ip−AlGaAs vary in these four heterojunctions? Which one would you use as thebase-emitter junction in an n-p-n HBT?Assume the dielectric constant of AlGaAs to be the same as that of GaAs.

Problem 5.26 In an attempt to increase the collector breakdown voltage of ann-AlInAs/p-GaInAs/i-GaInAs/n+-GaInAs HBT, I replace the i-GaInAs collector withi-InP. Unfortunately, this introduced a potential barrier in the conduction band ofΔEC = 0.2eV . I decide to linearly grade the barrier over a distance of 50nm for GaInAs(Eg = 0.7eV ) to InP (Eg = 1.4eV ). Design the electrostatics so that there is no barrier toelectron from over the graded region. Assume that EF = EV in the p base and EF = EC

in the n+ subcollector. How would the desing change if I decided to grade the regionparabolically as shown in figure 5.15.

5.8. FURTHER READING 245

Linear Parabolic

EC EC

EV EV

50nm 50nm

GaInAs GaInAsInP InP

Figure 5.15: Figure for problem 5.26.

5.8 FURTHER READING

• D. A. Neamen, Semiconductor Physics and Devices: Basic Principles (Irwin, Boston,1997).

• M. S. Tyagi, Introduction to Semiconductor Materials and Devices (John Wiley and Sons,New York, 1991).

• R. S. Muller and T. I. Kamins, Device Electronics for Integrated Circuits (Wiley, NewYork, 1986).

Chapter 6

BIPOLAR JUNCTIONTRANSISTORS

6.1 INTRODUCTION

The bipolar junction transistor was the first three-terminal device in solid state electronics andcontinues to be a device of choice for many digital and microwave applications. For a decadeafter its invention, the bipolar device remained the only three-terminal device in commercialapplications. However, as the Si-SiO2 interface improved, the MOSFET has become dominant.Heterojunction bipolar devices now have very high performance in terms of frequency and gain.In figure 6.1 we show the structure and device performance parameters of a state of the artInGaAs/InP heterojunction bipolar transistor. In a three terminal device the goal is to use a smallinput to control a large output. The input could be an incoming weak signal to be amplified,or a digital signal. The workings of a three terminal device can be understood by examininghow the flow of water can be controlled. In one case, let’s say the water was to flow in a pipeof fixed diameter while in another, it could flow over an open channel. In figure 6.2 we showtwo different ways one could design a system to control the water flow. On the left-hand sidesequence of figure 6.2 we show how a change in the ground potential can be used to modifythe water flow. Only the fraction of water that is above the bump will flow across the potentialprofile. The value of the potential bump could be controlled by an independent control input.

Water flow can also be controlled by a faucet in which the faucet controls the constriction ofthe pipe and thus the water flow. In a bipolar device one controls the potential profile in thecurrent flow channel by using the base current as a controlling agent. In a FET on the other handone controls the channel constriction by applying a gate bias.

As noted earlier, an important requirement for an electronic device is that a small change inthe input should cause a large change in the output, i.e., the device should have a high gain.This requirement is essential for amplification of signals, tolerance of high noise margins indigital devices, and the ability to have a large fan-out (i.e., the output can drive several additionaldevices). Another important requirement is that the input should be isolated from the output. For

246

6.1. INTRODUCTION 247

0

1

2

3

4

5

6

7

0 0.5 1 1.5 2 2.50

4

8

12

16

Je

(mA

/mm

2 )

Vce

(V)

Ajbe

= 0.6 x 4.3 μm2

Ib step

= 85 uA

Vcb

= 0 V

Ic (mA

)

Peak fτ, f

max

0

5

10

15

20

25

30

35

109 1010 1011 1012

Gai

ns

(dB

)

Frequency (Hz)

ft = 391 GHz, f

max = 505 GHz

U

H21

Ajbe

= 0.6 x 4.3 um2

Ic = 13.2 mA, V

ce = 1.54 V

Je = 5.17 mA/um2, V

cb= 0.6 V

200

300

400

500

1 2 3 4 5 6

GH

z

Je (mA/um2)

ft

fmax

Vcb

= 0.6 V

(a)

(b)

(c)

E

B

C

Figure 6.1: State of the art n-InP/p+-InGaAs/n−-InP double heterojunction bipolar transistor(DHBT). (a)SEM image of device, (b) dc I-V characteristics, and (c) high frequency currentgain and power gain. For this device, the average β ≈ 36 and VBR,CEO = 5.1 V (measured atIC = 50 μA). Figures courtesy of M. Rodwell and Z. Griffith, UCSB.

the faucet example, these two requirements mean we should be able to turn the faucet on and offwith little effort and the water should not leak out of the faucet head!

In this chapter we will discuss static characteristics of the bipolar transistor.

248 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

Fluid flow Fluid flow in a confined region

A potential energy profile created to stop flowOFF state

Constriction is controlled by a “gate”OFF state

A reduced profile allows flow

Opening in constriction allows flow

⇒ Field effect transistors channel constriction iscontrolled by gate bias.

⇒BJT, HBTs potential energy profile is controlled by base-emitter voltage

Controlling flow by potential energy change

Controlling flow by altering a constriction

Figure 6.2: Two different ways to control flow of a fluid. The bipolar and field effect transistorsuse these two approaches to control current flow.

6.2 BIPOLAR TRANSISTOR: A CONCEPTUAL PICTURE

The bipolar junction transistor employs two back to back p − n diodes which with cleverdesign rules can have a high amplification and can operate at high frequency. It can also act as adigital device and as a microwave device.

6.2. BIPOLAR TRANSISTOR: A CONCEPTUAL PICTURE 249

Emitter contact

n+

n+

n+

n+

p

B

E

C

p

p+

p+

p+

p+

p

n epitaxyn+

buried layerp-type substrate

Base contact

Collector contact

n+

n+

n epitaxy

n epitaxy

n+ n+p

n

E B C

Cross-sectional view

Base width

Figure 6.3: A schematic of the structure and doping profiles of a bipolar junction transistor alongwith a simplified view of the cross-section.

We have shown a state of the art bipolar device. A schematic of the device is shown infigure 6.1. The device could have a doping of the form n+ − p-n or p+ − n-p. We will focus onthe n+ − p-n device. The emitter is heavily doped n−type, the p-region forms the base, and thelower n region is the collector. The emitter doping Nde is much larger than the base doping Nab

to ensure that the device has a high current gain, i.e., that a small base current change producesa large collector current change.

To understand how the device can have gain, let us consider a BJT where the emitter basejunction (EBJ) is forward biased and the base collector junction (BCJ) is reverse biased. Thisbiasing creates the forward active mode. The band profile of the device is shown in figure 6.4.Note that the base width Wb is much smaller than the diffusion length of electrons in the p-type base region. So that when electrons are injected from the emitter, most cross the basewithout recombining with holes. The strong electric field these electrons see once they reach thecollector, cause them to be swept away and form the collector current.

250 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

+ + + + +

– – – – – –– – – – –

n = Ndc~

n = Nde~

p = Nab~

Wb

Electron current

Hole current = Base current

n

n

p

(a)

(b)

EMITTER BASE COLLECTOR

– – – – –

– – – – – –– – – – –

– – – – – – – – – –

+ + + ++

–

–

–

–

– – –

Figure 6.4: (a) Band profile of an unbiased n+p-n BJT. (b) Band profile of a BJT biased in theforward active mode, where the EBJ is forward biased and the BJT is reverse biased.

We remind ourselves that if the EB diode is asymmetrically doped, the forward bias currentis essentially made up of injection of electrons into the p-side. This forward-biased currentcan also be altered by a very small change in the forward bias voltage since the current dependsexponentially on the forward bias value. The forward-biased n+ emitter injects electrons into thep-base. Some of the electrons recombine in the base with the holes, but if the base region is lessthan the diffusion length of the minority carriers, most of them reach the depletion region of thep-n base-collector diode and are swept out to form the collector current. The collector current isproportional to the minority carriers (electrons) that reach the edge of the p−n depletion region,as shown in figure 6.4b. Since the injected minority carriers are due to the emitter current, we

6.2. BIPOLAR TRANSISTOR: A CONCEPTUAL PICTURE 251

haveIC = BIEn (6.2.1)

where IEn is the electron part of the emitter current and the factor B is called the base transportfactor. In the absence of e-h recombination, the emitter current is made up of electrons injectedfrom the n- to p-sides (IEn) and holes injected from p- to n-sides (IEp). Since the BCJ is reversebiased, the collector current is related only to the electrons injected and we define the emitterefficiency γe as

γe =IEn

IEn + IEp(6.2.2)

For optimum devices, γe and B should be close to unity. The ratio between the collector andemitter currents is the current transfer ratio, α

IC

IE=

BIEn

IEn + IEp= Bγe = α (6.2.3)

This ratio is close to unity in good bipolar devices. In figure 6.5 we show a typical circuit fora BJT in the forward-bias active mode. A change in the base current alters the minority carrierdensity np in the base and causes a large change in the collector current. The ratio between thecollector current and the controlling base current is of great importance since this represents thecurrent amplification . The base current is made up of the hole current injected into the emitter(IEp) and the hole current due to the recombination in the base with injected electrons from theemitter (= (1−B)IEn). Thus

IB = IEp + (1 − B)IEn (6.2.4)

The base-to-collector current amplification factor, denoted by β is then

β =IC

IB=

BIEn

IEp + (1 − B)IEn=

B(IEn/IE)

1 − B(IEn/IE)

=Bγe

1 − Bγe(6.2.5)

This gives for the current gain

β =α

1 − α(6.2.6)

The factor β can be quite large for the bipolar transistor. In the next section we will discuss themathematical derivation of the device characteristics.

252 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

CIC

R2

B

n

p

n

E

R1

V1

V2

IB

IE

Collector current

Collector

Base

Emitter

Base current (leads to changes in base charge)

(a)

(b)

Figure 6.5: A schematic showing how the change in base current affects the majority carrierinjection density and the collector current in a bipolar device. (a) A circuit using a bipolar tran-sistor. (b) The effect of base current variation on the injected minority charge and the collectorcurrent. The collector current is much larger than the base current.

6.3 STATIC CHARACTERISTICS: CURRENT-VOLTAGERELATION

We will now develop a model for the current flow in a BJT. Initially we will use a simplemodel which captures the essence of the device performance. Later we will discuss secondaryissues. In the bipolar device carriers from the emitter are injected “vertically” across the base

6.3. STATIC CHARACTERISTICS: CURRENT - VOLTAGE RELATION 253

while the base charge is injected from the “side” of the device, as can be seen in figure 6.6. Ifwe assume that the emitter width is wide, the device can be understood using a one-dimensionalanalysis. We will use the following simplifying assumptions.

1. The electrons injected from the emitter diffuse across the base region and the field acrossthe base is small enough that there is no drift.

2. The electric fields are nonzero only in the depletion regions and are zero in the bulk mate-rials.

3. The collector injection current is negligible when the BJT is reverse biased.

4. In describing voltages, we use the following notation. The first subscript of the voltagesymbol represents the contact with respect to which the potential is measured. For exam-ple, VBE > 0 means the base is positive with respect to the emitter.

In general, a number of currents can be identified in the bipolar device, (figure 6.6) as follows:

• Base current:Is made of holes that recombine with electrons injected from the emitter(Component I) and holes that are injected across the emitter-base junction into the emitter(Component II). Once again we ignore the BCJ for the forward active region.

• Emitter current: Consists of the electron current that recombines with the holes in the baseregion (III), the electron current which is injected into the collector (IV), and the holecurrent injected from the base into the emitter (II).

Minority electron (V) and hole (VI) currents flow in the base-collector junction and are im-portant when the emitter current goes toward zero. In our analysis, we will assume that all thedopants are ionized and the majority carrier density is simply equal to the doping density. Thesymbols for the doping density are (for the npn device): Nde—donor density in the emitter;Nab—acceptor density in the base; Ndc—donor density in the collector. If the ionization of thedopants is not complete we need to adjust for the ionization efficiency.

The back to back p − n diodes in the bipolar device can operate in four possible biasingmodes as shown in table 6.1. Depending upon the applications, the bipolar device operationmay span one or all of these modes. For example, for small-signal applications where one needsamplification one only operates in the forward active mode, while for switching applications thedevice may have to operate under cutoff and saturation modes and pass through the active modeduring the switching.

6.3.1 Current Flow in a BJT

Since the bipolar device is based on p − n diodes, we will use our understanding of currentflow of p − n diodes. Note that we will assume the emitter width is long compared to hole

254 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

Emitter contact

Basecontact

SiO2

A A'

p

n

n

IC

nIEB = Emitter current injected into the base = IEn

nIBC = Electron current injected across reverse-biased base collector junction

IBE = Base current injected into the emitter = IEpp

IBE = Recombination current in the base region R

IBC = Hole current injected across reverse-biased base collector junction p

InC = Electron current coming from the emitter (= IC)~

Electron flowIEBn

n n

IBEp

p

IBER

IBCp

IBCn

InC

IB

IE

Hole flow

III

III

IV

VIBER

++BE

A

A'

CB

VI

Collectorcontact

Figure 6.6: A schematic of an Si BJT showing the three-dimensional nature of the structure andthe current flow. Along the section AA′, the current flow can be assumed one-dimensional. Thevarious current components in a BJT are discussed in the text.

diffusion length while the base width is small compared to the electron diffusion length. We willuse the different axes and origins shown in figure 6.7. The distances are labeled xe, xb, and xc

as shown and are measured from the edges of the depletion region. The base width is Wb, butthe width of the “neutral” base region is Wbn as shown. We assume that Wb and Wbn are equal.

6.3. STATIC CHARACTERISTICS: CURRENT - VOLTAGE RELATION 255

Mode of operation EBJ bias CBJ biasForward active Forward (VBE > 0) Reverse(VCB > 0)Cutoff Reverse (VBE < 0) Reverse (VCB > 0)Saturation Forward (VBE > 0) Forward (VCB < 0)Reverse active Reverse (VBE < 0) Forward (VCB < 0)

Table 6.1: Operation modes of the npn bipolar transistor. Depending upon the particular appli-cation, the transistor may operate in one or several modes.

Later we will study the effect of the two widths being different. Using the p-n diode theory,we have the following relations for the excess carrier densities in the various regions are(see ourdiscussion on carrier decay in chapter 3 and chapter 4):

δpe(xe = 0) = excess hole density at the emitter side of the EBJ

= peo [exp (eVBE/kBT ) − 1] (6.3.1)

δnb(xb = 0) = excess electron density on the base side of the EBJ

= nbo [exp (eVBE/kBT ) − 1] (6.3.2)

δnb(xb = Wbn) = excess electron density at the base side of the CBJ

(collector-base junction)

= nbo [exp (−eVCB/kBT ) − 1] (6.3.3)

δpc(xc = 0) = excess hole density at the collector side of the CBJ

= pco [exp (−eVCB/kBT ) − 1] (6.3.4)

As shown in figure 6.7 in these expressions the subscripts peo, nbo, and pco represent theminority carrier equilibrium densities in the emitter, base, and collector, respectively. The totalminority carrier concentrations pe in the emitter, nb in the base, and pc in the collector are shownschematically in figure 6.7b. Assuming 100% ionization of the dopants, the majority carrierdensities are neo = Nde, pbo = Nab, and nco = Ndc for the emitter, base, and collector. Wewill assume that the emitter and collector regions are longer than the hole diffusion lengths Lp,so that the hole densities decrease exponentially away from base regions.

To find the current flow we have to calculate the spatial variation of carrier densities. Inthe base region, the excess electron density is given at the edges of the neutral base region byequation 6.3.2 and equation 6.3.3 To obtain the electron density in the base we must solve thecontinuity equation using these two boundary conditions, as discussed in section 3.9. The excessminority carrier density in the base region is given by

δnb(xb) =nbo

sinh(

Wbn

Lb

) {sinh

(Wbn − xb

Lb

)[exp

(eVBE

kBT

)− 1

]

+ sinh

(xb

Lb

) [exp

(−eVCB

kBT

)− 1

]}(6.3.5)

256 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

pe(xe = 0) nb(x)

Emitter VBE Base VCB Collector

peo

pbo nco

pco

IE

|EBJ| | CBJ |depletion layer

depletion layer

(a)

nbo

Equ

ilibr

ium

de

nsity

Wbn

neo

– – ++

xcxe

(b)

nbopeo

xe = 0xb= 0 xb =Wbn xc = 0

xb

pco

Wb

ICIB

Forward bias Reverse bias

Figure 6.7: A forward active mode BJT. (a) The equilibrium carrier concentrations of electronsand holes and positions of the junction depletion regions in the npn transistor. (b) Minoritycarrier distributions in the emitter, base, and collector regions.

The profile of the total minority carrier densities (i.e., background and excess) is shown in fig-ure 6.7b. The electron distribution in the base is almost linear, as can be seen, and is assumedto be so for some simple applications. Once the excess carrier spatial distributions are knownwe can calculate the currents as we did for the p-n diode. We assume that the emitter-base cur-rents are due to carrier diffusion once the device is biased. We have, for a device of area A and

6.3. STATIC CHARACTERISTICS: CURRENT - VOLTAGE RELATION 257

diffusion coefficients Db and De in the base and emitter, respectively,

IEn = IEBn = eADb

dδnb(x)

dxb

∣∣∣∣xb=0

(6.3.6)

IEp = IBEp = −eADe

dδp(x)

dxe

∣∣∣∣xe=0

(6.3.7)

These are the current components shown in figure 6.6 and represent the emitter current compo-nents II, III, and IV. Assuming an exponentially decaying hole density into the emitter, we have,as in the case of a p-n diode ,

IEp = −A

(eDepeo

Le

)[exp

(eVBE

kBT

)− 1

](6.3.8)

Using the electron distribution derived in the base, we have for the electron part of the emittercurrent

IEn = − eADbnbo

Lb sinh(

Wbn

Lb

) {cosh

(Wbn − xb

Lb

)[exp

(eVBE

kBT

)− 1

]

− cosh

(xb

Lb

) [exp

(−eVCB

kBT

)− 1

]}∣∣∣∣at xb=0

= − eADbnbo

Lb sinh(

Wbn

Lb

) {cosh

(Wbn

Lb

)[exp

(eVBE

kBT

)− 1

]

−[exp

(−eVCB

kBT

)− 1

]}(6.3.9)

For high emitter efficiency we want IEn to be much larger than IEp. This occurs if the emitterdoping is much larger than the base doping. The total emitter current becomes

IE = IEn + IEp = −{

eADbnbo

Lbcoth

(Wbn

Lb

)+

eADepeo

Le

}[

exp

(eVBE

kBT

)− 1

]+

eADbnbo

Lb sinh(

Wbn

Lb

) [exp

(−eVCB

kBT

)− 1

](6.3.10)

The collector current components can be obtained by using the same approach. Thus we have

IBCn = eADb

dδnb(xb)

dxb

∣∣∣∣xb=Wbn

(6.3.11)

IBCp = eADp

dδp(xc)

dxc

∣∣∣∣xc=0

(6.3.12)

258 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

Using the results shown in the first part of equation 6.3.9 at xb = Wbn, we have

IBCn = − eADbnbo

Lb sinh(Wbn/Lb)

[exp

(eVBE

kBT

)− 1

]+

eADbnbo

Lbcoth

(Wbn

Lb

)[exp

(−eVCB

kBT

)− 1

](6.3.13)

The hole current on the collector side is the same as for a reverse-biased p-n junction:

IBCp = −eADcpco

Lc

[exp

(−eVCB

kBT

)− 1

](6.3.14)

From the way we have defined the currents, the two current components flow along +x direction.If we define IC as the total current flowing from the collector into the base, we have

−IC =

[eADcpco

Lc+

eADbnbo

Lbcoth

(Wbn

Lb

)][exp

(−eVCB

kBT

)− 1

]− eADbnbo

Lb sinh(

Wbn

Lb

) [exp

(eVBE

kBT

)− 1

](6.3.15)

The base current is the difference between the emitter and collector currents: (IB = IE − |IC |).It is interesting to point out that if the base region Wbn is much smaller than the diffusion length,the electron gradient in the base region can be simplified by using the approximations

sinh(α) =eα − e−α

2= α +

α3

3!+

α5

5!+ · · ·

cosh(α) =eα + e−α

2= 1 +

α2

2!+

α4

4!· · ·

For the forward active mode if we ignore the current flow in the reverse-biased BCJ we get

IE =−eADbnb0

Lbcoth

(Wbn

Lb

)[exp

(eVBE

kBT

)− 1

]−eADepe0

Le

[exp

(eVBE

kBT

)− 1

](6.3.16)

Here the first part is due to electron injection from the emitter into the base (III and IV) and thesecond part is due to the hole injection from the base into the emitter (II). The collector currentis

IC =eADbnb0

Lb sinh(

Wbn

Lb

) [exp

(eVBE

kBT

)− 1

](6.3.17)

Assuming that Wbn � Lb, we can expand the hyperbolic functions as noted above. The basecurrent is the difference between the emitter and collector current. We find that

IB =eADepe0

Le

[exp

(eVBE

kBT

)− 1

]+

eADbnb0Wbn

2L2b

[exp

(eVBE

kBT

)− 1

](6.3.18)

6.3. STATIC CHARACTERISTICS: CURRENT - VOLTAGE RELATION 259

The first part represents the hole current injected from the base into the emitter and the secondpart represents the hole current recombining with electrons injected from the emitter .

Having derived the current components, in the next section we will examine how materialproperties and doping levels can be manipulated to improve device performance. It is useful torecast the prefactor of the first term in the emitter current (equation 6.3.16) in a different form.The prefactor, which we will denote by IS (we assume that Wbn � Lb so that coth α = 1/α),is

IS =eADbnbo

Wbn=

e2A2Dbn2i

eANabWbn=

e2ADbn2i

eQG

where QG is called the Gummel number for the transistor. It has a value

QG = NabWbn (6.3.19)

and denotes the charge in the base region of the device (assuming full ionization). As we willsee later, the Gummel number has an important effect on device performance.

To understand the operation of a BJT as an amplifier or a switching device it is useful to ex-amine the device under conditions of saturation, forward active (or reverse active), and cutoff. Infigure 6.8 we show the band profile and the minority carrier distribution for each of these modes.Note that in saturation where both EBJ and BCJ are forward biased, a large minority carrier den-sity (electrons for the npn device) is injected into the base region. This plays an important rolein device switching, as will be discussed later. In the cutoff mode there is essentially no minoritycharge in the base, since the EBJ and BCJ are both reverse biased. In the forward active mode,the mode used for amplifiers, the EBJ is forward biased while the BCJ is reverse biased. Underthis mode IC � IB , providing current gain.

6.3.2 BJT Biasing in circuits

The three terminal bipolar transistor can be biased in one of three different configurationsshown in figure 6.9a. The configuration chosen depends upon the applications. As shown, oneof the terminals can be chosen as a common terminal between the input and output terminals.The full I-V characteristics of a BJT in the common-base and the common-emitter configurationare shown in figure 6.9b. In the common-base configuration the cutoff mode occurs when theemitter current is zero. Note that the emitter current is finite, the collector current does not goto zero at VCB = 0. The BCJ has to be forward biased at the turn on voltage (∼ 0.7 V for Sidevices) to balance the injected emitter current.

In the common-emitter mode, the cutoff mode occurs when the base current is zero and indi-cates the region where the EBJ is no longer forward biased. The saturation region is representedby the region where VCE = VBE and both EBJ and BCJ are forward biased.

6.3.3 Current-Voltage: The Ebers-Moll Model

It is useful in circuit applications to represent the I − V characteristics derived by us in termsof a simple physical model. Several models have been developed to do so. Here we will discuss

260 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

Minority charge density

Holes

ElectronsHoles

peo

nbonco

IE

IB

IC

Minority charge density

Holes

ElectronsHoles

IB ~ 0

Minority charge density

Holes

ElectronsHoles

SATURATION FORWARD ACTIVE CUTOFF

Forward Forward Forward Reverse

Reverse Reverse

Figure 6.8: The band profile and minority charge distribution in a BJT under saturation, forwardactive, and cutoff modes.

the Ebers-Moll model. We can write the currents given in equation 6.3.10 and equation 6.3.17as

IE = −IES

[exp

(eVBE

kBT

)− 1

]+ αRICS

[exp

(−eVCB

kBT

)− 1

](6.3.20)

IC = αF IES

[exp

(eVBE

kBT

)− 1

]− ICS

[exp

(−eVCB

kBT

)− 1

](6.3.21)

where

IES =eADbnbo

Lbcoth

(Wbn

Lb

)+

eADepeo

Le(6.3.22)

ICS =eADcpco

Lc+

eADbnbo

Lbcoth

(Wbn

Lb

)(6.3.23)

αF IES = αRICS =eADbnbo

Lb sinh(

Wbn

Lb

) (6.3.24)

Notice the symmetry underlying these equations. This symmetry allows us to develop a simplemodel described in figure 6.10. The parameter αF represents the common-base current gain inthe forward active mode, ICS gives the reverse-bias BCJ current, αR is the common-base currentgain for the inverse active mode (i.e., EBJ is reverse biased and CBJ is forward biased) and IES

6.3. STATIC CHARACTERISTICS: CURRENT - VOLTAGE RELATION 261

VEB

Common base Common emitter Common collector

E

B

CE

B

CE

B

CIE IC

VBCIB

VEC

VECVEB

IE

VCBIC

IB

VBC

IB

VEB

VEC

IC

IE

IE4

IE3

IE2

IE1IE = 0

VBC~0.7 V 0

IC

Cutoff

Saturation

}

Active

IB2

IB1

IB = 0

IB2

IB1

IB = 0

Reverse active

Cutoff

Saturation

Active

VBC = 0

VEC

IC

Common base Common emitter

(a)

(b)

Forward active

Figure 6.9: (a) Three possible configurations under which a BJT can be used in circuits. (b)A schematic of the current-voltage characteristics of a BJT in the common-base and common-emitter configuration.

gives the reverse-bias EBJ current. These equations represent two diodes that are coupled toeach other. The Ebers-Moll model is primarily useful to develop a physical description of thebipolar device.

An important application of the Ebers-Moll model is to find the conditions for the saturationmode. In the common-emitter mode, the saturation condition is given by

VCE(sub) = VBE + VCB = VBE − VBC (6.3.25)

Note that both VBE and VBC (= −VCB) are positive.We also have the current conservation expression:

IE + IB + IC = 0 (6.3.26)

262 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

[ ( ) ] IR = ICS exp –1[ ( ) ]

αRIR αFIF

VΒΕ– +

VΒC+ –

IΕ IC

E C

IR

IF = IES exp –1 eVBE kBT

eVBC kBT

IF

B

Figure 6.10: The Ebers-Moll equivalent circuit of a bipolar transistor looks at the device as madeup of two coupled diodes.

Using this equation to eliminate IE from equation 6.3.20, we can obtain the values of VBE andVBC in terms of IC , IB , and the parameters IES , ICS , αR, and αF . This gives for VCE(sat)

VCE(sat) = VBE − VBC =kBT

e�n

[IC(1 − αR) + IB

αF IB − (1 − αF )IC· ICS

IES

](6.3.27)

Substituting for ICS/IES from equation 6.3.24, we get

VCE(sat) =kBT

e�n

[IC(1 − αR) + IB

αF IB − (1 − αF )IC· αF

αR

](6.3.28)

Typical values of VCE(sat) are 0.1 to 0.2 V, as can be seen in example 6.2.

6.4 DEVICE DESIGN AND DEVICE PERFORMANCE PA-RAMETERS

In this section we will examine how device design influences performance of a BJT. Throughmaterial and geometric parameters we can control are doping densities, base width, device area,and in some cases material choice (e.g. Si or GaAs etc.). Usually it would be difficult to changethe material system since it is difficult to alter the processing technology. The main performanceparameters one wants to improve are the current gain, and device operation frequency. Addition-ally there are issues related to high voltage biasing that we will discuss later. We will focus on

6.4. DEVICE DESIGN AND DEVICE PERFORMANCE PARAMETERS 263

the forward active mode of the device so that we have the conditions

eVBE � kBT (6.4.1)

eVCB � kBT (6.4.2)

In a well-designed bipolar transistor we always have Wb � Lb.

Emitter Injection Efficiency

Bipolar transistor gain is intimately tied to emitter efficiency. The emitter injection efficiencyis the ratio of the electron current (in the npn BJT) due to the electron injection from the emitterto the total emitter current. Thus,

γe =IEn

IEn + IEp(6.4.3)

For high emitter efficiency, IEp should be minimal. Under the voltage approximations made wehave from Eqns. 6.3.16 and 6.3.18,

IEp = −eADepeo

Leexp

(eVBE

kBT

)(6.4.4)

IEn∼= − eADbnbo

Lb tanh(

Wbn

Lb

) exp

(eVBE

kBT

)(6.4.5)

Thus the emitter efficiency becomes

γe =1

1 + (peoDeLb/nboDbLe) tanh (Wbn/Lb)(6.4.6)

If the base width is small compared to the electron diffusion length, the tanh (Wbn/Lb) can bereplaced by (Wbn/Lb) and we have

γe∼= 1

1 + (peoDeWbn/nboDbLe)∼ 1 − peoDeWbn

nboDbLe(6.4.7)

Thus for γe to be close to unity, we should design the device so that Wbn � Le and peo � nbo.Thus a small base width and a heavy emitter doping compared to the base doping are essential.Of course, the base width cannot be arbitrarily reduced.

Base Transport Factor

The second part of the device gain is related to how electrons injected from the emitter moveover the base. The base transport factor is the ratio of the electron current reaching the base-collector junction to the current injected at the emitter-base junction. As the electrons travelthrough the base, they recombine with the holes so that the base transport factor is less than

264 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

unity . We have from equation 6.3.16 and equation 6.3.17 (in the forward active mode, thecollector current is essentially due to electron injection from the emitter)

B =IC

IEn

∼= 1

cosh(

Wbn

Lb

) (6.4.8)

For small base width we have

B ∼= 1 − W 2bn

2L2b

(6.4.9)

Note that the base transport factor depends upon the neutral base width, not the chemical basewidth. Thus it depends upon the bias conditions. This causes the Early effect discussed later.

Collector Efficiency γc

The collector efficiency is the ratio of the electron current that reaches the collector to thebase-collector current. Due to the high reverse bias at the base-collector junction, essentially allthe electrons are swept into the collector so that the collector efficiency can be taken to be unity.

Current Gain

Since we know how the expression for the emitter efficiency and base transport factor we cannow examine the current gain. We are primarily interested in the ratio of the collector currentand the base current. The parameter α defined as the ratio of the collector current to the emittercurrent is given by

α =IC

IE=

BIEn

IEn + IEp= γeB

=

[1 − peoDeWbn

nboDbLe

] [1 − W 2

bn

2L2b

](6.4.10)

The ratio of the collector current to the base current is extremely important since it is the basecurrent that is used to control the device state. This is given by

β =α

1 − α(6.4.11)

We can see that heavy emitter doping and narrow base width are critical for high β. Animportant parameter characterizing the device performance is the transconductance, which de-scribes the control of the output current (IC) with the input bias (VBE). The transconductance is(IC ∝ exp (eVBE/kBT ))

gm =∂IC

∂VBE=

eIC

kBT=

eβIB

kBT(6.4.12)

The transconductance of bipolar devices is extremely high compared to that of field-effect tran-sistors of similar dimensions. This is because of the exponential dependence of IC on VBE incontrast to a weaker dependence of current on “gate bias” for field effect transistors.

6.5. BJT DESIGN LIMITATIONS: NEED FOR BAND TAILORING 265

6.5 BJT DESIGN LIMITATIONS: NEED FOR BANDTAILORING AND HBTs

So far in this chapter we have assumed that the emitter, base, and collector are made from thesame material, Of course this need not be the case since as we have noted in previous chaptersheterostructures can be fabricated with ease. In this section we will see the tremendous advan-tages of using heterostructure concepts in bipolar transistors. In the BJT, once a material systemis chosen the only flexibility one has in the device design is the doping levels and the devicedimensions. This is not optimum for high-performance devices. Let us examine the materialparameters controlling the device performance parameters. We have seen that for the narrowbase width case

α =

[1 − peoDeWbn

nboDbLe

] [1 − W 2

bn

2L2b

](6.5.1)

and the current gain β is

β =α

1 − α(6.5.2)

We have already noted that for β to be high, it is essential that: (i) the emitter doping be muchhigher than the base doping, i.e., for an npn device (neo � pbo); and (ii) the base width be assmall as possible. In fact, the product pboWb, called the Gummel number, should be as small aspossible. However, a small base with relatively low doping (usually in BJTs neo ∼ 102-103pbo)introduces a large base resistance, which adversely affects the device performance. From thispoint of view, the Gummel number should be as high as possible.

One may argue that the emitter should be doped as much as possible maintaining neo � pbo

and yet having a high enough base doping to ensure low base resistance. However, a seriousproblem arises from the bandgap shrinking of the emitter region that is very heavily doped.

If we assume that hole injection across the EBJ is a dominant factor, the current gain of thedevice becomes

β =α

1 − α nboDbLe

peoDeWbn(6.5.3)

If the emitter bandgap shrinks by |ΔEg| due to doping, the hole density for the same dopingchanges by an amount that can be evaluated using the change in the intrinsic carrier concentra-tion,

nie (Eg − |ΔEg|) = nie (Eg) exp

( |ΔEg|2kBT

)(6.5.4)

where ΔEg is positive in our case. Thus the value of peo changes as

peo (Eg − |ΔEg|) ∝ n2ie (Eg − |ΔEg|) (6.5.5)

= peo (Eg) exp

( |ΔEg|kBT

)(6.5.6)

The bandgap decrease with doping is given for Si by (Nd is in units of cm−3)

|ΔEg| = 22.5

(Nd

1018· 300

T (K)

)1/2

meV (6.5.7)

266 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

The expression is reasonable up to a doping of 1019cm−3. At higher doping levels, thebandgap shrinkage is not so large. For example, at a doping of 1020 cm−3the shrinkage is ∼160 meV and not 225 meV as given by the equation above. As a result of the bandgap decrease,the gain of the device decreases according to the equation

β =DbNdeLe

DeNabWbnexp

(−|ΔEg|

kBT

)(6.5.8)

were we have assumed full ionization, i.e.

peo

nbo=

Nab

Nde(6.5.9)

As a result of this for a fixed base doping, as the emitter doping is increased, initially the currentgain increases, but then as bandgap shrinkage increases, the current gain starts to decrease. Fromthe discussion above, it is clear that the conflicting requirements of heavy emitter doping, lowbase doping, small base width, etc., as shown in figure 6.11, cannot be properly met by a BJT inwhich the same bandgap semiconductor is used for the emitter and the base. This led Shockleyand Kroemer in the 1950s to conceive of the heterojunction bipolar transistor (HBJT or HBT),where the emitter is made from a wide-gap material. In a typical HBT the emitter is made froma material that has a bandgap that is, say, > 0.2 eV larger than the bandgap of the material usedin the base. Near the base side, the emitter material composition is graded so that there is asmooth transition in the bandgap from the emitter side to the base side. A typical example ofan HBT structural layout is shown in figure 6.12a. In the case shown, the emitter material isAlGaAs, which has a larger bandgap than GaAs, used for the base and the collector. We havediscussed the heterojunction in detail in section 5.6. There we realized that the maximum benefitis obtained by grading the E-B junction such that the full bandgap differential can be used.

In figure 6.12b we show the band profile for the emitter and the base region. We can see thatif ΔEg is the bandgap difference between the emitter material bandgap and the base materialbandgap, this difference appears across the valence band potential barrier, seen by holes. Thus,holes in the base see an increased barrier for injection into the emitter. As a result, the emitterefficiency dramatically increases. The suppression of hole injection current is given by

IEp(HBT )

IEp(BJT )= exp

(−ΔEg

kBT

)The gain β in the device increases by the exponential factor. We have for β in an HBT

β =DbNdeLe

DeNabWbnexp

(ΔEg

kBT

)[1 − w2

bn

L2b

](6.5.10)

Typically the values of ΔEg/kBT are ∼ 10, so that β improves by∼ 104. Due to the heavydoping now allowed in wide emitter HBTs, the base can be made narrow without too large abase resistance or the danger of punch through. This also avoids secondary effects such as Kirkeffect and Early effect discussed later.

6.5. BJT DESIGN LIMITATIONS: NEED FOR BAND TAILORING 267

CHALLENGESNEEDS

DEMANDS AND PROBLEMS FOR A

BIPOLAR JUNCTION TRANSISTOR

• High gain • High emitter efficiency • High speed

Heavy emitter doping

• Low base doping• Narrow base width

Bandgap shrinkage causing base injection

High base resistance

SOLUTION: HETEROJUNCTION BIPOLAR TRANSISTORS

Figure 6.11: Figure showing the conflicting requirements for high-performance BJTs. Het-erostructure devices offer reconciliation of all these requirements.

Example 6.1 Consider an npn GaAs BJT that has a doping ofNde = 5 × 1017 cm−3, Nab = 1017 cm−3. Compare the emitter efficiency of this devicewith that of a similarly doped HBT where the emitter is Al0.3Ga0.7As and the base isGaAs. The following parameters characterize the devices at 300 K:

Electron diffusion constant in the base, Db = 100 cm2s−1

Hole diffusion constant in the emitter, De = 15 cm2s−1

Base width, Wb = 0.5 μmBandgap discontinuity, ΔEg = 0.36 eVMinority carrier length for holes, Le = 1.5 μm

268 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

B arrier forelectron injection

B arrier forhole injection

HOMOJUNCT ION

E mitter(n)

B ase(p)

E mittern+ GaA s

n GaA lA s

p GaA s

n GaA s

n+ GaA s

n+ GaA s

L arge bandgap emitter material

Small bandgap base region

Small bandgap collector region

E mitter(n)

B ase(p)

B arrier forelectron injection

B arrier forhole injection

Ege

Egb

HE T E R OJUNCT ION

(a)

(b)

Figure 6.12: (a) A structural schematic of a heterojunction bipolar transistor made from GaAsand AlGaAs. (b) The band profile for a homojunction and heterojunction transistor. In the HBT,grading is used to avoid a potential “notch”.

For GaAs we have the emitter and base minority carrier concentrations

peo =n2

i

Nde=

(2.2 × 106)2

5 × 1017= 9.7 × 10−6 cm−3

nbo =n2

i

Nab=

(2.2 × 106)2

1017= 4.84 × 10−5 cm−3

The emitter efficiency is

γe = 1 − peoDeWb

nboDbLe= 1 − (9.7 × 10−6)(15)(0.5 × 10−4)

(4.84 × 10−5)(100)(1.5 × 10−4)

= 0.99

In the HBT, the value of peo is greatly suppressed. The new value is approximately

peo(Al0.3Ga0.7As) =n2

i (GaAs)

Ndeexp

(−ΔEg

kBT

)= peo(GaAs) exp

(−ΔEg

kBT

)= 9.4 × 10−12 cm−3

In this case the emitter efficiency is essentially unity.

6.5. BJT DESIGN LIMITATIONS: NEED FOR BAND TAILORING 269

6.5.1 The Generalized Moll-Ross Relationship

This very important relationship first developed by Moll and Ross, and subsequently gener-alized by Kroemer, is derived in this section. The Moll-Ross Relationship links the collectorcurrent density to the applied base-emitter voltage VBE and to the Gummel number QG. It is avery powerful relationship, since it shows that the nature of the doping in the base is inconse-quential as far as the output current is concerned. Rather, the total number of dopants in the baseis the controlling factor. Kroemer’s generalization expands this to heterostructure devices.

Let us assume an n-p-n transistor with a high current gain such that the hole current Jp ≈ 0.In the base of the transistor, we can write

Jn = μnndEFn

dx(6.5.11)

and

Jp = μppdEFp

dx(6.5.12)

Since Jp is assumed to be approximately zero, dEF p

dx ≈ 0, and so equation 6.5.12 can be rewrittenas

Jn = μnnd

dx(EFn − EFp) (6.5.13)

Inserting Einstein’s relationship

μn = Dne

kBT(6.5.14)

and using the relations

EFn − Ei = kBT ln

(n

ni

)(6.5.15)

and

Ei − EFp = kBT ln

(p

ni

)(6.5.16)

we getd

dx

[ln

(np

n2i

)]=

Jn

eDnn(6.5.17)

or

d

[ln

(np

n2i

)]=

Jn

e· p

Dnn2i

· dx (6.5.18)

Let us integrate equation 6.5.18 from x = 0 to the edge of the neutral base x = Wbn.

np

n2i

∣∣∣∣Wbn

− np

n2i

∣∣∣∣x=0

= − np

n2i

∣∣∣∣x=0

=Jn

e

∫ Wbn

0

p(x)

Dnn2i

dx (6.5.19)

Here, because of Shockley boundary conditions, we have assumed np/n2i

∣∣Wbn

can be neglected.

The quantity np/n2i

∣∣x=0

is given by the law of the junction

np

n2i

∣∣∣∣x=0

= exp

(eVBE

kBT

)(6.5.20)

270 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

This leads to the generalized Moll-Ross relation

Jn = −e · exp

(eVBE

kBT

)∫ Wbn

0

(p(x)

Dnn2i

)dx

(6.5.21)

where the integration is over the extent of the neutral base. In the case where ni and Dn areconstant throughout the base, or equivalently the material is homogeneous,

Jn = − eDnn2i∫ Wbn

0p(x)dx

exp

(eVBE

kBT

)= −eDnn2

i

QGexp

(eVBE

kBT

)(6.5.22)

where

QG =

∫ Wbn

0

p(x)dx ∫ Wbn

0

Nadx (6.5.23)

is the Gummel number, defined as the total number of acceptor atoms in the neutral base.

6.5.2 How much β do we need?

This question is very important, but it really has no universal answer. Different applicationshave different minimum tolerances for β . This will be illustrated in the four examples shownbelow. Because an understanding of these applications requires some knowledge of bipolarfrequency response, it is recommended that the reader examine chapter 7 before reading thissection. We thank Prof. Mark Rodwell for discussions on this topic.

Microwave power amplifiers

In figure 6.13, we show a basic BJT small-signal model. As derived in chapter 7,

Cin = Cπ + CBE =τB + τC

re+ CBE (6.5.24)

We will assume that Cπ >> CBE , so that Cin can be written as

Cin ≈ τB + τC

re= (τB + τC) gm (6.5.25)

At a small signal frequency ω, the input current Iin is given by

Iin =

{jω [(τB + τC) gm] +

gm

β

}Vin (6.5.26)

For an efficient transistor, one wants the first term in this expression to dominate, or

ω (τB + τC) >1

β(6.5.27)

6.5. BJT DESIGN LIMITATIONS: NEED FOR BAND TAILORING 271

IntrinsicTransistor

Cin b0re

Rbb

Figure 6.13: Basic BJT small-signal model for microwave power amplifiers.

If τB + τC is the dominant delay, then we may assume τB + τC (ωT )−1. Equation 6.5.27 can

then be written asω

ωT>

1

β(6.5.28)

Since power amplifiers are rarely operated at frequencies a factor of 20 below the transit fre-quency, β ∼ 20 is in most instances adequate for these applications.

Microwave low noise amplifiers

The noise figure of low noise amplifiers is determined by the shot noise at the input. For BJTsthis is the shot noise of the base current 2eIB , while for FETs it is that of the gate current 2eIG,were IB is the base current of the BJT and IG is the reverse leakage current of the gate diodeof the FET. Since the forward bias base current IB = IC/β is typically much larger than thereverse bias current IG, the minimum noise figure attainable at low frequencies (f << fT ) islimited by β, as shown in figure 6.14. Hence a high β (typically β > 100) is desirable for lownoise applications.

Logic applications

To explain the relevant issues in logic circuits, we will use a representative logic family, CML.Let us assume one gate driving n gates, connected as shown in figure 6.15. Also assume thatnode A is at a high. In the absence of base current, the difference between the voltage high andthe voltage low ΔVL = IoRL. However, in the presence of base current, since node C is high, acurrent nIB is sourced by the node. Hence the voltage at node C is VCC −nIBRL. This reducesthe logic difference to

ΔVL = − (VCC − IoRL) + (VCC − nIBRL) = (Io − nIB) RL = Io

(1 − n

β

)RL (6.5.29)

To provide adequate noise margin, it is necessary that

n

β<< 1

272 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

FET

BJT

Fmin 1+b -1/2

1

f

Figure 6.14: Minimum noise figure versus frequency for a BJT.

RL

n

A

B

C D

RL

RL RL

Io

Io

Ib

Figure 6.15: One gate driving n gates in a CML circuit.

Typically, β ∼ 50 is desirable in such applications.

Flash analog-to-digital converters

An m-bit flash ADC is shown in figure 6.16 to illustrate the need for high β’s in comparatorsusing BJT-based differential amplifiers. These architectures are based on using N = 2m resistorsin a reference ladder connected to a reference voltage Vref and comparing each node voltage tothe input voltage Vin. If the input voltage is between Vj and Vj+1, the comparators A1 throughAj will produce a 1 at their output, and the rest will produce a zero. This output is connected viaa decoder to a digital output. It is imperative that the voltage at any node, say Vj , be a predictable

6.5. BJT DESIGN LIMITATIONS: NEED FOR BAND TAILORING 273

IB

A1

A2

IB

IB

Aj

Aj+1

IB

IB

VRef Vin

AN

Dec

oder

DigitalOutput

Rμ

Rμ

Rμ

Rμ

Rμ

Vj

Vj+1

V1

V2

VN

2m comparators

Figure 6.16: Circuit diagram of an m-bit flash analog-to-digital converter, N = 2m.

function of the number of resistors, i.e.

Vj =(j − 1)

NVref

However, the base current flowing into the comparators causes a deviation from this linear be-havior. It is clear that the nodes 1 and N have minimum deviation, since they are proximal tothe voltage supplies. However, as the nodes progress away from 1 and N toward the center ofthe array, the deviation increases because of a continuously increasing fraction of base currentIB drawn by the comparators. The maximum deviation is thus instinctively understood to be atthe center node j = N/2 and is

〈ΔV 〉 =1

8N2RuIB (6.5.30)

Therefore IB should be reduced as much as possible, and hence β should be maximized. β >100 is desirable for such applications.

274 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

6.6 SECONDARY EFFECTS IN REAL DEVICES

In the derivations of the bipolar device characteristics, we have made a number of simplifyingassumptions. There are important secondary effects that make the device characteristics deviatefrom those derived so far. These deviations have important effects on circuit design as well ason the limits of device performance.

6.6.1 High Injection: The Kirk Effect

As will be shown in our high frequency analysis of the bipolar transistor in chapter 7, in orderto achieve high frequency device operation, it is essential to operate the device at high currentdensity. The reason for this in essence is that many important delays in the transistor have theirorigin in charging capacitances of the form

C =εAj

wd(6.6.1)

where Aj is the area of the capacitor (typically the area of the p-n junction) and wd is the junctiondepletion depth. Delays in the device are of the form

τ = rj · C (6.6.2)

where

rj =∂V

∂I=

kBT

eI(6.6.3)

is the ac resistance of the junction. The delay time τ can therefore be written as

τ =kBT

eI· εAj

wd=

kBT

e

ε

wd· 1

J(6.6.4)

where J = I/Aj is the current density. Thus it is imperative to increase J if one needs to reduceτ and hence increase the maximum device operating frequency.

There is, however, a maximum current density that the device can be operated at, above whichthe β of the transistor and the device frequency response drop catastrophically. Essentially, oncethe current density reaches this maximum value, the effective base length (i.e. the length betweenthe emitter and the collector which electrons must diffuse across) becomes wider as a result ofspace-charge injection into the collector. This phenomenon is known as the Kirk Effect, and theassociated current density at which it occurs is called the Kirk Threshold , JKirk. We will nowexplain why this occurs.

The basic analysis of bipolar transistors carried out in this chapter involved applying Shock-ley boundary conditions at the reverse biased base-collector junction. Under this assumption,the minority carrier density drops to zero at the collector edge of the base region and is zeroeverywhere within the base-collector depletion region. This of course is physically not possible,because having zero minority carriers within the junction requires carriers to travel at extremelyhigh velocities as dictated by current continuity.

JC = enp,Cve (6.6.5)

6.6. SECONDARY EFFECTS IN REAL DEVICES 275

as np,C → 0

ve → ∞where np,C is the electron concentration at the base-collector junction. Since in reality the bulkvelocity in the base will saturate at some value vs, np,C cannot drop to zero, but instead drops toa value

np,C =JC

evs(6.6.6)

Because electrons in the depleted collector all travel at the saturated velocity vs, the injectedcarrier concentration in the collector will everywhere be equal to np,C , and the net charge densityin the collector

NC,net = Nd,C − np,C (6.6.7)

The resulting charge profile, as well as electric field profile in the collector region, for a deviceunder dc bias with collector doping Nd,C is shown in figure 6.17. Here we have assumed thatthe device is biased such that the n− collector region is fully depleted (this is typically the casefor bipolars in modern circuits). As indicated in figure 6.17c, the slope of the electric field in thecollector region is given by

dEdx

=eNC,net

ε(6.6.8)

We will now consider the effect that increasing the collector current density JC has on thecharge distribution and electric field in the structure. We assume that the voltage across the base-collector junction maintains a constant value VCB , implying that the total potential drop acrossthe junction is VCB + Vbi. Under this assumption, the area underneath the electric field curve infigure 6.17c always maintains a constant value VCB + Vbi. The voltage drops in the p+ and n+

regions at the edge of the base-collector depletion region are very small relative to the voltage inthe n− layer, and hence the area of the shaded region in figure 6.17c is assumed to be VCB +Vbi.Equivalently, the total base-collector depletion depth wd,BC can be assumed to be approximatelyequal to the collector width wC .

As JC increases, the injected charge density in the collector np,C must increase to maintaincurrent continuity, as indicated by equation 6.6.6. This causes the net charge in the collectorNC,net to decrease (equation 6.6.7). Hence the slope of the electric field profile in the collector,which is proportional to NC,net, decreases. At the critical current density

Jcrit = eNd,Cve (6.6.9)

the injected mobile charge np,C exactly balances the ionized donor charge Nd,C , resulting inzero net charge as well as a constant electric field in the collector (see figure 6.18). Concur-rently, the depletion region depth at the base edge xpC decreases, since the electric field at thebase edge of the collector must decrease in order for the shaded area in figure 6.17c to remainconstant. Similarly, the depletion region in the n+ subcollector xnC increases, as the region hasto terminate a higher electric field.

As JC > Jcrit, the slope of the electric field reverses sign, as NC,net = Nd,C − np,C is nownegative. This process continues until another critical current threshold is reached, when the

276 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

|E|

dEdx = e

ε (Nd,C − np,C)

Figure 6.17: (a) Schematic diagram of a typical bipolar transistor structure. The EBJ is forwardbiased, and the BCJ is reverse biased such that the collector is fully depleted. (b) Correspondingcharge profile in the device. The space charge in the device results from depletion charge (lightgray) and injected mobile charge (dark gray). (c) Electric field in the collector region.

electric field at the base-edge reaches zero (and equivalently the depletion region width xpC =0). The current density when this condition occurs is called the Kirk threshold current densityand is given the symbol JKirk. Its value can be readily calculated by solving equation 6.6.6-equation 6.6.8 subject to the conditions that the electric field at the base edge of the collector is

6.6. SECONDARY EFFECTS IN REAL DEVICES 277

JC < Jcrit

JC = Jcrit

JC = JKirk

wC xnCxpC

|E|

Figure 6.18: Electric field profile in the collector when JC < Jcrit, JC = Jcrit, andJC = JKirk. The depletion extension into the base and subcollector are labeled xpC and xnC ,respectively. xpC and xnC shown in this figure correspond to the profile with JC = Jcrit.

zero and the area underneath the electric field is VCB + Vbi. From that we get the following setof equations.

1

2EmaxwC = VCB + Vbi (6.6.10)

Emax

wC=

dEdx

=e

ε(nKirk − Nd,C) (6.6.11)

nKirk =JKirk

evs(6.6.12)

Combining these equations and solving for JKirk gives us

JKirk =

[2ε

ew2C

(VCB + Vbi) + Nd,C

]evs (6.6.13)

Let us examine the consequence of reaching the Kirk threshold. If one assumed that theprocess of electric field modification with increasing current density described in this sectionwere to continue, then a situation occurs where the direction of the electric field reverses in aregion wrev near the base-collector edge, as shown in figure 6.19a. This corresponds to the banddiagram shown in figure 6.19b. However, this is an unphysical situation for homojunctions, asthere is no blocking barrier for holes. Hence the holes from the base would flood the collector toachieve the physical situation of the holes being contained within a region ΔwB in the collector.Here, they neutralize the injected negative charge, resulting in zero electric field within thisregion. This is shown in figure 6.20.

278 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

JC > JKirk (hypothetical)

JC = JKirk

wC

(a)

EC

EF,n

EV

EF,p

(b)

eVBC

|E|

Figure 6.19: (a) Hypothetical electric field profile in the collector if the electric field were tocontinue evolving as described earlier after JC > JKirk. (b) Band diagram corresponding toJC > JKirk above.

Now, electrons diffusing across the base must diffuse over a distance wB + ΔwB beforethey are swept into the collector by the electric field in the depletion region. This effectiveextension of the base region is called base widening. The consequence is a rapid increase inbase recombination or a decrease in β for JC > JKirk. It it therefore critical that JKirk bemaximized. From equation 6.6.13, we can see that this can be achieved by

6.6. SECONDARY EFFECTS IN REAL DEVICES 279

JC > JKirk

JC = JKirk

wB

(a)

EC

EF,n

EV

EF,p

(c)

eVBC

ΔwB

eNd,C

-enp,C

injected charge

in collector

Q

(b)

holes

from base

|E|

Figure 6.20: (a) Electric field profile, (b) charge profile, and (c) band diagram in the collectorregion when JC > JKirk.

280 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

1. Minimizing wC

2. Maximizing Nd,C

3. Maximizing vs

Increasing Nd,C and decreasing wC both lead to higher electric fields in the collector, thusdecreasing the breakdown voltage. Therefore, materials with larger bandgaps and higher electronvelocity characteristics (such as InP) are preferred for collector regions.

In figure 6.1c, we showed the current-gain cutoff frequency fT versus drain current JC for astate-of-the-art InP-based bipolar transistor. Indeed, we see that initially, fT increases with JC .However, as JC becomes larger, fT saturates and eventually begins to drop once JC > JKirk.

6.6.2 High Injection: Thermal Effects

At high injection levels there is thermal heating of the bipolar device since a power level ofICVBC is dissipated. As the temperature of the device changes the current usually increasesfurther. This is due to the exponential dependence of the injection current and the increase inthe recombination time (which increases faster than the increase in the base transit time), whichincreases the base transport factor. As the current increases, a further increase in heat dissipationoccurs until the device can be burnt out if proper design considerations are not met.

6.6.3 Base Width Modulation: The Early Effect

As seen clearly in our discussion of the Kirk Effect, the quantity Wbn that appeared in ourderivation for the current-voltage characteristics is not the metallurgical base width Wb, but thedistance which electrons must diffuse before they are swept into the collector by large electricfields. For Wbn � Lb we can see from equation 6.3.17 that the collector current

IC ∝ 1

Wbn

We saw that Wbn can be affected by the collector current density IC for high injection conditions.Additionally, Wbn (and therefore IC) also vary with the applied base-collector bias VBC . Thisnon-ideal behavior is known as the Early Effect. The physical reason for it is illustrated infigure 6.21. An increase in VBC at a fixed emitter-base voltage results in an increase in the base-collector depletion width and a subsequent decrease in Wbn. This results in an increase in theslope of the minority carrier profile in the base, resulting in an increased collector current IC . Ascan be seen in figure 6.21b, the Early Effect results in a finite output resistance of the transistor,which we will now show is

Ro =VA

IC(6.6.14)

where VA is called the Early voltage.

6.6. SECONDARY EFFECTS IN REAL DEVICES 281

(b)

(a)

n - E p+ - B n- - C n+

WbnΔWbn

VBC +ΔVBC

VBC

IC

VA

ideal

characteristics

Figure 6.21: (a) Slope of the electron profile in the base increases when VBC is increased,resulting in an increase in IC . (b) Device dc I-V characteristics when Early Effect is accountedfor.

Using the Moll-Ross relationship in equation 6.5.22, the variation of IC with respect to VBC

can be written as

∂IC

∂VBC= −eDnn2

i AE exp

(eVBE

kBT

)· ∂

∂x

(1∫ Wbn

0p(x)dx

)(6.6.15)

= +eDnn2i AE exp

(eVBE

kBT

)· p(Wbn)[∫ Wbn

0p(x)dx

]2

∂(Wbn)

∂VBC(6.6.16)

Collecting terms, we can simplify this expression to

∂IC

∂VBC= −IC

[p(Wbn) · 1∫ Wbn

0p(x)dx

· ∂Wbn

∂VBC

]= − IC

VA=

IC

|VA| (6.6.17)

282 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

where

VA =

∫ Wbn

0p(x)dx

p(Wbn) ∂Wbn

∂VBC

(6.6.18)

is defined as the Early voltage. It is clear that VA is a bias-dependent quantity and hence is bestdefined for a particular base-collector voltage, which is chosen to be VBC = 0. It turns out thatfor heavily doped base regions (used in most high performance devices), the variation of VA withVBC is small.

Let us now study the expression for VA. The quantity∫ Wbn

0

p(x)dx

was defined as the Gummel number QG(cm−2). If we take the derivative of QG with respect toVBC , we get

∂QG

∂VBC=

∂

∂VBC

(∫ Wbn

0

p(x)dx

]= p(Wbn)

(∂Wbn

∂VBC

)(6.6.19)

So VA can be rewritten as

VA =QG

∂QG/∂VBC(6.6.20)

The change in base charge with respect to VBC is by definition the base-collector depletioncapacitance CBC , or

CBC =e∂QG

∂VBC(Fcm−2) (6.6.21)

Thus VA can be written as

VA =eQG

CBC(6.6.22)

Both QG and CBC are measured at VBC = 0. Variations in QG due to changes in VBC

are considered negligible, giving a constant VA independent of bias. In actuality, the outputconductance always increases with VBC because the decrease in CBC with bias tends to besmaller than the decrease in QG, since CBC is determined dominantly by the depletion layerthickness in the collector.

To minimize the output conductance, or equivalently increase the Early voltage, one mustincrease the Gummel number QG and decrease CBC . The path with least penalty is to increaseQG, because a decrease in CBC is equivalent to an increase in the collector depletion regionthickness, which in high frequency transistors may result in an unacceptable collector transitdelay.

6.6.4 Drift Effects in the Base: Nonuniform Doping

We have assumed so far that the base doping is uniform and consequently there is no built-inelectric field in the base region. In real devices the doping can be quite nonuniform, especially ifthe doping is done by ion implantation. The nonuniform doping causes a built-in field that can

6.6. SECONDARY EFFECTS IN REAL DEVICES 283

COMMON BASE:During breakdown, emitter current is not affected

COMMON EMITTER:At very low multiplication, base current starts to increase, causing the emitter current to rise, and the collector current starts to run away

12

10

8

6

4

2

00 20 40 60 80

ICBOIE = 0

IE = 10 mA

I C(m

A)

VBC (V)

12

10

8

6

4

2

00 20 40 60 80

ICEOIB = 0

IB = 0.06 mA

I C(m

A)

VEC (V)

0.05

0.04

0.03

0.02

0.01

Figure 6.22: Avalanche breakdown related characteristics of a bipolar transistor in the common-base and common-emitter configurations.

help or hinder the carriers injected into the base from the emitter. Of course, if the doping canbe made non-uniform in a controlled manner, it can be exploited to shorten the base transit time.

6.6.5 Avalanche Breakdown

Just as in the case of the p-n diode, the avalanche process limits the collector-base voltagethat the transistor can sustain. This then sets the limit on the power that can be obtained bythe transistor. The breakdown due to the impact ionization (avalanching) is reflected in theI-V characteristics of the transistor in a manner shown in figure 6.22. In the common-baseconfiguration, the breakdown occurs at a well defined collector-base voltage BVCBO. On theother hand, for the common-emitter configuration, the breakdown is not as sharply reflectedin the device output characteristics. The breakdown in the common-emitter configuration alsooccurs at a lower value of VCE than it does in the common-base configuration.

284 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

In the common-base configuration, as VCB is increased, the breakdown is essentially similarto that of a single p-n junction discussed in chapter 4. The current coming from the emitter haslittle effect on the breakdown. However, in the common-emitter configuration, as soon as theimpact ionization process starts, say, in an npn BJT, the secondary holes are injected into thebase and act as a base current, leading to increased emitter current and eventual current runawayas the process snowballs.

6.6.6 Low Injection Effects and Current Gain

In our calculations for the BJT junction currents we have assumed that in the space chargeregion, the junctions are “ideal,” i.e., there is no current flow due to recombination-generationeffects. In chapter 5, we discussed how non-ideal effects arising from recombination genera-tion in the depletion region alter the current flowing in the junction. This effect is particularlyimportant under low injection (i.e., low values of VEB) conditions.

If we examine the forward-biased EBJ for a device operating in the forward active mode, thebase current will have an “ideal” current component and a “non-ideal” current component arisingfrom generation-recombination. We can write

IB =eADenoe

Lexp

(eVEB

kBT

)+

eAniWEBJ

2τexp

(eVEB

2kBT

)where the second term is due to recombination in the emitter-base junction depletion region(WEBJ ). The recombination time is τ . The base current may be written as

IB = IS exp

(eV

mkBT

)where m is the junction ideality factor.

The collector current is not greatly influenced by the recombination-generation process. Atlow injection the recombination-generation part of the base current dominates and as a result,the current gain β is reduced. As the injection (VEB value) is increased, the recombination partbecomes negligible and the value of β reaches its ideal value calculated earlier.

In section 6.3.3 we discussed the Ebers-Moll model for bipolar transistors. This model doesnot account for some of the issues discussed in this section. A more advanced model that includesmore realistic effects is the Gummel-Poon model. Three important effects are incorporated inthe Gummel-Poon model:

• Recombination current in the emitter depletion region under low injection levels.• Reduction of current gain at high injection levels.• Finite output conductance in terms of an Early voltage, VA.

6.6.7 Current Crowding Effect

The picture we have developed for the BJT is a one-dimensional picture. In reality, the basecurrent flows along the directions perpendicular to the emitter, as can be seen from figure 6.6.

6.6. SECONDARY EFFECTS IN REAL DEVICES 285

BASE

EMITTER

Emitterterminal

Baseterminal

Cross-section

p base

n collector

n n n n n

Top view

High powerBJT device

Interdigitated finger contacts

Figure 6.23: Top view and the cross-section of a typical device using an interdigitated emitter.

There is a voltage drop IR across the base cross-section that becomes increasingly important athigh injections and high frequencies. As a result of this potential drop, the edge of the emittermay be forward biased but the “core” of the emitter region may not be forward biased. Highercurrent densities would thus flow along the edges of the emitter. This effect is called emittercrowding and, because of it, the high injection effects discussed above can be important even atlow total current values.

Emitter crowding has an adverse effect on power transistors where high current values arerequired. It is essential for these transistors that the emitter be properly designed. Computersimulation techniques are used to study the current flow so that an optimum emitter can beused. The emitter crowding effects can be suppressed by increasing the perimeter-to-area ratioof the emitter. This is often done by using long fingers for the emitter and base contacts in the“interdigitated” approach shown in figure 6.23.

Example 6.2 Consider an npn silicon transistor at 300 K with a base doping of5×1016 cm−3 and a collector doping of 5×1015 cm−3. The width of the base region is 1.0μm. Calculate the change in the base width as VCB changes from 1.0 to 5.0 V. Alsocalculate how the collector current changes and determine the Early voltage. Assume thatDb = 20 cm2/s, VBE = 0.7 V, and Wb � Lb.

286 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

The depletion width at the base-collector junction is shared between the base and thecollector region. The extent of depletion into the base side is given by

ΔWb =

{2εs(Vbi + VCB)

e

(Ndc

Nab(Nab + Ndc)

)}1/2

The built-in voltage Vbi is given by

Vbi =kBT

eln

NabNdc

n2i

= (0.026(V )) × �n(1.1 × 1012)

= 0.721 V

For an applied bias of 1 V, we get

ΔWb =

{2 × (8.84 × 10−14 × 11.9 F/cm)(1.72 V)

(1.6 × 10−19 C)× 1

5.5 × 1017 cm−3

}1/2

= 6.413 × 10−6 cm = 0.064 μm

The neutral base width is thusWbn = 0.936 μm

When the collector-base voltage increases to 5 V, we get

ΔWb = 0.117 μm

The neutral base width isWbn = 0.883 μm

In the limit of Wbn � Lb we have for the collector current density (using equation 6.3.17with sinh (Wbn/Lb) ∼ Wbn/Lb)

JC =eDbnbo

Wbnexp

(eVBE

kBT

)where

nbo =n2

i

Nab=

2.25 × 1020

5 × 1016= 4.5 × 103 cm−3

For the base-collector bias of 1 V, we have Wbn = 0.936 μm. The collector current densityis then

JC =(1.6 × 10−19 C) × (20 cm2 s−1) × (4.5 × 103 cm−3)(4.93 × 1011)

(0.936 × 10−4 cm)

= 75.8 A/cm2

When the collector-base bias changes to 5 V, the current density becomes

JC = 80.35 A/cm2

6.6. SECONDARY EFFECTS IN REAL DEVICES 287

The slope of the JC vs. VCE curve is then

dJC

dVCE

∼= ΔJC

ΔVCE

∼= 80.35 − 75.8

4Acm−2 V−1

We define the Early voltage VA through the relation

dJC

dVCE=

JC

VCE + VA

Equating the two relations, we get

VA∼= 64.9 V

Example 6.3 Consider a npn Si-BJT at 300 K with the following parameters:

Nde = 1018 cm−3

Nab = 1017 cm−3

Ndc = 5 × 1016 cm−3

Db = 30.0 cm2s−1

Lb = 15.0 μm

De = 10.0 cm2s−1

Le = 5.0 μm

(i) Calculate the maximum base width, Wb, that will allow a current gain β of 100 whenthe EBJ is forward biased at 1.0 V and the BCJ is reverse biased at 5.0 V.(ii) Describe two advantages and two disadvantages of making the base smaller.

Since the base width is much smaller than the base diffusion length, we have for theemitter and collector current

IE =

[eADbnb0

Wbn+

eADepe0

Le

] [exp(

eVBE

kBT) − 1

]

IC =

[eADbnb0

Wbn

] [exp(

eVBE

kBT) − 1

]The base current is the difference of these and the current gain β is

β =IC

IB=

Dbnb0Le

Depe0Wbn= 100

This gives for Wbn

Wbn = 1.5 × 10−4 cm

288 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

This is the neutral base width. The actual base width will be larger and we need tocalculate the depletion on the base side at the BCJ due to the biasing of the device. Sincethe EBJ is strongly forward biased, there is essentially no depletion of the base at thisjunction.

The built-in voltage on the BCJ is

Vbi =kBT

eln

(NabNdc

n2i

)= 0.8 V

Using the Vbi value we find that the depletion width on the base side of the EBJ for a 5 voltbias at the base collector junction is

ΔW (V = 5 V) = 1.59 × 10−5 cm

and the base width becomes

Wb = Wbn + 1.59 × 10−5 = 1.659 × 10−4 cm

(ii) Two disadvantages of a shorter base:• The output conductance will suffer and the collector current will have a strongerdependence on VCB .• The device may suffer punch through at a lower bias.

Two advantages:• The current gain will be higher.• The device speed will be faster.

Example 6.4 Consider a npn Si-BJT at 300 K with the following parameters:

Nde = 1018 cm−3

Nab = 1017 cm−3

Ndc = 1016 cm−3

Db = 30.0 cm2s−1

Lb = 10.0 μm

Wb = 1.0 μm

De = 10 cm2s−1

Le = 10.0 μm

Emitter thickness = 1.0 μm

Device area = 4.0 × 10−6 cm2

Calculate the emitter efficiency and gain β when the EBJ is forward biased at 1.0 V andthe BCJ is reverse biased at 5.0 V.

Calculate the output conductance of the device defined by

go =ΔIC

ΔVCB

6.6. SECONDARY EFFECTS IN REAL DEVICES 289

To solve this problem we need to calculate the neutral base width in the device. Also notethat since the emitter thickness is small compared to the carrier diffusion length in theemitter, we will use the narrow diode theory to calculate the emitter efficiency. .

Using the parameters given, the built-in voltage in the BCJ is

Vbi =kBT

eln

(1017.1016

2.25 × 1020

)= 0.757 V

The depletion width on the base side of the BCJ is found to be

δW (5.0 V) = 8.296 × 10−6 cm

andδW (6.0 V) = 8.981 × 10−6 cm

Thus the neutral base width is

Wbn(5.0 V) = 9.17 × 10−5 cm

The emitter efficiency is (for a narrow emitter of width We)

γe = 1 − pe0DeWbn

nb0DbWe= 0.969

We find that the base transport factor is

B = 1 − W 2bn

2L2b

= 0.996

This givesα = γeB = 0.9656

and the current gain is

β =α

1 − α= 28

The collector current is

IC =eADbnb0

Wbn

[exp

(eVBE

kBT

)− 1

]− eADbnb0Wbn

2L2b

[exp

(eVBE

kBT

)− 1

]with the second part being negligible.

We find thatIC(5.0 V) = 23.79 A

We now calculate the neutral base width when the BCJ is reverse biased at 6.0 V. This is

Wbn(6.0 V ) = 9.1 × 10−5 cm

This givesIC(6.0 V ) = 23.973 A

The output conductance is nowgo = 0.183 Ω−1

290 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

6.7 PROBLEMS

Temperature is 300 K unless otherwise specified.

• Section 6.3

Problem 6.1 An npn HBT, shown in figure 6.24, is illuminated leading to an opticalgeneration of 1020 1

cm3s . τN = τP = 1ns. Assume Shockley boundary conditions.

1. Assume that all the light is absorbed in the collector depletion region. How willIB , IC , and IE be different from the case where there is no illumination?

2. Now assume that all the light is absorbed in the (short) neutral base region. Againexplain how IB, IC , and IE be different from the case where there is noillumination? Assume that the emitter injection efficiency is 1.

A

Emittern

Base p

Collector n

B

Emittern

Base p

Collector n

Figure 6.24: Figure for problem 6.1.

Problem 6.2 Consider an npn transistor with the following parameters:

Db = 20 cm2 s−1 De = 10 cm2 s−1

Nde = 5 × 1018 cm−3 Nab = 5 × 1016 cm−3

Ndc = 5 × 105 cm−3 Wb = 1.0 μm

τB = τE = 10−7 s n2i = 2.25 × 1020 cm−6

A = 10−2 cm2

6.7. PROBLEMS 291

Calculate the collector current in the active mode with an applied emitter base bias of0.5 V. What is the collector current when the base current is now increased by 20%?

Problem 6.3 An Si npn transistor at 300 K has an area of 1 mm2, base width of 1.0 μm,and doping of Nde = 1018 cm−3, Nab = 1017 cm−3, Ndc = 1016 cm−3. The minoritycarrier lifetimes are τE = 10−7 = τB ; τC = 10−6 s. Calculate the collector current in theactive mode for (a) VBE = 0.5 V, (b) IE = 2.5 mA, and (c) IB = 5 μA. The base diffusioncoefficient is Db = 20 cm2s−1.

Problem 6.4 An npn silicon transistor is operated in the inverse active mode (i.e.,collector-base is forward biased and emitter base is reverse biased). The dopingconcentrations are Nde = 1018 cm−3; Nab = 1017 cm−3, and Ndc = 1016 cm−3. Thevoltages are VBE = −2 V, VBC = 0.6 V. Calculate and plot the minority carrier distributionin the device. Also calculate the current in the collector and the emitter. The deviceparameters are: Wb = 1.0 μm, τE = τB = τC = 10−7s, Db = 20 cm2s−1, De =10 cm2s−1, Dc = 25 cm2s−1, A = 1 mm2.

Problem 6.5 Calculate the error made in the emitter efficiency expression (i.e., equation6.4.7 versus equation 6.4.6) when one makes the approximation given in the text for tanh.Obtain the error as a function of the ratio of Lb to Wbn.

Problem 6.6 Plot the dependence of the base transport factor in a bipolar transistor as afunction of Wb/Lb over the range 10−2 ≤ Wb/Lb ≤ 10. Assume that the emitterefficiency is unity. How does the common-emitter current gain vary over the same range ofWb/Lb?

Problem 6.7 In an npn bipolar transistor, calculate and plot the dependence of the emitterefficiency on the ratio of Nab/Nde in the range 10−2 ≤ Nab/Nde ≤ 1. Calculate theresults for the cases: (a) De = Db, Le = Lb,Wb = Lb, and (b)De = 0.2Db, Le = 0.2Lb,Wb = 0.1Lb.

Problem 6.8 In a uniformly doped npn bipolar transistor, the following current values aremeasured (see figure 6.6 for the current definitions):

IEn = 1.2 mA IEp = 0.1 mA

IC = InC = 1.19 mA IRBE = 0.1 mA

Determine the parameters α, β, γe for the transistor.

Problem 6.9 Consider an npn bipolar transistor at 300 K with the following parameters:

Nde = 5 × 1018 s; Nab = 5 × 1016 cm−3; Ndc = 1015 cm−3

De = 10 cm2 s; Db = 15 cm2 s; Dc = 20 cm2 sτE = 10−8 s; τB = 10−7s; τC = 10−6 sWb = 1.0 μm; A = 0.1 mm2

Calculate the emitter current and the collector current as well as the values of α, γe, β forVBE = 0.6 V; VCE = 5 V.

292 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

Problem 6.10 The mobility of holes in silicon is 100 cm2/V·s. It is required that a BJT bemade with a base width of 0.5 μm and base resistivity of no more than 1.0 Ω-cm. It is alsodesired that the emitter injection efficiency be at least 0.999. Calculate the emitter dopingrequired. The various device parameters are

Lb = 10 μm

Le = 10 μm

De = 10 cm2s−1

Db = 20 cm2s−1

What is the current gain β of the device? Assume Wbn = Wb.

Problem 6.11 Consider a npn Si-BJT at 300 K with the following parameters:

Nde = 1018 cm−3

Nab = 1017 cm−3

Ndc = 5 × 1016 cm−3

Db = 30.0 cm2s−1

Lb = 15.0 μm

De = 10.0 cm2s−1

Le = 5.0 μm

(i) Calculate the maximum base width, Wb, that will allow a current gain β of 100 whenthe EBJ is forward biased at 1.0 V and the BCJ is reverse biased at 5.0 V.(ii) Describe two advantages and two disadvantages of making the base smaller.

Problem 6.12 The VCE(sat) of an npn transistor decreases as the base current increasesfor a fixed collector current. In the Ebers-Moll model, assume αF = 0.995, αR = 0.1, andIC = 1.0 mA. At 300 K, at what base current is the VCE(sat) value equal to (a) 0.2 V, (b)0.1 V?

Problem 6.13 Consider an npn bipolar device in the active mode. Express the basecurrent in terms of αF , αR, IES , ICS , and VBE , using the Ebers-Moll model.

Problem 6.14 Derive the expressions for the emitter and collector current for a pnptransistor in analogy with the equations derived in the text for the npn transistor.

Problem 6.15 An npn silicon bipolar device has the following parameters in theEbers-Moll model at 300 K:

αF = 0.99; αR = 0.2

Calculate the saturation voltage VCE for IC = 5 mA and IB = 0.2 mA. Why is IC/IB notequal to αF /(1 − αF )?

6.7. PROBLEMS 293

• Section 6.5

Problem 6.16 Consider an npn silicon bipolar transistor in whichWb = 2.0 μm, Le = Lb = 10.0 μm, and De = Db = 10 cm2s−1. Assume thatNab = 1016 cm−3. What is the emitter injection efficiency for Nde = 1018, 1019 and 1020

cm−3 when (a) bandgap narrowing is neglected, (b) bandgap narrowing is included?

Problem 6.17 A silicon npn bipolar transistor is to be designed so that the emitterinjection efficiency at 300 K is γe = 0.995. The base width is 0.5 μm andLe = 10Wb, De = Db, and Nde = 1019 cm−3. Calculate the base doping required withand without bandgap narrowing effects.

Problem 6.18 Consider a GaAs/AlGaAs HBT in which an injector efficiency of 0.999 isrequired at 300 K. The emitter and base doping are both 1018 cm−3. The base width is 0.1μm. The carrier diffusion coefficients are Db = 60 cm2s, and De = 20 cm2s. The carrierlifetimes are τB = τE = 10−8s. Calculate the Al fraction needed in the emitter of theHBT.

Problem 6.19 Due to the high base doping possible, the base of an HBT can be verynarrow. Consider a GaAs/AlGaAs HBT where the GaAs base is 500 A. The minoritycharge diffusion coefficient is 100 cm2/V·s in the base. Calculate the base transit timelimited cutoff frequency of this device.

Problem 6.20 Consider an n-p-n bipolar transistor where the base is graded fromAl0.04Ga0.96As at the emitter end to GaAs at the collector end. The emitter material isAl0.22Ga0.78As and it is graded to Al0.04Ga0.96As at the base.(a) Sketch the detailed band diagram of the HBT in equilibrium, and under forward activebias. What is the quasi-electric field, Equasi,B, in the base?(b) Solve the drift-diffusion equation to obtain an expression for the base minority carrierconcentration, n(x), in terms of the total current JC , Equasi,B, and WB . Assume μ =1000 cm2/Vs.

Problem 6.21 Due to an error during growth, the emitter-base grade in the transistorshown in the figure 6.25 below was started after the emitter n-type dopant cell shutter wasopened. As a result, there was a thin n-type GaAs region between the p-type base and thegrade.

1. Construct the equilibrium band diagram of this structure taking into account quasi-electric and electrostatic fields. What is the β of this transistor at zero emitter-basebias?

2. Now, the transistor is operated under high-injection conditions. If an emitter-basebias of 1V is applied, how will the β be affected? Draw field and potential profiles toexplain your result.

294 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

AlGaAsEg = 1.7 eV

ΔEc = 0.2 eV

n-type: 1017 cm-3

Graded region

n-type: 1017 cm-3

Base

p+ - GaAs

0.2 μm 0.1 μm

Emitter

n - GaAs

n-type: 1017 cm-3

Figure 6.25: Figure for problem 6.21.

• Section 6.6

Problem 6.22 A silicon pnp transistor at 300 K has a doping ofNae = 1018 cm−3, Ndb = 5 × 1016 cm−3, Nac = 1015 cm−3. The base width is 1.0 μm.The value of Db is 10 cm2/s and τB = 10−7 s. The emitter base junction is forward biasedat 0.7 V. Using the approximation that the minority carrier distribution in the base can berepresented by a linear decay, calculate the hole diffusion current density in the base at (a)VCB = 5 V (reverse bias), (b) VCB = 15 V.

Problem 6.23 A uniformly doped npn bipolar transistor is fabricated to withinNde = 1019 cm−3 and Ndc = 1016 cm−3. The base width is 0.5 μm. Design the basedoping so that the punch through voltage is at least 25 V in the forward active mode.

Problem 6.24 An npn silicon bipolar transistor has a base doping of 1016 cm−3 and aheavily doped collector region. The neutral base width is 1.0 μm. What is the basecollector reverse bias when punch through occurs?

Problem 6.25 The punch through voltage of a Ge pnp bipolar transistor is 20 V. The basedoping is 1016 cm−3, and the emitter and collector doping are 1018 cm−3. Calculate thezero bias base width. If τB = 10−6 s, what is the α of the transistor at a 10 V reverse biasacross the collector-base junction at 300 K? The hole diffusion coefficient in the base is 40cm2s−1.

Problem 6.26 In a silicon npn transistor, the doping concentrations in the emitter andcollector are Nde = 1018 cm−3 and Ndc = 5 × 1015 cm−3, respectively. The neutral basewidth is 0.6 μm at VBE = 0.7 V and VCB = 5 V. When VCB is increased to 10 V, theminority carrier diffusion current in the base increases by 5%. Calculate the base dopingand the Early voltage if Db = 20 cm2/s and τB = 5 × 10−7s.

6.7. PROBLEMS 295

Problem 6.27 Consider a npn Si-BJT at 300 K with the following parameters:

Nde = 1018 cm−3

Nab = 1017 cm−3

Ndc = 1016 cm−3

Db = 30.0 cm2s−1

Lb = 10.0 μm

Wb = 1.0 μm

De = 10 cm2s−1

Le = 10.0 μm

Emitter thickness = 1.0 μm

Device area = 4.0 × 10−6 cm2

Calculate the emitter efficiency and gain β when the EBJ is forward biased at 1.0 V and theBCJ is reverse biased at 5.0 V. Calculate the output conductance of the device defined by

go =ΔIC

ΔVCB

Problem 6.28 An important advance in Si bipolar transistors is the use of polysiliconemitters. If a normal ohmic contact is made to an emitter, the injected minority densitygoes to zero at the ohmic contact boundary. In polysilicon emitters, heavily dopedpolysilicon forms the contact to the emitter. The minority density does not go to zero at thepolysilicon contact, but decreases to zero well inside it. This allows one to have very thinemitter contacts for high-speed operation. Discuss the disadvantage of such a contact overa normal ohmic contact in a thin emitter. (Consider the emitter efficiency and how it isaffected by a thin emitter by using the discussions in chapter 5 on the narrow p-n diode.)

Problem 6.29 Consider an npn BJT with a base width of 0.5 μm and base doping of1017 cm−3. The hole mobility is 200 cm2/V·s. An emitter stripe of 25 μm ×100 μm isplaced to form the EBJ. If a base current of 100 μA passes in the device and the EBJ isforward biased at 0.7 V at the edge of the emitter, estimate the value of the forward bias ofthe EBJ at the middle of the emitter. Discuss the possible problems that the biasingdifference could cause. (Assume that the base current is flowing through an area 100 μm×0.5 μm.)

Problem 6.30 From our discussions of narrow p-n diodes, the importance of the boundaryconditions imposed on the injected minority charge at the contact is quite obvious. Wehave used the condition that the minority charge density goes to zero at the contact. This isa reasonable approximation for the metal contact. One approach to defining the boundaryconditions at any interface is through the concept of a recombination velocity. Therecombination velocity vrecom is defined via the relation (say, for holes as minority charge)

Jp |boundary = e vrecom δp|boundary

296 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

where the current and the excess charge are evaluated at the boundary. Using theexpression for minority current in terms of the diffusion coefficient and the charge densitygradient, we have

Dpd(δp)

dx|boundary = vrecom δp|boundary

Consider the case where an excess hole density of δp(x1) is injected across a depletionregion into an n-side. The boundary of the contact is at a position x2. The distance(x2 − x1) � Lp so that the hole concentration can be assumed to decrease linearly.Express δp(x2) in terms of the surface recombination velocity, δp(x1), and the diffusioncoefficient Dp and (x2 − x1).

Problem 6.31 Consider an npn bipolar transistor where the base is graded fromAl0.04Ga0.96As at the emitter end to GaAs at the collector end. The emitter material isAl0.22Ga0.78As and it is graded to Al0.04Ga0.96As at the base.(a) Sketch the detailed band diagram of the HBT in equilibrium, and under forward activebias. What is the quasi-electric field, EB, in the base?(b) Solve the drift-diffusion equation to obtain an expression for the base minority carrierconcentration, n(x), in terms of the total current JC, EB, and WB. Assume μ =1000 cm2/Vs.

Problem 6.32 An npn HBT has a collector consisting of slabs of two different materials,A and B. The velocity in material A is vs while that in material B is vs

2 . The thickness ofthese slabs is equal, ie. WA = WB = WC

2 , where WC is the total collector width. Assumethat the doping in the collector is ND, and that the voltage VCB depletes the entirecollector region.(a) Consider the case when slab A is adjacent to the base. Draw the charge, electric fieldand potential profiles in the collector when the Kirk threshold current is reached. What isthe Kirk threshold of this transistor? How does it compare with a transistor whosecollector is made up of material A throughout?(b) Repeat the above but now with slab B adjacent to the base. Compare the two cases andexplain the result.(c) Assume that the breakdown field in material A is less than in material B. Whichmaterial should be placed adjacent to the base to maximize the breakdown voltage underhigh injection?

Problem 6.33 For some unknown reason, possibly dislocated assisted diffusion, the basedoping in the bipolar transistor diffuses back into the collector forming a base profileshown in figure 6.26.(a) Calculate the transit time across the depletion region of the base-collector junction forthis transistor.(b) Assuming that the collector remains fully depleted, and that the current density ismeasured by the collector current divided by the collector area, how is the Kirk currentthreshold for the transistor affected? Comment on your answer. Assume vs = 107cm/sand μ = 1000cm2/V.s for electrons. Apply both the impulse function and charge control

6.7. PROBLEMS 297

B-C JUNCTION

Figure 6.26: Figure for problem 6.33.

methods to arrive at the answer. For the impulse function, make sure the impulse charge isinitiated at the base-emitter junction by the application of an impulse voltage. Think abouthow the charge density is distributed based on the fact that the base has a varying width.

Problem 6.34 An n-p-n AlGaAs-GaAs HBT is grown with the emitter-base junctiongraded from Al0.2Ga0.8As to GaAs over 0.19 μm. Assume that the emitter is doped5 × 1016 cm−3, and that the base is doped at 1018 cm−3. Assume the conduction bandoffset between Al0.2Ga0.8As and GaAs to be 0.16 eV, and the bandgap of Al0.2Ga0.8Asand GaAs to be 1.67 eV and 1.4 eV respectively.(a) Draw the equilibrium band diagram of the emitter-base junction, indicating the bandbending due to depletion charges and quasi-electric field. Calculate the depletion width ofthe junction.(b) Calculate β for this device.(c) Now, if a forward bias of 1 V is applied to this junction, what is the new depletionwidth? Calculate the conduction band profile and draw the band diagram for the device.(d) Calculate the β when the emitter-base junction is forward biased.

Problem 6.35 Consider a GaAs npn BJT with the structure shown in figure 6.27. In thisproblem, we consider the effect of a non-zero lateral base resistance, RB . The effectiveemitter base potential, VBE(x), drops along the lateral direction x (shown in the figure)

298 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

Base

Emitter

x

z

XE = 2 μm

XB = 6 μm

WB = 100 nm

LBE = 0.5 μm

LBE

Figure 6.27: Figure for problem 6.35.

changing the current gain of the transistor. Note: You may ignore the vertical baseresistance in this problem.(a) Write the expression for the minority charge, n(x, z), and integrated minority charge,q(x) =

∫n(x, z)dz (in cm−2) in the base as a function of the varying emitter-base

potential VBE(x).(b) Derive the differential equation that relates the emitter base potential VBE(x) to q(x)in terms of the base resistance, RB , and recombination time, tN . What are the boundaryconditions?(c) Using your results from (a) and (b), derive an expression for n(x, z), q(x), and the basecurrent IB(x).(d) What is the total emitter current and base current for this transistor? Find theexpression for the current gain, β, in terms of RB and tN . Assume ideal emitter injectionefficiency.

Problem 6.36 Consider an npn transistor where the base is open (figure 6.28). Assumethat the β of the transistor is not impacted by recombination in the base. Show that thebreakdown voltage, VCEO, in this configuration is reduced from the normal breakdownvoltage of the base-collector junction, VCBO. Derive an analytical expression for VCEO.State all your assumptions.

Problem 6.37 Consider a GaAs n-p-n transitor shown in figure 6.29. I make a mistake andduring the growth and insert a 10nm thick quantum well in the center of a 100 nm base.The result of this mishap is to reduce the lifetime of the injected minority carriers to 0.1 ns

6.7. PROBLEMS 299

Figure 6.28: Figure for problem 6.36.

in the quantum well region compared to 1 ns in the rest of the base. The emitter is doped at5 × 1017cm−3. The collector is doped at 5 × 1016cm−3. Assume that the elctron mobilityis 5000 cm2

V s and that the device is operate at room temperature. Calculate and sketch theelectron current and charge profile in the structure at an emitter-base bias of 0.5 eV.Compare with the case of a homogeneous base. Next, calculate the early voltage oftransistors with and without the quantum well in the base . Comment on all your solutions.

E

B

CQW

10 nm

50 nm

Figure 6.29:

Problem 6.38 Consider the transistors with two different collector doping profiles asshown in figure 6.30. Assume that the same base-collector bias, VBC , is applied in bothcases. You may also assume that the collector is fully depleted, and that the saturatedvelocity in both devices is vSAT . Calculate the difference between the current densities atthe Kirk threshold of transistors A and B. Give a physical explanation of your result usingcharge and electric field profiles.

Problem 6.39 The base-collector junction in a bipolar transistor has the structure shownin figure 6.31.

300 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

ND

W

A

ND/2

W

B

2W2W 00

Figure 6.30: Figure for problem 6.38.

p++ i n n++

0.4 μm 0.1 μm

Figure 6.31: Figure for problem 6.39

1. Draw the band diagram of this base collector junction at zero bias. Assume that thebase is heavily doped so that the entire voltage falls in the collector region. Thebuilt-in voltage is 1.4 eV.

2. Since the Γ − L valley spacing in GaAs is 0.3 eV, we would like to make the voltagedrop in the intrinsic collector adjacent to the base to be equal to that number. Thiswould lead to high electron velocities without intervalley transfer. Is it possible toachieve this by adding a single sheet of acceptors or donors to this structure? Drawcharge, electric field and energy band profiles to explain your answer. Calculate theacceptor or donor sheet charge density you would use.

6.8. DESIGN PROBLEMS 301

6.8 DESIGN PROBLEMS

Problem 6.1 Consider a npn Si-BJT at 300 K with the following parameters:

Nde = 1018 cm−3

Nab = 1017 cm−3

Ndc = 1016 cm−3

Db = 30.0 cm2s−1

Lb = 10.0 μm

Wb = 1.0 μm

De = 10 cm2s−1

Le = 5.0 μm

electron mobility in the emitter = 500 cm2 V−1 s−1

area = 5.0 × 10−7 cm2

Calculate the emitter efficiency and gain β when the EBJ is forward biased at 1.0 V andthe BCJ is reverse biased at (a): 5.0 V and (b) 10.0 V.

For high-speed operation, it is found that the BJT discussed above has too large an emitterresistance. The device designer wants to limit the emitter resistance (keeping the areaunchanged) to 2.0 Ω. Calculate the emitter efficiency and β for the new device using thecase (a) given above.

Problem 6.2 Consider a npn Si-BJT at 300 K with the following parameters:

Nde = 1018 cm−3

Nab = 1017 cm−3

Ndc = 5 × 1016 cm−3

Db = 30.0 cm2s−1

Lb = 15.0 μm

De = 10.0 cm2s−1

Le = 5.0 μm

Design the maximum base width, Wb, that will allow a current gain β of 100 when theEBJ is forward biased at 1.0 V and the BCJ is reverse biased at 5.0 V. You may make thefollowing approximations:• The reverse bias collector current is zero.• Wb is much smaller than Lb.

302 CHAPTER 6. BIPOLAR JUNCTION TRANSISTORS

Problem 6.3 Consider a npn Si-BJT at 300 K with the following parameters:

Nde = 1018 cm−3

Nab = 1017 cm−3

Ndc = 1016 cm−3

Db = 30.0 cm2s−1

Lb = 10.0 μm

Wb = 1.0 μm

De = 10 cm2s−1

Le = 10.0 μm

emitter thickness = 1.0 μm

device area = 4.0 × 10−6 cm

(a) Calculate the emitter efficiency and gain β when the EBJ is forward biased at 1.0 V andthe BCJ is reverse biased at 5.0 V.(b) Calculate the output conductance of the device defined by

go =ΔIC

ΔVCB

Problem 6.4 Consider an npn Si-BJT at 300 K with the following parameters:

Nde = 1018 cm−3

Nab = 1017 cm−3

Ndc = 5 × 1016 cm−3

Db = 20.0 cm2s−1

Lb = 15.0 μm

De = 10.0 cm2s−1

Le = 5.0 μm

emitter dimensions = 100 μm × 100 μm

(a) Calculate the base width, Wb, that will allow a current gain β of 200 when the EBJ isforward biased at 0.8 V and the BCJ is reverse biased at 5.0 V. Design the base width sothat the gain goal is achieved and the base resistance is minimum.(b) Estimate the base resistance. Note that the base hole current flows sideways into thedevice (figure 6.6). The hole mobility in the base is 300 cm2/V·s.You may make the following approximations :• The reverse bias collector current is zero.• Wb is much smaller than Lb.

6.9. FURTHER READING 303

6.9 FURTHER READING

• General

– D. A. Neaman, Semiconductor Physics and Devices, Basic Principles (Irwin, Boston,1997).

– G. W. Neudeck, The Bipolar Junction Transistor (Vol. 3 of the Modular Series onSolid State Devices, Addison-Wesley, Reading, MA, 1989).

– D. J. Roulston, Bipolar Semiconductor Devices (McGraw-Hill, New York, 1990).

– B. G. Streetman and S. Bannerjee, Solid State Electronic Devices (Prentice-Hall,Englewood Cliffs, NJ, 2000).

– D. A. Hodges and H. G. Jackson, Analysis and Design of Digital Integrated Circuits(McGraw-Hill, New York, 1988).

Chapter 7

TEMPORAL RESPONSE OFDIODES AND BIPOLARTRANSISTORS

7.1 INTRODUCTION

In chapters 4-6, we studied the dc properties of diodes and bipolar transistors. In practice,these devices are used in circuits for both digital and analog applications, such as the circuitpictured in figure 7.1. In digital circuits, the devices will constantly be switched from the “on”(conducting) state to the “off” (non-conducting) state and back. The speed at which the circuitcan process bits of data is largely determined by the switching speed of the devices.

In analog applications, the circuit is biased at some dc value, and then a small ac signal vin isapplied at the input. The input signal is amplified by the circuit, resulting in a signal vout at theoutput. The gain of the devices in the circuit is frequency dependent and compresses at higherfrequencies. Therefore, in order to design high frequency circuits, it is important to understandthe frequency response of the devices.

In this chapter, we derive the frequency response of diodes and bipolar transistors. We addressissues for both large-signal switching applications and small-signal high frequency applications.We will see that in many cases, there are trade-offs between achieving superior dc performanceand being able to operate at higher frequencies.

7.2 MODULATION AND SWITCHING OF A P -N DIODE:AC RESPONSE

In chapter 5, we discussed the dc characteristics of the p-n diode. However, many applicationsof diodes will involve transient or ac properties of the diode. The transient properties of the diode

304

7.2. MODULATION AND SWITCHING OF A P -N DIODE: AC RESPONSE 305

clock clock

clock clock

Ref Ref Ref RefRdataRef,clk Ref,clk

Rclk Rclk

to buffer

R,load

R,load R,load

R,load

R,load

R,load

RefRefRefRef Rdata Ref,clkRef,clk

R,load

R,load

L,peak

L,peak

L,peak

L,peak

L,peak

L,peak

L,peak

L,peak

Q1Q3

Q2Q4

Q5Q6

RclkRclk

Inductor

HBT

Resistor(a)

(b)

Figure 7.1: (a) Photograph of a 142 GHz master-slave latch, along with (b) the correspondingcircuit diagram. The circuit is based on the InP HBT technology illustrated in figure 7.1 Figurescourtesy of M. Rodwell and Z. Griffith, UCSB.

306 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

are usually not very appealing, especially for high-speed applications. This is one of that reasonsthat diodes have been replaced by transistors and Schottky diodes (to be discussed later) in manyapplications.

A homojunction p-n diode is a minority carrier device, i.e., it involves injection of electronsinto a p-type region and holes into an n−type region. In forward-bias conditions where thediode is in a conducting state, the current is due to the minority charge injection. In figure 7.2a,we show the minority charge (hole) distribution in the n-side of a forward-biased p-n diode. Ifthis diode is to be switched, this excess charge must be removed. The device time response,therefore, depends upon how fast one can alter the minority charge that has been injected. Infigure 7.2b we show how the minority charge can be extracted. As noted in this figure, one canspeed up the process either by introducing defects that speed up the recombination or by usingvery narrow diodes. Both these approaches have problems. A high defect density causes non-ideal diode behavior and increases reverse leakage and a narrow diode has a large reverse-biascurrent.

For the reverse-biased case, where no minority charge injection occurs, the device speed canbe quite high and is dominated by the device RC time constant. Let us examine the response ofthe p − n diode to large and small signals.

7.2.1 Small-Signal Equivalent Circuit of a p-n Diode

We will start by developing a model for the diode small-signal capacitance and resistance.The diode capacitance arises from two distinct regions of charge: i) The junction capacitancearises from the depletion region where there are regions of fixed positive and negative charge;and ii) The diffusion capacitance is due to the region outside the depletion region where minoritycarrier injection has introduced excess charges. The diffusion capacitance due to injected carriersdominates under forward-bias conditions. While in the reverse bias case the junction capacitancedominates. The small signal capacitance is in general defined by the relation

C =

∣∣∣∣dQ

dV

∣∣∣∣ (7.2.1)

It is important to note that by definition, capacitance is a lossless energy storage element.This implies that any charge which is stored in a capacitor must be reclaimable . Charge whichis lost during modulation (for example through electron-hole recombination) is not reclaimedand therefore does not contribute to the capacitance defined in equation 7.2.1. We will see in thissection that in p-n diodes, only a fraction of the stored charge is reclaimed during high frequencyoperation. This impacts the diode small-signal response.

We will now use the equations derived in chapter 4 to calculate the capacitance. The junctiondepletion width of the p-n diode is

W =

[2ε(Vbi − V )

e

(Na + Nd

NaNd

)]1/2

(7.2.2)

The depletion region charge is

|Q| = eA WnNd = eA WpNa (7.2.3)

7.2. MODULATION AND SWITCHING OF A P -N DIODE: AC RESPONSE 307

δp(x)

T = 0

Increasing time

x

(a)

How fast can minority charge be removed?

Electron-hole recombination

• τ ~ 10–6 sec forindirect gap materials• τ ~ 10-9 sec for

direct gap materials

Impurity enhanced recombination

• τ can approach a few picoseconds problems with non-ideal behavior

Short devices

• τ dominated by diffusion time problems with high reserve current

(b)

δn(x)Minority charge injection

Device response:How fast is excess minority charge removed?

Figure 7.2: (a) The minority hole distribution in a forward-biased p-n diode. If the diode is to beswitched, the excess holes have to be extracted. (b) A schematic of what controls device responseof minority-carrier-based devices. Three approaches used to speed up the device response aredescribed.

where we showed earlier (see equation 4.2.22 through equation 4.2.24)

Wn =Na

Na + NdW ; Wp =

Nd

Na + NdW (7.2.4)

Thus

|Q| =eA NaNd

Nd + NaW = A

[2eε(Vbi − V )

NdNa

Nd + Na

]1/2

(7.2.5)

308 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

The small signal junction capacitance is then

Cj =

∣∣∣∣dQ

dV

∣∣∣∣ =A

2

[2eε

(Vbi − V )

NaNd

Na + Nd

]1/2

=Aε

W=

Cjo

(1 − VVbi

)1/2(7.2.6)

where Cjo is the capacitance at zero applied bias. Since the depletion width depends upon theapplied bias, the diode capacitance can be tailored electronically. This voltage-dependent diodecapacitor is called a varactor is useful for tuning frequency of a resonant cavity electronically.

In real diodes, the doping in the n-side and p-side gradually changes from n−type to p−type.In such cases, the depletion capacitance of the diode is written as

Cj =Cjo(

1 − VVbi

)m (7.2.7)

where m is a parameter called the grading parameter. For abrupt junctions, m = 1/2 as can beseen in equation 7.2.6. For linearly graded junctions, m = 1/3.

For the forward-biased diode, the injected charge density can be large and can dominate thecapacitance. The injected hole charge is (see Eqn. 5.3.12 for the forward bias hole current;remember that charge is Iτp and use τpDp = L2

p; we also ignore 1 in the forward-bias state)

Qp = Iτp = eA Lppn eeV/kBT (7.2.8)

The diffusion capacitance is then

dQp

dV=

e2

kBTA Lppn eeV/kBT =

e

kBTIτp (7.2.9)

Using the diode equation for small-signal ac response, the ac conductance of the diode is

Gs =dI

dV=

e

kBTI(V ) (7.2.10)

from the definition of the I(V ) function. We will show later that this expression only holds atlow frequencies. At room temperature the conductance is (rs is the diode resistance)

Gs =1

rs=

I(mA)

25.86Ω−1 (7.2.11)

Consider now a p-n diode that is forward-biased at some voltage Vdc, as shown in figure 7.3a. Ifan ac signal is now applied to the diode, the current changes as shown schematically. The smallsignal equivalent circuit of the diode is shown in figure 7.3b and consists of the diode resistancers (= G−1

s ), the junction capacitance, and the diffusion capacitance. At first glance, it would

7.2. MODULATION AND SWITCHING OF A P -N DIODE: AC RESPONSE 309

appear that the diffusion capacitance in figure 7.3b is given by equation 7.2.9. However, thisis not the case, since when an ac signal is applied, not all of the injected minority charge isreclaimed through the junction. Some of the charge simply recombines in the neutral region. Inthe forward-bias condition, the diffusion capacitance will dominate and we have the followingrelation between the current is and the applied voltage signal vs:

is = Gsvs + Cdiffdvs

dt(7.2.12)

If we assume an input voltage with frequency ω (vs ∼ vos exp (jωt)), we get

is = Gsvs + jωCdiffvs (7.2.13)

and the admittance of the diode becomes

y =isvs

= Gs + jωCdiff (7.2.14)

To find Gs and Cdiff in equation 7.2.14. it is necessary to calculate the admittance y bysolving the time-dependent continuity equation, and then Gs and Cdiff can be extracted. Wefirst solve the continuity equation to find the ac part of the injected charge distribution when abias V (t) = Vdc + vo

s exp (jωt) is applied to the diode. From this we can determine the acpart of the current and thus calculate the admittance. The general form for the time-dependentcontinuity equation is

∂p

∂t= −1

e∇ · J + G − R (7.2.15)

We assume here that we have a wide base diode (base >> (Dpτp)1/2), and we are applying a

voltage V (t) = Vdc + vos exp (jωt). The continuity equation then takes the form

eA∂ (Δp)

∂t= −eA

Δp

τp− ∂Ip

∂x(7.2.16)

Assuming our current Ip is purely diffusion (Ip = −eADpd(Δp)

dx ), the continuity equation be-comes

∂ (Δp)

∂t= −Δp

τp+ Dp

∂2 (Δp)

∂x2(7.2.17)

Under dc bias, the left hand side of this equation is zero, and our solution was given by

(Δp)dc = Δp (0) e−x/Lp (7.2.18)

where x = 0 is at our depletion region edge and Lp = (Dpτp)1/2. When an ac signal is added,

we assume a solution of the form

Δp = (Δp)dc + (Δp)ac = Δp (0) e−x/Lp + Δp(x)ejωt (7.2.19)

310 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

Cp

(a) (b)

Input ac signal vs

Vdc

isI

Cj Cdiffrs

Rs

Diode equivalent circuit

Figure 7.3: (a) A p-n diode is biased at a dc voltage Vdc and a small signal modulation is appliedto it. (b) The equivalent circuit of a forward-biased diode

where Δp(x) is the amplitude of the ac hole concentration due to the small signal. Plugging thisback into equation 7.2.16 and simplifying, we get

jωΔp(x) = −Δp(x)

τp+ Dp

d2(Δp(x)

)dx2

(7.2.20)

Equation 7.2.19 allows us to solve for the ac part of the injected charge distribution. Thegeneral solution to this equation is

Δp(x) = C1e−x/λ + C2e

+x/λ (7.2.21)

where λ is the ac diffusion length and is given by

λ =

[jω

Dp+

1

Dpτp

]−1/2

(7.2.22)

Applying appropriate boundary conditions (Δp = 0 when x → ∞ and Δp = Δp(0) whenx = 0) results in

C2 = 0 (7.2.23)

C1 = Δp(0) (7.2.24)

and the ac injected charge distribution becomes

(Δp)ac =

[Δp(0) exp

(−x

√jω

Dp+

1

Dpτp

)]exp (jωt) (7.2.25)

7.2. MODULATION AND SWITCHING OF A P -N DIODE: AC RESPONSE 311

Δp(0) can be calculated by noting that the total injected charge at x = 0, Δptot(0), is the sum

of the dc and ac components(Δpdc(0) = pn0 exp

[eVdc

kBT

]).

Δptot(0) = Δpdc(0) + Δp(0) = pn0 exp

(e (Vdc + vs)

kBT

)= pn0 exp

(eVdc

kBT

)exp

(evs

kBT

)= Δpdc(0) exp

(evs

kBT

)(7.2.26)

Since we are assuming vs to be small, exp(

evs

kBT

) 1 + evs

kBT . Inserting this into equation

7.2.25 and solving for Δp(0) gives us

Δptot(0) = pn0eeVdckBT

(1 +

evs

kBT

)(7.2.27)

Δp(0) = Δpdc(0) · evs

kBT(7.2.28)

Notice that the time-independent part of the ac injected charge in equation 7.2.25 has the sameform as the dc injected charge, only with a complex diffusion length, λ. It is interesting to notethat λ is frequency dependent; when ω = 0, λ = Lp, and as ω increases, λ decreases, since theinjected charge can be reduced via reclamation through the junction during the negative swingof the ac voltage.

Using the results of equation 7.2.25 and equation 7.2.28, we can find the current is that resultsfrom our applied voltage signal vs. The total current is is given by the diffusion current at x = 0.

is = −eADpdΔp(x)

dx

∣∣∣∣∣x=0

= eADpΔp(0)

√jω

Dp+

1

Dpτp(7.2.29)

=eaDp

LpΔpdc(0) · evs

kBT

√1 + jωτp (7.2.30)

=eIvs

kBT

√1 + jωτp (7.2.31)

From this equation, we calculate the small signal admittance

y =isvs

=eI

kBT

√1 + jωτp (7.2.32)

The admittance, as well as the small signal parameters Cdiff and Gs, take different forms atlow frequencies (ωτp < 1) and at high frequencies (ωτp > 1). At low frequency, the admittanceis

y eI

kBT

[1 +

jωτp

2

](7.2.33)

312 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

and Gs and Cdiff are given by (see equation 7.2.14)

Gs =eI

kBT(7.2.34)

Cdiff =e

2kBTIτp =

1

2

(dQp

dV

)(7.2.35)

While the diode conductance Gs is the same for low frequency ac response as its value at dc

(equation 7.2.10), we see that the diffusion capacitance Cdiff = 12

(dQp

dV

)(see equation 7.2.9),

indicating that only half of the injected charge is reclaimed through the junction. The other halfrecombines in the neutral region. A similar analysis can be carried out for narrow base diodes toshow that in that case, 2/3 of the injected charge is reclaimed through the junction. In general,the diffusion capacitance of the small-signal description can be written as

Cdiff = Ke

kBTIτp (7.2.36)

where K is a factor which is 1/2 for long base diodes and 2/3 for narrow base devices.At high frequencies, the admittance becomes

y eI

kBT

√jωτp =

eI

kBT

√ωτp

2+ jω

eI

kBT

√τp

2ω(7.2.37)

and Gs and Cdiff are given by

Gs =eI

kBT

√ωτp

2(7.2.38)

Cdiff =eI

kBT

√τp

2ω(7.2.39)

We see that at high frequencies both the small signal resistance rs = G−1s and capacitance Cdiff

decrease with ω as 1√ω

.In figure 7.3b we show the equivalent circuit of a packaged diode where we have the additional

series resistance Rs associated with the diode n and p−type neutral regions and a capacitanceCp associated with the diode packaging. As discussed, at forward bias the diffusion capacitancedominates, while at reverse bias the junction capacitance is dominant.

7.2.2 Switching characteristics of diodes

In many approaches the diode is switched from the conducting state to its non-conductingstate. Large-signal switching occurs in digital technology, in pulse shaping, and in optoelectron-ics. Accurate time responses of current to voltage switching are complex series solutions to thetime-dependent semiconductor equations. However, simplified approaches give a good insightto the problem and will be discussed.

7.2. MODULATION AND SWITCHING OF A P -N DIODE: AC RESPONSE 313

In the forward-biased state, minority charge is injected across the depletion region. In thereverse-bias state, the excess minority charge is below the equilibrium value. Thus in diodeswitching, minority charge has to be removed and injected, and the diode temporal response iscontrolled by the time it takes to inject and remove the minority charge.

To understand the time response of the diode, we use the relationship between the excessminority charge and the current in the diode. We will assume an asymmetrically doped diode(p+ − n) so that hole lifetime will limit the device response. The total charge Qp injected intothe n-region for a long diode is

Qp = eA

∫ ∞

Wn

δpn(x)dx (7.2.40)

Using the relation between the charge and the voltage across the diode, we have

Qp = eALppno

(eeV/kBT − 1

)(7.2.41)

In steady state the current is related to the charge by

I =Qp

τp(7.2.42)

where τp is the hole recombination time. For a narrow diode the relevant time is the carrierextraction time from the neutral n-region of width Wln − Wn, which is given by:

τT =|Wln − Wn|2

2Dp(7.2.43)

A change in density with time defines the current. This give the equation

i(t) =Qp

τp+

dQp

dt(7.2.44)

where the first term is due to e − h recombination and the second is due to the change in theminority charge with time.

Turn-ON Response

We will start by examining how a p − n diode switches to its ON state. Consider the circuitof figure 7.4 where a diode is driven by a square wave pulse with the voltage switching betweenVF and VR. The voltage VF is much larger than the voltage across the diode under forward-biasconditions. Let us consider how the diode responds when the voltage pulse switches to VF . Asshown in figure 7.4a, the voltage switches at t = t1. Once the diode is forward biased, thecurrent becomes

i(t) =VF − V1

R(7.2.45)

314 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

+R

i(t)

v(t)

VR

VF

0

t1Time

–

+

–

(a)

(b)

i(t)

VFR

t1Time

(c)

t

Current in the diode reaches IF =

Increasing time

EX

CE

SS

MIN

OR

ITY

CH

AR

GE

n-side x

Δpn

0

Minority carrier density builds up on the n-side as the diode is forward biased

(d)

Voltage across the diode builds up to its final value

t1Time

t

v(t) V1 ~kBT n

t< t1

( )IFIo

TURN ON

e

∼2τp

Figure 7.4: Turn-ON characteristics of a p-n diode: (a) The voltage switches from VR to VF asshown at t = t1. (b) Current response (c) Time evolution of the minority charge injected into then-side. (d) Voltage across the p − n diode.

7.2. MODULATION AND SWITCHING OF A P -N DIODE: AC RESPONSE 315

where V1 is the voltage across the diode and is related to the minority charge by the relation (seeEqn. 5.3.5)

V1(t) = kBT ln

(p(Wn)

pn

)(7.2.46)

Since turn on voltage of the diode is small compared to VF

i(t) ∼ VF

R(7.2.47)

It is important to note that upon turn-on, the diode current reaches its peak value almost instantly,as shown in figure 7.4b.

The minority charge in the n-region increases gradually, and is controlled by diffusion, asshown in figure 7.4c. From equation 7.2.46 we see that the voltage across the diode also increasesand saturates at

V1 = kBT ln

(IF

Io

)(7.2.48)

The time taken for the voltage to saturate to V1 is approximately 2τp. The voltage across thediode starts from zero and grows to V1 as shown in figure 7.4d.

Turn-OFF

We now discuss the turn-off behavior of the diode as shown in figure 7.5a. The voltage isswitched from VF to VR at t = t2. To understand the diode response to this turn-off, we note therelation between the excess hole density on the n-side and the voltage across the diode:

δp(Wn) = pn

[exp

(eV

kBT

)− 1

](7.2.49)

An important outcome of this equation is that as long as δp(Wn) is positive, the voltage acrossthe diode is essentially the forward bias voltage (∼ 0.7 V). The diode current is

t < t2 : i(t) = IF =VF − V1

R

t = t2 : i(t) = IR =VR − V1

R(7.2.50)

Since the diode is in the forward-biased state before the diode is reverse biased, there is excessminority charge (holes) stored in the n-side. The diode response is controlled by the rate atwhich this charge is removed. If t3 is the time at which the excess minority charge is extracted,then up to this time, the diode cannot be reverse biased (see equation 7.2.49). To examine thetime response, let us examine the charge control equations

t < t2 : i(t) = IF =Qp

τp

t = t2 : i(t) = IR =Qp

τp+

dQp

dt(7.2.51)

316 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

+R

i(t)

v(t)

VR

VF

0t2

Time t

–

+

–

(a)

(b)

i(t)

T/2t2

tt3

τsd τt

–IR

IF

0

i

I0

I

–IR

IF

Va

0

Static current

Switching current

(d)

t2

Time

t

τsdτt

VR

v(t)

V0

Diode voltage

(c)

Increasing timeEX

CE

SS

MIN

OR

ITY

CH

AR

GE

n-region x

pn

0

Current

t< t2

t =

pno

TURN OFF

Dynamic current in the diode

Figure 7.5: Turn-OFF characteristics of a p − ndiode: (a) The external voltage switches fromVF to VR at t = t2. (b) A schematic of the current in the circuit and the current path (right)superimposed on the steady state I-V of a diode. (c) Minority charge distribution change. (d)Voltage across the diode.

7.3. TEMPORAL RESPONSE OF A SCHOTTKY DIODE 317

The general solution of the equation is

Qp(t) = iRτp + Ce−t/τp (7.2.52)

To obtain the constant C, we note that at time just before t2,

Qp(t) = iF τp = iRτp + Ce−t2/τp

orC = τp (iF − iR) et2/τp (7.2.53)

The time dependence of the minority charge becomes

t > t2 : Qp(t) = τp

[iR + (iF − iR) e(t2−t)/τp

](7.2.54)

At t = t3, the entire excess minority charge is removed, i.e., Qp(t3) = 0. This gives us

iR + (iF − iR) e−(t3−t2)/τp = 0

For the long diode, we get

t3 − t2 = τp lniF − iR

iR= τsd (7.2.55)

The time (t3 − t2) it takes to remove the stored minority charge is called the storage delay timeτsd. Until this time, the diode remains forward biased. For the short diode, the time τp is replacedby the transit time defined in equation 7.2.43. We have, for the short diode,

t3 − t2 = τT lniF − iR

iR= τsd (7.2.56)

Once the minority charge has been removed, the diode reverse biases in a time controlled by thecircuit resistance and the average depletion capacitance of the diode. This time, known as thetransition time, is

τt ∼ 2.3 RCj (7.2.57)

where R is the resistance in the circuit and Cj is the average depletion capacitance.The discussion of the turn-off process is represented schematically in figure 7.5.

7.3 Temporal Response of a Schottky Diode

In chapter 5 we have examined the Schottky diode. The key difference between the Schottkydiode and the p − n diode is that the Schottky diode is a majority carrier device and as a resultminority carrier injection and extraction is not an issue. The small-signal equivalent circuit of aSchottky diode is shown in figure 7.6. One has the parallel combination of the resistance

Rd =dV

dI(7.3.1)

318 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

Cgeom

LsCd

Rd

Rs

Figure 7.6: Equivalent circuit of a Schottky diode.

and the differential capacitance of the depletion region. The depletion capacitance has the form:

Cd = A

[eNdε

2(Vbi − V )

]1/2

(7.3.2)

As noted earlier, there is no diffusion capacitance. These circuit elements are in series with theseries resistance Rs (which includes the contact resistance and the resistance of the neutral dopedregion of the semiconductor) and the parasitic inductance. Finally, one has to include the devicegeometry capacitance:

Cgeom =εA

L(7.3.3)

where L is the device length. The absence of the diffusion capacitance that dominates theforward-bias capacitance of a p-n diode allows a very fast response of the Schottky diode.

7.4 BIPOLAR JUNCTION TRANSISTORS:A CHARGE-CONTROL ANALYSIS

In our dc analysis of the bipolar transistor , we saw that when the device is under bias, currentflows through each of the terminals, and a stored charge profile is established within the structure(figure 6.8). When an ac signal is applied, the stored charge and the current are modulated.However, the stored charge cannot be modulated instantaneously; once a signal is applied, afinite amount of time is required for the corresponding charge distribution to be established.Determining the switching behavior of a bipolar transistor essentially boils down to finding the

7.4. BIPOLAR JUNCTION TRANSISTORS: A CHARGE-CONTROL ANALYSIS 319

relationship between the currents and the stored charge, the charge control model, and thendetermining the delays associated with modulation of stored charge. We shall discuss the smallsignal model of the bipolar transistor after the charge control model, since that allows the readerto better appreciate setting up the continuity equations for the minority carriers.

The charge-control model, presented in this section, establishes relationships between thecurrents and stored charge in the device. These relationships are quite useful for calculatingdelays. In section 7.5 the response of bipolar transistors to small signals is derived using thecharge-control framework.

The two junctions of the BJT can be biased in several ways to produce four operating modesfor the transistor, as was shown in figure 6.8. When the device is used for small-signal amplifica-tion, it remains biased in forward active mode. Hence, the analysis of the device in this mode issufficient for deriving the response of the device to small signals (section 7.5). For large-signalapplications, in addition to forward active mode, the device will also at times switch to saturationand cutoff modes. We will now briefly discuss behavior in all four modes and concentrate on theforward active mode in section 7.5.Forward Active ModeIn this mode the emitter-base junction (EBJ) is forward biased, while the base-collector junction(BCJ) is reverse biased. We will use the subscript F to denote various terms in the forward activemode. The currents are given by the Ebers-Moll model discussed in section 6.3.3 (eVCB � kBTin this mode):

IE = IES exp

(eVBE

kBT

)+ αRICS

IC = αF IES exp

(eVBE

kBT

)+ ICS (7.4.1)

Here we assume that the emitter and collector current have the same direction. If we expressIES exp (eVBE/kBT ) in the second equation using the first equation, we can write

IC = αF (IE − αRICS) + ICS

= αF IE + ICS (1 − αF αR) (7.4.2)

Using IE = IB + IC , we have

IC = αF IB + αF IC + ICS (1 − αF αR) (7.4.3)

or

IC =αF

1 − αFIB +

ICS (1 − αF αR)

1 − αF

= βF IB + (βF + 1) ICS (1 − αF αR) (7.4.4)

whereβF =

αF

1 − αF(7.4.5)

βF represents the forward active current gain IC/IB for the transistor.

320 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

It is useful to examine the charge in the device in the forward active mode. In figure 6.8bwe showed the minority charge injected in the emitter, base, and collector. The excess minoritycharge injected into the base region is given by

QF =eAWbnnb0

2

(exp

eVBE

kBT− 1

)(7.4.6)

We can define the collector current in terms of the excess charge by defining a time constant τF

which is the forward transit time of minority carriers through the base. We have

QF = τF IC (7.4.7)

In other words, for a collector current IC to be maintained, the excess minority charge in thebase QF must be replaced every τF seconds. As discussed in chapter 3 , the forward transit timeis

τF =W 2

bn

2Db(7.4.8)

The base current IB is due to recombination in the neutral base with the minority charge andhole injection into the emitter. These two effects can be summarized by a time constant τBF andwe can write

IB =QF

τBF(7.4.9)

The current gain is then

βF =IC

IB=

τBF

τF(7.4.10)

Now let us examine what happens when the junction voltages are modulated. Consider thetransistor connected in a common emitter configuration shown in figure 7.7. When the emitter-base voltage is increased by ΔVBE , the current and the stored charge in the device both change.The collector current increases by some amount ΔIC , causing the collector voltage vout to dropby an amount Δvout = ΔIC · RCC . This decreases the reverse bias across the base-collectorjunction, causing the base-collector depletion region to become narrower, as illustrated in fig-ure 7.7b. Additionally, because VBE has increased, the emitter-base depletion region becomesnarrower, and the injected minority charge in the base QF increases in magnitude. The variationin emitter-base and base-collector depletion widths implies a change in the amount of storedcharge in each of the depletion regions, as indicated in figure 7.7b.

Figure 7.7c shows a schematic diagram of the current at each of the three terminals. Additionalstored charge in the emitter, base, and collector regions must be supplied by the emitter, base,and collector currents. Including the current required to supply the additional stored charge, iC ,iB , and iE can be written as

iC =QF

τF− dQBC

dt

iB =QF

τBF+

dQF

dt+

dQBC

dt+

dQBE

dt

iE = iC + iB = QF

(1

τF+

1

τBF

)+

dQF

dt+

dQBE

dt(7.4.11)

7.4. BIPOLAR JUNCTION TRANSISTORS: A CHARGE-CONTROL ANALYSIS 321

VCC

RCC

voutC

B

vin E

(a)

(b)

n+ - E p - B n- - C

-ΔQBE +ΔQBE +ΔQBC BC

-ΔQF

(c)

n+ - E p - B n- - C

iB

iCiE

n+

n+

wB wd,BC

−ΔQ'

Figure 7.7: Charge control model for forward active mode. (a) Bipolar transistor biased incommon emitter configuration. (b) Charge components corresponding to a change in base-emitter voltage ΔVBE . Because of charge injection into the base-collector depletion region,ΔQBC �= ΔQ

′

BC (c) Currents at each of the three transistor terminals.

322 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

This is valid at current densities much below the Kirk threshold density (section 6.6.1) whereΔQBC ≈ ΔQ

′

BC (see figure 7.7).Reverse Active ModeIn the reverse active mode the EBJ is reverse biased while the BCJ is forward biased. Note thatbipolar devices are asymmetrically doped, i.e., Nde � Ndc, and the reverse active mode has apoor current gain. The current and excess minority charge can be written, in analogy with theforward active mode case (note that the collector is now acting as the emitter):

QR =eAWbnnb0

2

[exp

(eVBC

kBT

)− 1

]iE =

−QR

τR+

dQV E

dt

iB =QR

τBR+

dQR

dt+

dQV C

dt+

dQV E

dt

iC = −QR

(1

τR+

1

τBR

)− dQR

dt− dQV C

dt(7.4.12)

Cutoff ModeIn the cutoff mode, both junctions are reverse biased and we may write

IE = −IES + αRICS

IC = −αF IES + ICS (7.4.13)

In the cutoff mode the terminal currents are extremely small and there is an effective open circuitat the terminals.Saturation ModeIn the saturation mode the EBJ and the BCJ are both forward biased. In this case a good approx-imation to the current-voltage equations is

IE = IES exp

(eVBE

kBT

)− αRICS exp

(eVBC

kBT

)IC = αF IFS exp

(eVBE

kBT

)− ICS exp

(eVBC

kBT

)(7.4.14)

In saturation there is charge injected into the base from the emitter (QF ) and the collector (QR).The charge in the depletion region charge is negligible, since the junction voltages do not changemuch once the device is in saturation. The current-charge relations can be written as

iC =QF

τF− QR

(1

τR+

1

τBR

)− dQR

dt

iB =QF

τBF+

QR

τBR+

d

dt(QF + QR) (7.4.15)

7.4. BIPOLAR JUNCTION TRANSISTORS: A CHARGE-CONTROL ANALYSIS 323

Forward-biased EBJ

Total minority charge

Forward-biased BCJ

QA

QSQR

QF

Figure 7.8: Minority charge in the base of a BJT in saturation mode. Charge is injected fromthe emitter and the collector into the base. The figure on the right shows a representation of thecharge in terms of a uniform charge QS and charge QA.

The charges QF and QR are shown in figure 7.8. The total base charge may be written as shownon the right-hand side of figure 7.8:

QB = QF + QR

= QA + QS (7.4.16)

where QA represents the charge at the edge of saturation (EOS) and QS is the overdrive chargethat drives the device into saturation. The charge QA can be written as

QA = τF IC(EOS) = τBF IB(EOS)

IC(EOS)

IB(EOS)= βF (7.4.17)

The overdrive charge QS can be written as

QS = τSIBS (7.4.18)

where IBS is the base current over and above IB(EOS) that brings the device to the edge ofsaturation. The time τS is the weighted mean of τBF and τBR.

The static base current in saturation is

IB = IB(EOS) + IBS (7.4.19)

The instantaneous value of the base current is

iB(t) =QA

τBF+

QS

τS+

dQS

dt(7.4.20)

We can use the relationQA

τBF=

τF IC(EOS)

τBF=

IC(EOS)

βF(7.4.21)

324 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

so that we have

iB(t) − IC(EOS)

βF=

QS

τS+

dQS

dt(7.4.22)

We will see later that in the switching characteristics of the BJT, the overdrive charge and thetime constant τS appearing in the equation above play a critical role.

7.4.1 Junction Voltages at Saturation

Having discussed the various operating modes of the BJT, we will now obtain expressions forthe junction voltages as the device goes into the saturation mode. These voltages are useful instudying the behavior of BJTs for logic elements. In figure 7.9 we show a simple model of theBJT in the saturation mode. Let us apply Kirchhoff’s voltage law (KVL) to the voltage values:

VCE = VCB + VBE

= −VBC + VBE (7.4.23)

ThusVCE(sat) = VBE(sat) − VBC (7.4.24)

To obtain VBE(sat) we multiply the second of Eqns. 6.68 by αR and subtract the resultingequation from the first of Eqns. 5.68. This gives

IE − αRIC = IES(1 − αF αR)eeVBE/kBT (7.4.25)

Using IE = IB + IC , we find

IB + IC(1 − αR) = IES(1 − αF αR)eeVBE/kBT (7.4.26)

This gives for VBE(sat)

VBE(sat) =kBT

eln

[IB + IC(1 − αR)

IEO

](7.4.27)

whereIEO = IES(1 − αF αR) (7.4.28)

In a similar manner, the value of VBC(sat) is

VBC(sat) =kBT

eln

[αF IB − IC(1 − αF )

ICO

](7.4.29)

withICO = ICS(1 − αF αR) (7.4.30)

From these values of VBE(sat) and VBC(sat) we have

VCE(sat) =kBT

eln

[IB + IC(1 − αR)

αF IB − IC(1 − αF )· ICO

IEO

](7.4.31)

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 325

B

VBE(sat)

E

C

VCE(sat)

CB

E

+

–

+

–

Figure 7.9: The BJT and a simple model for a device in the saturation mode.

Note thatICO

IEO=

ICS

IES=

αF

αR(7.4.32)

The equation for VCE(sat), after some simple manipulation, can be written as

VCE(sat) =kBT

eln

[1

αR+ IC

IB

1−αR

αR

1 − IC

IB

1−αF

αF

](7.4.33)

We finally substitute for the current gains βR = αR/(1 − αR), βF = αF /(1 − αF ) to get

VCE(sat) =kBT

eln

[1

αR+ IC

IB

1βR

1 − IC

IB

1βF

](7.4.34)

Typical values of VCE(sat) from the expression derived here are ∼ 50 mV. If one adds to thisvalue the voltage drop across the neutral regions of the emitter and the collector, we find thatVCE(sat) is ∼ 0.1 V. For silicon devices typical values for the various junction voltages, are

VBE(sat) ∼ 0.8 V

VCE(sat) ∼ 0.1 V (7.4.35)

7.5 HIGH-FREQUENCY BEHAVIOR OF A BJT

An important application of bipolar transistors is in the amplification of high-frequency smallsignals. For this application, the device is biased as shown in figure 7.7a, and a signal vin is

326 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

applied at the base terminal, resulting in an output voltage vout at the collector terminal. Thedevice remains in forward active mode at all times, so the charge control framework developedfor this mode is sufficient to derive the small-signal response.

When the emitter current in the device is modulated by an amount ΔiE , the collector currentdoes not respond immediately. The delay in establishing the change in collector current ΔiC isa result of the finite time required to modulate the various stored charge elements in the device.The total emitter to collector delay τEC is given by

τEC = τBE + τB + τBC (7.5.1)

where τBE is the EBJ capacitance charging time, τB is the total delay in the quasi-neutral baseregion, and τBC is the delay associated with the base-collector capacitance (which includes thecontribution due to change in mobile charge in the collector, which is equivalent to the collectortransit delay). It will be shown later in section 7.5.3 that the current gain cutoff frequency fτ ofthe device is given by

fτ =1

2πτEC(7.5.2)

This is the maximum frequency at which it is possible to achieve current gain in the device.To calculate the delays in the device, we apply the following rule. The ratio of the change in

stored charge to the change in current is the delay associated with the element. We are interestedin the delay in setting the output current. We can write the ac portions of equation 7.4.11 as

|ΔiE | =ΔQF

τB+

ΔQBE

τBE

|ΔiC | =ΔQBC

τBC(7.5.3)

The delay element τBE can be written as

τBE =ΔQBE

ΔIE= CBE

(ΔVBE

ΔIE

)∼= CBE

(ΔVBE

ΔIC

)(7.5.4)

where (ΔVBE

ΔIC

)−1

= gm0 = (re)−1 ∼= eIC

kBT(7.5.5)

is the transconductance of the device. τBE is therefore given by

τBE = reCBE =

(kBT

eIC

)CBE (7.5.6)

The base delay τB is the time required to supply the additional charge ΔQF to the quasi-neutral base region. If we assume Shockley boundary conditions (np(wB) = 0), then τB can bewritten as

τB =w2

B

2DnB(7.5.7)

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 327

(a)wB0

Δnp(0) |ΔQF|

(b)wB0

Δnp(0) |ΔQF|

Δnp(wB)

Figure 7.10: Charge profile in the base when device is modulated. (a) Approximate base chargeprofile with Shockley boundary conditions. (b) Base charge profile when velocity saturation inthe collector is included.

where ΔQF for this case is shown in figure 7.10a. However, as we saw in the case of the Kirkeffect, the carrier density cannot drop to zero at the collector side of the neutral base. Instead,np(wB) is given by

np(wB) =IC/AE

evsat(7.5.8)

where vsat is the electron saturation velocity in the material and AE is the emitter area. If weincrease the current in the device by an amount ΔIC , the electron density at the collector sideof the base also rises, as indicated in figure 7.10b. This results in additional charge that mustbe supplied to the base region. In figure 7.10b, the charge above the dotted line is equal tothe total charge supplied when Shockley boundary conditions are assumed (figure 7.10a). Thecharge below the dotted line is the additional charge due to velocity saturation in the collector.Including velocity saturation effects, τB can be written as

τB =w2

B

2DnB+

wB

vsat(7.5.9)

In the base-collector depletion region, the change in stored charge ΔQBC results from twoseparate effects.

1. The base-collector depletion width changes due to the variation in the base-collector volt-age, as was illustrated in figure 7.1b. We will refer to the associated change in space chargeas ΔQBC1.

2. As discussed in the derivation of τB , because of velocity saturation, the mobile chargedensity in the base-collector depletion region must also increase when IC increases (thisis the origin of Δnp(wB) in figure 7.10b). Because this increased mobile charge cannotresult in a change in voltage across the depletion region (the voltage is fixed by the biasconditions), the base-collector depletion widths are adjusted by an additional amount to

328 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

RC

B

E

C

RE

AC short

Figure 7.11: Biasing circuit for calculation of τBC1.

accommodate the mobile charge. Stated differently, each electron introduced into the base-collector depletion region must be imaged at the depletion edges. Because the inducedcharge due to this effect at both ends of the depletion region is positive, the total chargeat the base end increases, while the charge at the collector end decreases in magnitude(becomes less negative). Hence referring to figure 7.7b,ΔQBC �= ΔQ

′

BC . Since thecharge at the base end (ΔQBC) is the one which must be supplied at the input to inducea change in the output current, it is this charge that we are interested in calculating. Wewill call the change in the base-collector depletion charge associated with finite electronvelocity in the collector, ΔQC .

The total change in charge in the base-collector depletion region ΔQBC = ΔQBC1 + ΔQC .We will split the base-collector delay into two components, τBC = τBC1 + τC , where

τBC1 =ΔQBC1

ΔIC(7.5.10)

τC =ΔQC

ΔIC(7.5.11)

τC is commonly referred to as the collector delay . To determine τBC1, we refer to the circuitshown in figure 7.11. Delay analysis is by convention carried out with the collector incrementallyshorted to the emitter. Assuming a change in the base-emitter voltage ΔVBE leads to a changein collector current ΔIC , we can write the following expression for ΔVBC .

ΔVBC = ΔVBE + ΔIC (RE + RC) (7.5.12)

By definition,ΔQBC1 = CBCΔVBC (7.5.13)

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 329

Inserting the above equation and equation 7.5.12 into equation 7.5.10 gives us for τBC1

τBC1 =CBCΔVBC

ΔIC=

CBC (ΔVBE + ΔIC (RE + RC))

ΔIC(7.5.14)

=

(ΔVBE

ΔIC

)CBC + (RE + RC) CBC

τBC1 = (rE + RE + RC) CBC (7.5.15)

In calculating τC , we will assume that the electron velocity profile in the base-collector deple-tion region does not necessarily need to remain constant. This would, for example, be the case ifthe material composition in the collector was varied, such as in a double heterojunction bipolartransistor structure, or in the case of non-stationary transport in short collectors. The increasedelectron concentration in the collector Δn(x) as a function of ΔIC is then given by

Δn(x) =ΔIC

AEeve(x)(7.5.16)

where AE is the emitter area and ve(x) is the electron velocity at a point x in the collector.figure 7.12 shows a schematic plot of Δn(x) in the collector for an arbitrary velocity distributionve(x).

We first need to calculate ΔQC . To do this, we find the induced charge d (ΔQC) at x = 0caused by a sheet of charge −eΔn(x)dx at a point x, and integrate from x = 0 to x = wC , asillustrated in figure 7.13a (note that we assume wd,BC wC , since the base and subcollectorare doped highly and the collector is typically fully depleted when the device is under bias).The electric field induced in the depletion region by each sheet charge element is shown infigure 7.13b. Using Gauss’ Law, we can relate d(ΔQC) and eΔn(x)dx to dE+(x) and dE−(x).

dE+(x) =d (ΔQC)

εAE(7.5.17)

dE+(x) + dE−(x) =eΔn(x)dx

ε(7.5.18)

Also, since the change in voltage in the collector due to the induced charge must be zero, thearea under dE+(x) in figure 7.13b must equal the area above dE−(x), or

x · dE+(x) = (wC − x) dE−(x) (7.5.19)

Solving for ΔE−(x) in this equation gives us

dE−(x) =

(x

wC − x

)dE+(x) (7.5.20)

We can then substitute this result into equation 7.5.18 to get

dE+(x) +

(x

wC − x

)dE+(x) =

eΔn(x)dx

ε(7.5.21)

330 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

(a)

ve(x)

wd,BC

x

(b)

|eΔn(x)|

wd,BC

x

ΔQC

CΔQ'

Figure 7.12: (a) Arbitrary velocity profile ve(x) in the base-collector depletion region. (b) In-jected charge Δn(x) corresponding to this velocity profile, along with the image charges at thedepletion edges. AE

∫ wd,BC

0|eΔn(x)|dx = ΔQC + ΔQ

′

C (charge neutrality)

Solving for dE+(x) and using equation 7.5.16 to substitute for Δn(x) gives us

dE+(x) =

(1 − x

wC

)ΔIC

εAEve(x)dx (7.5.22)

Substituting equation 7.5.17 into the equation above and integrating both sides, we can nowsolve for ΔQC .

d (ΔQC) =

(1 − x

wC

)ΔIC

ve(x)dx (7.5.23)

ΔQC = ΔIC

∫ wC

0

(1 − x

wC

)1

ve(x)dx (7.5.24)

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 331

(b)

E(x)

wC

x

(a)

|eΔn(x)|

wC

x

d(ΔQC) d(ΔQ'C)

dx

dE+(x)

dE-(x)

Figure 7.13: Induced (a) image charge and (b) electric field due to an injected sheet charge−eΔn(x)dx at a point x.

Finally, we can solve for τC .

τC =ΔQC

ΔIC=

∫ wC

0

(1 − x

wC

)1

ve(x)dx (7.5.25)

For the case of a constant electron velocity vs, τC is given by

τC =wC

2vs(7.5.26)

The delay analysis for bipolar transistors presented here accurately describes the frequencylimitations of the device and provides us with the tools required to design devices for high fre-quency operation. However, it does not give us any information about how the device willperform at frequencies less than fτ . Since these transistors will ultimately be used in circuits,we need to be able to determine the frequency response of a circuit containing these devices. Itis therefore necessary to derive a small-signal model of the device that can then be applied incircuit simulations. We will see in the next section that the discrete components of the bipolarequivalent circuit can be written in terms of the delays that we have derived.

332 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

Example 7.1 Consider an npn transistor with the following properties at 300 K:

Emitter current, IE = 1.5 mAEBJ capacitance, Cje = 2pFBase width, Wb = 0.4 μmDiffusion coefficient, Db = 60 cm2/sWidth of collector depletion region, Wdc = 2.0 μmCollector resistance, rC = 30ΩTotal collector capacitance, (Cs + Cμ) = 0.4pFSaturated electron velocity, vs = 5 × 106 cm/s

Calculate the cutoff frequency of this transistor. How will the cutoff frequency change (i)if the emitter current level is doubled? (ii) if the base thickness is halved?

The emitter resistance r′e is given by (see equation 7.5.11 for the resistance of a

forward-biased diode)

r′

e =dIE

dVBE

∼= kBT

eIE=

0.026

1.5 × 10−3= 17.3 Ω

This givesτe = r

′

eCje = (17.3)(2 × 10−12) = 34.6 ps

The base transit time is

τt =W 2

b

2Db=

(0.4 × 10−4)2

2 × 60= 13.3 ps

The collector transit time is

τC =Wdc

2vs=

(2.0 × 10−4)

1 × 107= 10 ps

The collector charging time is

τc = rc(Cμ + Cs) = 30(0.4 × 10−12) = 12 ps

The total time isτec = 34.6 + 13.3 + 10 + 12 = 69.9 ps

The cutoff frequency is

fτ =1

2πτec=

1

2π(69.9 × 10−12 s)= 2.3 GHz

If the emitter current is doubled (assuming no other change occurs), the time τe is reducedby half. This gives a cutoff frequency of 2.54 GHz. Similarly, if the base width is reducedby half, the base transit time becomes 3.3 ps and the cutoff frequency becomes 2.65 GHz.In this problem the dominant source of delay is the emitter junction.

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 333

n+ - E p - B n- - C n+

wB wd,BC

iB

iCiE

iω(0) iω(wB)

VCE

VBE (t)

Figure 7.14: Current components in a bipolar transistor when a small signal vin is applied. Thedirection of the arrows shows the direction of the electron flux.

7.5.1 Bipolar Transistor Small-Signal Equivalent Circuit

In figure 7.14, we show a schematic diagram of various current components in a bipolar tran-sistor when a small signal vin(t) is applied. The total base-emitter voltage VBE(t) is givenby

VBE(t) = Vdc + vin(t) (7.5.27)

where we assume vin(t) to be of the form

vin(t) = vωejωt (7.5.28)

This generates a small-signal current iE at the emitter. The current entering the base is denoted asiω(0). In general, iω(0) differs from iE because of the delay in the emitter-base depletion region.Electrons then continue through the base, where they undergo a transit delay τB , resulting in aflux iω(wB) leaving the base. Finally, the delay in the base-collector region results in an outputcurrent iC at the collector. We are interested in determining the output current iC as a functionof the input voltage vin.

We continue to make the assumption that the current in the base is purely diffusive and istherefore given by

iω(x) = eAEDn∂nω(x)

∂x(7.5.29)

where iω(x) and nω(x) are the position-dependent amplitudes of the ac current and charge. Thusto determine iω(x), we must first calculate nω(x). In order to do this, it is necessary to solve thetime-dependent continuity equation for electrons, which in the case of zero recombination takesthe form

∂n(x, t)

∂t= − ∂

∂x

(Ie(x, t)

−eAE

)= Dn

∂2n(x, t)

∂x2(7.5.30)

334 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

We assume solutions of the form

n(x, t) = ndc(x) + nω(x)ejωt (7.5.31)

where ndc(x) is the dc component of the current calculated above and nω(x, t) = nω(x)ejωt. Ifwe insert the ac part of equation 7.5.30 back into equation 7.5.29, the result can be written in theform

d2nω(x)

dx2=

nω(x)

λ2e

(7.5.32)

where λe is the frequency dependent diffusion length and is given by

1

λe=

√jω

Dn= (1 + j)

√ω

2Dn(7.5.33)

Assuming nω(wB) = 0 (Shockley boundary conditions), the solution for nω(x) in equation7.5.31 is given as

nω(x) = nω(0)sinh [(wB − x) /λe]

sinh [wB/λe](7.5.34)

where nω(0) is the amplitude of the the ac portion of the electron concentration at x = 0.The value of nω(0) obviously depends on the magnitude of the ac voltage, which we have

called vω . Again assuming Shockley boundary conditions, n(0, t) can be written as

n(0, t) = np0exp

[eVBE(t)

kBT

]= np0exp

(eVdc

kBT

)exp

(evωejωt

kBT

)(7.5.35)

Assuming vω is small, we can linearize the second exponential in this equation, such that

exp

(evωejωt

kBT

) 1 +

evω

kBTejωt (7.5.36)

We may then write equation 7.5.35 as

n(0, t) = ndc(0) + nω(0)ejωt (7.5.37)

where

ndc(0) = np0exp

(eVdc

kBT

)(7.5.38)

and

nω(0) = np0exp

(eVdc

kBT

)· evω

kBT= ndc(0)

evω

kBT(7.5.39)

Now that we know our ac charge distribution nω(x), we can calculate the amplitudes of theac currents iω(0) and iω(wB). If we insert nω(x) from equation 7.5.34 into equation 7.5.29 andevaluate the derivative at x = 0, we get

iω(0) = −eAEDnnω(0)

λecoth

[wB

λe

](7.5.40)

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 335

We see that the injected current amplitude is complex, indicating that the current has both aconductive (real) and capacitative (imaginary) part. If the frequency is sufficiently low such thatwB <<

√ω/(2Dn), the hyperbolic cotangent term may be expanded in the following manner:

α coth α = 1 +α2

3+ H.O.T. (7.5.41)

This gives us for iω(0)

iω(0) = −eAEDnnω(0)

wB

[1 + jω

w2B

3Dn

](7.5.42)

If we insert the expression for nω(0) from equation 7.5.38 into equation 7.5.41, we can expressiω(0) in terms of our input signal vω

iω(0) = −eAEDnndc(0)

wB

e

kBT

[1 + jω

w2B

3Dn

]vω (7.5.43)

or

iω(0) = − eIE

kBT

[1 + jω

w2B

3Dn

]vω (7.5.44)

where IE is the dc emitter current. iω(0) may also be written in the form

iω(0) = − (Gs + jωCdiff ) vω (7.5.45)

where

Gs =1

re=

eIE

kBT(7.5.46)

is the emitter-base diode conductance , and

Cdiff =2

3

∂QF

∂VBE=

2

3CB =

eAEndc(0)wB

3

e

kBT(7.5.47)

is the diffusion capacitance measured at the emitter terminal. As was discussed in section 7.2,the diffusion capacitance is 2/3 the value of the apparent diffusion capacitance (CB), since fora short-base diode only 2/3 of the charge stored in the base is reclaimable. Finally, recognizingthat CB can be written related to the base transit time τB by

τB = re · CB (7.5.48)

we may express iω(0) as

iω(0) = − 1

re

(1 + jω

2τB

3

)vω (7.5.49)

336 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

ΔJc

ΔJc=eΔn(x)Δx/τ

τ = Wc/vs

ΔQc

ΔQc

vs

Δn(x)

Wc

Δ x

x

BASE

Figure 7.15: The induced charges and collector current versus time for a sheet of charge travelingat a constant velocity vs.

Now, to calculate the flux leaving the base iω(wB), we insert nω(x) from equation 7.5.34into equation 7.5.29 and evaluate the derivative at x = wB . If we Taylor expand the result andneglect higher order terms, we can express iω(wB) as

iω(wB) = − 1

re

(1 − jω

τB

3

)vω (7.5.50)

Note that the reactive part of iω(wB) corresponds to a negative capacitance. This behaviorresults from the fact that any rise in current at the emitter end of the base appears at the collectorend with a delay of one transit time τB , as can be seen by examination of equation 7.5.49 andequation 7.5.50.

Now all that remains is to calculate the collector current iC . We showed in our time delayanalysis (see figure 7.13) that electrons which are injected into the base-collector depletion re-gion have a finite velocity and thus require a finite amount of time to transit this region. As theelectrons travel through the depletion region, they induce image charges at the depletion edges,as illustrated in figure 7.13a. The collector current is equal to the time rate of change of theinduced charge at the collector end of the depletion region.

7.5.2 Attenuation and Phase Shift of a Traveling Electron Wave

To analyze the delay introduced due to velocity saturation in the collector, we first derive thecurrent, ΔJc induced by a sheet of charge of areal density Δn(x) · Δx traveling with a velocityvs and a distance x from the edge of the base as shown in figure 7.15.

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 337

Following the analysis in section 7.5 (equation 7.5.16 through equation 7.5.26) and using

ΔJc

v(x)= eΔn(x) · Δx (7.5.51)

we see that the charge induced on the base is

ΔQc = (1 − x

Wc) · eΔn(x) · Δx (7.5.52)

and the image on the collector is by charge neutrality

ΔQ′

c = Δn(x)Δx − ΔQc = eΔn(x)Δx · x

Wc(7.5.53)

The displacement current flowing in the external circuit, ΔJc is given by

ΔJc =d

dtΔQ

′

c = eΔn(x)Δx · dx

dt· 1

Wc(7.5.54)

Using dxdt = vs we arrive at an important relationship also known as the Ramo-Shockley theorem

ΔJc =eΔn(x)Δx

τ(7.5.55)

The current carrying electrons in the collector can be assumed to comprise of several sheetcharges of magnitude Δn(x)Δx. Hence the net induced current due to the electrons will be asum (integral) of all the induced currents. The total current per unit area is therefore obtained byintegration over all sheets:

J = −e · (v/w) ·∫

n(X) · dX (7.5.56)

We apply (equation 7.5.56) to a traveling electron wave of the form

n(x, t) = n0 exp [jω(t − x/v)] (7.5.57)

It clearly corresponds to a wave of (angular) frequency ω traveling with a uniform speed v.The convection current in the plane x = 0 is evidently

iω(wB) = −en0v · exp (jωt) (7.5.58)

this is the current density that would be flowing if the capacitor were infinitesimally thin and thetransit time of the electrons through the capacitor were zero. With the help of equation 7.5.58we may write equation 7.5.57 as

n(x, t) = −(

iω(wB)

ev

)exp (−jωx/v) (7.5.59)

338 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

If this is inserted into equation 7.5.56, and the integration executed, one finds readily

J = iω(wB)exp (−jωt) − 1

−jωt(7.5.60)

where we have introduced the electron transit time through the capacitor,

τ = w/v (7.5.61)

The expression equation 7.5.60 is easily transformed into the product of an amplitude factor anda phase factor:

J = iω(wB) ·[sin(ωτ/2)

ωτ/2

]exp (−jωτ/2) (7.5.62)

The two factors following iω(wB) indicate the attenuation and the phase shift of the currentleaving the capacitor by the finite transit time through the capacitor.

We note first of all that the signal delay is only one-half the transit time of the electronsthemselves. We also note that there is an attenuation, due to the destructive interference betweendifferent portions of the traveling wave. For ω = 2π/τ the amplitude factor is zero, and nocurrent is collected at all. This is the case when the wavelength λ = 2πv/ω of the travelingwave is equal to the capacitor plate separation w.

The two terms following iω(wB) indicate that that the signal passing through the base-collectordepletion capacitor has been both attenuated and phase shifted as a result of the finite transit timethrough this region.

Substituting for iω(wB) we can express the output current iC in terms of the input signal vω .

iC = −vω

re

(1 − jω

τB

3

)· sin (ωτC)

ωτC· exp (−jωτC) (7.5.63)

If the frequency ω is sufficiently small, this may be written as

iC = −vω

re· sin (ωτC)

ωτC· exp

[−jω

(τB

3+ τC

)](7.5.64)

The device transconductance, gm, is defined as

gm =∂iC∂vω

(7.5.65)

Inserting equation 7.5.65 into equation 7.5.63, we get for the bipolar transistor transconductance

gm = gm0 · sin (ωτC)

ωτC· exp

[−jω

(τB

3+ τC

)](7.5.66)

where gm0 = r−1e is the device transconductance at dc.

The base current iB in figure 7.14 is simply the difference in iE and iC , or

iB = iE − iC = iω(0) − iC (7.5.67)

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 339

B

rπCπ CBE

CBC

gmVBE

R0

C

E

Element

re

rπ

Cπ

R0

IE

kBT

b0re

Value

IC

VA

retB+tC

Figure 7.16: Small-signal model of a bipolar transistor.

Inserting our expressions from , we get

iB = −vω

re

[(1 + jω

2τB

3

)−

(1 − jω

τB

3− jωτC

)](7.5.68)

where we have assumed ω to be small so that

iC −vω

re

[1 − jω

(τB

3+ τC

)](7.5.69)

Simplifying equation 7.5.57 gives us for iB

iB = −jω(τB + τC)

revω = −jωCπvω (7.5.70)

whereCπ =

τB + τC

re(7.5.71)

which illustrates how collector delay adds to the input capacitance.

340 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

= rπCπ CBE

CBC

Iin ( jω)

vBE

Iin ( jω) Io ( jω)

vBE gmVBE

Io ( jω)

Figure 7.17: Bipolar equivalent circuit for calculating fτ .

Now that we have derived all of the small-signal currents in the device and expressed them interms of conductive and capacitative components, it is relatively straightforward to construct asmall-signal equivalent model. This model is shown in figure 7.16.

7.5.3 Small Signal Figures of Merit

Current gain cutoff frequency fτ

As stated earlier, the current gain cutoff frequency fτ is defined as the frequency at which theshort circuit current gain becomes 1. We assumed earlier that fτ could be found by summing allthe delays in the device (see equation 7.5.1 and equation 7.5.2). We will now show why this isthe case.

The value of fτ is obtained by applying nodal analysis to the bipolar equivalent circuit forthe termination shown in figure 7.17. The input capacitance Cin = Cπ + CBE . The frequencydependent current gain of the device β (jω) is given by

β (jω) =Io (jω)

Iin (jω)(7.5.72)

We define the input impedance zin as

zin = rπ

∣∣∣∣∣∣∣∣ 1

jωCin=

rπ

1 + jωrπCin(7.5.73)

We can then write Iin and Io as

Iin (jω) =

[vBE

zin+ jωvBECBC

](7.5.74)

Io (jω) = vBE [gm − jωCBC ] (7.5.75)

Using gm = r−1e

Io (jω)

Iin (jω)=

zin

re

[1 − jωCBCre

1 + jωCBCzin

](7.5.76)

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 341

This expression reduces to

Io (jω)

Iin (jω)=

rπ

re

[1 − jωCBCre

1 + jωrπ (Cin + CBC)

](7.5.77)

Neglecting the zero introduced by reCBC , since re and CBC are both small, β (jω) can bewritten as

β (jω) =β0

1 + jωrπ (Cin + CBC)=

β0

1 + jωβ0re (Cin + CBC)(7.5.78)

or

β (jω) =β0

1 + jβ0

(ω

ωT

) (7.5.79)

where

ωT =1

re (Cin + CBC)(7.5.80)

It is readily seen that

1

ωT= re (Cin + CBC) = re [(Cπ + CBE) + CBC ]

= re (CBE + CBC) + τB + τC (7.5.81)

= τEC

where τEC is the total delay from the emitter to the collector.Let us examine our expression for β (jω) in equation 7.5.79. When ω < ωT /β0, the denomi-

nator in equation 7.5.79 is approximately equal to 1, and |β(jω)| is given by the dc current gainβ0. Once ω > ωT /β0, we can ignore the 1 in the denominator, and β(jω) is approximatelygiven by

β (jω) ωT

jω(7.5.82)

So we see that at ω = ωT , |β| = 1, or the current gain is unity. ωT is the transit frequency anddetermines the current gain cutoff frequency as ωT = 2πfτ , or

fτ =1

2πτEC(7.5.83)

Maximum frequency of oscillation fmax

fτ is a very important figure of merit because it is determined by the intrinsic delay in the de-vice and is therefore related intimately to material parameters such as carrier velocity, lifetimes,etc. However, when used as an amplifier, in many cases the device can amplify power beyondfτ , because often voltage gain can be achieved at frequencies higher than fτ . The maximumfrequency of operation beyond which the power gain is less than 1 is termed fmax. Beyond thisfrequency, the device dissipates more power than it outputs.

342 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

(a)

(b)

rπ Cin

CBC

gmVBE

vBE

rb

ib

Cin

CBC

vBE

rb

Zin

ib

ib

jωTω ib( ) V0

V0 I0

Figure 7.18: Equivalent circuit for determining (a) the input impedance and (b) the outputimpedance of a BJT biased in the common emitter configuration.

In well designed transistors, fmax is larger than fτ , though it is possible (but undesirable) tohave fmax < fτ . Since an amplifier functions by delivering power to a load, the calculationof fmax is carried out under conditions of the load being conjugately matched to the output ofthe device. Let us calculate the input and output impedances of a BJT via its equivalent circuitin the common emitter configuration. For these calculations, we refer to the circuit diagrams infigure 7.18.

The input impedance (calculated by applying a test generator at the input and an open circuitat the output as in figure 7.18a) is seen to very rapidly approach rb for

ω >1

rπCin

The circuit used in the output impedance calculation is shown in figure 7.18b. Here, the inputmay be terminated with any impedance under the assumption that

1

jωCin< rb

so that the current flow through rb is negligible. Applying a test voltage Vo, we can calculate the

7.5. HIGH-FREQUENCY BEHAVIOR OF A BJT 343

Zo CBC1

ωT CBC

Figure 7.19: Equivalent circuit representation of the output impedance Zo.

output impedance

Zo =Vo

Io(7.5.84)

From nodal analysis, we get the following expression for Io:

Io =−jωT

ω· iB + iB =

[−jωT

ω+ 1

]iB (7.5.85)

We now assume CBC << Cin, and since

iB = jωCBC (Vo − vBE)

andiB = jωCinvBE

we can combine these expressions to show that

vBE =

(CBC

Cin + CBC

)Vo

This shows that vBE << Vo, and so iB jωCBCVo.We can now write Io as a function of Vo.

Io =

[−jωT

ω+ 1

]· jωCBCVo

= [ωT CBC + jωCBC ] Vo (7.5.86)

= [Gs + jX] Vo

This shows us that the output impedance can be expressed as a resistor 1/(ωT CBC) in parallelwith a capacitor CBC , as shown in figure 7.19. The dc output conductance

R−1o =

IC

VA

344 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

Zo CBC1

ωT CBC

Figure 7.20: Equivalent circuit representation of the intrinsic device with the dominant extrinsicelements outside.

is also in parallel to the ac components in figure 7.19 but is typically very small compared to theac conductance. The transistor can now be represented as an intrinsic device with the dominantextrinsic elements outside, as shown in figure 7.20.

Power gain is always calculated for the case of a conjugately matched load ZL = Z∗o to

enable maximum power transfer to the load. The conjugately matched load ZL for the outputimpedance shown in figure 7.19 is illustrated in figure 7.21. Since the output current in the loadis one-half of the short circuit current,

iCiB

=iC(short)

2· 1

iB=

β

2(7.5.87)

The power gain can be written as

G =Pload

Pin=

|iC |2 Rload

|iB |2 Rin

=

(iCiB

)2

· 1

ωT CBC· 1

rb(7.5.88)

or

G =|β|24

· 1

ωT CBC· 1

rb(7.5.89)

Substituting |β| = ωT /ω (equation 7.5.82) and using ω = 2πf , we get

G =fτ

8πrbCBC· 1

f2(7.5.90)

fmax is defined as the frequency at which G → 1. This gives us

fmax =

√fτ

8πrbCBC(7.5.91)

where rb is the total base resistance of the device including contact resistance, sheet resistanceof the extrinsic base, and the intrinsic base resistance of the device.

7.6. BIPOLAR TRANSISTORS: A TECHNOLOGY ROADMAP 345

Zo

CBC1

ωT CBC

1

ωT CBCRL=

1

ω2CBC

ZL=Zo*

Figure 7.21: Conjugately matched load ZL (right) for the output impedance Zo shown on theleft.

7.6 BIPOLAR TRANSISTORS: A TECHNOLOGYROADMAP

In this section we will discuss some of the important design considerations in the performanceof bipolar devices. Bipolar devices must compete with the field effect transistor (FETs) and inmany respects the two classes of families carry out similar functions. This puts a tremendouspressure on the BJT and HBT device designers to design the best devices in a given materialsystem.

Bipolar devices are exploiting both fabrication techniques and new material systems to pro-duce superior devices. A survey of the development of advanced devices was given in figure 7.22.We will now give a brief overview of these developments.

7.6.1 Si Bipolar Technology

In spite of the superior performance of HBTs, the Si bipolars continue to be the workhorsedevices for both digital and some microwave applications. The advances in Si technology havecome from two directions. The first direction relates to advanced fabrication technology and thesecond one relates to the use of polysilicon as a contact for the emitters.

The fabrication-technology-related advances in Si bipolars have resulted from: (i) self-alignedemitter and base contacts, which allow extremely precise placement of the base contact next tothe emitter contact and thus reduce parasitic resistances; (ii) trench isolation, which allows verydense packing of the transistors without cross-talk. This involves etching narrow grooves aroundthe transistor down to the substrate, lining them with SiO2, and filling them with polysilicon.This greatly reduces the isolation capacitance; (iii) sidewall contact process, which dramaticallyreduces the extrinsic base collector capacitance. In this process polysilicon is used to contact thebase and is isolated from the collector by a thick oxide. The device becomes essentially one-dimensional as a result and also becomes quite symmetric between the emitter and the collector.

The second source of improvements in Si bipolar devices is the use of polysilicon to con-tact the emitter. The advantages of polysilicon over metal contacts arise from the boundary

346 CHAPTER 7. TEMPORAL RESPONSE OF DIODES AND BIPOLAR TRANSISTORS

Silicon bipolar technology• Advanced fabrication techniques are allowing devices with fT ~25GHz

Advanced fabrication techniques• Self-aligned emitter base• Trench isolation to avoid cross-talk (SiO2 fills the "trenches").• Sidewall contacts. Polysilicon is used to contact the base.• Polysilicon emitter contact provides low recombination at the contact and suppresses base injection into